ENGINEERING COMPOSITE MATERIALS Bryan Harris The Institute of Materials, London 1999
CONTENTS1 THE NATURE OF COMPOSITE MATERIALS....................................................................... 5 1.1 WHAT ARE COMPOSITES? ..............................................................................................................................5 1.2 CONVENTIONAL MATERIALS AND THEIR LIMITATIONS ..................................................................................6 1.3 STRONG FIBRES..............................................................................................................................................7 1.3.1 Glass fibres ..........................................................................................................................................8 1.3.2 Carbon fibres.......................................................................................................................................8 1.3.3 Silicon carbide.....................................................................................................................................9 1.3.4 Alumina and alumina/silica compounds............................................................................................10 1.3.5 Organic Fibres ..................................................................................................................................10 1.3.6 Styles of reinforcement ......................................................................................................................11 1.4 THE SCOPE FOR REINFORCEMENT OF CONVENTIONAL MATERIALS................................................................12 1.4.1 Functions of the matrix......................................................................................................................12 1.4.2 Metals ................................................................................................................................................13 1.4.3 Polymeric materials...........................................................................................................................13 1.4.4 Glasses, ceramics and cement ...........................................................................................................14 1.4.5 Carbon...............................................................................................................................................15 1.5 REFERENCES TO CHAPTER 1 .........................................................................................................................15 1.5.1 General bibliography ........................................................................................................................16 1.5.2 Sources of data ..................................................................................................................................172 MAKING COMPOSITE MATERIALS .................................................................................... 18 2.1 THE COMBINING OF MATERIALS ...................................................................................................................18 2.2 THE INTERFACE ...........................................................................................................................................19 2.3 MANUFACTURING PROCESSES ......................................................................................................................20 2.3.1 Polymer-matrix composites ...............................................................................................................20 2.3.2 Metal-matrix composites ...................................................................................................................22 2.3.3 Ceramic-matrix composites ...............................................................................................................23 2.3.4 Hybrid composites .............................................................................................................................24 2.4 DEFECTS IN MANUFACTURED POLYMERIC COMPOSITES ...............................................................................25 2.5 METHODS OF NON-DESTRUCTIVE EVALUATION FOR POLYMER COMPOSITES.................................................28 2.5.1 Optical inspection..............................................................................................................................28 2.5.2 Radiographic methods.......................................................................................................................28 2.5.3 Thermal imaging................................................................................................................................28 2.5.4 Ultrasonic techniques ........................................................................................................................29 2.5.5 Optical fibre sensors..........................................................................................................................29 2.5.6 Microwave methods. ..........................................................................................................................30 2.5.7 Dynamic mechanical analysis. ..........................................................................................................30 2.5.8 Acoustic emission methods. ...............................................................................................................31 2.6 THE USE OF COMPOSITES ..............................................................................................................................31 2.7 REFERENCES TO CHAPTER 2 .........................................................................................................................313 ELASTIC PROPERTIES OF FIBRE COMPOSITES............................................................. 33 3.1 SIMPLE MICROMECHANICAL MODELS ...........................................................................................................33 3.2 THE HALPIN-TSAI EQUATIONS .....................................................................................................................36 3.3 THE COMPRESSION MODULUS.......................................................................................................................38 3.4 THE ANISOTROPIC PROPERTIES OF A THIN LAMINA .......................................................................................39 3.5 ORIENTATION-DEPENDENCE OF THE ELASTIC PROPERTIES OF A UNIDIRECTIONAL LAMINA...........................42 3.6 MULTI-PLY LAMINATES................................................................................................................................44 3.7 SHORT-FIBRE COMPOSITES ...........................................................................................................................48 3.8 HYBRID COMPOSITES ...................................................................................................................................51 3.9 RESIDUAL STRAINS ......................................................................................................................................54 3.10 TEXTILE COMPOSITES ..............................................................................................................................56 3.11 PLIANT COMPOSITES ................................................................................................................................58 3.12 REFERENCES TO CHAPTER 3 ....................................................................................................................594 THE STRENGTH OF FIBRE COMPOSITES................................................................................ 61
4.1 TENSILE STRENGTH ......................................................................................................................................61 4.1.1 Unidirectional continuous-fibre composites......................................................................................61 4.1.2 The problem of the strength of brittle fibres ......................................................................................63 4.1.3 Progressive damage and failure in unidirectional composites..........................................................65 4.1.4 Calculation of the tensile strength of a unidirectional composite .....................................................67 4.1.5 Transverse strength ...........................................................................................................................69 4.1.6 Orientation-dependence of composite strength .................................................................................71 4.1.7 The strengths of multi-ply laminates..................................................................................................72 4.1.8 Short-fibre composites .......................................................................................................................75 4.1.9 Hybrid composites .............................................................................................................................79 4.2 COMPRESSION STRENGTH.............................................................................................................................80 4.2.1 Compression strength after impact....................................................................................................84 4.3 SHEAR STRENGTH ........................................................................................................................................85 4.3.1 The shear strength of the interfacial bond.........................................................................................87 4.4 FLEXURAL STRENGTH ..................................................................................................................................92 4.5 FAILURE CRITERIA FOR COMPLEX STRESSES .................................................................................................93 4.6 THE STRENGTH OF CERAMIC-MATRIX COMPOSITES ......................................................................................94 4.7 REFERENCES TO CHAPTER 4 .........................................................................................................................965 FRACTURE AND TOUGHNESS OF COMPOSITES ............................................................ 99 5.1 STRUCTURAL ASPECTS OF COMPOSITES FAILURE ...........................................................................................99 5.1.1 Fracture formalisms ..........................................................................................................................99 5.2 FRACTURE PROCESSES IN COMPOSITES .......................................................................................................100 5.2.1 Matrix effects ...................................................................................................................................100 5.2.2 Fibre effects .....................................................................................................................................101 5.2.3 Simple fibre/matrix addition effects.................................................................................................101 5.3 TOUGHNESS DERIVING FROM COMPOSITE ACTION ......................................................................................102 5.3.1 Toughening mechanisms in fibre-reinforced plastics......................................................................102 5.3.2 Toughness of hybrid composites......................................................................................................111 5.3.3 Toughness of laminated structures ..................................................................................................112 5.4 TOUGHNESS OF PRACTICAL REINFORCED PLASTIC LAMINATES ...................................................................115 5.4.1 Short-fibre composites .....................................................................................................................117 5.4.2 Design of damage-tolerant composites ...........................................................................................118 5.5 TOUGHNESS OF CERAMIC-MATRIX COMPOSITES .........................................................................................118 5.5.1 Matrix cracking ...............................................................................................................................119 5.5.2 Fibre bridging..................................................................................................................................119 5.5.3 Fibre pull-out...................................................................................................................................120 5.6 APPLICATION OF FRACTURE MECHANICS TO COMPOSITES ..........................................................................121 5.6.1 Strength of notched composites and notch sensitivity .....................................................................121 5.6.2 The application of fracture mechanics .................................................................................121 5.6.3 Application to specific composites...................................................................................................122 5.7 CONCLUSION ..............................................................................................................................................125 5.8 REFERENCES TO CHAPTER 5 .......................................................................................................................1276. FATIGUE BEHAVIOUR OF FIBRE COMPOSITES ........................................................... 130 6.1 INTRODUCTION ..........................................................................................................................................130 6.2 DAMAGE IN COMPOSITES ...........................................................................................................................131 6.2.1 Definition of failure and experimental scatter.................................................................................132 6.3 REVIEW OF SOME CLASSICAL FATIGUE PHENOMENA.................................................................................132 6.3.1 Stress/life curves ..............................................................................................................................132 6.3.2 Constant-life diagrams ....................................................................................................................133 6.3.3 Statistical aspects of the analysis of fatigue data ............................................................................133 6.3.4 Cumulative damage laws.................................................................................................................135 6.5 FATIGUE OF REINFORCED PLASTICS ...........................................................................................................136 6.4.1 Constant-stress fatigue curves.........................................................................................................136 6.4.2 Materials factors affecting fatigue behaviour of reinforced plastics...............................................139 6.4.3 Other factors affecting the fatigue of reinforced plastics ................................................................143 6.4.4 Damage accumulation and residual strength.....................................................................148 6.4.5 Fatigue under conditions of variable stress: block loading ............................................................151
6.4.6 Life prediction..................................................................................................................................152 6.5 FATIGUE OF METAL-MATRIX COMPOSITES ..................................................................................................153 6.6 FATIGUE OF CERAMIC-MATRIX COMPOSITES ..............................................................................................156 6.7 CONCLUSION ..................................................................................................................................................160 6.8 REFERENCES TO CHAPTER 6 .......................................................................................................................1607 ENVIRONMENTAL EFFECTS............................................................................................... 164 7.1 INTRODUCTION ..........................................................................................................................................164 7.2 HYGROTHERMAL SENSITIVITY OF REINFORCED PLASTICS .........................................................................166 7.2.1 Fibre effects .....................................................................................................................................166 7.2.2 Resin effects .....................................................................................................................................167 7.2.3 Composite effects .............................................................................................................................168 7.3 TIME-DEPENDENT EFFECTS ........................................................................................................................170 7.3.1 GRP in Corrosive Environments .....................................................................................................171 7.4 HIGH-TEMPERATURE STRENGTH AND CREEP OF COMPOSITES ...................................................................171 7.4.1 Introduction .....................................................................................................................................171 7.4.2 Creep ...............................................................................................................................................173 7.5 REFERENCES TO CHAPTER 7 .......................................................................................................................182APPENDIX 1......................................................................................................................................... 185 ORIENTATION-DEPENDENCE OF THE ELASTIC PROPERTIES OF A SINGLE UNIDIRECTIONAL LAMINA ......................185APPENDIX 2......................................................................................................................................... 189 STATISTICAL ASPECTS OF THE STRENGTH OF BRITTLE SOLIDS ............................................................................189 The Weibull Model..........................................................................................................................................189 REFERENCES TO APPENDIX 2 ...............................................................................................................................192APPENDIX 3......................................................................................................................................... 193 SOME APPLICATIONS OF COMPOSITES..................................................................................................................193 Aerospace .......................................................................................................................................................193 Automotive Engineering .................................................................................................................................193 BioEngineering ...............................................................................................................................................193 Chemical Engineering ....................................................................................................................................194 Civil/Structural Engineering...........................................................................................................................194 Domestic .........................................................................................................................................................194 Electrical Engineering....................................................................................................................................194 Marine Engineering........................................................................................................................................195 Sport................................................................................................................................................................195
1 THE NATURE OF COMPOSITE MATERIALS1.1 WHAT ARE COMPOSITES?C omposite materials are extending the horizons of designers in all branches of engineering, and yet the degree to which this is happening can easily pass unperceived. The eye, after all, does not see beyond the glossy exterior or the race performance of a GRP1 yacht, nor does it sense the complexity of the structure of a composite helicopter rotor blade or of a modern CFRP2 tennisracket. Nevertheless, this family of synthesized materials offers the possibility of exciting new solutionsto difficult engineering problems. In composites, materials are combined in such a way as to enable us to make better use of theirvirtues while minimising to some extent the effects of their deficiencies. This process of optimisationcan release a designer from the constraints associated with the selection and manufacture of conventionalmaterials. He can make use of tougher and lighter materials, with properties that can be tailored to suitparticular design requirements. And because of the ease with which complex shapes can bemanufactured, the complete rethinking of an established design in terms of composites can often lead toboth cheaper and better solutions. The ‘composites’ concept is not a human invention. Wood is a natural composite material consistingof one species of polymer — cellulose fibres with good strength and stiffness — in a resinous matrix ofanother polymer, the polysaccharide lignin. Nature makes a much better job of design and manufacturethan we do, although Man was able to recognize that the way of overcoming two major disadvantages ofnatural wood — that of size (a tree has a limited transverse dimension), and that of anisotropy(properties are markedly different in the axial and radial directions) — was to make the compositematerial that we call plywood. Bone, teeth and mollusc shells are other natural composites, combininghard ceramic reinforcing phases in natural organic polymer matrices. Man was aware, even from theearliest times, of the concept that combining materials could be advantageous, and the down-to-earthprocedures of wattle-and-daub (mud and straw) and ‘pide’ (heather incorporated in hard-rammed earth)building construction, still in use today, pre-date the use of reinforced concrete by the Romans whichforeshadowed the pre-tensioned and post-tensioned reinforced concretes of our own era. But it is only inthe last half century that the science and technology of composite materials have developed to providethe engineer with a novel class of materials and the necessary tools to enable him to use themadvantageously. The simple term ‘composites’ gives little indication of the vast range of individual combinations thatare included in this class of materials. We have mentioned some of the more familiar ones, but thediagram Figure 1.1 gives a clearer idea of the scope for ingenuity which is available to the MaterialsScientist and his customer, the Design Engineer. First, within each group of materials — metallic,ceramic and polymeric — there are already certain familiar materials which can be described ascomposites. Many members of the commonest and largest group of engineering materials, the family ofsteels, consist of combinations of particles of hard ceramic compounds in a softer metallic matrix. Theseparticles are sometimes plate-like, sometimes needle-shaped, and sometimes spherical or polygonal.Polymers, too, are often two-phased, consisting of a matrix of one polymer with distributions of harderor softer particles contained within it; wood is a perfect example of this, as we have seen. And concreteis a classic example of a ceramic/ceramic composite, with particles of sand and aggregate of graded sizesin a matrix of hydrated Portland cement. These materials have been well known for many years, andMaterials Scientists have learned to control their properties by controlling their microstructures; that is tosay, the quantity, the form, and the distribution of what we might refer to as the ‘reinforcing phase’. Theidea of mixing components across the materials class boundaries is a natural extension of this idea.Making additions of hard, or fire-resistant, or simply cheap, ceramic powders to plastics to make filled__________________________________________________________________________________1 GRP is the usual abbreviation for glass-fibre-reinforced plastics2 CFRP is carbon-fibre-reinforced plastic
chapter one — The nature of composites 6 METALS AND ALLOYS: metal-matrix composites, metal-filled plastics ceramic-matrix composites, steels, (particulate and fibre fill) (including ordinary reinforced aluminium alloys, copper & brasses, concrete and steel-fibre rein- titanium, etc. forced concrete) PLASTICS: CERAMICS & resins (epoxies, etc.), GLASSES thermoplastics, rubbers, glass, foams, fired ceramics, textile fibres concrete, fibre-reinforced plastics (including GRP, CFRP, glass/PTFE coated fabrics), FRP-reinforced concrete Figure 1.1. Relationships between classes of engineering materials, showing the evolution of compositespolymers; and making additions of very hard, or abrasive, or thermally stable ceramic particles to metalsto make the class of materials known as ‘cermets’ to produce machine tool tips capable of cutting hardmetals at high speeds or high temperatures; are only two examples of important developments in ourexploitation of these materials. But even more significant is the extension of this principle to incorporatefilamentary metals, ceramics and polymers into the bulk forms of any of these three classes of materialsto make fibre composites — reinforced plastics, like CFRP and GRP, metal-matrix composites (MMCs)like silicon-carbide-fibre-reinforced aluminium, and ceramic-matrix composites (CMCs) like carbon-fibre-reinforced glass. Ideally, the properties of engineering materials should be reproducible and accurately known. Andsince satisfactory exploitation of the composite principle depends on the design flexibility that resultsfrom tailoring the properties of a combination of materials to suit a particular requirement, we also needto be able to predict those properties successfully. At the present time some of the more importantengineering properties of composites can be well predicted on the basis of mathematical models, butmany cannot.1.2 CONVENTIONAL MATERIALS AND THEIR LIMITATIONS It is difficult to draw up a table of materials characteristics in order to assess the relative strengths andweaknesses of metals, plastics and ceramics because each of these terms covers whole families ofmaterials within which the range of properties is often as broad as the differences between the threeclasses. A comparison in general terms, however, can identify some of the more obvious advantages anddisadvantages of the different types of material. At a simplistic level, then:• Plastics are of low density. They have good short-term chemical resistance but they lack thermal stability and have only moderate resistance to environmental degradation (especially that caused by the photo-chemical effects of sunlight). They have poor mechanical properties, but are easily fabricated and joined.• Ceramics may be of low density (although some are very dense). They have great thermal stability and are resistant to most forms of attack (abrasion, wear, corrosion). Although intrinsically very rigid and strong because of their chemical bonding, they are all brittle and can be formed and shaped only with difficulty.• Metals are mostly of medium to high density — only magnesium, aluminium and beryllium can compete with plastics in this respect. Many have good thermal stability and may be made corrosion-
chapter one — The nature of composites 7 resistant by alloying. They have useful mechanical properties and high toughness, and they are moderately easy to shape and join. It is largely a consequence of their ductility and resistance to cracking that metals, as a class, became (and remain) the preferred engineering materials. On the basis of even so superficial a comparison it can be seen that each class has certain intrinsicadvantages and weaknesses, although metals pose fewer problems for the designer than either plastics orceramics.1.3 STRONG FIBRES The engineer who uses materials for structural or load-bearing purposes is quickly aware of animportant feature of engineering solids, which is that they are never as strong as we would expect themto be from our knowledge of the strengths of the chemical bonds which hold them together. The reasonfor this is that all materials contain defects of various kinds which can never be entirely eliminated inpractical manufacturing operations. For example, the strength of bulk glass and other ceramics isdetermined not by their strong covalent or ionic bonds, but by the many tiny pores or sharp cracks thatexist either on the surface or in the interior. The most highly polished and dense bulk ceramic will rarelyhave a strength that exceeds one thousandth of the theoretically predicted strength. Similarly, metalscontain faults in the stacking of atoms in their crystalline arrays, and the most damaging of theseimperfections — dislocations — cause most bulk metal samples to deform plastically at loads which are,again, perhaps a thousandth or less of the theoretically calculated shear strength. The strength of any sample of a glass or ceramic is actually determined by the size of the largestdefect, or crack, which it happens to contain. Roughly, the strength is proportional to the inverse squareroot of the length of the largest flaw, a relationship developed in a thermodynamic argument by Griffithin the 1920s. The relationship in its simplest form is: 2EγF σmax = ..................................................................................................... [1.1] πawhere σmax is the strength of the material, E is its elastic stiffness (Youngs modulus), γF is the workrequired to fracture the sample (a slight modification of Griffiths original idea that it represented thesurface free energy of the material), and a is the flaw size. Since materials of this kind inevitablycontain cracks and other defects with a wide range of sizes, one of the unfortunate consequences of theGriffith model is that the measured strengths of a batch of supposedly identical samples of a brittlematerial will be very variable simply because of the spread of flaw sizes. If the flaw sizes can be reduced by careful control of the manufacturing process, the general level ofstrength of the material will be raised and its variability reduced. Glass fibres, for example, aremanufactured by drawing molten glass very rapidly down to form fine filaments of the order of only tenmicrons (10μm) in diameter. The resulting freshly formed surface is free of macroscopic defects and thefibre itself is too fine to contain any defects of the size that are found in bulk glass. Carefulmeasurements of the strengths of freshly drawn glass fibres shows them to be up to 5GPa by comparisonwith the very modest 100MPa or so of bulk glass. The fresh fibre needs to be protected from abrasion bycontact with hard objects and from corrosion by moisture in the atmosphere, both of which would resultin the reintroduction of surface flaws and loss of the high strength achieved by drawing. Similarly, the strengths of polymeric filaments, such as the polyacrylonitrile fibres used to make‘acrylic’ textiles, are limited by the weak chemical bonding between the molecular chains which makeup the filament and by the defects caused by the manufacturing process. By subjecting such filaments tocarefully controlled stretching, oxidation and carbonisation processes, however, the polymer can beconverted into fibres which are chemically almost entirely carbon, and with a crystal structure that isapproximately that of graphite, in which the proportion of strong C—C bonds that lie in the direction ofthe fibre axis is very great. The load-bearing ability of these filaments, which are about 7μm in diameter,is high, and the sizes of the residual defects are very small. As a result, each filament, finer than a human
chapter one — The nature of composites 8hair, is capable of supporting a load of 10-20g without breaking, which is equivalent to strengths of up to5GPa. And so it is with the many other types of fibres, organic and inorganic, that are used in compositematerials. The finer the filament that can be made from a given solid, the stronger it will be. The theoretical strength of a given type of solid is determined by the strengths of the atomic ormolecular bonds that hold the solid together. And although the practical strengths of solids aredetermined by the defects which they contain, it is nonetheless necessary to seek materials with thestrongest chemical bonds if we are to have the best chance of exploiting the principle of compositematerials construction. An appreciation of the nature and magnitude of chemical bonding leads us toscan the Periodic Table for elements in which there is a high density of covalent or mixed covalent/ionicbonds, and we naturally alight on the area containing light elements with directional bonds. Theelements most likely to provide what we seek are those like carbon, boron and silicon. In the 1950s,when ideas about composite materials were first being formulated, the plain elements would not havebeen considered to be particularly promising as high-performance structural materials, but the inventionof carbon fibres at the Royal Aircraft Establishment, Farnborough, in the UK, and the simultaneousdevelopment of high-strength boron fibres at Texaco in the USA, resulted in a very rapid expansion ofresearch and development programs to exploit these new filamentary materials in engineeringcomposites. Silicon also appears unpromising as a structural material, but in combination with another ‘light’element, oxygen, as the compound silica (SiO2), it was long familiar as a high-strength filament in theform of melt-drawn glass or quartz fibres. And the list of other combinations of light-weight elementsthat have been successfully exploited in the search for high-performance reinforcing filaments includesalumina (Al2O3), silicon carbide (SiC), and silicon nitride (Si3N4) to name but three of the moreimportant ceramic fibres. Polymeric fibres in which the strength and stiffness are due to the strong C—Cbond are also utilized in fibre composites, and perhaps the two most important are highly drawn forms ofthe humble polyethylene and the more exotic aromatic polyamides (related to Nylon, but possessingmuch greater thermal stability). Table 1.1 gives a rough comparison of the mechanical properties ofsome of the more important commercial reinforcing fibres. Taking steel, in the form of piano wire, as abasis for comparison, it is clear why some of the new fibrous materials are of such interest to engineers,especially those concerned with light-weight structures. On a strength/density or stiffness/density basis,the comparison is almost startling. Since it is the reinforcing fibres that provide the means of creating composite materials of highstrength and stiffness, combined with low density, it is worth-while examining in a little more detail thenature of these fibres and their origins. Information can be obtained on these and other fibres from thepublications edited by Bunsell (1988) and Mai (1994).1.3.1 Glass fibres Glass fibres are manufactured by drawing molten glass into very fine threads and then immediatelyprotecting them from contact with the atmosphere or with hard surfaces in order to preserve the defect-free structure that is created by the drawing process. Glass fibres are as strong as any of the newerinorganic fibres but they lack rigidity on account of their molecular structure. The properties of glassescan be modified to a limited extent by changing the chemical composition of the glass, but the only glassused to any great extent in composite materials is ordinary borosilicate glass, known as E-glass. Thelargest volume usage of composite materials involves E-glass as the reinforcement. S-glass (called R-glass in France) has somewhat better properties than E-glass, including higher thermal stability, but itshigher cost has limited the extent of its use. Wallenberger and Brown (1994) have recently described theproperties of experimental calcium aluminate glass fibres with stiffnesses as high as 180GPa.1.3.2 Carbon fibres By oxidising and pyrolysing a highly drawn textile fibre such as polyacrylonitrile (PAN), preventingit from shrinking in the early stages of the degradation process, and subsequently hot-stretching it, it ispossible to convert it to a carbon filament with an elastic modulus that approaches the value we wouldpredict from a consideration of the crystal structure of graphite, although the final strength is usually
chapter one — The nature of composites 9well below the theoretical strength of the carbon-carbon chain (Watt, 1970). The influence of strength-limiting defects is considerable, and clean-room methods of production can result in substantial increasesin the tensile strength of commercial materials. Prior to sale, fibres are usually surface-treated bychemical or electrolytic oxidation methods in order to improve the quality of adhesion between the fibreand the matrix in a composite. Depending on processing conditions, a wide range of mechanicalproperties (controlled by structural variation) can be obtained, and fibres can therefore be chosen fromthis range so as to give the desired composite properties. Although the fibre is highly organized andgraphite-like, the structure is not identical with that of graphite and the fibres should not, strictlyspeaking, be referred to by that name, although this is common in the US (and in UK advertising jargonfor sports equipment!). Recent developments in this field have led to the use of pitch as a precursor inplace of textile fibres, and these newer materials have extremely high stiffnesses, compared to PAN-based fibres, but rather lower strengths (Fitzer and Heine, 1988). Table 1.1. Typical properties of some familiar reinforcing fibres Material Trade name Density, Fibre Youngs Tensile 103 kg.m-3 diameter, Modulus, Strength, µm GPa GPa High-carbon steel wire eg. piano wire 7.8 250 210 2.8 Short fibres: α-Al2O3 (whisker crystals) 3.96 1-10 450 20 δ-Al2O3 + SiO2 (discontinuous) Saffil (UK) 2.1 3 280 1.5 Continuous fibres:(inorganic) α-Al2O3 FP (US) 3.9 20 385 1.8 Al2O3 + SiO2 + B2O3 (Mullite) Nextel480 (US) 3.05 11 224 2.3 Al2O3 + SiO2 Altex (Japan) 3.3 10-15 210 2.0 Boron (CVD on tungsten) VMC (Japan) 2.6 140 410 4.0 Carbon (PAN precursor) T300(Japan) 1.8 7 230 3.5 Carbon (PAN precursor) T800(Japan) 1.8 5.5 295 5.6 Carbon (pitch precursor) Thornel P755(US) 2.06 10 517 2.1 SiC (+O) Nicalon(Japan) 2.6 15 190 2.5-3.3 SiC (low O) Hi-Nicalon(Japan) 2.74 14 270 2.8 SiC (+O+Ti) Tyranno(Japan) 2.4 9 200 2.8 SiC (monofilament) Sigma 3.1 100 400 3.5 Silica (E glass) 2.5 10 70 1.5-2.0 Silica (S or R glass) 2.6 10 90 4.6 Silica (Quartz ) 2.2 3-15 80 3.5 Continuous fibres (organic) Aromatic polyamide Kevlar 49 (US) 1.5 12 130 3.6 Polyethylene (UHMW) Spectra 1000 (US) 0.97 38 175 3.0 Carbon fibres are inherently expensive, since they are produced from relatively costly precursorfilaments. Since their introduction, however, their price has fallen from several hundred £/kg to tens of£/kg, depending upon quality, and although carbon is still an expensive reinforcement, more so thanglass, for example, it is now much cheaper than most other common reinforcing fibres. The costs of thefibres listed in Table 1.1 vary from about £30 per kg for PAN-based carbon to over £5,000 per kg forboron.1.3.3 Silicon carbide. Continuous SiC monofilaments were first produced by pyrolytic decomposition of gaseous silanesonto fine filaments of carbon or tungsten. These are thick fibres, of the order of 100μm in diameter,which continue to be of major interest to manufacturers of metal- and ceramic-matrix composites. Thealternative production method, analogous to that for carbon described earlier, is based on the controlledthermal degradation of a polymer precursor (Yajima, 1980). This process typically takes a precursorsuch as some mixture of dimethyl dichlorosilane and diphenyl dichlorosilane and converts it in anautoclave to a polycarbosilane from which a continuous fibre is made by melt-spinning. The fibre is then
chapter one — The nature of composites 10converted by pyrolysis at 1300°C into a fibre consisting mainly of β-SiC of about 15µm diameter. Thecharacteristic commercial fibre of this type is that known as Nicalon which is marketed by the NipponCarbon Company. It has a rough surface, making for good fibre/matrix adhesion, but is somewhatreactive towards oxygen. It is well wetted by molten metals and is reasonably stable as a reinforcementfor MMCs based on aluminium and copper although it lacks long-term thermal stability. There havebeen various attempts to improve this feature of the fibre, for example by reducing the oxygen content(Hi-Nicalon; see Toreki et al, 1994) and by adding titanium (Tyranno fibre).1.3.4 Alumina and alumina/silica compounds The earliest work involving Al2O3 as a reinforcement for composite materials concerned the use oftiny filamentary crystals, of the order of 50μm long and a few microns in diameter, which could begrown from the vapour phase in a highly perfect state and which, in consequence, had great strength andstiffness. These crystals, known as ‘whiskers’, proved to be very expensive and difficult to handle inprocessing operations, and their potential could not be satisfactorily realized. The DuPont Company inthe USA subsequently developed an improved alumina fibre in the form of a polycrystalline yarn knownas FP fibre (Dhingra, 1980). These filaments, which were manufactured by a sol-gel process, had amodulus comparable with those of boron and carbon, and a strength of the order of 1.8GPa. Like SiC,this fibre also had a rough surface and was potentially well-suited for the reinforcement of metals suchas aluminium and magnesium on account of its chemical inertness, high-temperature stability, and itsability to form a good bond with matrix alloys. As far as can be ascertained at present, however, FP hasnever been an economic prospect for its manufacturer, and alternative forms of alumina, usuallycontaining other constituents, like Sumitomo’s Altex fibre, for example, are currently preferred. Manyof the oxide-based reinforcing filaments available at present are compounds of alumina and silica, andWallenberger and Brown (1994) have given a useful graphical plot, drawn in modified form in Figure1.2, showing how the tensile stiffness of this particular family of materials varies with composition.Some of the points in the diagram are labelled with their familiar trade names. An alternative form of alumina-based reinforcement known as Saffil, a δ-Al2O3 containing certainimpurities which were advantageous for processing MMCs, was introduced in 1979 by ICI in responseto the need for a reinforcing filament that was cheaper than those currently available. This discontinuousfibre was manufactured in the form of a continuous mat which could be used as layers or preforms, or asa shredded material, with controlled fibre aspect ratios (the ratio of length to diameter) ranging from50:1 to 500:1. The material combined ease of handling with low cost (up to one tenth the cost ofcontinuous reinforcing fibres), and unlike competing fibres was produced on a large-scale. Its intrinsicproperties were as good as those ofsome competing fibres, but the fact that 500it was produced as a random mat meant monocrystallinethat the potential strength of composites Saphicon Elastic modulus, E, GPacontaining it was more limited. It has 400 FPbeen used for the selectivereinforcement of MMC components, but polycrystalline Safimax 300not on any large scale. Themanufacturers have since relinquished Nextel 480their interest in the material. 200 Altex Nextel 3121.3.5 Organic Fibres S glass 100 Bulk polymers have elastic modulino greater than 100MPa, but if the E glass amorphouspolymer is spun into fibres and cold 0drawn so as to develop a high degree of 0 20 40 60 80 100molecular orientation, substantial Alumina content, wt%improvements in both strength andrigidity can be achieved. In particular, Figure 1.2. Elastic modulus of SiO2/Al2O3 fibres as a function ofpolyolefin fibres with an exceptionally composition (after Wallenberger & Brown, 1994)
chapter one — The nature of composites 11highly oriented, extended molecular chain structure can be achieved by superdrawing in the solid state(Ward, 1980). In this process, both the crystalline and non-crystalline phases of the initially isotropicpolymer are stretched out and aligned and there is an increase in crystal continuity. Such fibres havehigh strengths, and their elastic moduli are similar to those of glass and aluminium. Apart from theirexcellent mechanical properties such fibres have the important advantage over inorganic fibres that theyare not brittle. The other major development in organic fibres over the last three decades has been the production byDuPont of aromatic polyamide fibres, collectively known as aramids, of which the best known for manyyears in the composites industry has been Kevlar-49 (Yang, 1993). These polymers are based on p-oriented diamine and dibasic acid intermediates which yield liquid crystalline solutions in amide andacid solvents. These solutions contain highly-ordered extended-chain domains which are randomly-oriented in the absence of force, but which may be oriented by inducing shear forces in the liquid.Highly-oriented fibres can therefore be produced by wet-spinning these solutions, andpoly(paraphenylene terephthalamide) fibres such as Kevlar and Twaron have strengths of the order of2.6GPa and moduli up to 130GPa, depending on the degree of alignment of the polymer chains. Havingproperties intermediate between those of carbon and glass, aramids offer an extra degree of flexibility incomposite design. One important characteristic of the fibre is that it is extremely difficult to cut onaccount of its fibrillar structure. Laser and water-jet methods are essential for trimming bare fabrics andcomposites containing them. Kevlar/resin composites are noted for their extremely high levels oftoughness and resistance to impact damage. One disadvantage of aramids, by comparison with carbonfibres, for example, is that they are sensitive to moisture.1.3.6 Styles of reinforcement Many reinforcing fibres are marketed as wide, semi-continuous sheets of ‘prepreg’ consisting ofsingle layers of fibre tows impregnated with the required matrix resin and flattened between paper carriersheets. These are then stacked, as discussed in chapter 3, the orientations of each ‘ply’ being arranged inaccordance with design requirements, and hot pressed to consolidate the laminate. This process is able tocope with curved surfaces, provided the degree of curvature is not too great, but there may be apossibility of local wrinkling of the fibres when prepregs are pressed into doubly curved shapes. Onemeans of overcoming this problem is to use the reinforcement in the form of a woven cloth since textilematerials can readily be ‘draped’ over quite complex formers. Many of the fine filamentary reinforcingfibres like glass, carbon and SiC can be readily woven into many kinds of cloths and braids, the fibresbeing effectively placed by the weaving process in the directions required by the designer of the finalcomposite structure. In simple designs, this may call for nothing more elaborate than an ordinary plainweave or satin weave, with fibres running in a variety of patterns but in only two directions, say 0° and90°, but weaving processes to produce cloths with fibres in several directions in the plane of the cloth areall readily available. Fibres of different types may also be intermingled during the weaving processes toproduce mixed-fibre cloths for the manufacture of some of the ‘hybrid’ composites that will bediscussed later. Most of the continuous fibres that we have considered are expensive raw materials, and it is oftenonly the fact that the overall cost of a manufactured composite product may nevertheless be lower than acompeting product made from cheaper, conventional materials by more costly processes that makes acomposites design solution an attractive alternative. Thus, although large quantities of glass fibres aresupplied in chopped form for compounding with both thermoplastic and thermosetting matrix polymers,it may not seem economical to chop the more expensive types of reinforcement. Nevertheless, there aresome advantages in using even these fibres in chopped form, provided they can be arranged in thecomposite in such a way as to make good use of their intrinsically high strengths and stiffnesses. Parrattand Potter (1980) described a process for producing both chopped fibres, like glass and carbon, andnaturally short filaments, like whiskers or asbestos fibres, in the form of prepreg sheets with fibres thatwere very well aligned in either unidirectional or poly-directional patterns. These prepregs also haveexcellent ‘drapability’ and can be used to form complex shapes, as discussed by Tsuki et al. (1997). Aswill be seen in chapter 4, provided the short fibres are well above some critical length, which for carbon,for example, may be of the order of only a millimetre, they are able to contribute a high fraction of their
chapter one — The nature of composites 12intrinsic properties to the composite without the loss that occurs with woven reinforcements as a result ofthe out-of-plane curvature of the fibres.1.4 THE SCOPE FOR REINFORCEMENT OF CONVENTIONAL MATERIALS The composite matrix is required to fulfil several functions, most of which are vital to theperformance of the material. Bundles of fibres are, in themselves, of little value to an engineer, and it isonly the presence of a matrix or binder that enables us to make use of them. The rôles of the matrix infibre-reinforced and particulate composites are quite different. The binder for a particulate aggregatesimply serves to retain the composite mass in a solid form, but the matrix in a fibre composite performs avariety of other functions which must be appreciated if we are to understand the true composite actionwhich determines the mechanical behaviour of a reinforced material. We shall therefore consider thesefunctions in some detail.1.4.1 Functions of the matrix• The matrix binds the fibres together, holding them aligned in the important stressed directions. Loads applied to the composite are then transferred into the fibres, the principal load-bearing component, through the matrix, enabling the composite to withstand compression, flexural and shear forces as well as tensile loads. The ability of composites reinforced with short fibres to support loads of any kind is dependent on the presence of the matrix as the load-transfer medium, and the efficiency of this load transfer is directly related to the quality of the fibre/matrix bond.• The matrix must also isolate the fibres from each other so that they can act as separate entities. Many reinforcing fibres are brittle solids with highly variable strengths. When such materials are used in the form of fine fibres, not only are the fibres stronger than the monolithic form of the same solid, but there is the additional benefit that the fibre aggregate does not fail catastrophically. Moreover, the fibre bundle strength is less variable than that of a monolithic rod of equivalent load-bearing ability. But these advantages of the fibre aggregate can only be realized if the matrix separates the fibres from each other so that cracks are unable to pass unimpeded through sequences of fibres in contact, which would result in completely brittle composites.• The matrix should protect the reinforcing filaments from mechanical damage (eg. abrasion) and from environmental attack. Since many of the resins which are used as matrices for glass fibres permit diffusion of water, this function is often not fulfilled in many GRP materials and the environmental damage that results is aggravated by stress. In cement the alkaline nature of the matrix itself is damaging to ordinary glass fibres and alkali-resistant glasses containing zirconium have been developed (Proctor & Yale, 1980) in an effort to counter this. For composites like MMCs or CMCs operating at elevated temperature, the matrix would need to protect the fibres from oxidative attack.• A ductile matrix will provide a means of slowing down or stopping cracks that might have originated at broken fibres: conversely, a brittle matrix may depend upon the fibres to act as matrix crack stoppers.• Through the quality of its ‘grip’ on the fibres (the interfacial bond strength), the matrix can also be an important means of increasing the toughness of the composite.• By comparison with the common reinforcing filaments most matrix materials are weak and flexible and their strengths and moduli are often neglected in calculating composite properties. But metals are structural materials in their own right and in MMCs their inherent shear stiffness and compressional rigidity are important in determining the behaviour of the composite in shear and compression. The potential for reinforcing any given material will depend to some extent on its ability to carry outsome or all of these matrix functions, but there are often other considerations. We consider now thelikely qualities of various classes of matrix materials.
chapter one — The nature of composites 131.4.2 Metals Metals owe their versatility as engineering materials to the fact that they can be plastically deformedand can be strengthened by a variety of methods which, by and large, act by inhibiting the motion ofdislocations. As a consequence of the non-directional nature of the metallic bond, dislocations are highlymobile in pure metals which are therefore very soft. But by controlling the number and distribution ofdislocations the materials scientist can adjust the properties of a metal or alloy system to suit specificrequirements. There are limitations, however. Increases in strength can usually be achieved only at theexpense of the capacity for plastic deformation, with the consequence that the strongest alloys often lacktolerance of defects or other stress-concentrators. Since brittleness is a drawback no designer daresunderestimate, this leads to the use of large safety factors which, in turn, means that the full potential ofhigh-strength alloys is often not utilisable in practice. Many solid-state hardening methods used in alloys involve producing a material in a metastablestate which may subsequently revert to a more stable but unstrengthened condition if sufficient thermalenergy is provided. Alloys strengthened by precipitation hardening, such as the strong aluminium alloys,alloys depending on phase transformations of the martensitic type, such as steels, and heavily cold-worked metals which depend simply on the presence of a high dislocation density, as in piano wires andlamp filaments, will all soften at elevated temperatures. The strongest aluminium alloys lose theirstrength at temperatures little over 150°C, for example. Many conventional metallic materials are relatively heavy. For land-based engineering projects thismay be of no consequence, but economic arguments relating to pay-loads (in civil aircraft) and tacticalarguments relating to manoeuvrability (in military aircraft) have always been a powerful incentive forthe use of low-density materials in aerospace engineering, and in these energy-conscious times theeconomic incentive for lightening automobiles has considerably influenced the motor car designer. For structural applications involving compression or flexural rather than tensile loads, the relevantstructural stiffness index is not simply Youngs modulus, E, or the modulus/density ratio, E/ρ, but mayinstead be either of the ratios E/ρ2 or E/ρ3 (Gordon, 1968 and 1978, Ashby and Jones, 1980). Foraerospace applications modifications to materials that result in lowered density may therefore be moreprofitable than attempts simply to improve their strength or stiffness. These features show why it is worthwhile to attempt to use light, strong, stable fibres to reinforcesome of the lighter engineering metals and alloys.1.4.3 Polymeric materials Few polymers are thermally stable by comparison with metals or ceramics and even the most stable,like the polyimides, or poly(ether ether ketone) (known as PEEK) are degraded by exposure totemperatures above about 300°C, as illustrated by some of the data in Table 1.2. There is nothing thatreinforcement can do to combat chemical degradation, but the associated fall in strength and increase intime-dependent (creep or visco-elastic) deformation, a feature common to all polymers, though lessserious in cross-linked resin systems than in thermoplastics, can be delayed by fibre reinforcement.
chapter one — The nature of composites 14 Table 1.2. Thermal Stability of some Matrix Polymers Type and Polymer Symbol Crystallinity Glass transition Max use temp, Tg, ° C temp, °C Thermosets: Polyester PE no 80 -100 50 Epoxy Ep no 120-180 150 Phenolic Ph no 130-180 200 Bismaleimide BMI no 180-200 220 Polyimide PI no 300-330 280 Thermoplasts: Polyamide (Nylon) PA yes 80 125 Poly(phenylene sulphide) PPS yes 100 260 Poly(ether ether ketone) PEEK yes 143 250 Polycarbonate PC no 145 125 Polysulphone PS no 190 150 Poly(ether imide) PEI no 210 170 Poly(ether sulphone) PES no 230 180 Thermoplastic polyimide TPI no 270 240 A more serious problem in polymers is their very low mechanical strength and stiffness in bulk form:and, like metals, the weakest plastics tend to be ductile but the strongest tend to be brittle, although thereare exceptions. Polymers are traditionally insulators and in their application as such strength is usually a secondaryconsideration. The electrical conductivity of plastics reinforced with carbon fibres is of importance inmany aeronautical applications, however, where protection of avionics systems from external electricalactivity (eg. lightning strike) is of importance. Most polymers are already low-density materials, and theaddition of fibres confers no density advantage. It is in the reinforcing of polymers that most developments have been made so far, and it is likelythat there is still scope for improvement. There is a thriving, international reinforced plastics Industry,for which both the science and technology are highly advanced. And although the level of awareness ofthe merits of reinforced plastics on the part of designers in general engineering seems to be low, thesame is not true of the aerospace industry for which the potential benefits of very high strength andstiffness, combined with low density, are easily recognized.1.4.4 Glasses, ceramics and cement Glasses have high chemical stability, but many lose their mechanical strength at relatively lowtemperatures as they pass through the glass transition. Special glasses have been developed with hightransition temperatures (Tg), however, and many are at least as resistant as some of the less stable steels.The principal problem with glassy materials is that they are always brittle and their measured strengthsare very variable at ordinary temperatures. They are not able to relieve stress concentrations at crack tipsby plastic deformation and they are not, therefore, fail-safe. A constant disadvantage, aggravated by lowthermal conductivity, is that glass usually has poor thermal shock resistance unless, like borosilicateglass, it also has a low thermal expansion coefficient. Many of these difficulties can be overcome byreinforcement with fibres like carbon, and with the added bonus of a saving in weight (Phillips et al,1972). Most ceramics suffer from the same defects as glasses in that, although they are potentially high-strength solids, they are also brittle and notch-sensitive. Most ceramics retain their strength to very hightemperatures, however, unlike glasses, and several have good resistance to thermal shock. Improvingtoughness and reducing notch sensitivity are the main reasons for attempting to reinforce ceramics sincetheir stiffnesses are not very different from those of the best reinforcing fibres. For high-temperaturestability we might expect that the best possibility for reinforced ceramics would be an equilibriumsystem in which whisker-like crystals of a reinforcing phase were grown within the polycrystalline
chapter one — The nature of composites 15matrix of a chemically-related ceramic. Most recent work has followed the more established route,however, in attempting to reinforce a variety of glasses (such as borosilicate) and glass-ceramics (such ascalcium aluminosilicate (CAS) and lithium aluminosilicate (LAS)) with fibres like carbon, siliconcarbide and alumina (Prewo and Brennan, 1980; Phillips et al, 1972), the fibres being impregnated by aslurry of fine glass powder and subsequently hot-pressed (Sambell et al, 1970, 1972). Critical control ofmanufacturing conditions is needed in order to produce appropriate interfacial conditions for theoptimum combination of strength and toughness. Once control of the glass-making technique isestablished, development of the process to include a glass-ceramic transformation is the logical next stepin the production of a continuous-fibre composite. The advantage of the glass-ceramic route is thatrelatively modest processing temperatures are involved. For high-temperature exposure of suchcomposites, however, or for work involving the production of CMCs by conventional pressing methods,there remains the problem of compatibility. At the time of writing, the concept of all-oxide CMCs isbeing strongly argued, although we already have comparative examples of stable pairings in the FrenchSiC/SiC materials (Frety and Boussuge, 1990). After a period of intense activity in fibre-reinforced glassand glass-ceramic research with an eye on the gas-turbine industry, it has still not been possible forengineers to come to terms with the concept, already explored in the 1970s (Aveston et al, 1971), that inthese materials the matrix will crack at worryingly low stress levels (Harris et al, 1992) leaving thereinforcing filaments exposed to any hostile environment. Concrete is a particulate ceramic composite in which aggregate particles of graded sizes areembedded in a glassy or microcrystalline silicate matrix. Like most ceramics and glasses it is brittle andexhibits a very low tensile failure strain which engineers cope with by using it in compression or withmacroscopic reinforcing bars to carry tensile loads. In design, the tensile load-bearing ability of theconcrete is ignored. Reinforcement of concrete in the composite sense has been widely studied, withattempts to produce stronger, stiffer and tougher structural materials by adding fibres of asbestos, glass,steel, polymeric materials, and carbon. Improved properties can be obtained, although usually only at theexpense of a severe economic penalty, given the fact that concrete is the cheapest structural materialavailable. The addition of even a few percent of the cheapest reinforcing fibres may still raise the pricesufficiently to lead the engineer to use a thicker section of plain concrete in preference to a moreexpensive thinner section of reinforced concrete. Such small additions do little to increase the crackingstress or elastic modulus of cement, but by introducing complex cracking and failure modes they cansubstantially improve the work of fracture. The scope for improvement of bulk poured concrete isprobably negligible: it is much more likely that the present trend towards changes in design philosophyand the use of speciality products in fibre-reinforced concrete will continue. High volume fractions ofwell-aligned fibres can be obtained by vacuum dewatering and filament-winding and the products ofthese processes can be used in much thinner sections than is normal with concrete. Traditional attitudesand design procedures are of course no longer applicable for such materials.1.4.5 Carbon Carbon is a unique material with many attractive engineering qualities. It can be prepared in a varietyof forms — conventional hot-pressed carbons and graphites, densified impermeable graphite, pyroliticgraphite, and vitreous carbon — with a wide range of engineering properties. It is valuable for itslubricating properties, its electrical properties, its nuclear characteristics and, in the pyrolytic andvitreous forms, for high strength and resistance to oxidative and chemical attack (Cahn and Harris,1969). The opportunity to improve the mechanical properties of such an important material and reduceits brittleness somewhat has been the driving force for the development of an invaluable material,carbon-fibre-reinforced carbon (Savage, 1993) that has been used for rocket nozzles, aerospacecomponents (including the ablative shields of space vehicles), and surgical implants.1.5 REFERENCES TO CHAPTER 1 Ashby MF and Jones DRH, 1980, Engineering Materials, (Pergamon, Oxford) Atzori B, Quaresimin M and Trattenero G, 1994, in Proc 2nd International Seminar Experimental Techniques and Design in Composite Materials (editor MS Found) Sheffield, Sept 1994, (Sheffield Academic Press, Sheffield, UK), 193-211.
chapter one — The nature of composites 16 Aveston J, Cooper GA and Kelly A, 1971, Proceedings of NPL Conference on The Properties of Fibre Composites, (IPC Science and Technology Press Ltd, Guildford), 15-26 Cahn RW and Harris B, 1969, Nature, 221, 132-141 Dhingra AK, (1980), in New Fibres and their Composites, Watt W, Harris B and Ham AC (editors), (Royal Society of London), Phil Trans Roy Soc Lond, A294, 411-417. Fitzer E and Heine M, 1988, in Fibre Reinforcements for Composite Materials, Composite Materials Series, volume 2, (editor AR Bunsell), (Elsevier, Amsterdam), 73-148. Frety N and Boussuge M, 1990, in Ceramic-Matrix Composites: Components, Preparation, Microstructure and Properties, Naslain R and Harris B (editors), Special Issue of Composites Science and Technology, 37, 177-190. Gordon JE, 1968, Structures, (Penguin, Harmondsworth, Middlesex) Gordon JE, 1978, The New Science of Strong Materials, (Penguin, Harmondsworth, Middlesex) Griffith AA, 1920, Phil Trans Roy Soc, A221, 163-198. Harris B, Habib FA and Cooke RG, 1992, Proc Roy Soc (Lond), A437, 109-131. Parratt NJ and Potter KD, 1980, Advances in Composite Materials (Proc ICCM3) vol 1 (editors AR Bunsell, C Bathias, A Martrenchar, D Menkes and G Verchery), (Pergamon, Oxford), 313-326. Phillips DC, Sambell RAJ, Bowen DH, 1972, J Mater Sci, 7, 1454-1464, Prewo KM, Brennan JJ, 1980, J Mater Sci, 15, 463-468, Proctor B and Yale B, 1980, in New Fibres and their Composites, Watt W, Harris B and Ham AC (editors), (Royal Society of London), Phil Trans Roy Soc Lond, A294, 427-436. Sambell RAJ, 1970, Composites, 1, 276-285. Sambell RAJ, Briggs A, Phillips DC and Bowen DH, 1972, J Mater Sci, 7, 676-681. Savage G, 1993, Carbon-Carbon Composites, (Chapman & Hall, London). Toreki W, Batich CD, Sacks MD, Saleem M, Choi GJ and Morrone A, Compos Sci & Technol, 51, 145-159. Tsuji N, Springer GS and Hegedus I, 1997, J Compos Mater, 31, 428-527. Wallenberger FT and Brown SD, 1994, Compos Sci & Tech, 51, 243-264. Ward IM, 1980, in New Fibres and their Composites, Watt W, Harris B and Ham AC (editors), (Royal Society of London), Phil Trans Roy Soc Lond, A294, 473-482. Watt W, 1970, Discussion Meeting on Strong Fibrous Solids, Proc Roy Soc Lond, A319, 5-15. Yajima S, 1980, in New Fibres and their Composites, Watt W, Harris B and Ham AC (editors), (Royal Society of London), Phil Trans Roy Soc Lond, A294, 419-426. Yang HH, 1993, Kevlar Aramid Fibre, (John Wiley, Chichester)1.5.1 General bibliography Agarwal BD and Broutman LJ, 1990, Analysis and Performance of Fibre Composites, second edition, (John Wiley, New York). Astrom BT, 1997, Manufacturing of Polymer Composites, (Chapman & Hall, London). Bunsell AR, (editor), 1988, Fibre Reinforcements for Composite Materials, Composite Materials Series, volume 2, (Elsevier, Amsterdam). Chawla KK, 1993, Ceramic Matrix Composites, (Chapman & Hall, London). Chou TW, 1992, Microstructural Design of Fibre Composites, (Cambridge University Press). Clyne TW and Withers PJ, 1993, An Introduction to Metal-Matrix Composites, (Cambridge University Press). Eckold G, 1994, Design and Manufacture of Composites, (Woodhead, Abington, UK). Everett RK and Arsenault RJ (editors), 1991, Metal-Matrix Composites; volume 1, Processing and Interfaces, volume 2, Mechanisms and Properties, (Academic Press, Boston). Hull D, 1981, An Introduction to Composite Materials, (Cambridge University Press). Jones RM, 1975, Mechanics of Composite Materials, (Scripta Books, Washington DC) Kelly A and McMillan NH, 1986, Strong Solids (3rd Edition), (Clarendon Press, Oxford).
chapter one — The nature of composites 17 Mai YW (editor), 1994, Advances in Inorganic Fibre Technology, Special Issue of Composites Science and Technology, 51, 123-296. Matthews FL and Rawlings RD, 1994, Composite Materials: Engineering and Science, (Chapman & Hall, London). Naslain R and Harris B (editors), 1990, Ceramic-Matrix Composites, (Elsevier Science Publishers, London and New York). Piggott MR, 1980, Load-Bearing Fibre Composites, (Pergamon Press, Oxford) Powell PC, 1994, Engineering with Fibre-Polymer Laminates, Chapman & Hall, London). Warren R (editor), 1992, Ceramic Matrix Composites, (Blackie, Glasgow). Watt W, Harris B and AC Ham (editors), 1980, New Fibres and their Composites, (The Royal Society of London), Phil Trans Roy Soc Lond, A2126.96.36.199 Sources of data Hancox NL and Meyer RM, 1994, Design Data for Reinforced Plastics, (Chapman & Hall, London). Kelly A (Editor), 1989, Concise Encyclopaedia of Composite Materials, (Pergamon, Oxford). Lubin G (Editor), 1982, Handbook of Composites, (Van Nostrand Reinhold, New York).
2 MAKING COMPOSITE MATERIALS2.1 THE COMBINING OF MATERIALSI n considering the scope for reinforcing conventional materials, we have already examined the functions of the matrix in a composite and the general nature of available reinforcing filaments. The problem facing the manufacturer of composites is to develop suitable methods for combining the matrix and the reinforcement so as to obtain the required shape of component with propertiesappropriate to the design requirements. In the early days of the subject, attention was focused on firstproducing a ‘piece’ of the composite — a sheet, or rod, or billet, with the fibres arranged in one or moredirections — and then using that intermediate product to construct a finished ‘component’ in much thesame way as steel castings were bolted together to build a car engine or steel plates were welded togetherto make a pressure vessel. Early use of composites in practical applications was on the basis of piece-meal substitution of the composite for a metallic part of identical shape without any consideration of thespecial nature of the composite, notably its anisotropic mechanical properties. The idea of bolting GRP‘top-hat’ stiffeners to the underside of GRP ship decking seems ridiculous now, but the procedure wascertainly investigated in the 1970s. It is essentially the reinforcement ‘architecture’ that determines the load-bearing characteristics of afibre composite, and the beauty of modern composites design and manufacturing procedures is that inmany cases the composite material and the finished component can be created and final in a singleoperation. A typical example is in the process of resin-transfer moulding (RTM) which we shall discusslater. A fibre preform — a skeleton of the approximate shape of the finished component with the fibresarranged in the directions determined by the design requirements — is placed into a closed mould, andpre-catalysed resin is injected into the mould, which is often pre-heated. The resin cures in a short time,and the finished component, requiring only final cleaning up, is removed from the mould, the compositematerial and the finished article being formed in a single operation. The rate-controlling step in this near-net-shape manufacturing process is probably the manufacture of the fibre preform. In the filament-winding of hollow containers, fibres wetted by catalysed resin are wrapped onto a mandrel and, again, asthe resin cures the component and the material are formed simultaneously. In this case, the locations ofthe fibres may have been determined by a computer programme and the same computer code can then beused to control an automatic filament-winding machine — a good example of CADCAM. The range of processes used for manufacturing composites is now wide. Almost all of the basicmetal, polymer and ceramic forming processes have been adapted, with greater or less success, and foreach class of composites — fibre-reinforced plastics (FRPs), MMCs and CMCs — there is a range ofpreferred techniques, depending on the required product. In many cases, there has been technologytransfer from one field to another, so that similar processes, suitably modified, may be used for differenttypes of composite. The RTM process for FRPs is clearly related to the liquid-metal infiltration processwhich is used for MMCs and to the sol-gel process for CMCs. Almost all successful processes involveliquid-phase reactions — molten metal, liquid glass, ceramic sol — although many processes for ceramiccomposites are gas-phase processes, as in the chemical vapour deposition (CVD) processes for preparingcarbon/carbon composites and some of the monofilament-reinforced ceramics like the SiC/SiCcomposites made by SEP in France. What is feasible for the manufacturer is often limited by the available forms of the reinforcingfilaments. The thick monofilamentary reinforcements like boron and SiC are produced in continuoussingle filaments and because of their diameters they cannot easily be handled except as regular arrays ofcontinuous fibres. But the majority of the fine, continuous reinforcements are manufactured ascontinuous tows, often containing thousands of individual fibres, and these can be manipulated by well-established textile handling techniques. They can be chopped into short lengths for mechanical blendingwith matrix resins and fillers, for example, or they can be woven into many kinds of cloths and braids,the fibres being effectively placed by the weaving process in the directions required by the designer. Insimple designs, this may call for nothing more elaborate than an ordinary plain weave or satin weave,
Chapter two Making composite materials 19with fibres running in a variety of patterns but in only two directions, say 0° and 90°. But weavingprocesses to produce cloths with fibres in several directions in the plane of the cloth — eg. triaxialweaves with three groups of fibres at 120° to each other, and so-called 4D and 5D fabrics — are allreadily available. The study of textile-based composites is currently a much researched topic (see, forexample, Masters and Ko, 1996). Fibres of different types may also be intermingled during the weavingprocesses to produce mixed-fibre cloths for the manufacture of some of the ‘hybrid’ composites that willbe discussed later.2.2 THE INTERFACE In materials where the mechanical response depends on loads being shared between two or moreseparate constituents or ‘phases’ and where paths for the propagation of cracks will be affected by thedifferent mechanical properties of the components, the manner in which these adhere to each otherbecomes an important consideration. When we come to discuss the strength and toughness ofcomposites, we shall see that the strength of the interfacial bond between the fibres and the matrix maymake all the difference between a satisfactory material and an inadequate one. The problem is that theideal situation for load sharing — a perfect bond between the fibre and the matrix, forcing them todeform as one, which is the first assumption that we shall make in attempting to calculate the elasticmodulus of a fibre composite — often results in a lower tensile strength than expected because of theway cracks run in such a composite. In the early days of carbon-fibre technology, it was quicklyestablished that the greater the degree of order in the graphitized fibre structure the poorer was theadhesive bond between the new high-modulus fibres and the existing polyester and epoxy resins. As aconsequence, the higher the fibre stiffness the poorer the extent to which the composite was able to resistshear forces acting in the plane of a laminate ie. the lower the interlaminar shear strength (ILSS). Hastyattempts were made to improve the ILSS by a variety of surface treatments, including coating withpolymers, high-temperature and electrolytic oxidation, and vapour deposition of other compounds ontothe fibre surface. Electrolytic treatment became the established method, but the need for control over theextent of the treatment was not appreciated and some early fibres were supplied by manufacturers withheavily oxidised surfaces that were very well wetted by the resins. This facilitated manufacture, butresulted in composites that were disastrously brittle, causing a serious set-back for aeronautical use ofcarbon fibres. In early work on the use of carbon fibres as reinforcements for aluminium alloys, thechoice of an aluminium/silicon alloy as matrix (on account of the well-known fluidity of these alloys)led to a rapid reaction between the silicon and the carbon fibre, with the result that a very strong bondwas created but the fibre properties were ruined. This kind of interaction between the fibre surfacecharacteristics and the fibre/matrix bond, and frequently also the effect of processing, has probablyexercised the minds of composites workers more than most other aspects of the technology. It would be wrong, then, to consider the fibres and the matrix as the only important constituents of acomposite, even of a simple two-phased composite where no other actual component is intentionallypresent. The interface between two solids, especially when thermal or chemical processes have beeninvolved in putting them together, is rarely a simple boundary between two materials of quite differentcharacter. Over a certain range, which will vary in dimensions depending upon the chemical andphysical natures of the fibres and the matrix, there will be some modification of either chemical orphysical characteristics, or both, resulting in a region, perhaps only of molecular dimensions, perhapsmany microns, which has properties quite different from those of either of the two major components.Sometimes this occurs fortuitously, as when the two components in a ceramic-matrix composite, whichhas to be fired at elevated temperature to achieve compaction, react chemically together, or it may bedeliberately engineered, as when, in the case of GRP materials, we apply a size coating to the fibres afterdrawing in order to make them adhere more readily to the resin matrix. Whatever the origin of thisregion, which we often refer to as an ‘interphase’, it is important in that its properties determine themanner in which stresses are transferred from matrix to fibres and, in consequence, many of thechemical, physical and mechanical properties of the composite itself. Control of this interphase, orinterface region, is a major concern to developers and suppliers of commercial composite materials.
Chapter two Making composite materials 202.3 MANUFACTURING PROCESSES This book is not about manufacturing, yet it is necessary to know something of the nature of the mainprocessing methods used in order to appreciate how what happens during processing may affect theproperties of the product. In this chapter, therefore, we shall take only a very general look at the majorprocesses currently being used to produce composite artefacts. There will be no attempt to discuss thebasic engineering of the individual processes, and further details of manufacturing processes may beobtained from publications listed in the General Bibliography for Chapter 188.8.131.52 Polymer-matrix composites The wide range of processes used to produce reinforced plastics is partly new, and partly derivedfrom established methods of processing ordinary polymeric materials. The manner of combining fibresand matrix into a composite material depends very much on the particular combination in question andon the scale and geometry of the structure to be manufactured. The commoner varieties of thermoplastic-based materials, like glass-filled Nylon and glass-filledpolyacetal, are made largely by the injection moulding of granules of material in which the choppedfibres and matrix have been pre-compounded. The principal problem in such cases is that the flow ofmaterial during moulding may be non-uniform, especially in moulds of complex geometry. There maybe regions in which the fibres are highly oriented and others where the degree of orientation is almostnil, as well as variations in fibre content from place to place. Preferential fibre orientation is often useful,but only if it can be adequately controlled. Some very sophisticated recent developments in multiplelive-feed injection moulding by Bevis and co-workers have enabled the inventors to produce short-fibre-filled thermoplastics with very well aligned fibre arrays in different parts of a moulding with the resultthat the properties of these materials can compete favourably with those of many continuous-fibrecomposites (Allan & Bevis, 1987). Continuous-fibre thermoset composites are produced by quite different methods. Cylindricallysymmetric structures such as pressure vessels, tanks, rocket-motor casings, centrifuge cylinders, and avariety of pipes, can be made by winding fibres or tapes soaked with pre-catalysed resin onto expendableor removable mandrels. Winding patterns may be simple or complex and may be accurately calculated toresist a prescribed stress system. (eg. a given ratio of hoop stress to longitudinal stress) in service.Variations in winding pattern or in the combination of stresses subsequently applied to the structure willclearly change the extent to which the fibres are loaded purely in tension or to which shear stresses areintroduced between separate layers of winding. After the resin has hardened the mandrel is removed and,if size permits, the product may be post-cured at an elevated temperature. Extremely large vessels can bemade by this method, but these must usually be left to cure at ambient temperature. Since the windingprocedure can be closely controlled, a high degree of uniformity is possible in the fibre distribution offilament-wound structures, but planes of weakness sometimes occur between winding layers, especiallyif resin-rich pockets are allowed to form. An important feature of this process is that after a structure hasbeen designed according to well-defined principles based on stress analysis of composite materials, thedesign software can be extended to provide instructions to a computer or numerically-controlled windingmachine to manufacture the vessel to close tolerances (Eckold, 1994; Jones et al, 1996). Large panels and relatively complex open structural shapes are easily constructed by hot-pressingsheets of pre-impregnated fibres or cloth between flat or shaped platens, or by vacuum autoclaving withthe aid of atmospheric pressure to consolidate a stack of ‘prepreg’ sheets against a heated, shaped die.Woven reinforcements are particularly useful for constructing shapes with double curvature since theycan readily be ‘draped’ over quite complex formers, unlike unidirectional prepregs which may wrinklebecause of their anisotropy. Pressing must be carried out carefully to produce intimate association of thefibres in different layers, with expulsion of trapped air (and of excess resin unless the prepreg is of the‘zero-bleed’ variety containing no excess resin), and the time/temperature cycle must be controlled so asto ensure final curing of the resin only when these conditions have been met. Higher fibre contents areobtainable with non-woven laminates than with woven-cloth composites, and the characteristics of thetwo types of material are quite different. The orientation of the fibres in the separate laminations is
Chapter two Making composite materials 21varied to suit the specific load-bearing characteristics required of the laminate or moulding. Althoughthis is a common process and a great deal of experience has been accumulated in its use, control of theautoclave cycle is sometimes difficult to establish since there is a complex interaction between thekinetics of the resin cure, the resin curing exotherm, and the externally applied pressure and temperature.Research is currently in progress to develop the use of in situ fibre-optic sensors for closed-loop controlof the autoclave (Roberts and Davidson, 1993; Crosby et al, 1995). For complex aeronautical and similar structures, the relationship between computer-based designprocedures and robotic or computer-controlled manufacturing processes has considerably improved theproduction engineering of composites. In particular, the construction of the stacked laminates ready forprocessing or autoclaving may be carried out by a computer-controlled tape-laying machine which canlay up components rapidly, accurately, and with minimum waste of raw materials. Such a system permitsof greater design flexibility than is possible in manual production and can consistently produce parts ofhigher strength. Most other operations, including prepreg trimming, transfer between operations,autoclaving, component trimming, and assembly can also be carried out with a high level of softwarecontrol (see, for example, Hadcock and Huber, 1982). In the pultrusion process, tightly packed bundles of fibres, soaked in catalysed resin, are pulledthrough a shaped die to form highly aligned, semi-continuous sections of simple or complex geometry.Curing of the resin in the die may be achieved either by heating the die itself or by the use of dielectricheating. Solid and hollow sections may be produced by this process, and because of the high fibrecontent (70% by volume is achievable) and the high degree of fibre alignment resulting from the tensileforce used to pull the fibre bundle through the die, extremely high mechanical properties can beobtained. In more recent developments of the process, off-axis fibres may also be introduced into thestructure. A detailed description of this process has been given by Spencer (1983). Another familiar process for producing high-quality mouldings of complex shape is resin-transfermoulding or RTM. Pre-catalysed resin is pumped under pressure into a fibre preform which is containedin a closed (and often heated) mould. The preform may be made of any kind of reinforcement, butusually consists of woven cloths or fibre mats, arranged as required by the design. Thick componentscontaining foamed polymer cores can also be produced in this way. The ease with which this can bedone successfully (Harper, 1985) belies the complexity of the process which involves non-Newtonianflow of a resin (which may be curing at a significant rate during short-cycle operations) through apreform in which the fibre distribution results in flow paths of markedly different geometries in the in-plane and through-thickness directions. In high-speed versions of the process favoured by theautomobile industry the cycle time may be reduced to a minute or less, and there are problems inobtaining complete wetting and uniform cure throughout the heated mould cavity. The mould cavity isoften evacuated to assist wetting out. This is an important, high-volume, automatable process which,when used in association with automated fibre-preform manufacture, offers considerable advantages inthe production of low-cost engineering components from GRP (Rudd et al, 1990; Turner et al, 1995). Awide range of low-viscosity resins — polyesters, vinyl esters, epoxies, urethane-acrylates, etc. — arenow commercially available for use in this process. A commercially important class of thermoset moulding compounds, the polyester dough-mouldingcompounds or DMC, consist of chopped glass fibres blended into a dough with a pre-catalysed resin anda substantial quantity of inert filler, like chalk. These compounds (also referred to as bulk mouldingcompounds or BMC) may be manufactured to final shape by injection moulding or, more commonly, bythe simpler transfer-moulding process — squeezing to shape in hot dies. As in the case of the injection-moulded reinforced thermoplastics mentioned earlier, problems resulting from non-uniformity and fibre-orientation effects can also occur during the moulding of these materials. Lower quality composites reinforced with random-fibre chopped-strand mat (CSM) or continuous-filament mat (CFM) reinforcements may be press-laminated like the higher-performance CFRP and GRPlaminates but are more frequently laid up by hand methods, especially for irregularly shaped structures.Large structures, tanks, boats and pipes are often made in this way. The usual procedure is to coat a
Chapter two Making composite materials 22shaped former or mandrel with resin, allow the resin to gel and then build up the required shape andthickness by rolling on layer upon layer of resin-soaked cloth or mat. A final gel-coat is then applied andthe finished structure may be post-cured. The distribution of fibres in such structures will usually beuneven. Resin pockets and voids are invariably present in these materials.2.3.2 Metal-matrix composites The basic attributes of metals reinforced with hard ceramic particles or fibres are improved strengthand stiffness, improved creep and fatigue resistance, and increased hardness, wear and abrasionresistance, combined with the possibility of higher operating temperatures than for the unreinforcedmetal (or competing reinforced plastics). These properties offer potential for exploitation in a range ofpump and engine applications, including compressor bodies, vanes and rotors, piston sleeves and inserts,connecting rods, and so forth. Components of this type are still under development, but few are incommercial production (Feest, 1986) apart from one or two limited applications in Japaneseautomobiles. Thus, although a wide range of manufacturing methods has been used over the past twentyyears on a laboratory or development scale, at this stage relatively little can be said about large-scaleproduction processes for MMCs. Some of the techniques that have been described in detail are • Unidirectional solidification of eutectics or other constitutionally-appropriate alloys • Liquid-metal infiltration, often under vacuum, of pre-packed fibre bundles or other preforms • Liquid-phase infiltration during hot pressing of powder compacts containing whiskers or fibre bundles • Hot pressing of compacts consisting of matrix alloy sheets wrapped or interleaved with arrays of reinforcing wires • Hot pressing or drawing of wires pre-coated with the matrix alloy (eg. by electroplating, plasma spraying or chemical vapour deposition (CVI) • Co-extrusion of prepared composite billets The first of these processes relates to the manufacture of the so-called in situ composites which beganwith model systems, like Cu/Cr and Al/Al2Cu, in most of which thermodynamic constraints imposeserious restrictions on the range of materials that can be treated and in which the fibre contents are small.Better results were subsequently obtained with more complex systems such as the monovariant ternaryeutectic alloy (Co, Cr)-(Cr, Co)7 C3 which, in the directionally-solidified form, contains about 30 vol%of the fibrous carbide phase in a Co/Cr solid solution (Thompson et al,1970). Further developments werebased on complex superalloy systems in which the composition of the phases can vary widely withoutinhibiting the formation of an aligned two-phased structure during processing. Typical of these materialsare the carbide-reinforced systems exemplified by the NITAC (TaC in nickel) and COTAC (TaC incobalt) alloys developed at ONERA in France (Bibring et al, 1971). From the thermodynamic point ofview, composites of this kind possess the clear advantage that they are intrinsically stable underoperating conditions involving elevated temperature. There seems to be little current enthusiasm for thisprocess. With both liquid infiltration and solid-state bonding techniques, one of the main problems is that ofensuring the optimum degree of chemical contact (or wetting) between the fibres and the matrix. Inmany systems with practical potential, wetting is inhibited by oxide films or surface chemistry featuresof the reinforcing phase, and measures to improve the interfacial characteristics often result in anundesirable degree of fibre/matrix interaction and damage. Similar consequences of inherentthermodynamic incompatibility followed when many of the early MMCs were exposed to elevatedtemperatures. As a consequence of these wetting and stability problems, a considerable proportion of theearly research and development in this field was concerned with fibre treatments both to improve
Chapter two Making composite materials 23adhesion and to provide diffusion barriers — two clearly conflicting requirements — and theestablishment of conditions needed to obtain optimum interfacial bonding. Short-fibre-reinforced MMCs are commonly made by liquid-metal infiltration (LMI) or squeezecasting into fibre preforms, a net-shape forming technique that has much to recommend it for localisedor general reinforcement of components such as automotive pistons, connecting rods, etc. Powderprocessing is much less satisfactory because of the possibility of fibre damage. A useful practicaldevelopment in the liquid-state processing of metal-matrix composites was the introduction in 1984 of alow-cost short-fibre reinforcement consisting of δ-alumina containing a few percent of silica, calledSaffil by the manufacturers, ICI plc. These fibres, said to be some 45% stronger than other availablecontinuous α-alumina fibres, are easily wetted by a range of aluminium alloys and can be fabricated intopractical engineering composite components by pressure die-casting or squeeze-casting an alloy matrixinto pre-formed fibre arrays located in the mould. A number of announcements of practical applicationsof the material followed, but ICI’s interest in composite materials proved as transitory as those of almostevery other major UK company which had a composites programme in the 1970s and 1980s, and thematerial is no longer obtainable. Products requiring continuous reinforcement, such as boron/aluminium composite panels andsections that have been under consideration for aerospace applications (Renton, 1977) are preferablyproduced by solid-state processes such as diffusion bonding or hot pressing in which criticalpressure/time/temperature cycles are needed to obtain optimum quality. Structures can be fabricatedrelatively easily (by comparison with thermoset resin matrix composites) by brazing, welding, diffusionbonding or mechanical fastening. There is now a wide range of continuous fibres available that aresuitable for reinforcement of MMCs, and a variety of production techniques, including liquid-metalinfiltration, squeeze casting, electroplating, diffusion bonding of plasma-sprayed tapes, and evenexplosive welding, has been developed to make use of them, in addition to conventional roll-bondingand hot-pressing. At the time of writing. however, there are few genuine large-scale applications forcomposites of this kind. unlike their resin-matrix equivalents. Of the recently renewed activity in MMCs, not all is associated with fibre-reinforced materials, muchwork having been done on particulate MMCs, a class of materials that was formerly familiar tometallurgists as ‘cermets’, although the classical cermet — the cemented carbides and other metal-bonded ceramic materials mostly used for cutting tools — contained a very low proportion of themetallic phase by comparison with modern MMCs. The most familiar of the modern MMCs are made bythe incorporation of SiC particles (after treatment to improve particle/matrix adhesion) at volumefractions of 0.1 to 0.3 into aluminium alloys by various routes, including co-spraying, powdermetallurgy, and liquid infiltration. These materials are claimed to show significant increases in specificstiffness and strength, although at the expense of ductility and toughness, with the advantage (eg. overreinforced plastics) that they can be processed by conventional metal-forming methods. A recent surveyof the manufacturing processes used for MMCs has been published by Everett and Arsenault (1991).2.3.3 Ceramic-matrix composites Fabrication processes are complex and need to be carefully optimised because of the inevitablesensitivity of materials properties to microstructures controlled by processing conditions andinteractions. Much of the recent work on CMCs in the US, Japan and Europe has largely followedrelatively familiar routes in attempting to reinforce glasses (like borosilicates) and glass-ceramics (likelithium aluminosilicate or LAS and calcium aluminosilicate or CAS) with fibres such as the commercialNicalon and Tyranno varieties of silicon carbide. Substantial improvements in mechanical propertieshave been achieved, by comparison with early carbon-fibre/glass composites. The fibres are usuallyimpregnated with a slurry of fine glass powder and subsequently hot-pressed (Dawson et al, 1987). If thematrix is a glass-ceramic, the final stage in manufacture is the ‘ceramming’ process, the final heattreatments to convert the glass to a fully dense ceramic. Companies like Corning in the US offer suchmaterials for commercial sale. Critical control of manufacturing conditions is needed to produceappropriate interfacial conditions for the optimum combination of strength and toughness. Theadvantage of the glass-ceramic route is that relatively modest processing temperatures are involved,
Chapter two Making composite materials 24although even so a typical residual thermal stress of the order of only 200MPa may still be sufficient tocause cracking of the matrix in as-manufactured or lightly-loaded composites. Much of the research onmonofilament-reinforced ceramics like the French SiC/SiC materials, for example (Naslain and Langlais,1986), and on the production of carbon/carbon composites (Fitzer, 1987), has been directed towardschemical vapour infiltration (CVI) and related processes. Commercial quantities of these materials havebeen available for a considerable time although CVI is normally a very slow process and componentsproduced in this way are very costly. However, for all work involving the production of ceramic-fibre-reinforced ceramic composites byconventional pressing methods, there remains the problem of compatibility. Nicalon fibre with a startingstrength as high as 3GPa, for example, may lose half its strength when pressed into composites with aCAS or borosilicate glass matrix, and following high-temperature exposure in service this load-bearingability may be further impaired. Current developments in the field involve the search for reliablediffusion-barrier coatings (plus ça change!). It is perhaps also worth remarking that although the driving force for developments in the CMC fieldhas most frequently been the needs of high-temperature applications in the aerospace industry, there aremany other branches of engineering—automotive, chemical, marine, and general engineering, forexample—where there is a need for reliable economic components possessing good mechanicalproperties and reasonable wear and corrosion resistance, in combination with adequate impact andthermal shock resistance at ordinary or only slightly raised temperatures. For many such applicationsthere is no need for high-temperature stability, and the problems relating to fibre/matrix interactions athigh temperatures are not as serious as in gas-turbine applications, for example, provided processingmethods can be developed which do not require the high firing temperatures normally associated withceramics manufacture. One such process is the sol-gel process in which low-viscosity sols are convertedto solid ceramics in a manner analogous to the curing of organic resins. And by extension of the analogy,composite materials may be made by techniques of casting, filament winding and sol-transfer moulding,as described by Russell-Floyd et al (1993).2.3.4 Hybrid composites Reference to hybrid composites most frequently relates to the kinds of fibre-reinforced materials,usually resin-based, in which two types of fibres are incorporated into a single matrix. The concept is asimple extension of the composites principle of combining two or more materials so as to optimise theirvalue to the engineer, permitting the exploitation of their better qualities while lessening the effects oftheir less desirable properties. As such, the definition is much more restrictive than the reality. Anycombination of dissimilar materials could in fact be thought of as a hybrid. A classic example is the typeof structural material in which a metal or paper honeycomb or a rigid plastic foam is bonded to thin skinsof some high-performance FRPs, the skins carrying the high surface tensile and compressive loads andthe core providing lightweight (and cheap) structural stability. The combination of sheets of aluminiumalloy with laminates of fibre-reinforced resin, as in the commercial product ARALL (aramid-reinforcedaluminium, Davis, 1985) is a related variety of layered hybrid, and the mixing of fibrous and particulatefillers in a single resin or metal matrix produces another species of hybrid composite. Some hybrids of current interest represent attempts to reduce the cost of expensive compositescontaining reinforcements like carbon fibre by incorporating a proportion of cheaper, lower-qualityfibres such as glass without too seriously reducing the mechanical properties of the original composite.Of equal importance is the reverse principle, that of stiffening a GRP structure with a small quantity ofjudiciously placed carbon or aromatic polyamide fibre, without inflicting too great a cost penalty. Inhigh-technology fields the question of cost may be insignificant by comparison with the advantages ofoptimising properties. In aerospace applications, a familiar purpose of using hybrids is to utilise thenatural toughness of GRP or of Kevlar-fibre-reinforced plastics (KFRP) to offset a perceived brittlenessof typical CFRP. From the designers point of view the important aspect of using hybrids is that providedthere is adequate understanding of the underlying mechanisms of stiffening, strengthening andtoughening, they allow even closer tailoring of composite properties to suit specific requirements thancan be achieved with single-fibre types of composites.
Chapter two Making composite materials 252.4 DEFECTS IN MANUFACTURED POLYMERIC COMPOSITES All practical reinforced plastics composites are likely to contain defects of various kinds arising fromthe processes of manufacture. Indeed, composites are noted for the variability of mechanical propertiesthey exhibit unless they have been produced under the most rigorously controlled conditions. Thevariability of material produced by hand lay-up methods is more marked than that of composites madeby mechanised processes. The specific nature and severity of the defects found in any manufacturedproduct will also be characteristic of the manufacturing process. In addition, any composite consisting ofmaterials of widely different thermal expansion coefficients which is heated during manufacture may, oncooling, develop residual stresses sufficiently high to crack a brittle matrix. The defects that may bepresent in manufactured composites include: • incorrect state of resin cure, especially that resulting from variations in local exotherm temperatures in thick or complex sections during autoclaving • incorrect overall fibre volume fraction • misaligned or broken fibres • non-uniform fibre distribution, with resultant matrix-rich regions • gaps, overlaps or other faults in the arrangement of plies • pores or voids in matrix-rich regions • disbonded interlaminar regions • resin cracks or transverse ply cracks resulting from thermal mismatch stresses • disbonds in thermoplastic composites resulting from failure of separated flows to re-weld during moulding • mechanical damage around machined holes • local bond failures in adhesively bonded composite componentsand we shall discuss some of these in more detail in the context of particular manufacturing processes. In the moulding of shaped artefacts from materials such as dough-moulding and sheet-mouldingcompounds (DMC and SMC) there are two main kinds of possible defects. The first results from failureof the process to control resin cure and flow, perhaps as a consequence of the use of a mouldingcompound that is past its shelf-life or because of incorrect control of the temperature/pressure cycle. Theconsequences are poor consolidation, incomplete filling of the mould, and perhaps also the failure ofseparated flow streams to re-amalgamate in complex mouldings. The second problem may arise eitherfrom the non-uniform filling of the mould cavity (a manual operation) prior to pressing or from poorattention to the flow patterns that will occur during pressing. In either case there may again be non-uniformity of fibre content in the finished artefact, and/or local preferred orientation of the short fibres,with resultant anisotropy in mechanical properties. If this anisotropy is not allowed for in the design, thecomponent may fail to meet the design specification. Similar considerations apply, of course, to theinjection moulding of short-fibre-reinforced thermoplastics. Typical defects in RTM mouldings include porosity resulting from bubbles injected with the resin,‘washing’ or movement of the preform, especially near injection points or corners, failure of the resin topenetrate the preform uniformly, poor wetting-out of the fibres by the resin, distributed porosity, andpremature gelation. Porosity is a particular problem, since the process relies on the flow of resin tosweep out the air contained within the mould and the fibre preform, and when filled matrix resins arebeing injected into a tightly packed fibre preform, there is sometimes a tendency for the filler particles tobe filtered out of resin. The quality of RTM mouldings is considerably improved, however, by slightlyreducing the air pressure in the mould cavity. In the so-called vacuum-assisted RTM process (VARTM)it is sufficient to maintain the mould cavity pressure at only 0.7 bar in order to improve considerably thewetting out of the preform and reduce the level of residual porosity in the moulding to a fraction of a
Chapter two Making composite materials 26percent for relatively little extra cost. Figure 2.1 1.6shows how the mechanical properties of a typical RTM withglass/polyester composite vary with the levels of vacuum Property value, relative to the 1.4porosity characteristic of different processing value for hand lay-up hand compression RTMconditions. The average porosity levels in moulding lay-upVARTM mouldings are comparable with those 1.2obtainable in high-quality autoclaved materials. 1.0 A schematic illustration of some of the typicalfaults that occur in the laying up of prepreg Flexural strength 0.8 Flexural modulusmaterials is shown in Figure 2.2. The finite Short-beam shear strengthdimensions of the prepreg will require, from timeto time, that joins (a) will have to be made. 0.6 4 3 2 1 0Closely butted joins are clearly more satisfactory Porosity, vol%than overlapped (b) or widely separated (c)prepreg ends since these will result in resin-rich Figure 2.1. Variation of mechanical properties of GRPregions, as shown. Rigorous quality-control materials as a consequence of variations in porosity levelsprocedures should prevent the incorporation of introduced during manufacturing. In each case the fibreinclusions such as bits of rubbish (d), but a volume fraction is approximately 0.4. (Hayward and Harris, 1990)common problem with prepregs is the occurrenceof small bundles of fibre debris, known as ‘whorls’, which are sometimes attached to the surface of thesheet and subsequently become incorporated in the laminate as small regions of random fibre alignment.These are considered to be damaging to composite strength, and an aerospace manufacturer maytypically specify that such defects should not occur more than once in, say, ten metres of prepreg roll.Their effect is modest, however. In samples of [(0/90)2]S glass/epoxy laminate hot-pressed fromcommercial prepreg, with deliberate concentrations of whorls to the extent of 3 defects per prepreg plyin a 150mm x 150mm x 1mm plate, the tensile strength was reduced by only about 6%, and the failurestrain by about 2%, the stiffness being unaffected (Ellis, 1985). Failure to achieve a consistent level of pressure over the whole surface of a sheet during autoclavingmay result in small regions where the plies are imperfectly bonded (e). These disbonds are particularsources of weakness in laminates subjected to compression or impact forces. Voids or imperfectly curedresin regions near the surface of a laminate may absorb moisture during service in wet conditions, withthe result that hydrostatic pressure could develop inside the region and push out the surface layer or gelcoat to create blisters (f). Poorly stored prepregs or prepregs that are draped over a former which is toosharply curved may become wrinkled (g), and this may again lead to poor surface quality or weaknessesresulting from resin-rich regions in the laminate. The last feature shown in Figure 2.2 is a deliberatelyintroduced ‘defect’ rather than an adventitious manufacturing fault. It is often required to change thedimensions of a structure, and since the individual ply effectively represents a ‘quantum’ of laminatethickness, such changes can only be made by gradually reducing or increasing the number of plies in across section. This design procedure by the introduction of ‘ply drop-offs’ (h) nevertheless presents aproblem for the stress engineer since the ply ends result in local stress concentrations the effects ofwhich must be accounted for (see, for example, Curry et al, 1985; Cui et al, 1994). The prepregsthemselves may also be a source of defects if the strictest quality control procedures are not employed.Broken or damaged fibre-tows, accumulations of debris (eg. the ‘whorls’ mentioned above), and out-of-date resin are examples of prepreg defects that can lead to poor quality in the final laminate.
Chapter two Making composite materials 27 Since most composites consist of materials of widely different thermal expansion coefficients they may, if heated and cooled during manufacture, develop residual stresses sufficiently high to crack a brittle matrix. Early high-performance CFRP laminates were frequently found to have suffered multiple internal cracking unless proper care was taken to control the production cycle. This type of problem has been eliminated to a large extent for polymer composites by the advent of ‘modified’ or ‘toughened’ resins with high failure strains, but such problems will inevitably be of more concern for users of such materials as CMCs. The advantages of using hybrid laminates may be both structural and economic, as we have seen, but there is also a potential disadvantage. Over the temperature range of about 150°C from conventional Figure 2.2. Some typical defects in composite curing temperatures down to ambient, the axial thermal laminates manufactured from prepreg sheets. expansion coefficient of most carbon fibres is close to zero, while that of an aramid fibre like Kevlar-49 isnegative, about –3 x 10-6 K-1, and that of E-glass is positive, 0.7 x 10-6 K-1. Thus, in hybrid laminatescontaining various mixtures of these fibres, there will be a tendency to develop thermal stresses whichmay become great enough to cause marked undulations in the plies subject to compression — the Kevlarplies in a carbon/Kevlar hybrid, for example. A consequence of this is that the wavy plies are unable tocontribute their full share of load-bearing in tension, and the compression strength of a hybrid may alsobe reduced because the waviness facilitates a common compression kinking mechanism (see chapter 4). One of the virtues of polymer composites is that complex shapes can often be manufactured in single-shot operations, thereby eliminating much of the need for the joining operations that characterise mostconventional manufacturing with metallic materials. Joining and machining operations may not alwaysbe completely avoidable, however, and in such cases there is always likely to be the possibility ofbonding failures in imperfectly prepared adhesive joints (in thermoset composites), disbonds in weldedthermoplastic composite plates, and machining damage (in sawn or drilled components, for example).But while machining damage will usually be at cut edges, and therefore visible, poor joints will rarely bedetectable from the exterior. Any of these defects can locally reduce the strength of the material below the required componentdesign stress. They may then act as sites for the initiation of fatigue damage, or may facilitate the growthof a fatigue crack during cyclic loading. A comprehensive assessment of the quality of a compositematerial prior to putting it into service is therefore as important as the monitoring of the levels of damageaccumulated in a composite structure during service. The use of non-destructive evaluation methods isthus of great importance in composite materials technology, and modern aerospace design proceduresincreasingly relate to the establishment of zero-growth thresholds for manufacturing and service defects.Many of the defects associated with hand lay-up or manual operation may be avoided, where the extracost is justifiable, by the use of computer-controlled tape-laying machines which are able to construct aprepreg stack for autoclaving to very high standards of quality and repeatability. Similarly, errors ofcontrol in pressing can be avoided to some extent by the use of automated autoclaves with pressure-temperature cycles carefully programmed from detailed chemical knowledge of the gelation andviscosity characteristics of the resin in use. It is largely only in the aircraft industry that the high initialcosts of such equipment can be borne, however. Of particular importance to the manufacturer and user is the associated question of what are likely tobe the consequences of the presence of a particular defect. At present, there is no easy way to quantifythis. A few isolated spherical pores a micron or so in diameter may have no effect on any physicalproperty, and may not therefore affect the tensile or flexural mechanical performance of a composite.
Chapter two Making composite materials 28But a distribution of innocuous looking pores may markedly reduce the interlaminar shear strength of amaterial, and by providing sites for accumulation of moisture may also ruin the electrical or dielectricperformance of the material. A minor delamination between plies in a complex laminate may have noeffect on the tensile strength of the material, but such defects are frequently injurious to the compressionperformance of laminates and, as indicated above, may grow rapidly to eventual ruin of the compositeunder cyclic loading conditions. The question of critical size or quantity of defects must therefore beaddressed with specific reference to the particular composite and service conditions involved in a givenapplication.2.5 METHODS OF NON-DESTRUCTIVE EVALUATION FOR POLYMER COMPOSITES Since the presence of defects in reinforced plastics, either ab initio or as a consequence of damage inservice, is to some extent inevitable, it follows that manufacturers and users need sensitive techniques forthe detection of these defects and damage. Much of the technology previously developed for metallicengineering materials and structures has been transferred across, with appropriate modifications, for usewith fibre composites. Some of these techniques are more useful than others, and it is often goodpractice to use a back-up technique where possible rather than to rely on a single method. Harris andPhillips (1983, 1990) have given summaries of some of the more common methods in current use, but atthe time of writing there is a high level of activity in R & D work on fibre-optic sensors specifically foruse with reinforced plastics. Brief details of some of these NDT tools are given below.2.5.1 Optical inspection In translucent GRP, inspection by transmitted light can give indications of the presence of pores, poorwetting-out, delaminations, and gross inclusions. Light transmission can also sometimes be correlatedwith the fibre content, Vf. Loss of transparency (stress-whitening) is associated with the development offibre/resin debonding and resin cracking. In non-translucent composites the only feasible visual-inspection techniques relate to observation of surface damage. The detection of surface cracking may beenhanced by dye-penetrant methods. Moiré methods require photographic grids to be printed on thesurface of the composite and irradiated with coherent light. The resulting interference fringes give clearindications of local stress concentrations and deformation, including those arising from sub-surfacedamage. Laser holographic methods and electronic speckle-pattern interferometry (ESPI) are also usedfor non-translucent materials.2.5.2 Radiographic methods Radiography is not easily applied in the field, but information about composite quality can beobtained by x-ray inspection. Contact radiography with sources of 50kV or less yields high-contrastphotographs from low-density materials like GRP because of their low inherent filtration. The linearabsorption coefficient of glass is about twenty times that of most resins, and film density measurementscan be correlated with Vf if the material is unpigmented. The fibre distribution, quality of weave, and thepresence of large laminating defects can be easily investigated. Contact radiographs showing fibredistributions have also been analyzed by optical diffraction methods to give quantitative informationabout the fibre distribution. The sensitivity of contact radiography can be improved by impregnating thecomposite with a radio-opaque material, usually an alcoholic solution of zinc iodide. By this technique,resolution of cracks of the order of a few mm long and 0.1 mm deep is feasible in GRP and CFRP, anddelaminations are easily resolved.2.5.3 Thermal imaging When a uniform heat flux is supplied to a plate, any anomalous variations in the resulting temperaturedistribution in the plate are indications of structural flaws in the material. Similarly, in an otherwiseuniform material working under variable loads, local damage will give rise to changes in the hystereticthermal losses in the body of the material. Thermal imaging, with limiting detection of temperaturedifferences of about 0.2°C, is easily carried out by means of infra-red television photography. Damagehas been detected in glass/epoxy laminates at low stresses and frequencies, but in materials of higherthermal conductivity detection is more difficult. Testing frequencies greater than 5Hz are needed in
Chapter two Making composite materials 29order to detect damage in CFRP because of their high thermal conductivity. Thermal imaging equipmentis routinely available and is widely used in the aerospace industry. The technique has the advantage overmany other methods that it is a remote monitoring technique. The use of thermography has beenextended in recent years by the use of transient heat sources and rapid scanning of the induced thermalfields by TV/video-compatible infra-red imagers which forms the basis of the pulse video thermography(PVT) technique. This is a convenient and versatile extension of conventional thermography capable ofrapid detection of near-surface defects. An associated thermal NDE method is that of thermoelastic stressanalysis which makes use of the familiar thermoelastic effect, where a temperature change accompaniesadiabatic elastic deformation of a body. This technique is said to offer spatial resolution down to 1mmand temperature discrimination of about 0.002°C for stress changes of about 2MPa in steel, although incomposites there are potential problems of interpretation resulting from their anisotropic nature.2.5.4 Ultrasonic techniques Ultrasonic inspection techniques are perhaps the most widely-used NDE methods for composites.The velocity and attenuation of an ultrasonic pulse passing through a material provide information aboutthe general physical properties (ie. the stiffness) and the structure (ie. the defect/damage state) in amaterial, provided certain basic features of the material, such as the anisotropy, are taken into account.Most composites are highly dispersive, often having regular structural patterns at several levels of scale(fibres, fibre tows, weave of cloth, laminate stacking sequence), an array of interfaces (fibre/resininterface, interlaminar interface) and an inherent distribution of defects. Ultrasonic waves in compositesare therefore highly attenuated and their velocity and attenuation are dependent on frequency, thisfrequency-dependence being affected by the construction of the laminate. The propagation of ultrasonicwaves may be affected by frequency, composite structure, structural defects, and damage induced byloading. The problem of high attenuation is overcome by the use of broad-band transducers and lowwave frequencies which give shorter, more highly penetrating pulses with less pronounced near-fieldinterference effects. As a result of the low pulse intensities used in composites testing it is generallynecessary to use higher amplification than is needed for other materials, but most of the commonultrasonic techniques, including pulse-velocity measurements, echo methods, goniometry, and ultrasonicinterferometry, are used with composites. The most highly developed ultrasonic NDE method, based on measurements of through-thicknessattenuation, is the C-scan technique, which is used routinely for inspecting large panels. Synchronizedraster-scanning motions of the transmitter and receiver (either in a water bath or with irrigated water-jetprobes) on opposite sides of the plate enable measurements of the intensity of the transmitted wave to bemade as a function of position. It is common to use a focused transmitter, focusing on the back face ofthe plate, with the receiver as close to the front face as possible The transmitted intensity is used tomodulate the brightness of a visual display, or the density of ink on a diagram, so as to build up a pictureof plate quality. The resolution of the technique is limited by dispersion in the composite and by thebeam dimensions. It is necessary to use something like a focused 4MHz probe to detect defects withdimensions of the order of 1mm, and as a consequence C-scanning is more reliable as an indicator ofgeneral quality than as a detector of specific defects. Large voids, distributions of fine porosity, areas ofvariation in fibre content, and delaminated regions will usually be revealed by a C-scan, but forassessment of the severity of specific defects it is necessary to make standard test plates containing flat-bottomed drilled holes of various depths and diameters for calibration purposes. Conventional C-scanning is a slow process, but new techniques for real-time operation are now on the market.2.5.5 Optical fibre sensors Optical fibre sensors have a number of advantages over other types of sensor in that they are immunefrom electromagnetic interference, they can be embedded in a composite material during manufacturerather than simply being surface mounted, they can be used to monitor several parameters, includingtemperature, pressure, strain, and chemical characteristics, and they offer important possibilities for on-line application, both for process optimization and in-service health monitoring (Fernando, 1998).
Chapter two Making composite materials 302.5.5.1 Cure monitoring The mechanical properties of composites are strongly dependent upon the chemical and rheologicalevents occurring during the cure cycle. There is considerable current interest in the possibility of usingfibre-optic sensors embedded in the composite itself to carry out in situ measurements of cure state, curekinetics, resin viscosity and residual stress build-up in real time during manufacture. It is expected thatthe signal processing procedures that are involved could, eventually, form the basis for intelligentprocessing of composites (Roberts & Davidson, 1993). Techniques that are being explored includerefractive-index-based sensors (Crosby et al, 1995), evanescent-wave spectroscopic sensors (Powell etal, 1996), and transmission or reflection infra-red spectroscopy sensors (Crosby et al, 1996). Thesesensors are able to evaluate changes in the optical properties, and hence the state of cure, of the resinsurrounding a stripped length of embedded fibre, or of the resin in a gap between two lengths of fibre, orof resin at the end of a single embedded fibre.184.108.40.206 Sensing of deformation and damage (health monitoring) The simplest form of assessment of impact damage is based on the fact that optical fibres will fracturewhen the composite in which they are embedded suffers an impact event, and this reflects the relateddamage that will be sustained by the main load-bearing fibres. More sensitive assessment of the presenceof strain or a rise in temperature of the composite can be obtained by the use of fibres which have Bragggratings written into their cores or the somewhat cheaper Fabry-Perot sensors in which changes in thelength of an air gap are measured by interferometry (Greene et al, 1995). These provide a means ofmonitoring strain with a high degree of accuracy and resolution. They can also be used for on-linelocation of the position of impact events — Greene et al cite an ability to locate an impact with aresolution of 0.5mm and an accuracy better than 5mm. Provided the separate effects of thermalexpansion and elastic strain can be isolated, sensors of this kind can also provide information abouttemperature changes in the material. They also therefore offer the possibility, mentioned in section220.127.116.11, of closer monitoring and intelligent control of processing procedures, feedback methods beingused to control the severity of the resin curing exotherm and therefore the quality of the finished product.2.5.6 Microwave methods. The dielectric constant of glass is much greater than those of resins at microwave frequencies, andany technique for measuring the average dielectric constant of a GRP composite can therefore becorrelated reasonable satisfactorily with the glass content of the material. A typical instrument consistsof an open-ended coaxial resonator which can be applied to a GRP surface in order to close the resonantcavity. As the instrument is moved over the surface, changes in the local average glass content areindicated by changes in the resonant frequency. Since any defect which affects the microwavepenetration will also cause a resonance shift, the method is capable of monitoring the deterioration of astructure under load, once its dielectric response in the undamaged state is known.2.5.7 Dynamic mechanical analysis. When stresses and strains can be continuously monitored in service, we might expect that changes inelastic modulus would give non-destructive indications of deterioration of properties caused by theaccumulation of damage. However, the change in stiffness of a composite as a result of cycling dependson the type of composite and the extent to which the matrix, fibres and interface are directly loaded.Measurement of the modulus itself, either by strain gauges or by ultrasonic pulse-velocitymeasurements, may therefore prove to be relatively insensitive to changes in the damage state in certaincases, although relative changes in resonant frequency and of the damping capacity can give more subtleindications of damage accumulation. If a structure can be made to resonate in a reproducible manner, itsfrequency spectrum can be rapidly analysed to establish its characteristic ‘sound’. Any damage to thestructure will change this characteristic spectrum in a recognisable way and this provides the basis of asimple ‘coin-tap’ test which can be used to monitor damage in composites. One of the oldest-established NDE methods is the principle embodied in the Fokker debond testermanufactured by Wells-Krautkramer. This machine uses swept-frequency probes generating shear wavesof constant amplitude and compares the response of the test material with that of a standard. The
Chapter two Making composite materials 31resonant frequency and amplitude of the transducer response are recorded in contact with the standard,and any shifts that occur when the probe is subsequently coupled to the test sample are noted. Theseshifts must be calibrated against some known or measurable property. The technique is said to becapable of giving more sensitive indications of the presence of flaws, voids, weak bonds, porosity,delaminations, incorrect cure conditions, poor wetting, and poor gap-filling in joints than any otherultrasonic method.2.5.8 Acoustic emission methods. Any sudden structural change within a composite, such as resin cracking, fibre fracture, rapiddebonding, or interlaminar cracking, causes dissipation of energy as elastic stress waves which spread inall directions from the source. The technique of detection of these acoustic emissions (AE) by suitabletransducer/amplifier systems is now well-established and triangulation methods may be used to locateflaws in large structures and to assess their severity. There are several ways of analysis of theinformation obtained by AE monitoring of structures under load, some of which offer suitablequantitative procedures for proof testing or life prediction, and some of which provide deeper insightinto the mechanisms of damage accumulation in composites.2.6 THE USE OF COMPOSITES In order to make good use of engineering materials, we have to understand their behavioursufficiently well to be able predict performance in both the short term and the long term. In the contextof composite materials, this means developing mathematical models which represent reasonably closelythe known experimental response of real composites to applied stresses and environmental conditions. Ifwe can predict the behaviour of any given composite accurately as a result of this modelling, then wecan have confidence that the material we have designed will meet the service requirements of theapplication concerned. One of the problems with composites is that there is such a diverse range ofmaterials, and it is necessary to have a thorough understanding of each class: we cannot simply readacross from the characterisation of one group of composites to another without carrying out extensivechecks of the validity of the old models for the newer materials. Theories of the elastic behaviour ofcomposite materials are very well developed, and predictions of elastic response are often verysatisfactory. Problems arise, however, when attempts are made to predict processes of failure. Thefailure of composites is almost always a complex process. Damage accumulates in a widespread fashionin composites, and many individual processes occur at the microstructural level. The strength of acomposite is determined by the conditions which determine the climax of this damage accumulationprocess, and modelling of these conditions is far from perfect at the present time. As a consequence,there is still a certain lack of confidence on the part of designers, a reluctance to use some of these newmaterials for which we have not, as yet, the operating experience that instils confidence, and this leads toa measure of inefficient (and often uneconomic) design for which the only cure is better understanding. From the point of view of the designer who is using composites, there is an important constraint:composites do not behave like metals. Conventional notions of materials behaviour and design methodsare therefore unlikely to be appropriate. The use of composites offers the designer a range of newsolutions to engineering problems of many kinds, but it is vital to use the opportunity to rethink theapproach. It is rarely a good idea simply to carry out a piece-meal substitution of composites parts forexisting metallic parts. This kind of approach will certainly not liberate the designer from the oldconstraints, will often lead to more expensive rather than cheaper solutions, and may result in unsafedesigns. In the application of composites, as in other areas of materials engineering, it is important to considerthe selection of the materials and the choice of manufacturing process as a vital and integrated part of thedesign process.2.7 REFERENCES TO CHAPTER 2 Allan PS and Bevis MJ, 1987, Plastics Rubber & Composites: Processing & Applications, 7, 3-10.
Chapter two Making composite materials 32 Bibring H, Trottier JP, Rabinovitch M and Siebel G, 1971, Mém Sci de la Revue de Métall, 68, 23-41. Crosby P, Powell G, Spooncer R and Fernando G, 1995, Proc SPIE Conference on Smart Structures and Materials, (Society for Optical Engineering, vol. 2444, 386-395. Crosby PA, Powell GR, Fernando GF, Spooncer RC, France CM and Waters DN, 1996, In situ cure monitoring in advanced composites using evanescent wave spectroscopy, J Smart Mater and Struct, 5, 415-428. Cui W, Wisnom MR and Jones M, 1994, Compos Sci & Technol, 52, 39-46, Curry JM, Johnson ER and Starnes JH, 1985, Proc 28th Conference on Structures, Structural Dynamics and Materials, Monterey, California, (AIAA/ASME/ASCE/AHS), paper AIAA 87-0874, 737-747. Davis JW, 1985, ARALL — from development to a commercial material, in Progress in Advanced Materials and Processing, editors G Bartelds and RJ Schlickelman (et al) (Elsevier, Amsterdam), 41-49. Dawson DM, Preston RF and Purser A, 1987, Ceram Eng Sci Proc, 8, 815-820. Doyle C and Fernando GF, 1997, Condition monitoring engineering materials with an optical fibre vibration sensor system, SPIE, 3042, 310-318. Eckold GC, 1994, Design and Manufacture of Composite Structures, (Woodhead Publishing Ltd, Abington, UK). Ellis KRJ, 1985, The effect of structure and defects on FRP laminate materials, unpublished report, School of Materials Science, University of Bath. Everett RK and Arsenault RJ (editors), 1991, Metal Matrix Composites: I Processing and Interfaces, (Academic Press Boston). Feest EA, 1986, Mater Des, 7, 58-64. Fernando G, 1998, Materials World, 6 (5), 340-342. Fitzer E, 1987, Carbon, 25, 163-190. Greene JA, Tran TA, Bhatia V, Gunther MF, Wang A, Murphy KA, Claus RO 1995, Smart Mater & Struct, 5, 93-99. Hadcock R and Huber J, 1982, Practical Considerations for Design, Fabrication and Tests for Composite Materials, NATO (AGARD) Lecture Series 124, papers 11 and 12, (AGARD, Neuilly, France). Harper A.,1985, Proceedings of Conference Hands Off GRP ll, Nottingham, (Plastics & Rubber Institute, London), paper 4. Harris B and Phillips MG, 1983, in Developments in GRP Technology (editor B Harris), (Applied Science Publishers London), 191-247. Harris B and Phillips MG, 1990, in Analysis and Design of Composite Materials and Structures (Editors Y Surrel, A Vautrin and G Verchery), (Editions Pluralis, Paris), Part I, chapter 15. Hayward JS and Harris B, 1990, Compos Manuf, 1, 161-166; also 1990, SAMPE Journal, 26(3), 39-46. Jones DT, Jones IA and Middleton V, 1996, Composites, A27, 311-317. Masters JE and Ko FK (Editors), 1996, Textile Composites, Special Issue of Composites Science and Technology, Compos Sci & Technol, 56 (3), 205-386. Naslain R and Langlais F, 1986, in Proc Conf on Tailoring Multiphase and Composite Ceramics (editors RT Tessler, GL Messing and CG Pantano and RE Newham) July 1985, (Plenum Press, New York), 145-164. Powell GR, Crosby PA, Fernando GF, France CM, Spooncer RC and Waters DN, 1996, Optical fibre evanescent-wave cure monitoring of epoxy resin, SPIE, 2718, 80-92. Renton WJ, (editor), 1977, Hybrid and Select Metal-Matrix Composites, (AIAA, New York). Roberts SSJ and Davidson R, 1993, Compos Sci & Technol, 49, 265-276. Rudd CD, Owen MJ and Middleton V, 1990, Mater Sci & Technol, 6, 656-665. Russell-Floyd RS, Harris B, Cooke RG, Wang TH, Laurie J, Hammett FW and Jones RW, 199), J Amer Ceram Soc, 76, (10), 2635-2643. Spencer RAP, 1983, in Developments in GRP Technology (editor B Harris), (Applied Science Publishers, London), 1-36. Thompson ER, Koss DA and Chesnutt JC, 1970, Metall Trans, 1, 2807-2813. Turner MR, Rudd CD, Long AC, Middleton V and McGeehin P, 1995, Advances Compos Lett, 4, 121-124.
3 ELASTIC PROPERTIES OF FIBRE COMPOSITES3.1 SIMPLE MICROMECHANICAL MODELST he simplest method of estimating the longitudinal modulus, E c stiffness of a composite in which all of the fibres are aligned in the direction of fibre matrix the applied load (a unidirectional load,composite) is to assume that the structure is a P csimple beam, as in Figure 3.1, in which the twocomponents are perfectly bonded together so Figure 3.1. Simplified parallel model of a unidirectional composite.that they deform together. We shall ignore thepossibility that the polymer matrix can exhibit time-dependent deformation. The elastic (Young) moduliof the matrix and reinforcement are Em and Ef, respectively. We let the cross-sectional area of the fibre‘component’ be Af and that of the matrix component be Am. If the length of the beam is L, then we canrepresent the quantities of the two components in terms of their volume fractions, Vf and Vm , which ismore usual, and we know that their sum Vf + Vm = 1. The fibre volume fraction, Vf, is the criticalmaterial parameter for most purposes. The subscript ‘c’ refers to the composite. The load on the composite, Pc, is shared between the two phases, so that Pc = Pf + Pm, and the strain inthe two phases is the same as that in the composite, εc = εf = εm (ie. this is an ‘iso-strain’ condition).Since stress = load/area, we can write: σcAc = σfAf + σmAmand from the iso-strain condition, dividing through by the relevant strains, we have: σc A c σ f A f σm A m = + εc εf εm or Ec = Ef Vf + Em(1 - Vf ) ................................................................................ [3.1] This equation is referred to as the Voigt estimate,but is more familiarly known as the rule of mixtures. 400It makes the implicit assumption that the Poisson W/Al-4%Cu Young modulus, E c , GParatios of the two components are equal (νf = νm), glass/epoxythus ignoring elastic constraints caused by 300differential lateral contractions. More sophisticatedmodels have been developed which allow for sucheffects, the most familiar being that of Hill (1964) 200which shows that the true stiffness of aunidirectional composite beam would be greater than 100the prediction of equation 3.1 by an amount which isproportional to the square of the difference inPoisson ratios, (νf – νm)2, but for most practical 0purposes this difference is so small as to be 0 0.2 0.4 0.6 0.8 1.0negligible. For example, for high-performance Fibre volume fraction, Vfreinforced plastics, νm ≈ 0.35 and νf ≈ 0.25, and for afibre volume fraction, Vf, of about 0.6, the correction Figure 3.2. Confirmation of the rule-of-mixtures relationship forneeded to account for the Poisson constraints is only the Young moduli, Ec, of undirectional composites consistingabout 2%. A good indication of the validity of the of tungsten wires in Al-4%Cu alloy and glass rods in epoxy resin.mixture rule for the longitudinal moduli of two
chapter three Elastic Properties 34composites of quite different kinds is given in transverse modulus, E tFigure 3.2. fibre matrix To estimate the transverse modulus, Et, we load,use a similar approach with a block model such Pcas that shown in Figure 3.3, with the sameconstraints as before, ie. well-bonded Figure 3.3. Simple series model of a composite.components with similar Poisson ratios, and novisco-elastic response from the matrix. This is now an ‘iso-stress’ model, so that σc = σf = σm. The totalextension of the model is the sum of the extensions of the two components: εcLc = εf Lf + εm LmIf the cross-sections of both phases are the same, L ≡ V, so dividing through by the stress (andremembering that Vf + Vm = 1) we have: εc ε f Vf εm Vm = + σc σf σm or 1 Vf Vm = + Et Ef EmThis is referred to as the Reuss estimate, sometimes called the inverse rule of mixtures: the transversemodulus is therefore: Ef Em Et = ............................................................................................ [3.2] Em Vf + Ef (1 − Vf )and the relationship between the Voigt and Reuss models can be seen in Figure 3.4. The Reuss estimateis sometimes modified to account for the Poisson effect in the matrix by introducing a ‘constrained’matrix modulus, effectively by dividing Em by(1 – ν2m) , so that: 80 1 Vf Vm (1 − νm ) ………..........….[3.3] 2 = + rule of mixtures, or Et Ef Em Voigt estimate, Ec Young modulus, E, GPa 60The relatively small effect of this correction isalso shown in Figure 3.4. 40 modified The problem with the Reuss model for the series modeltransverse case is that the geometry shown inFigure 3.3 in no way resembles that of a fibre 20 Reuss seriescomposite perpendicular to the fibres. And in model, Etassuming that the Poisson ratios of the phasesare the same, it ignores constraints due to 0strain concentrations in the matrix between 0 0.2 0.4 0.6 0.8 1.0the fibres. As a consequence, although it Volume fraction of reinforcement, Vfappears to give the correct form of thevariation of Et with Vf, the values predictedseldom agree with experimental Figure 3.4. Predicted variations of the longitudinal elastic modulus, Ec, and the transverse modulus, Et, of composites ofmeasurements. The model also implicitly glass and epoxy resin connected in parallel and in series. Theassumes that the transverse stiffness of the solid curves give the Voigt (parallel) and Reuss (series)fibre is the same as its longitudinal stiffness, estimates. The dashed line represents the Reuss estimateand while this is true of isotropic fibres like modified to include the effect of matrix Poisson constraint.
chapter three Elastic Properties 35glass, it is not true of reinforcements with a textileorigin like carbon and Kevlar. The need for a more refined procedure is apparentif we look at even an idealised model of the structureof a composite loaded transverse to the fibres, asshown in Figure 3.5. A model based on hexagonal(close-packing) geometry would clearly give differentresults from this square-packing model, and both Figure 3.5. Idealised square packing geometry in awould be different from the true packing geometry of transverse section of a unidirectional composite. any real composite (see Figure 3.6, for example) which will almost always tend to be much less regular than either of these idealised geometries. In practice the true transverse modulus lies some way above the lower bound given by the Reuss estimate. In discussing the behaviour of anisotropic materials, it becomes inconvenient to continue using subscripts like c and t and we resort to using a numerical index system associated with orthogonal axes, x1, x2 , and x3. We choose the x1 direction to coincide with the fibre axis and the x2 direction to coincide with the transverse in-plane direction (assuming that we are dealing, as is usually the case, with a thin plate of material). The longitudinal Figure 3.6. Real packing geometry: the cross-section of a unidirectional SiC/CAS laminate of Vf stiffness of a unidirectional composite is then referred to≈ 0. 4. The magnification can be judged from the as E1 and the transverse stiffness is E2. Since in most fibre diameter, 15μm. practical reinforced plastics composites, Ef » Em the Reuss and Voigt estimates of stiffness given in equations 3.1 and3.2 can be usefully approximated (in the new notation) by the relationships: E1 ≈ Ef Vf........................................................................................................... [3.4]a E2 ≈ Em (1 – Vf )-1 ............................................................................................. [3.4]bfrom which it is clear that the stiffness in the fibre direction is dominated by the fibre modulus, whilethat in the transverse direction is dominated by the matrix modulus. The Poisson ratio, ν, of an isotropic material is defined as the (negative) ratio of the lateral strain, ε2,when a stress is applied in the longitudinal (x1) direction, divided by the longitudinal strain, ε1,ie. ν = –ε2/ε1. Consideration of equations 3.1 and 3.2 shows that in a unidirectional composite laminathere will be two in-plane Poisson ratios, not one as in isotropic materials, and it is convenient to labelthese ν12 , called the major Poisson ratio (relating to the lateral strain, ε2, when a stress is applied in thelongitudinal (x1) direction) and ν21, the minor Poisson ratio (relating to the strain in the x1 direction whena stress is applied in the x2 direction). The two are not the same, since it is obvious that ν12 must be muchlarger than ν21. By means of arguments similar to those above for the determination of E1, it can beshown that for a stress applied in the x1 direction only, the major Poisson ratio is given by: ν12 = νf Vf + νm(1 - Vf).......................................................................................... [3.5]ie. it also obeys the rule of mixtures. Further thought will show that the minor Poisson ratio must berelated to ν12 by the equation: ν21 / E2 = ν12 / E1 .................................................................................................. [3.6]
chapter three Elastic Properties 36Values of the fibre and matrix Poisson ratios rarely differ bya great deal, so that neither matrix nor fibre characteristicsdominate these two elastic constants. When a unidirectional fibre composite is loaded by an in-plane (x1x2) shear force, it distorts to a parallelogram, asshown in Figure 3.7. The shear stress in the fibre direction, τ12, is matched by its complementary shear stress, τ21. Thesimplest model assumes that the fibres and matrix carry thesame stress: τ12 = G12 γ12 = Gf γf = Gm γm Figure 3.7. Definition of a shear relative to the x1 x2 Cartesian axes.and the (apparent) in-plane shear modulus, G12, is given by: 1 V (1 − Vf ) ..................................................................................................................... [3.7] = f + G12 Gf GmBy analogy with equation 3.2 for the transverse Youngs modulus, it can be seen that the matrix shearstiffness again dominates the composite shear modulus unless the fibre volume fraction is very large.3.2 THE HALPIN-TSAI EQUATIONS The models in the last section are simple models, although, if treated with care, they can give usefulapproximations to the behaviour of many composites. There have been many more formal treatments,however, based on more realistic models of the transverse fibre distribution, which yield results ofvarying degrees of complexity. These more rigorous approaches may give predictions of elasticproperties that are closer to experimentally observed values than the simple models of section 3.1, butthey are seldom easy to use in practice. For design purposes it is more useful to have simple and rapidcomputational procedures for estimating ply properties rather than more exact but intractable solutions.Convenient interpolation procedures have been developed by Halpin and Tsai (1968; see also Halpin,1992) who showed that many of the more rigorous mathematical models could be reduced to a group ofapproximate relationships of the form: E1 ≈ EfVf + Em(1 - Vf) ........................................................................................... [3.8] ν12 ≈ νfVf + νm(1 - Vf)............................................................................................. [3.9] (1 + ζηVf ) ............................................................................................... [3.10] E2 = Em (1 − ηVf ) (1 + ζηVf ) G12 = Gm ........................................................................................... [3.11] (1 − ηVf )The first two of these equations are the same rules of mixtures that we have already discussed. In thesecond two equations, ζ is a factor, specific to a given material, that is determined by the shape anddistribution of the reinforcement (ie. whether they are fibres, plates, particles, etc. and what kind ofpacking geometry), and by the geometry of loading. The parameter η is a function of the ratio of therelevant fibre and matrix moduli (Ef/Em in equation 3.9 and Gf/Gm in equation 3.10) and of thereinforcement factor ζ, thus:
chapter three Elastic Properties 37 ⎛ Ef ⎞ ⎜ − 1⎟ η= ⎝ m ⎠ ..................................................................................................... [3.12] E ⎛ Ef ⎞ ⎜ + ζ⎟ ⎝ Em ⎠ The parameter ζ is the only unknown, and values must be obtained empirically for a given compositematerial, although they are also sometimes derived by a circular argument involving comparison ofequations 3.9 and 3.10 with one of the exact numerical solutions mentioned previously. ζ may vary fromzero to infinity, and the Reuss and Voigt models are actually special cases of equation 3.9 for ζ = 0 and ζ= ∞, respectively. A number of analyses have been carried out to compare the predictions of equations3.9 and 3.10 with elasticity-theory calculations, often with a great degree of success, and it is frequentlyquoted from the early work of Halpin and Tsai that for practical materials reasonable values of ζ are 1for predictions of G12 and 2 for calculations of E22. It is dangerous, however, to accept these valuesuncritically for any given composite. This can be illustrated by taking a specific example. Sensitive measurements have been made of the elastic properties of a sample of unidirectionalcarbon-fibre-reinforced plastic (CFRP) consisting of Toray T300 carbon fibres in Ciba-Geigy 914epoxide resin with a fibre volume fraction of 0.56 (Pierron & Vautrin, 1994). Measurements were alsomade of the properties of the unreinforced matrix resin. Table 3.1 gives the properties of the plain matrixand fibres. Table 3.1. Properties of T300 carbon fibres and 914 epoxy resin. Property Fibres Matrix Youngs modulus, E, GPa 220 3.3 Shear modulus, G, GPa 25 1.2 Poisson ratio, ν 0.15 0.37 The experimental values are first compared in Table 3.2 with the predictions of the simplemicromechanical models of section 3.1. It can be seen that the fibre-dominated modulus, E1, is wellpredicted by the simple rule of mixtures, while the other properties, E12, G12 and ν12, are less wellpredicted. It is to some extent accidental that the prediction of E2 in Table 3.2 is as good as it is. Thevery rigid carbon-carbon bonds in carbon fibres are well-aligned with the fibre length, but in thetransverse direction, the fibre is far less rigid, ie. it is highly anisotropic, with an anisotropy ratio (theratio of the axial to transverse moduli) of about 10. Inserting a more appropriate value of Ef (which isdifficult to measure) into equation 3.2 would actually result in a value of E2 for the composite that waseven lower than that predicted in Table 3.2. Table 3.2. Predictions of composite properties by simple micromechanics models Equation Relationship Predicted values Experimental values (moduli in GPa) (moduli in GPa) 3.1 E1 = Ef Vf + Em(1 - Vf ) (RoM) 124.7 125.0 3.2 1 V (1 − Vf ) 7.4 9.1 = f + E2 Ef Em 3.6 1 V (1 − Vf ) 2.6 5.0 = f + G12 Gf Gm 3.4 ν12 = νfVf + νm(1 - Vf) (RoM) 0.25 0.34
chapter three Elastic Properties 38 Calculations of E2 and G12 by the Halpin-Tsai approximate model (equations 3.9 and 3.10) depend onknowing ζ. By solving these equations for a range of ζ we can then see what values of ζ must be used inorder to obtain predicted moduli that agree with the experimental values. Taking the data from table 2,but substituting a more appropriate transverse fibre stiffness of about 22GPa for the axial stiffness givenin the table we find that the appropriate values of ζ are about 2 for E2 and 2.5 for G12, for this particularmaterial. Use of the usually recommended values of 2 and 1, respectively, would thus be accurate for E2but would result in a 25% underestimate for G12. This emphasises the importance of calibrating themodel against experimental data rather than against predictions of other models if the method is to bevalid for design purposes. As a second example, we consider results obtained from ultrasonic pulse-velocity measurements onmodel composites consisting of 3mm diameter glass rods arranged in regular hexagonal arrays in castblocks of epoxy resin. The velocity, v, of a compressional pulse travelling through a solid is given by: v = √(C/ρ)where C is an elastic constant and ρ is the density of the material. C is not exactly equal to theconventional engineering Young modulus, E, although it has been shown that for ultrasonic rod waves Cand E are practically identical for a wide range of GRP materials (Harris and Phillips, 1972). Figure 3.8shows some experimental values for the longitudinal and transverse moduli of the model composites,determined by this method, as a function of 80volume fraction of the glass rods (Shiel, E 1 (glass rods)1995). The E1 values are well represented by E 2 (glass rods)the rule-of-mixtures line joining the E (glass beads) Elastic modulus, GPa 60 Tsai-Halpin model (ζ = 2)experimental moduli of the plain resin andthe glass rods, but the E2 values lie well T-H model (fitted: ζ = 5.37)above the line representing the Reuss 40estimate (equation 3.2) and significantlyabove the predictions of the Halpin-Tsaiequation (3.9) with the recommended value 20 Voigtof ζ of 2. In order to obtain a good fit to the Reussdata points, a value of ζ of 5.37 is required.It is interesting to note that the stiffnesses of 0model ‘particulate’ composites consisting of 0 0.2 0.4 0.6 0.8 1.03mm diameter glass beads randomly Reinforcement volume fraction, V fdispersed in the same resin (Birch, 1995) arealmost indistinguishable from the transverse Figure 3.8. Comparison of experimental data for the elasticstiffnesses of the rod-reinforced resin moduli of model glass/resin composites with various theoreticalcomposites, as might be expected. Nielsen predictions. The upper and lower bounds (rule-of-mixtures and(1978) has discussed at length the inverse RoM) correspond to equations 3.1 and 3.2. The Halpin-applicability of the Halpin-Tsai equations to Tsai curve for ζ = 2 represents the commonly used function for the transverse modulus, E2 (equation 3.9) but a value of ζ = 5.37particulate composites. is necessary to obtain the best fit to the data.3.3 THE COMPRESSION MODULUS We might expect that the compression stiffness of a unidirectional composite would be similar to itstensile stiffness, until we remember that the fine-scale structures of certain fibres — particularly thosederived from textiles — are known often to result in unpredictable behaviour of these fibres under shearand bending conditions. We might take as an analogy the behaviour of a piece of rope: tensile forcesdraw the fibres into tighter bundles, but any attempt to squeeze a length of rope axially will force thefibres apart. Piggott and Harris (1980) illustrated the problem by measuring the compression moduli, Ec,of polyester-based composites reinforced with glass, Kevlar-49 and two varieties of carbon fibres. Theirresults, illustrated in Figure 3.9, show that the variation with Vf is linear up to only about 50 vol% ofreinforcement, and that beyond this the rate of increase of stiffness falls or even becomes negative,depending on the fibre. The change in behaviour is evidently related to the diminishing ability of the
chapter three Elastic Properties 39 300 1:1matrix to constrain the fibre bundles to HMS dEc /dVf , GPadeform axially as Vm falls. As the inset 200figure plotting the initial slopes of these glass HTScurves against the fibre tensile modulus 100shows, the rule of mixtures is not properly 200 Kevlar-49obeyed except by the homogeneous and 0 Compression modulus, GPa 0 100 200 300 400isotropic glass fibre. The slopes, dEc/dVf, of Fibre tensile modulus, GPathe curves for the two carbon-fibre 150composites fall slightly below the 1:1 rule-of-mixtures values, while that for the aramid HMS carbonfibre composite falls well below the RoM. 100These results confirm what we know of the HTS carbonstructures of these reinforcing fibres. Somerecent elegant experiments by Young et al 50 E glass(1996), who used laser Raman spectroscopyto study the strains in single filaments Kevlar-49embedded in transparent resin, clearly 0 0 0.2 0.4 0.6 0.8showed the markedly non-linearcompression behaviour of carbon and Fibre volume fraction, Vfaramid fibres, in keeping with the behaviour Figure 3.9. Variation of the compression moduli of polyester-matrixof the composites illustrated in Figure 3.9. composites with volume fraction of four species of reinforcing fibre.3.4 THE ANISOTROPIC PROPERTIES OF A THIN LAMINA Having considered the properties of a lamina parallel with and perpendicular to the fibres, it is clearthat the elastic properties of a piece of unidirectional composite must vary continuously with orientationbetween these two extremes, and that in order to be able to design with such anisotropic materials it isnecessary to have a means of predicting this angular variation. Most common engineering materials — metals, plastics or ceramics — are usually considered to beisotropic, which is to say that they have the same properties in whichever direction the property ismeasured. This is not strictly true: wood is an excellent example of an anisotropic material in which thestiffness in the axial direction (parallel to the trunk centre) is greater than the stiffness in any otherdirection. Cold-worked metals also often have different properties parallel with and perpendicular to thedirection of working, although designers usually treat them as isotropic. An isotropic material has fourcharacteristic elastic constants, the Young modulus, E, the shear or rigidity modulus, G, the bulkmodulus, K, and the Poisson ratio, ν. In isotropic bodies, however, only two of these are independentproperties. If, for example, we know E and ν, we can calculate the other two constants from the familiarrelationships (see, for example, Dugdale, 1968): E E G= K= 2(1 + ν ) 3 (1 − 2 ν ) In an anisotropic fibre composite material these simple relationships cannot be valid. But in order todiscuss anisotropy, we first need a frame of reference, and we choose for convenience to use anorthogonal set of axes, (x1,x2,x3), in which the fibres are aligned in the x1 direction and transverse to thex2 direction, as shown in Figure 3.10. For this thin plate of composite, we might guess that there must be three values of Youngs modulus,E1, E2, and E3, three shear moduli, G12, G13, and G23, and six values of the Poisson ratio, ν12 and ν21, ν13and ν31, and ν23 and ν32, (not all of these are shown in Figure 3.10, for the sake of clarity) instead of thetwo independent constants that we need for an isotropic material. However, consideration of thegeometry of the laminate suggests that E3 is not likely to be very different from E2 and G13 is similar toG12, although G23 will probably be different from the other two shear moduli. Similarly, ν12 will be closein value to ν13 . By contrast with the shear moduli, however, for which symmetry implies that G12 = G21,
chapter three Elastic Properties 40it is clear, from the definition of Poissons ratio givenearlier, that ν12 » ν21, and so forth. The response of aunidirectional lamina, such as that shown in Figure 3.10, toapplied stresses must therefore be more complex than thatof an isotropic material. The general state of stress on a body can be written inthe form of a group of six independent components, σ1, σ2,σ3, τ12, τ23, τ31, where the single suffices represent normalcomponents (tension or compression) and the doublesuffices represent shear components (see Dugdale, 1968).Likewise, the strains form a similar series of sixcomponents, ε1, ε2, ε3, γ12, γ23, γ31. When a general stresssystem consisting of the six stress components acts on an Figure 3.10. Definition of elastic constants for anisotropic body, the familiar Hookes-law relationship anisotropic thin composite lamina.between stress and strain is usually written in the form of afamily of equations for the strain components: 1 ε1 = E [σ1 − ν(σ2 + σ3 )] 1 ε2 = E [σ2 − ν(σ3 + σ1 )] 1 ε3 = E [σ3 − ν(σ1 + σ2 )] ....................................... [3.13] 1 1 1 γ12 = τ12 γ 23 = τ23 γ 31 = τ31 G G G These equations can also be written in matrix format: ⎡ ε1 ⎤ ⎡ 1 E −ν E −ν E ⎤ ⎡ σ1 ⎤ ⎢ε ⎥ ⎢ −ν E 1 E −ν E ⎥ ⎢ ⎥ ⎢ 2⎥ ⎢ ⎥ ⎢ σ2 ⎥ ⎢ ε3 ⎥ ⎢ −ν E −ν E 1 E ⎥ ⎢ σ3 ⎥ ..................................... [3.14] ⎢ ⎥ = ⎢ ⎥ x ⎢ ⎥ ⎢ γ 23 ⎥ ⎢ 1G ⎥ ⎢ τ23 ⎥ ⎢ γ 31 ⎥ ⎢ 1G ⎥ ⎢ τ31 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ γ12 ⎥ ⎣ ⎦ ⎢ ⎣ 1 G⎥ ⎢ τ12 ⎥ ⎦ ⎣ ⎦ The order of the stress and strain components is arbitrary, and the sequences above are thoseconventionally used. In this form, the individual terms in the matrix of constants relating strain and stressare referred to as compliances and, as we have already said, there are only two independent elasticconstants in the matrix. The blanks in the matrix, which are really zeros, show that the normal stresscomponents do not cause shear deformations, and the shear stresses do not cause tensile or compressivedeformations. For a thin rod of isotropic material under a simple tension stress, σ1, equations 3.12 and3.13 reduce to the familiar form of Hookes law given by: σ1 = E ε1and for a thin plate subject to a plane-stress state only, since no stress components containing a suffix 3are then of any importance (σ3 = τ13 = τ23 = 0), the Hookes law relationship of equation 3.13 reduces to:
chapter three Elastic Properties 41 ⎡ ε1 ⎤ ⎡ 1 E −ν E 0 ⎤ ⎡ σ1 ⎤ ⎢ ε ⎥ = ⎢ −ν E 1 E 0 ⎥ ⎢ σ ⎥ ......................................................................... [3.15] ⎢ 2⎥ ⎢ ⎥ ⎢ 2⎥ ⎢ γ12 ⎥ ⎢ 0 ⎣ ⎦ ⎣ 0 1 G⎥ ⎦ ⎢ τ12 ⎥ ⎣ ⎦ By contrast, in an anisotropic solid like a fibre composite, each of the strain components has to berelated to all of the stress components, and it is possible that all of the elements in the matrix ofequations 3.13 could have real values — a total of 36 elastic constants. In reality, however, the symmetryof a unidirectional material makes it possible to reduce the number of constants and since the mostdemanding of current applications for composites call for the use of thin plates, the plane-stress stateallows further simplification. Since we shall want to make some limited use of the formal tensor theory of anisotropic elasticbehaviour, we must first introduce some new definitions. First, a unidirectional lamina, as discussed withreference to Figure 3.10, is regarded as transversely isotropic, that is to say that it has one major axis ofanisotropy — the fibre direction — and perpendicular to this the properties are independent oforientation (ie. E2 = E3, etc.). By convention we take the fibre axis to be parallel to x1 and the lamina isthen referred to as orthotropic. Second, in tensor notation the definitions of shear strains are slightlydifferent from the engineering definitions that we have been using so far. Although the engineering shearstress component identified as γ12 is the same as the tensor stress σ12, the tensor strain ε12 is only half theengineering strain γ12. For the orthotropic lamina loaded in plane stress, as we have seen, no stresscomponent with a suffix 3 is present, and the Hookes law tensor relationship, modifying equations 3.13,is then written: ⎡ ε1 ⎤ ⎡ S11 S12 0 ⎤ ⎡ σ1 ⎤ ⎢ ε ⎥ = ⎢S 0 ⎥ ⎢ σ 2 ⎥ ..................................................................... [3.16] ⎢ 2 ⎥ ⎢ 12 S22 ⎥⎢ ⎥ ⎢ ε12 ⎥ ⎢ 0 ⎣ ⎦ ⎣ 0 S66 ⎥ ⎢σ12 ⎥ ⎦⎣ ⎦or εij = Srs σkl.......................................................................................................... [3.17]where the Srs terms are referred to as the elastic compliances. A similar relationship gives stress as afunction of strain: σij = Crs εkl ........................................................................................................... [3.18]where the Crs terms are referred to as elastic constants or elastic coefficients, and it should be borne inmind that in general C is not simply the reciprocal of S.Note: although the suffices for stress and strain, as in ε1, ε12, etc. are directly related to the orthogonalaxis designations, x1, x2, those used for the Srs terms are not: they simply reflect the rows and columns inthe compliance tensor — hence, S66 simply corresponds to the last of the compliance components inequations 3.13. Again we see that the elasticity tensor contains some zero values: shear stresses do not cause normalstrains and normal stresses do not cause shear strains, and we describe this formally by saying that thereis no tension/shear coupling. The significance of this will become apparent later. The compliances, Srs,in equations 3.15 are related to our normal engineering elastic constants for the composite lamina: S11 = 1/E1 S22 = 1/E2 S66 = 1/2G12 S12 = –ν12/E1 = –ν21/E2
chapter three Elastic Properties 423.5 ORIENTATION-DEPENDENCE OF THE ELASTIC PROPERTIES OF A UNIDIRECTIONAL LAMINA Composites are rarely used in the form of unidirectional laminates, since one of their great merits isthat the fibres can be arranged so as to give specific properties in any desired direction. Thus, in anygiven structural laminate, predetermined proportions of the unidirectional plies will be arranged at somespecific angle, θ, to the stress direction. In order to calculate the properties of such a multi-ply laminate,it is first necessary to know how the elastic response of a single unidirectional lamina, such as that whichwe have been considering so far, will vary as the angle to the stress direction is changed. This is done bytransforming the x1x2 axes through some arbitrary angle, θ, a procedure that will familiar to anyone whohas studied the derivation of the Mohr’s circle construction. The derivation in given in Appendix 1, andfor our present purpose we need only the result of this analysis to illustrate the full anisotropic behaviourof a single unidirectional lamina. If both the stresses and the strains are transformed through an angle θfrom the x1,x2 co-ordinates to an arbitrary pair of axes (x,y), we find that the appropriate form ofHooke’s Law is now: ⎡ ε x ⎤ ⎡ S11 S12 S16 ⎤ ⎡ σ x ⎤ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ε y ⎥ = ⎢S12 S22 S26 ⎥ x ⎢ σ y ⎥ ...................................................................... [3.19] ⎢ε xy ⎥ ⎢S16 S26 S66 ⎥ ⎢σ xy ⎥ ⎣ ⎦ ⎣ ⎦ ⎣ ⎦ Except for the case when the (x,y) axes coincide with the composite orthotropic axes (the fibredirection, x1, and the transverse direction, x2) the compliance matrix, S rs , now contains six elasticconstants instead of the four in the matrix of equations 3.15. Since there are now no zeros in thecompliance matrix each component of stresswill contribute to all of the components ofstrain. A shear stress will therefore induce fibres at 30°normal strains and normal stresses will to plate edgeinduce shear strains. This shear-tensioncoupling has important consequences fordesigners since a thin plate of aunidirectional composite will show complexout-of-plane distortion if loaded off-axis.This is illustrated in Figure 3.11 for a plateof a unidirectional lamina with fibres at 30°to the loading axis which is subjected to acentral point bending load. The out-of-planedistortion is calculated by the commercial Figure 3.11. Out-of-plane distortion when an off-axislaminate analysis programme LAP unidirectional laminate is loaded in bending.(Anaglyph Ltd, UK). The compliance terms in the matrix in equations 3.18 are barred to remind us that these are no longermaterial elastic constants like the Srs in equations 3.15, but are functions of stress, as shown by thepresence of the matrix functions T and T-1 in their definitions (Appendix 1). It can be seen that if only atensile stress, σx, is applied, the strain measured in the direction of the stress, εx, is related to σx, by thefamiliar Hookes law, ie. ε x = S11σ xand the compliance S11 therefore represents the reciprocal Young modulus for this deformation: 1 S11 = Ex
chapter three Elastic Properties 43 But, clearly, S11 , and therefore also Ex, are functions of the orientation, θ. The matrix algebra needed to evaluate the barred compliances in equations 3.18 can be carried out painlessly with Mathcad, and it can be shown that the full expression for S11 is: S11 = S11 cos4 θ + S 22 sin4 θ + 2(S12 + S66 )cos2 θ sin2 θ ........................... [3.20] where the compliances S11, S22, S12, and S66 are the four elastic constants for the orthotropic lamina relative to the (1,2) axes, as defined in terms of the normal engineering constants at the end of section 3.3. If those definitions are substituted in equation 3.19, we have the orientation dependence of the elastic modulus, which we shall call E(θ): 1 cos 4θ sin4θ ⎛ 1 2ν ⎞ = + +⎜ − 12 ⎟ cos θ sin θ 2 2 ................................................ [3.21] E(θ) E1 E2 ⎝ G12 E11 ⎠ Similarly, the shear compliance component, S 66 , can be evaluated to obtain the orientation dependence of the shear modulus, G(θ): 1 ⎛ 1 + 2ν12 1 1 ⎞ 1 = 4⎜ + − ⎟ cos θ sin θ + 2 2 (cos4θ + sin4θ ) ..................................... [3.22] G(θ) ⎝ E1 E2 2G12 ⎠ G12 Equations 3.20 and 3.21 are plotted to show the angular SiO /epoxy 2 dependence (and the high degree 150 15 T300/914 carbon/epoxy of anisotropy) of two typical E(θ), GPa G(θ), GPa unidirectional laminates in Figure 3.13. It can be seen that the 100 10 stiffness of the unidirectional composite falls rapidly as the loading direction shifts away from 50 5 the fibre axis, the effect being more marked the higher the stiffness of the reinforcing fibres. 0 0 30 60 90 0 0 30 60 90 By contrast, the shear stiffness of the composite is less sensitive to Orientation, θ, degrees the fibre characteristics, as would be expected, being largely Figure 3.13. Dependence of Youngs modulus, E(θ) and the shear modulus, controlled by the matrix rigidity. G(θ), on the angle, θ, between the fibres and the stress axis for a carbon- fibre composite and a silica/epoxy composite. The shear modulus is a maximum, 60 however, in a direction at 45° to the fibre axis. The curve predicted by equation 3.20 validity of equations 3.20 and 3.21 for predicting the off- 50 experimental data for silica/epoxy axis elastic properties of laminates is usually very good, as can be judged from Figure 3.12 which compares the 40 predicted values of E(θ) for the silica/epoxy composite inE(θ), GPa Figure 3.13 with experimental data for this material 30 (Pabiot, 1971). 20 For most reinforced plastics composites, where the modulus ratio Ef/Em is large and the axial lamina 10 properties are dominated by the fibre stiffness, the influence of the values of in-plane shear modulus and 0 0 30 60 90 Poisson ratio on the form of the orientation dependence Orientation, θ, degrees defined by equation 3.20 is not significant. But in certainFigure 3.12. Comparison of predicted and experimentalresults for the angular variation of Youngs modulus of a unidirectional silica/epoxy composite (data of Pabiot, 1971)
chapter three Elastic Properties 44materials, like ceramic-matrix composites wherethe stiffnesses of the fibres and matrix are oftensimilar, variations in the value of Poisson’s ratio,caused by changes in processing conditions, for 140example, may modify the form of E(θ)substantially, as illustrated by the surface plot of 130 E(θ)E(θ) for a range of values of ν12 for a SiC- GPa 120reinforced calcium aluminosilicate CMCmanufactured by Corning (as shown in Figure 1103.14). 0.4 100 ν3.6 MULTI-PLY LAMINATES 0 0.3 tio , 30 ra n Unidirectional composites are rarely used in Orientati on, θ, de 60 90 0.2 iss o grees Popractice because of the high level of anisotropydemonstrated by Figure 3.13. In practice it is moresensible to make use of the versatility of Figure 3.14. Effect of the value of Poissons ratio on thecomposite materials by arranging the fibres in orientation dependence of Youngs modulus for SiC/CASdifferent directions to suit the design requirements. ceramic-matrix composites.There are various ways in which this is done, depending on the level of sophistication of the requiredproduct. It is useful at this stage, however, to refer to the most common procedure for producing high-performance laminates, which is to stack groups of single-ply laminae cut at various angles from thecontinuous sheet of prepreg — a continuous layer of fibres pre-impregnated with resin which is thendried (but not cured) — and then hot-press them between the heated platens, flat or shaped, of a press.The stacking sequence of such a laminate is described in short-hand form by formulae of the followingkind:(0)12 ─ a unidirectional composite with 12 plies 200 +θ(0,90)2s ─ a cross-plied laminate with four pairs of0/90 laminae arranged symmetrically (indicated 150 -34% cross-ply -θ E, GPaby the ‘s’) (0,90,0,90,90,0,90,0) 100 ud[(±45,02,902)2]s ─ a quasi-isotropic laminate with cross-ply θ24 plies arranged symmetrically 50 ud(+45,-45,0,0,90,90,+45,-45,0,0,90,90,90,90,0,0,-45,+45,90,90,0,0,-45,+45), the external ±45 plies 0 0 30 60 90providing protection against impact damage. 60 The choice of laminating sequence may varywidely, depending upon the particular design G, GPa 40 cross-plyrequirements, but an indication of the potential formodifying the lay-up to achieve a desired resultcan be seen by comparing the orientation 20 +225%dependence of the stiffness of a unidirectional udlaminate with the stiffness of a series of 0composites of lay-up ±θ, where in each case θ 0 30 60 90varies from 0 to π/2, as shown in Figure 3.15. Orientation, θ, degreesCross-laminating is a compromise solution whichresults in improved torsional and transverse Figure 3.15. The effect of cross-laminating on Youngsrigidity at the expense of some loss in longitudinal modulus and the shear modulus of a T300/5208 carbon-stiffness. It can be seen, for example, that by using fibre/epoxy composite.a ±20° laminate instead of a unidirectionalcomposite, for only a 34% loss in axial stiffness, the torsional rigidity may be doubled. The extent of theaxial stiffness reduction caused by cross-laminating is greater the stiffer the reinforcing filaments.
chapter three Elastic Properties 45Nielsen and Chen (1968) demonstrated the significance of this by showing the effect of randomising thefibre distribution in the plane of the laminate. The modulus, E(θ), given by equation 3.20, is randomisedover all θ: π/2 ∫ E(θ)dθ 1.0( E( = 0 π/2 …………...................[3.23] ∫ dθ 0 0.8 <E>/E1 0.6The solution to this equation, also obtained in GRP (Ef /Em = 22)Mathcad, for a pair of composites with 0.4different modulus ratios, Ef/Em is shown inFigure 3.16. For most practical purposes (Hull, 0.21981) the solution to equation 3.22 can be CFRP (Ef /Em = 70)approximated reasonably closely by: 0 0 0.2 0.4 0.6 0.8 〈E〉 = E1 + E 2 ...........................[3.24] 3 8 5 8 Fibre volume fraction, Vfwhere E1 and E2 are the known or calculated Figure 3.16. Effect of randomising the fibre orientations on thelongitudinal and transverse moduli for a stiffnesses of CFRP and GRP laminates.unidirectional lamina. An analogousapproximate expression can be obtained for the shear modulus of a random continuous-fibre composite: 〈G〉 = 8 E1 + 4 E2 ...........................[3.25] 1 1 Multi-ply laminates usually, but not always, consist of regular arrays of plies of the same materialand of the same thickness. When a laminate contains equal numbers of plies in each orientation, it is saidto be balanced. A (0,90)3 laminate is thus a balanced laminate, but such a laminate would have 0° and90° plies on opposite faces and may behave in unexpected ways if loaded in other than the 0° and 90°directions. Laminates that are arranged to have the plies on either side of a mid-plane matching in bothmaterial and orientation are described as symmetric: such laminates have the advantage that they remainflat after curing and during deformation. Symmetric laminates are therefore preferred for most purposes,but careful tailoring of a laminate lay-up can be used deliberately to produce a material that will changeshape in some desired manner under stress. For design purposes, it is necessary to have accurate methods of calculating the elastic properties of acomposite with a given lay-up as part of the process of tailoring a material to suit a given set ofrequirements. For a simple 0/90 lay-up it is a simple matter to treat the laminate as a parallelcombination of materials with two different elastic moduli and apply the mixture rule as given byequation 3.1, provided accurate values of the two moduli E1 and E2 are known. Thus, from dynamicmeasurements on an 11-ply unidirectional GRP composite of Vf = 0.64, values of E1 and E2 of 46.1GPaand 19.6GPa were measured (Harris et al, 1978: see Table 3.3). For an 11-ply 0/90 laminate from thesame manufacturer with the same raw material specifications, we may rewrite the rule of mixtures: E0 = 6 11 E1 + 11 E2 5 E90 = 5 11 E + 11 E2 6to give predicted values of E0 and E90 in the two orthogonal directions. As Table 3.3 shows, the estimateswould be adequate for most practical purposes.
chapter three Elastic Properties 46 Table 3.3. Comparison of some predicted and experimental elastic modulus values for typical GRP laminates. Material Vf Density Orientation Dynamic Predicted Model modulus, modulus, 3 -3 10 kg.m GPa GPa pultruded rod 0.7 2.09 0 54.4 51.3 RoM 0 90 24.7 9.1 inverse RoM 90 24.7 24.6 Halpin-Tsai (ζ = 4.6) ud 11-ply 0.6 2.04 0 46.1 47.2 RoM 4 Laminate 90 19.6 7.8 inverse RoM (Permali, UK) 90 19.6 19.6 Halpin-Tsai (ζ = 4) 45 20.4 12.6 Krenchel 0/90 11-ply 0.6 2.03 0 (6 plies) 35.3 34.0 RoM 3 Laminate 90 (5 plies) 30.5 31.6 RoM (Permali, UK) 45 21.6 12.6 Krenchel 0/90 woven 0.4 1.85 0 26.5 7 35-ply 90 27.5 laminate 45 16.7 (Permali, UK) A preliminary estimate of the elastic response of a general multi-ply laminate can often be obtainedby a netting analysis (Cox, 1952; Krenchel, 1964) which sums the contributions from each group offibres lying at a specific angle, θ, to the applied stress. If we assume that the fibres are continuous andthat there are no elastic Poisson constraints (νf = νm), each group of fibres (a proportion an of the totalfibre content) can be considered to have a reinforcing efficiency ancos4θ , and an overall compositeefficiency factor, ηθ, can be defined as: ηθ = Σan cos4 θ.......................................[3.26]The approximate composite modulus can then beobtained from a modified rule of mixtures as:Ec = ηθEf Vf + Em(1 - Vf) ………...........................[3.27]The fourth-power geometrical term in the efficiencyfactor clearly indicates its relationship with equation3.19. Shear and transverse behaviour is ignored, however,and the limitation of the model is therefore that it allowsno stiffness contribution from transverse fibres andignores interlayer constraints. For composites containinghigh volume fractions of high-stiffness fibres, none ofwhich are at 90° to the stress axis, it can give reasonable Figure 3.17. Values of the Krenchel efficiencyestimates of the laminate stiffness, but it is not acceptable factor for various fibre groupings.for detailed design purposes. For the GRP materialsreferred to in Table 3.3, for example, the predictions of the stiffnesses E45 are poor. Values of theefficiency factor, ηθ, for a range of fibre distributions are shown in Figure 3.17. For a 3-D random arrayηθ is about 1/6. It can be seen from Figure 3.16 that although the Krenchel factor is approximately inagreement with the more general randomisation model for GRP, it gives a poor prediction for CFRP.
chapter three Elastic Properties 47 In real laminates the individual plies which are stacked together to produce the multi-ply structure each have their own characteristic anisotropy. If a ply is at an angle to the load axis the simplified form of Hookes law for the orthotropic case (equation 3.15) is no longer applicable and the more complex form of equation 3.18 must be used. As we have seen, the zeros in equation 3.15 are replaced by non- zero values and there is then tension/shear coupling — ie. the application of a tensile force will induce shear strains and the application of shear forces will induce normal Figure 3.18. Out-of-plane distortion in an unsymmetric laminate consisting of a single pair of off-axis (±θ )plies. strains. This coupling can lead to unexpected The anisotropic shape changes induced in each separate distortions of composites under load and ply can only be accommodated in the laminate by the unless these are carefully balanced in distortion shown, accompanied by the development of constructing the laminate interlaminar shear interlaminar shear stresses. forces may be generated that are high enough to cause delamination (separation of the individual plies). A schematic illustration of the effect of shear/tension coupling in causing out-of-plane distortion in a simple ±θ laminate is shown in Figure 3.18 (Soden and Eckold, 1983). A full treatment of the elastic behaviour of thin composite laminates is beyond the scope of this book (readers are referred to the standard texts listed in the bibliography to Chapter 1) but an indication of the tk approach used in the classical theory may be given. Assuming symmetry about the centre line and in-plane t/2 th loads only, as shown in Figure 3.19, the elastic k ply response of the kth ply will, in the general case, be t/2 load described by equations A6 and A6a of Appendix 1, ie. [ ε ] k = ⎣S ⎦ k [ σ ] k ⎡ ⎤Figure 3.19. In-plane loading of a laminate of thickness t, and the location of the kth ply relative to the mid- plane. [ σ ] k = ⎣Q ⎦ k [ ε ] k ⎡ ⎤ in simplified form. The second of these relates each of the stress components to all of the strain components through a matrix of elastic coefficients: ⎡ σx ⎤ ⎡ εx ⎤ ⎢ ⎥ ⎢ ⎥ ............................................................................................. . [3.28] ⎢ σ y ⎥ = ⎡ A ij ⎤ ⎣ ⎦ ⎢ εy ⎥ ⎢σ xy ⎥ ⎢ε xy ⎥ ⎣ ⎦ ⎣ ⎦ where [Aij] is a stiffness matrix whose elements (the Q coefficients in equation A6a) are functions of the unidirectional lamina elastic constants E1, E2, G12, ν12, and the transformation angle θ. If the total composite is composed of a large number of evenly stacked layers, its properties can be determined by summing the stiffness matrices, [Aij], of each layer proportional to the number of plies lying in each direction: 1 k =n ⎡ A ij ⎤ = ∑ ( A ij )k .t k .......................................................................... [3.29] ⎣ ⎦ composite t k =1 where n is the number of plies, tk is the thickness of the kth ply, and t is the total laminate thickness.
chapter three Elastic Properties 48 On the other hand, if the laminate contains relatively few plies, the effect of stacking sequencebecomes important. Unsymmetric arrangements of plies, for example, may cause out-of-planedeformations (twisting or bending) such as that illustrated in Figure 3.18. These effects are mostlyundesirable, but on occasion they may be used to advantage, as in the aeroelastic tailoring of aircraftstructures, designing the lay-up so that it changes shape (and therefore its aerodynamic performance) in apredictable way in response to aerodynamic forces. In the full classical theory of thin laminates,therefore, it is necessary to obtain the resultant forces and moments acting on the laminate by integratingthe stresses in each ply through the laminate thickness. In addition to the A matrix of equation 3.27which relates in-plane forces to in-plane deformations, the full constitutional equation for laminatedeformation then includes relationships between in-plane forces, N, moments, M, in-plane deformations,ε, and curvatures, x, which are conveniently represented in the form of a partitioned matrix: ⎡N ⎤ ⎡ A B ⎤ ⎡ ε ⎤ ⎢M⎥ = ⎢ B D ⎥ ⎢ x ⎥ ............................................................................................ [3.30] ⎣ ⎦ ⎣ ⎦⎣ ⎦where A is the extensional stiffness matrix that we have already met, D represents the bendingstiffnesses, and B represents the stiffness matrix for coupling between these two. The calculations involved in analysing a complex laminate fully are tedious but straightforward, andare ideally carried out on one of the many pieces 60of computer software currently available. The SiO2/epoxy, udLAP programme by Anaglyph, UK, previously 50 glass/epoxy, 0/90, non-wovenmentioned is one such programme which glass/epoxy, 0/90, woven CSM/polyester, randomoperates under Microsoft Windows, but there 40 E(θ), GPaare many others, of different degrees ofsophistication, offering a variety of calculation 30facilities and graphics. 20 As an illustration of the general effects of 10structure and orientation on the elastic stiffnessof glass-fibre laminates, Figure 3.20 shows the 0variation with orientation of Youngs modulus 0 30 60 90for three types of laminate, the unidirectional Orientation, θ, degreessilica/epoxy material of Figure 3.12, the 0/90non-woven and woven glass/epoxy laminates Figure 3.20. Orientation-dependence of Youngs modulus forreferred to in Table 3.3, and an isotropic GRP four types of glass-fibre-reinforced plastic. The curves fittedlaminate made with randomly arranged to the upper three data sets correspond to equation 3.20.chopped-strand mat (CSM) reinforcement.3.7 SHORT-FIBRE COMPOSITES High-performance composites are generally made from continuous fibres, but there are manyapplications for which the requirements are less demanding, or for which the appropriate manufacturingroute cannot handle long fibres: it is then natural to consider using short fibres. Some reinforcing fibresare also available only in the form of short filaments. The ends of a fully-embedded short fibre cannot be fully loaded by shear at the fibre/matrix interface.This can be seen by embedding different lengths of a fibre in a resin block and attempting to pull the freeend out. The pull-out force is resisted by interfacial friction or bonding, and if the embedded length, x, isgreater than some critical length, lc the tensile stress in the fibre will break the free fibre before theembedded end can be pulled out. This critical length can be determined by considering the force requiredto pull an embedded length, x, of fibre of diameter, d, from a block of matrix (Figure 3.21). A force Papplied to the fibre develops a tensile stress σ = 4P/πd2 in the unembedded length and this is balanced bya mean shear force at the interface equal to τπdx. Thus, the ratio of embedded length to fibre diameter,
chapter three Elastic Properties 49x/d = σ/4τ. If the fibre can just be withdrawn fromthe matrix by a tensile load only marginallysmaller than the fibre breaking load, x must beequal to half the critical length, lc/2, since onlyone fibre end is concerned. Thus, the criticalaspect ratio is: Figure 3.21. Forces on a fibre being pulled from a block of l c σf …………….....................[3.31] matrix material. = d 2τiwhere σf is the breaking stress of the fibre and τi is the interfacial shear strength. This is a very simplisticmodel which assumes that all deformations are entirely elastic and that the shear stress is independent ofembedded length, but it gives useful insights into composite behaviour. We imagine an aligned array of short fibres ofidentical length embedded in a composite which isloaded parallel with the fibres, as shown in Figure3.22. Since the load on the composite must betransferred into the fibre by shear at the interface, itcan be seen that no transfer can occur at the Figure 3.22. Idealized short-fibre composite containingextremities of the fibre, and that the tensile stress in discontinuous but aligned fibres.the fibre will build up from zero at the ends. At thesame time, the interface shear stress will be high at the fibre ends, and will fall to zero when the fullextent of load transfer has been achieved, asshown in Figure 3.24. The calculations on which this figure isbased are the result of what is referred to asa ‘shear-lag’ analysis (Cox, 1952) whichinvolves determining the conditions forequilibrium of the shear and tensile forces ina simple twin-cylinder model such as that Figure 3.23. Concentric cylinder model used to determine theshown in Figure 3.23. For the results shown stress distributions, shown in Figure 3.24in Figure 3.24, Cox’s equations for the fibretensile stress and the interfacial shear stress have been used to simulate the situation for a 1mm length ofcarbon fibre (Young’s modulus 300GPa) embedded in an epoxy resin matrix. Other solutions for the stress distributions also exist, but the general validity of the functions which give lc/2 lc/2 3 rise to Figure 3.24 have been demonstrated fibre tensile stress, σ both by photoelastic experiments and, in 2 recent years, by means of laser Raman σ, GPa 0.2 spectroscopy which is able directly to 1 determine, at the molecular scale, the strain interfacial shear stress, τ 0.1 at any point along a single fibre embedded τ, GPa 0 0 in a resin block under external load (see, for 0 200 400 x, μm 600 800 1000 example, Galiotis, 1991). -0.1 Distance, x, from fibre end In the central portion of a long fibre, the -0.2 Cox stress functions vary only very slowly fibre length, l towards the fibre centre, so that we can usually make the assumption that there is aFigure 3.24. Variation of the tensile stress, σ, in the fibre and the plateau, as illustrated in Figure 3.24. The shear stress, τ, at the interface along the length of a short fibre ends of a short fibre thus constitute aembedded in a matrix. The calculations, based on the shear-lag notional ineffective length which reducesmodel of Cox (1952), relate to a 1000μm length of carbon fibre in the fibre reinforcement efficiency. The an epoxy resin matrix.
chapter three Elastic Properties 50contribution of these short, aligned fibres to the stiffness of the composite will therefore be less than therule-of-mixtures contribution, Ef Vf, by an amount that will depend on the efficiency of the stresstransfer, which is determined by the relative stiffnesses of the fibre and the matrix. Thus, the mixture-rule equation needs to be modified to allow for this fibre-end effect by introducinganother efficiency factor, usually designated ηl, so that: Ec = ηlEf Vf + Em(1 - Vf).................................................................................... [3.32]The Cox shear-lag model leads to a value for the efficiency factor, ηl, tanh ⎡ β2l ⎤ ⎣ ⎦ ηl = 1 − βl ........................................................................................... [3.33] 2where β, which determines the rate at which the tensile stress builds up at the fibre ends, is a function ofthe fibre and matrix stiffnesses and the composite geometry, viz. 2Gm Ef ............................................................................................... [3.34] β= 2 ro loge (R / ro ) In a regular fibre arrangement, the fibre radius, ro, and the matrix cylinder radius, R, are related to thefibre volume fraction. For example, if we assume a regular array, as in Figure 3.25, it can be seen thatthe triangle defines a unit cell which, if duplicated many times, would result in hexagonal symmetry.The area of the triangle is ½ (2R)2 sin60. This area contains three fibre sectors, each of area (πro2)/6, andthe total area of fibre is ½ πro2. From the definition of fibre volume fraction (and assuming Af ≈ Vf), itcan be seen that: ½ πro2 πro2 ....................................[3.35] Vf = 2 = ½( 2 R ) sin 60 2 3R 2and the value of R in equation 3.33 can therefore be written in termsof the fibre distribution. If equations 3.30 to 3.34 are now used todetermine values of the stiffnesses of typical GRP and CFRPcomposites reinforced with short fibres, the results can be plotted asfunctions of the fibre length or the fibre aspect ratio, l/d, as in Figure3.26, to show these stiffnesses as percentages of the moduli ofunidirectional laminates of the same composites but reinforced withcontinuous fibres, as given by the normal rule of mixtures, equation3.1. We see that ηl → unity as l → ∞, and the efficiency of stress Figure 3.25. Fibre packing in a simpletransfer is marginally higher in the GRP than in the CFRP. For hexagonal arrangement.aspect ratios of the order of 100 (ie. for fibre lengths of the order ofonly 1mm) some 95% of the full potential stiffening effect of fine reinforcing fibres like glass andcarbon can be achieved in composites reinforced with chopped, rather than continuous, fibres. In deriving Figure 3.26, we have ignored certain problems in applying the Cox model. It has beenpointed out (Galiotis and Paipetis, 1998) that in reality the matrix shear stiffness in equation 3.33 isaffected by interface chemistry, fibre surface treatments, elastic constraints due to fibre volume fraction,etc., and R is much more difficult to define for a real composite than is implied by equation 3.34. Ananalytic derivation of β is therefore questionable. They propose instead that β should be treated as anempirical index of the efficiency of stress transfer which can be considered as an ‘inverse length’. Forvalues of βl ≥ 10 the Cox hyperbolic equation for the fibre tensile stress, σ(x), which is plottedin Figure 3.24 can be simplified to give:
chapter three Elastic Properties 51 σ(x) = σ∞ (1 − exp( −β x) ................................................................................ [3.36]Direct estimates of β can be made by the laser-Raman spectroscopy technique mentioned earlier. If the short-fibre composite consists of layers of material with the fibres arranged at different anglesto the stress direction, equation 3.31 can be further modified by the inclusion of the appropriate value ofthe Krenchel factor, ηθ, thus: Ec = ηlηθEf Vf + Em(1 - Vf )............................................................................... [3.37]to give an estimate of the composite stiffness. The short-fibre composite model described above is clearly based on an idealised structure consistingof short fibres, all of identical length, arrangedin a unidirectional array. Although there aremanufacturing processes which can achieve such 100 95%structures (see chapter 1, section 1.3.6), they arerather specialised and composites reinforced 80with chopped or short fibres are, for the most Eshort / E long %part, likely to be of the type which are produced 60by the injection moulding of chopped-fibrereinforced thermoplastics or by the hot-press- 40 GRPmoulding of dough moulding compounds (eg.glass-fibre-filled polyester resins). During such 20moulding processes, there may well be some CFRPfibre alignment as a result of the high shear 0forces acting in the injection die or in the mould, 1 10 100 1000but the fibres will be imperfectly oriented, sothat the mean angle between the fibres and the Fibre aspect ratio, l/dmaterial flow direction will be greater than zero Figure 3.26. Variation with fibre aspect ratio, l/d, of theand the fibre lengths will be distributed about stiffnesses of aligned short-fibre composites of GRP andsome mean value as a result of damage leading CFRP for a fibre volume fraction of 0.5. The results areto fibre breakage during processing. Thus, in given as percentages of the normal continuous-fibre composite stiffnesses.order to estimate the elastic modulus of a short-fibre composite, the spreads of both the fibre orientations and the fibre lengths have to be taken intoaccount.3.8 HYBRID COMPOSITES Fibres of different types are sometimes mixed in a single matrix to produce hybrid composites. Themixing may occur at several structural levels, as illustrated in Figure 3.27, from skin-core structures,through ply-by-ply laminates to mixed-tow laminates.Random, intimately mixed fibre hybrids are rarelyconsidered. The purpose of hybridisation is to extend theconcept of tailoring the material’s properties to suitparticular design requirements, and to offset thedisadvantages of one component by the addition ofanother. For example, GRP are cheaper and tougher thanCFRP, but they are significantly less rigid, as we have Figure 3.27. Schematic illustration of three possible types of hybrid laminate structure: a)seen. In principle, then, the addition of a proportion of skin-core b) ply-by-ply c) tow-by-towglass fibres to a CFRP composite offers the possibility ofmaking the material cheaper while improving its toughness, ideally without paying too great a penalty interms of loss of stiffness. Reinforcing cloths and braids are available which are woven as hybridreinforcements with two or more species of fibre appropriately placed.
chapter three Elastic Properties 52 Skin-core structures are common in structural engineering and behave, in a sense, like I-beams, thecore playing the same rôle as the web of the I-beam and therefore being required to carry only shearforces, while the skin layers carry the major tensile and compression forces. In composite structures ofthis kind, the core may be a structural polymer foam or a paper or metal honeycomb. The bendingstiffness, EI, of a skin-core beam can be found in the usual way: n (EI)beam = ∑ EIi ............................................................................................... [3.38] i i=1provided the core is an isotropic material and the skin materials are symmetric and balanced laminates(Stavsky & Hoff, 1969; Marshall, 1982). For example, for a skin-core sandwich beam of width bconsisting of thin skins of a fibre composite of thickness t and a foamed polymer core of thickness c, thesecond moment of area of the core about the neutral plane is: bc 3 Ic = 12and that of each of the skins about the neutral plane is: bt 3 Is = + btz2 12where z is the distance from the neutral plane to the mid-plane of the skin. The bending stiffness of thesandwich beam is thus: (EI)beam = 2EsIs + EcIcWhen the skin thickness is small relative to that of the core, t2 << z2, and since Ec << Es the expressioncan be approximated to: (EI)beam ≈ 2Esbtz2which is sufficiently accurate for most purposes. Significant benefits are obtained by separating twoskins of a fibre composite with a lowstiffness core, as illustrated by the graph in 10 5Figure 3.28 which shows the variation ofbeam bending stiffness, given by equation 10 43.37, as a function of the ratio of the EIbeam /EIskinthicknesses of the core and the skin, c/t. 3 10The illustration is for a skin thickness, t, of1mm, a beam width, b of 10cm, and a 2polyurethane foam core of stiffness 1020MPa. The beam bending stiffness,(EI)beam, is normalised with respect to the 10 1bending stiffness, (EI)s, of the skinmaterial, and the graph is independent of 10 0the actual skin stiffness. For a 1mm skin 0 10 20 30 40 50and a 25mm core, the beam is over 4000 Ratio of thicknesses, core to skin, c/ttimes as stiff as the skin materials. Sincethe overall density of the beam falls as the Figure 3.28. The bending stiffness of a sandwich beam of width 10cm,ratio c/t increases, there is an optimum normalised with respect to the bending stiffness of the skin panels, asskin thickness for a beam of given weight, a function of the ratio of the thicknesses of the core and skin. The core is a polyurethane foam and the skin panels are 1mm thick. The normalised bending stiffness of the beam is independent of the stiffness of the skin material.
chapter three Elastic Properties 53as discussed by Farebrother and Raymond (1977). For simple hybrids consisting of unidirectional plies or mixed, aligned fibre tows, the tensile moduliobey the familiar rule of mixtures. With appropriate change of symbols, equation 3.1 becomes: Ehybrid = EAVA + EBVB + ECVC + ................................................................................................... [3.39]where EA , EB , EC ...... are the moduli of the individual component unidirectional composites (eg. CFRPand GRP in a carbon/glass/epoxy hybrid) and VA , VB , VC are the volume fractions of the componentsA, B, C, etc. As in the case of a simple composite, VA + VB + VC + = 1. An illustration of the validity ofthe mixtures rule for two varieties of unidirectional CFRP/GRP hybrid composites is given in Figure3.29. Two quite different composite structures are represented, one being an early pultruded polyesterrod material with intimately mixed E-glass and HM carbon fibres (Harris and Bunsell, 1975), and theother a laminate with alternate plies of E-glass/epoxy and XAS-carbon/epoxy (Dickson et al, 1989).When a mixed-ply laminate is tested in bending, the resulting flexural stiffness will clearly be affectedby the distributions of the different species of fibre. This was studied by Wagner et al (1982a and b) whofound apparent deviations from the mixtures rule in CFRP/GRP hybrid laminates. These deviationswere, however, predictable by their theoretical analysis based on the Hoff composite-beam model ofequation 3.37. Chamis and Lark (1977) have shown that fair agreement can be obtained betweenmeasured values of the flexural modulus of hybrid beams and those calculated by the formula: 1 k Ehybrid = ∑ ⎡zi3+1 − zi3 ⎤ Ei ......................................................................................... [3.40] 3t i=1 ⎣ ⎦where t is the laminate thickness, zi is the distance to the bottom of the ith ply and zi+1 is the distance tothe top of the ith ply.The tensile and flexural stiffnesses of most laminate hybrids are predicted satisfactorily by the methodsof classical thin-laminate theory, and most computer packages allow the construction of laminates fromplies of any given material for which the properties of the basic unidirectional ply are known. A detaileddiscussion of models of hybrid laminates is given by Chou (1992).3.9 RESIDUAL STRAINS Residual thermal strains occur in newlymanufactured composites as a result of 5differential thermal contraction during cooling ud composites (HM carbon) Normalised Youngs modulus,from the moulding, post-curing, or final heat- 4 [(±45,02)2]S laminates (XAS carbon)treatment temperature (eg. the ‘ceramming’temperature for a CMC with a glass-ceramic Ehybrid / EGRP 3matrix). The state of thermal stress will alsochange as a consequence of any temperature 2changes during service. Since the axialthermal expansion coefficient of many modern 1reinforcing fibres is small (slightly negative inthe case of carbon) and that of a resin matrix 0relatively large, the fibres in a composite 0 0.2 0.4 0.6 0.8 1.0laminate will be put into compression and the VCFRP/(VGRP+ VCFRP)matrix into tension during cooling from atypical curing temperature of 140°C. A roughestimate of the level of the axial stress in a Figure 3.29. Variation of the Youngs moduli of two families ofunidirectional composite can be obtained by unidirectional carbon/E-glass hybrid composites with composition. The rule of mixtures fits both sets of dataapplication of simple compound beam reasonably well.mechanics. The difference in the thermalstrains in the two components, Δε, is given by:
chapter three Elastic Properties 54 (εm – εf) = (αm – αf)ΔTor σm σf − = (αm − α f )ΔT Em Efwhere αm and αf are the coefficients of thermal expansion (CTEs) of the matrix and fibres, respectively,and ΔT is the temperature change. With the condition for equilibrium that no external load, P, is applied,the forces in the fibres and matrix will balance: P = Pf + Pm = σf Af + σm Am = 0where Af and Am are the cross-sectional areas of the two components, and equal to the respective volumefractions. Solving these two equations for the fibre and matrix residual stresses, σfr and σmr, we have: Ef Em Vm (α f − αm )ΔT σfr = Ec ...................................................................................... [3.41] Ef Em Vf (αm − α f )ΔT σmr = Ec Values of these residual stresses for a group of polymer- and ceramic-matrix composites are given inTable 3.4. It can be seen that in each case the fibre is in compression and the matrix in tension, asexpected. The fibre stresses are low compared with their tensile strengths, although it has been shownthat in very low-Vf resin-based composites fibres may be buckled or broken as a result of the residualstrains (Ferran and Harris, 1971). The matrix strains in the resin-based composites are also low, but itcan be seen that in the CMCs the residual matrix tensile stresses are of the order of 100MPa, which isclose to the expected matrix tensile strengths of these materials. As a consequence, matrix microcrackingoccurs very readily in CMCs under very small applied tensile loads (Harris et al, 1993), a matter of someconcern for users of these materials. Table 3.4. Residual thermal stresses in some typical unidirectional composites. Matrix Fibre Vf Temperature Fibre residual Matrix residual range, ΔT, K stress, MPa stress, MPa epoxy (high T cure) T300 carbon 0.65 120 -19 36 epoxy (low T cure) E glass 0.65 100 -15 28 epoxy (low T cure) Kevlar-49 0.65 100 -16 30 borosilicate glass T300 carbon 0.50 520 -93 93 CAS glass-ceramic Nicalon SiC 0.40 1000 -186 124 In addition to the axial residual stresses, differential thermal contraction also results in residual radialstresses which may make an important contribution to the mechanical behaviour of the composite sincethey provide one of the mechanisms whereby the matrix grips the fibre and therefore allows the transferof shear stress from matrix to fibre, as we saw in section 3.6. If there is no mechanical gripping of thiskind, the composite must rely exclusively on a chemical fibre/matrix bond. A rough estimate for theradial residual stress, Emαm ΔT, when a resin matrix of Em = 3GPa and CTE 100x10-6 K-1 contracts onto afibre of infinite rigidity as it cools through a temperature range, ΔT, of 100°C, is about 30MPa. If theenvironment surrounding the fibre were to be a homogeneous one having the transverse properties of acomposite instead of pure matrix, the effective stiffness of the matrix would be higher and its CTEwould be lower. The net effect on the radial residual pressure would therefore depend on relativechanges in E2 and α2 with increasing Vf. Harris (1978) used a simple micro-mechanical model to showthat the radial pressure was of the order of 25MPa in glass/resin systems, but a reworking of hiscalculation to incorporate more realistic models for the effects of Vf on the transverse stiffness (Halpin-Tsai) and CTE (Schapery, 1968, see below) suggests values as high as 40MPa for practical levels of Vf.
chapter three Elastic Properties 55These values are considerably higher than thosecommonly quoted from other models, but are in 1.0accord with experiments involving the pulling 0.8 ΔT = 100Kout of glass fibres from blocks of resin (Harris et Residual thermal strain, % 90° plyal, 1975). 0.6 0° plies One of the difficulties in carrying out such 0.4calculations is that of knowing precisely what 0.2value of ΔT to use. Although it is commonpractice to select the glass-transition temperature, tension 0Tg, or the post-cure temperature for a thermoset- compressionmatrix composite, it is known that some stress -0.2relaxation can occur in resins like epoxies some 0 0.2 0.4 0.6 0.8 1.0way below these temperatures. The actual Fibre volume fraction, Vfresidual stress levels in manufactured compositesare therefore likely to be considerably lower thanthose predicted from simple models. Figure 3.31. Residual thermal strains in the 0° and 90° plies in a 0/90/0 glass/epoxy laminate. The thermal expansion coefficients incomposite laminae will, like other elastic properties, be anisotropic. Schapery (1968) derived thefollowing expressions for the CTEs parallel with and transverse to the fibres in a unidirectional lamina: E f α f Vf + Em αm Vm ...................................................................................... [3.42] α1 = Ec α2 = (1 + νm )αm Vm + (1 + ν f )α f Vf − α1(ν f Vf + νm Vm ) ........................................ [3.43]α1 and α2 being, respectively, the axial and transverse CTEs. In polymer-matrix composites α1 is strongly fibre-dominated and falls much more 1.0 rapidly than a mixtures-rule prediction as Vf increases, whereas α2 initially rises slightly before Normalised residual stress ambient conditions 0.8 following an approximate mixtures rule between the fibre and matrix values. The maximum difference 0.6 between the CTEs occurs at a volume fraction of about 0.2 for a typical laminate of E-glass and epoxy 0.4 temperature/humidity resin. A consequence of the expansion anisotropy is cycling that laminates containing plies at different angles 0.2 will distort in unexpected ways unless care is taken to ensure that the constraints are always matched. A 0 single pair of unidirectional CFRP plies bonded 0 5 10 15 20 25 together at 0° and 90° will behave like a bimetallic Time, days strip during unconstrained cooling from the curing temperature — a phenomenon that can be used toFigure 3.30. Reduction in residual thermal stresses in a determine the residual stress levels in laminates byunidirectional carbon/glass/epoxy hybrid laminate under different hygrothermal conditions. direct measurements of the curvature that occurs. Equations 3.40 may also be used to calculate the residual stresses in 0/90 lay-ups or in mixed-plyhybrid laminates which can develop significant levels of thermal stress if the expansion coefficients ofthe two species are significantly different, as in a CFRP/GRP hybrid, for example. As an illustration,Figure 3.31 shows the predicted levels of thermal strain, as functions of the ply fibre content, in the pliesof a 0/90/0 GRP laminate. The values of the CTEs were obtained from equations 3.41 and 3.42 and thevalue of E2 required to determine the transverse strain in the 90° ply was obtained from the Halpin-Tsaiequation (equation 3.9) with ζ = 4. It can be seen that the 0° plies are in a modest state of compression,while for a practical Vf of 0.6 the strain level in the transverse ply is of the order of 0.5%. Similar resultswere obtained experimentally for model glass/resin laminates by Jones and Mulheron (1983). The
chapter three Elastic Properties 56development of residual thermal stresses in hybrid laminates has sometimes been observed to result in awaviness of the fibre tows in the laminae that are under compression as a consequence of in-planebuckling of the tows before the resin ceases to be capable of flow. Such a defect would be likely to haveserious consequences for the compression strength of the material (see Chapter 4). The thermal strains arising during either post-cure cooling or subsequent service at raisedtemperatures in both single-fibre and hybrid laminates can be determined satisfactorily by means of mostcommercial software applications, and the theoretical basis for the calculations can be found in standardtexts, such as that of Jones (1975). It should be born in mind, however, that most matrix resins are visco-elastic to some extent, and their ability to undergo time-dependent stress relaxation is accentuated byeven slightly elevated temperatures or exposure to moisture which plasticizes some thermosets. Residualstresses arising during initial manufacture may therefore fall to insignificant levels during storage underambient conditions. An illustration of this is shown in Figure 3.30 where the stresses determined fromthe curvature of two-ply strips of a unidirectional glass/carbon/epoxy laminate are observed to bedissipated as a result of hygrothermal conditioning treatments.3.10 TEXTILE COMPOSITES Although many high-performance composites are manufactured from prepreg sheet consisting of thinlayers of aligned fibres preimpregnated with semi-cured resin, thereare many practical advantages in using woven fabrics as thereinforcing medium. Textiles can be produced in a wide variety offorms, starting from simple plain-weave cloth, with equal numbersof tows of fibre in the warp and weft directions, via tubular braidedstructures, to cloths with fibres in three or five directions(sometimes confusingly called 3D and 5D weaves) and genuinelythree-dimensional fabrics with a proportion of fibres runningthrough the thickness. The characteristics of these materials asreinforcements may be of great value to composites designers,particularly since woven fabrics drape much more satisfactorilyover complex curved surfaces than unidirectional prepregs can. Adetailed mathematical treatment of textile composites manufacturedfrom woven products is given by Chou (1992), and an importantrecent collection of papers on the subject has been edited byMasters and Ko (1996). Figure 3.32. Photograph of a piece of commercial plain-weave glass cloth. Since, in woven cloths, varying proportions of the reinforcing filaments will be lying out of the plane of the laminate into which they are incorporated, the elastic reinforcing efficiency of the fabric will be somewhat lower than that of a ply derived from a prepreg sheet. This can be illustrated by way of a simple example for composites containing a 0/90 textile. The general appearance of a typical balanced plain- weave glass fabric is shown in Figure 3.32. The fibre tows in this fabric are flattened, and the extent to which they deviate from a single plane depends both on the degree of flattening and the tightness of the weave. In satin-weave fabrics, the ratio of the numbers of tows (or ends) lying in the 0° and 90° directions may be greater than unity, and the use of a satin-weave Figure 3.33. (a) Two-unit representative volume element reinforcement therefore allows the designer of a composite reinforced with a six-harness satin-weave greater flexibility in meeting service cloth. (b) Mechanical model of the RVE.
chapter three Elastic Properties 57requirements. A simple model to represent the structure of such a weave is shown in Figure 3.33 whichdepicts an idealised weave described as a six-harness satin weave. For a harness number of two, themodel is equivalent to a plain weave. Many models of woven-fabric composites treat the undulations ofthe warp fibres as they pass over and under the weft tows as a sine wave, but for a rough estimate we canreasonably adopt the simpler linear approach shown in Figure 3.33. The ‘representative volume element’ (RVE) shown in this figure can be modelled as two series-connected elements — the kinked section, component 1, and the unkinked section, component 2. Thefirst of these is itself a parallel-connected trio of elements, one at the out-of-plane angle θ to the maincomposite axis, the second at 90°, and the third a plain resin element. Component 2 is equivalent to asimple non-woven 0/90 laminate, also parallel connected. Thus, the mechanical analogue of the weave isillustrated in Figure 3.33. Component 2 is modelled as in section 3.5 of this chapter, the required values of E1 and E2 requiredto calculate the component stiffness, E(2), being determined from the Halpin-Tsai equations with ζ = 5for a notional Vf of 0.65. Simple geometrical considerations allow us to determine the volumes of theelements in component 1 and their effective fibre volume fractions. The kinked component is thenanalysed by a modified Krenchel approach: E(1) = cos4(θ) E1Vf(θ) + E2 Vf(90) + Em Vmwhere Vf(θ) and Vf(90) are the proportions of fibre at the two specified angles. Unlike the conventionalKrenchel estimate, this therefore includes a contribution from the 90° fibre tow. The overall modulus ofthe RVE is now obtained as a Reuss (series) 40estimate for the stiffness contributions of theappropriate proportions of components 1 and 2. 0/90 non-wovenThe harness number will clearly affect these 35 Elastic modulus, GPaproportions and the degree of flattening of thetows determines the angle θ and the overall 30 tthickness of the RVE. Figure 3.34 shows the wresults of these calculations, plotting the 25composite Young modulus as a function of θ° w/tharness number for various tow-flattening ratios, 14 4w/t (ratio of major to minor axes of the elliptical 20 18.5 3tow shape). Crude though this model is, the 26.5 2agreement with the stiffnesses of the plain- plain weave 15weave and 0/90 non-woven GRP laminates 1 10 100referred to in Table 3.3 is adequate for many Harness numberdesign purposes. Figure 3.34. Predicted moduli for satin-weave GRP composites3.11 PLIANT COMPOSITES as a function of harness number. The angle θ is the mean angle of deviation from the laminate long axis of the fibre tows in the Pliant composites are, generally speaking, weave cross-over sections. The flatter the fibre tows, the highertextile fabrics coated with waterproof polymers the aspect ratio, w/t, and the lower the misalignment angle, θ.which are used in various applications requiringflexibility, toughness, gas-tightness, etc. Typical applications include air-house membranes, dirigible air-ship envelopes, and rubber boats. Depending upon requirements, the reinforcement may be fabricswoven from either glass fibres or from conventional textiles, such as polyesters (eg. Terylene/Dacron) orpolyamides (Nylons). For special requirements, aramids like the lower-performance Kevlar fibres maybe appropriate. The range of possible fibre stiffnesses thus covers an order of magnitude or so, fromabout 5GPa for Nylon to 73GPa for glass. The coatings may be low-cost materials like PVC,polyurethanes and rubbers, or more expensive fluoroelastomers like Hypalon. The more costly and morerigid fluoropolymers like PTFE have excellent long-term weathering and fire-resistance properties.
chapter three Elastic Properties 58 The elastic behaviour of pliant composites is more difficult to characterise than that of rigidcomposites. When a typical uncoated, woven fabric is stretched the effective stiffness will includeapparent strain contributions from several mechanisms other than the true elastic extension of the fibresthemselves. These mechanisms, which do not occur to the same extent in rigid composites, may beidentified as follows. i) Yarn shear or rotation may occur if the principle stresses are not aligned with the warp and weft of the fabric. ii) Crimp interchange. If a highly crimped weft yarn is directly loaded it will not begin to extend elastically until it has lost the crimp which will in some measure be transferred to the originally straight warp yarns. A similar type of deformation occurs, although to a lesser extent, in woven cloth-reinforced resins. iii) Yarn flattening, leading to a reduction in effective yarn diameter. iv) Yarn compaction, resulting in an increase in packing density. v) Fibre straightening and/or rotation with the yarn structure. The first two occur at low stresses and depend on the principal stress ratios (not on their magnitudes),whereas the other mechanisms become active onlyat high stresses. In normal fabric behaviour true 500elastic extension of the individual filamentsprobably never occurs, and since this is the only 400 PVC/polyestermechanism considered in conventional netting PTFE/glassanalyses like that of Cox (1952) such analyses are Load, kg 300not useful for predicting the behaviour of fabricsor pliant composites. Shanahan et al (1978) have 200shown that in some respects fabrics may be treatedas sheets of an elastic continuum and have appliedthe basic framework of laminate theory. For 100 warpmembrane strains the tensile modulus, E(θ), from weftequation 3.18 gives a reasonable approximation to 0 0 5 10 15 20measured properties of some types of fabric, butcoupling between membrane modes of Strain, %deformation, bending and twisting, and large non-linear elastic strains cannot be dealt with by the Figure 3.35. Tensile load/strain curves for two types ofcontinuum model. architectural coated fabrics. Test strips were 5cm wide. The application of an extensible or rubber coating to a woven fabric is considered, for designpurposes, not to change the cloth characteristics. For small-strain extensional behaviour in the warp orweft directions this may be an acceptable assumption, but even a non-rigid matrix will significantly raisethe in-plane shear resistance of a coated fabric. The shear stiffness may also be affected by a stress-system which increases the inter-yarn frictional forces. The wall of an internally pressurised tube, forexample, appears to become stiffer as the internal pressure is increased and rotation of the yarns isinhibited by the increased inter-yarn friction (Topping, 1961). An illustration of the comparativestress/strain behaviour of two quite different types of coated fabric is shown in Figure 3.35 (Ansell andHarris, 1980): the effect of the matrix rigidity is clear. The generalised two-dimensional form of Hookes Law for a textile or coated fabric (Alley andFaison, 1972) contains nine stiffness coefficients. Since the straining of such materials is not necessarilyconservative (ie. the values of the coefficients may be dependent on the state of strain in the material andits loading history) all nine coefficients are independent, necessary, and multi-valued. Furthermore, in acoated fabric some of the coefficients are likely to be time dependent. In a non-linear anisotropicmembrane, then, it is not surprising that the setting up of practicable constitutive relationships should bean unwieldy process and of little practical use for design purposes. Useful surveys of the problems ofdesigning with coated fabrics are given in two published conference proceedings on air-supportedstructures (Evans et al, 1980, and Happold et al, 1984).
chapter three Elastic Properties 593.12 REFERENCES TO CHAPTER 3 Alley VL and Faison RW, 1972, J Aircraft, 9, 55-60 and 211-216 Ansell MP, Harris B, 1980, Air-Supported Structures: the State of the Art, (Institution of Structural Engineers London), 121-130. Birch SJ, 1995, Unpublished data, School of Materials Science, University of Bath. Chamis CC and Lark RF, 1977, Hybrid and Select Metal-Matrix Composites (ed. WJ Renton), (AIAA New York), 13-51. Chou TW, 1992, Microstructural Design of Fibre Composites, (The University Press, Cambridge). Cox HL, 1952, Brit J Appl Physics, 3, 72-79. de Ferran EM and Harris B, 1971, J Mater Sci, 6, 238-251. Dickson RF, Fernando G, Adam T, Reiter H and Harris B, 1989, J Mater Sci, 24, 227-233. Dugdale DS, 1968, Elements of Elasticity, (Pergamon, Oxford). Evans CJ, Bate SCC, Happold E and Piall GHA (editors), 1980, Proc. Symposium on Air-Supported Structures: the State of the Art, (Institution of Structural Engineers, London). Farebrother TH and Raymond JA, 1977, Polymer Engineering Composites (editor MOW Richardson), (Applied Science Publishers London), 198-235. Galiotis C, 1991, Compos Sci and Technol, 42, 125-150. Galiotis C and Paipetis A, 1998, J Mater Sci, 33, 1137-1143. Halpin JC and Tsai SW, 1969, Effects of Environmental Factors on Composite Materials, Report AFML-TR 67-423, (US Air Force Materials Laboratory, Dayton, Ohio). Halpin JC, 1992, Primer on Composite Materials Analysis (2nd edition), (Technomic Publishing Lancaster Pennsylvania USA). Happold E, Dickson MGT, Halstead DH, Tietz SB and Williams CJK, (editors), 1984, Proc. Symposium on The Design of Air-Supported Structures, (Institution of Structural Engineers London). Harris B and Bunsell AR, 1975, Composites, 6, 197-199. Harris B and Phillips MG, 1983, Developments in GRP Technology (ed. B Harris), (Applied Science Publishers, London), 191-247. Harris B, 1978, J Mater Sci, 13, 173-177. Harris B, Guild FJ and Brown CR, 1979, J Phys D: Applied Phys, 12, 1385-1407. Harris B, Habib FA and Cooke RG, 1992, Proc Roy Soc (Lond), A437, 109-131. Harris B, Morley J and Phillips DC, 1975, J Mater Sci, 10, 2050-2061. Hill R, 1964, J Mech Phys Solids, 12, 199-212 and 213-218. Hull D, 1981, An Introduction to Composite Materials, (University Press, Cambridge). Jones FR and Mulheron M, 1983, Composites, 14, 281-287. Jones RM, 1975, Mechanics of Composite Materials, (Scripta Book Co, Washington, & McGraw-Hill). Krenchel H, 1964, Fibre Reinforcement, (Akademisk Forlag, Copenhagen, Denmark). Marshall A, 1982, Handbook of Composites (ed. G Lubin), (Van Nostrand Reinhold New York), 557-560. Masters JE and Ko F, (editors), 1996, Compos Sci and Technol, 56, 205-386, Textile Composites Special Issue, (Elsevier Science, Oxford). Nielsen LE and Chen PE, 1968, J Materials, 3, 352-358. Nielsen LE, 1978, Predicting the Properties of Mixtures, (Marcel Dekker, New York). Pabiot J, 1971, Composite Materials Conference proceedings number 63, (AGARD/NATO, Neuilly, Paris), paper 6. Pierron F and Vautrin A, 1994, Compos Sci & Technol, 52, 61-72. Piggott MR, Harris B, 1980, J Mater Sci, 15, 2523-2538. Schapery J, 1968, J Compos Mater, 2, 380-404. Shanahan WJ, Lloyd DW and Hearle JWS, 1978, Textile Research J, 48, 495-505. Shiel D, 1995, Unpublished data, School of Materials Science, University of Bath.
chapter three Elastic Properties 60 Soden PD and Eckold GC, 1983, Developments in GRP Technology (ed. B Harris), (Applied Science Publishers, London), 91-159. Stavsky Y and Hoff NJ, 1969, Engineering Laminates (ed. AGN Dietz), (MIT Press, Cambridge, Mass), 5- 59. Topping AD, 1961, Aerospace Engng, 20, 53-58. Wagner HD, Roman I and Marom G, 1982a, Fibre Sci and Technol, 16, 295-308. Wagner HD, Roman I and Marom G, 1982b, J Mater Sci, 17, 1359-1363. Young RJ, Yallee RB and Andrews MC, 1996, Proc. 7th European Conference on Composite Materials: ECCM7, London, May 1996, (Woodhead Publishing, Abington, UK), vol. 2, 383-388.
4 THE STRENGTH OF FIBRE COMPOSITES S trength is more difficult to predict than elastic properties because it depends on the mechanisms of damage accumulation and failure as well as on the properties of the constituents, and the failure behaviour of fibre composites is often complex. The manner in which damage occurs in the material, and the way in which it accumulates to reach some critical level which precipitates final failure depends on many aspects of the composite construction, including the fibre type and distribution, the fibre aspect ratio, l/d, and the quality of the interfacial adhesive bond between the fibres and the matrix. Much of the software currently available for predicting the strengths of fibre composites must be treated with circumspection on account of this uncertainty relating to the modelling of failure. Because of the complex nature of failure in many types of composite, considerations of strength and toughness are closely inter-related. And although in this book we have opted, for the sake of clarity, to treat them in separate chapters, we should bear in mind when designing with composites that the strength and toughness may not be Figure 4.1. A simple unidirectional composite independent. lamina under tensile load. 4.1 TENSILE STRENGTH 4.1.1 Unidirectional continuous-fibre composites Consider a simple unidirectional composite lamina reinforced with continuous fibres which are initially well-bonded to the matrix so that under load fibres and matrix deform together (Figure 4.1). The load is shared between them and, following the argument at the beginning of chapter 3, we can write the stress on the composite, (σ)c, as: (σ)c = (σ)f Vf + (σ)m (1 – Vf) where (σ)f and (σ)m are the stress levels in fibres and matrix (as opposed to being properties of fibre and matrix), and are equal to Efε and Emε, respectively, where ε is the composite strain. What happens as loading continues depends on the nature of the individual components. There are two common situations which may be taken as examples, as illustrated in Figure 4.2. In most practical composites, the high- performance reinforcing fibres can usually be regarded as being brittle, ie. they deform elastically to failure, showing little or no non-linear deformation. In metal- and polymer-matrix composites, the unreinforced matrix is usually capable of some irreversible plastic deformation and in such materials the matrix failure strain is usually much greater than that of the fibres. By contrast, in ceramic- matrix composites the matrix is also brittle, and although much weaker than the reinforcing fibres it is often almost as rigid as the fibres. The matrix failure strain is therefore usually less than that of the fibres. As the diagram in Figure 4.2 shows, when the stress in the ductile matrix reaches the matrix Figure 4.2. Schematic illustrations of the stress/strain curves of two types of yield stress, σmy, the matrixcomposite, (a) with a ductile matrix and (b) with a brittle matrix, as derived from continues to bear load, although the stress/strain behaviour of the constituents. the slope of the stress/strain
chapter four Strength 634.1.2 The problem of the strength of brittle fibres The simple models that we have beenconsidering make the assumption that the 25 150 sam ples of Enka HTA carbon fibrereinforcing filaments have a unique failure m ean fibre strength:stress, σfu, and that they all fracture 20 2.7GPasimultaneously when the load on the Frequencycomposite reaches this critical level. In reality, 15since almost all of the common reinforcingfilaments exhibit brittle behaviour, there is a 10statistical distribution of fibre strengths ratherthan a unique value of σfu. The mean filament 5strength, σf u , and the spread of values isdetermined by the statistical distribution of 0defects or flaws in the fibre or on its surface. 0 1 2 3 4 5In general, the spread of strengths in any Fibre strength, GPacommercial tow of fine fibres is quite large, asshown in Figure 4.4 by some typical results Figure 4.4. Distribution of tensile strengths of 150 samplesfor commercial HTA carbon fibres of commercial Enka HTA carbon fibre. The sample testmanufactured by Enka. length was 3cm (Harris et al, 1992a Although we often speak of the ‘mean strength’ and the ‘standard deviation’ of the strengths of thefibres, the distributions are seldom Gaussian (or Normal) distributions. We usually use an exponentialdistribution described by Weibull (1951) which gives the probability of failure at a stress level, σ, of anysample from a given batch of fibres of identical length as: ⎡ ⎛ σ ⎞m ⎤ P(σ ) = 1 − exp ⎢ − ⎜ ⎟ ⎥ .................................................................................... [4.4] ⎢ ⎝b⎠ ⎥ ⎣ ⎦The parameters m and b are known as the shape and scale parameters, respectively*. The shape factor,m, sometimes called the Weibull modulus, relates to the uniformity of the distribution of flaws in abrittle material: a high value of m implies a highly uniform distribution of defect sizes and therefore alow level of variability of fibre strengths. Conversely, a low value of m implies highly variable flawsizes and a large spread of measured strengths, as in Figure 4.4. When the data are ranked and plotted asdescribed in Appendix 2 (see Figure 4.5), it can beseen that the two-parameter Weibull model of 2equation 4.4 provides a reasonable fit to the data, 1despite the fact that for carbon fibres one wouldexpect to find a minimum stress level (the location 0 Ln[-ln(1 - P)]parameter) below which no failures would occur. gauge length = 2cmThe parameters of the distribution shown are m = 6.3 -1 m = 6.3and b = 2.96GPa (cf. the arithmetic mean of2.76GPa). A value of 6.3 is very low when -2compared with the behaviour of normal engineeringmaterials (m ≈ 30 to 100), but it is not untypical of -3ceramics. -4 For composites users, there are two important 0 0.5 1.0 1.5consequences of the weakest-link model upon which Ln(strength, GPa)the statistical analysis is based. First, the breakingload of a large bundle of brittle fibres (tows of Figure 4.5. Two-parameter Weibull plot of strengths ofcarbon fibres typically contain between 3,000 and untreated ENKA carbon fibres: gauge length = 2cm.__________________________________________________________________________________*A brief introduction to the statistical background to this method of analysis is given in Appendix 2
chapter four Strength 6410,000 individual filaments) is lower than the arithmetic mean strength of all the filaments in the bundle.This can be shown by the following simplified argument. We assume that all of the filaments in a large bundle have the same length and the same elasticmodulus and are equally loaded. As a bundle is loaded, the weaker fibres in the bundle will fail at lowloads and the applied load must then be redistributed among the remaining fibres. At some point, thefailure of one more filament will mean that the load carried by those remaining is too great for them tosupport, and the bundle fails. Suppose that at a load, PF, on the bundle, n fibres out of a total of N havealready failed. The stress on the remaining filaments is then: σF = PF /AN-n......................................................................................................... [4.5] AN-n being the cross-sectional area of the remaining unbroken fibres. The ratio of unbroken fibre area tototal area, AN-n /AN , is 1 - n/N, and since this describes the same failure probability as that given by theWeibull function, P(σ), in equation 4.4, we can rewrite the expression for PF, the load on the remainingfibres in the bundle, in equation 4.5, as: ⎛ n⎞ ⎡ ⎛ σ ⎞m ⎤ PF = σF A N ⎜ 1 − ⎟ = σF A N exp ⎢ − ⎜ F ⎟ ⎥ ................................................................... [4.6] ⎝ N⎠ ⎢ ⎝ b ⎠ ⎥ ⎣ ⎦To find the critical load to fracture the bundle, we maximize PF by setting the derivative dPF/dσF = 0,with the result, after some arithmetic, that: σF = b(m)-1/mInserting this into equation 4.6, we obtain the maximum bundle load: PF(max) = b AN (m)-1/m e-1/mand the strength of the bundle, σB, which is given by PF(max)/AN, is therefore: σB = be-1/m m-1/m .................................................................................................... [4.7]In Appendix 2 we see that the mean (or first moment) of a Weibull distribution is given by the functionbΓ(1 + 1/m), Γ being the Gamma function. The ratio of the bundle strength to the mean filamentstrength, σf u , can therefore be found: −1 −1 −1 σB be m m m (m.e) m ...................................................................... [4.8] = = σ fu ⎛ 1⎞ ⎛ 1⎞ bΓ ⎜ 1 + ⎟ Γ ⎜1+ ⎟ ⎝ m⎠ ⎝ m⎠and this ratio is plotted as a function of m in Figure 4.6. As we see from the graph, the values of m forbrittle fibres like carbon and glass are typically less than 10, so that the strength of a bundle of suchfilaments may be only 70% of the mean fibre strength. Another consequence of the statistical model of failure of brittle solids is that their strengths dependon the size of the piece being tested and for samples of different sizes equation 4.4 contains a volumeterm, as shown in Appendix 2. For a batch of samples of fibres of reasonably constant cross-section, thissize-dependence manifests itself as a variation of strength with sample length. This can be shown byrestating equation 4.4 to include a term for the volume, V: ⎡ ⎛ σ ⎞m ⎤ P(σ) = 1 − exp ⎢− V ⎜ ⎟ ⎥ ……..Equation 4.1) ⎢ ⎝b⎠ ⎥ ⎣ ⎦
chapter four Strength 65 Assuming some fixed failure probability for two 1.0 groups of fibres of lengths l1 and l2, it is then easy to see that the ratio of the strengths of these two groups σB must be: σf 0.8 75% −m 1 σ(l1 ) ⎡ l1 ⎤ = ⎢ ⎥ …………….Equation 4.2) 65% σ(l 2 ) ⎣ l 2 ⎦ 0.6 The value of m alone thus determines the range for carbon magnitude of the strength/length effect. This effect is and glass fibres a feature common to all brittle filaments, and is 0.4 1 10 100 illustrated for some commercial carbon fibres in Weibull shape parameter, m Figure 4.7. It has always been a problem for designers of composites structures that when dealing Figure 4.6. Dependence of the strength of a bundle of fibres on the Weibull shape parameter, m. 4 with data from fibre manufacturers the fibre strength line predicted from m value should only be quoted in relation to the sample test Fibre strength, GPa 3 length. We see now that when trying to calculate the 2 composite strength the choice of the value of σfu that should be used in equation 4.1 is a matter of some Courtauld HMS carbon fibres concern. It is clearly not the mean fibre strength, and 1 m = 7.1 although it may seem that the fibre bundle strength, σB, is the appropriate value to use, this may also 0 prove to be an incorrect assumption. To try to 5 10 20 50 100 answer this question, we have to consider in more Fibre gauge length, mm detail the mechanism by which a composite breaks down under load. Figure 4.7. Variation of fibre strength with test length forsamples of Courtauld HMS carbon fibres (Dickson, 1980). 4.1.3 Progressive damage and failure in The straight line is predicted from the value of m of 7.1 obtained from individual fibre tests. unidirectional composites A fibre bundle embedded in a matrix does not behave like a free fibre bundle. When the local load level reaches the failure stress at a weak point in a given fibre it breaks and the load it carried is transferred back into the neighbouring matrix regions. But away from the broken ends the fibre carries its full share of the load, by contrast with what happens in an unbonded bundle. The stress carried by neighbouring fibres in the vicinity of the break will be perturbed, as shown schematically in Figure 4.8, but the stress concentration may not be great enough to break a neighbouring fibre (or fibres). As the load on the composite increases other fibre breaks will occur, but each fibre may break many times without seriously damaging the overall load-bearing ability of the composite since the tensile load supported by the broken fibre within a short distance, δ, known as the ineffective length, from each broken end, will rapidly build up again to its original level. Figure 4.8. Schematic illustration of the perturbation of the stresses in the neighbourhood of a broken fibre.
chapter four Strength 66 If the scatter in filament strengths is small (large value of m) and the fibres are closely spaced, the extra load carried across to a neighbouring fibre may be sufficient to break that one too. The local stress concentration is then even higher. If the process is repeated a number of times, the cross section where the breaks are occurring will rapidly become too weak to support the applied load and catastrophic brittle failure will follow. In reinforced plastics containing brittle fibres like glass or carbon, however, this mode of fracture rarely occurs. The second fibre seldom breaks at the same cross section as the first because the stress concentration adjacent to the first break is unlikely to coincide with a weak point in the second fibre. Instead, fibre breaks accumulate randomly throughout the whole sample or structure, and final failure may then occur when the number of breaks in any one cross section has effectively reduced the local Vf below that required to support the applied load at that instant. Figure 4.9. Model composite for studying the random failure of fibres leading to composite failure. Three adjacent fibre failures is assumed to be the failure condition (x = fibre failure). This process of damage accumulation may be illustrated in a simple fashion by considering the model composite shown in Figure 4.9. It represents a single ‘ply’ consisting of ten parallel fibres. In order to model the statistical distribution of flaws in the fibres, each fibre ‘chain’ is divided into ‘links’, each of which is of length lc (= 2δ): as we shall see later, this is the smallest length of fibre that can just be broken by a tensile force. In a realistic statistical model, such as the Monte Carlo treatment of Fukuda and Kawata (1977), each fibre section would be allocated a ‘strength’ value from a Weibull distribution, and a notional ‘load’ acting on the composite would be increased in small steps. The links would fail as the local stress reached the Weibull ‘strength’, and this process would be allowed to continue until some preset failure criterion was reached. A similar result can be demonstrated by simply using a random-number generator to cause random failures throughout the model, as displayed by the crosses in Figure 4.9. A suitable failure condition can be deduced from the work of Jamison (1985) who deconstructed samples of composite material that had been loaded to failure, or just below, and searched for groups of adjacent fibre fractures throughout the material. He concluded that since the largest groups that could be found were triplets, a group of four must constitute a critical-sized nucleus that led immediately to failure. If the computer running the simple stochastic failure model is programmed to recognise an appropriate group of adjacent failures, then the time to reach that condition (which may equally well represent an applied load on a composite being 2 loaded at a constant rate) is the composite life (or failure stress). The result of repeating such a simulation 100 times is shown in Figure 4.10: for 0 this simple model, the failure condition was three Ln[-ln(1 - P)] adjacent breaks, as illustrated, and, to -2 accommodate the effective-length concept, in-line chain links immediately adjacent to an existing failure were not allowed to break. The total P(x;b,m) = 1 - exp[-(x/b)m] -4 number of fibre breaks that may occur prior to m = 2.85 failure varies widely, from 19 to 147 in the case b = 34.5 of this series of simulated tests, and the times to -6 failure (or failure stresses) are also very widely 1.5 2.0 2.5 3.0 3.5 4.0 4.5 distributed as the figure shows. Somewhat Ln(time to failure), arbitrary units surprisingly, the data fit a two-parameter Weibull distribution. This is not a very realistic model: we Figure 4.10. Two-parameter Weibull plot of times to failure might ask, for example, whether three breaks in agenerated by a random-break computer program for a model row would be more damaging than two in a row fibre composite (100 tests). and one slightly oblique, and such matters have to
chapter four Strength 67be addressed in serious calculations. However, we can easily appreciate the progressive nature ofdamage from such a model and the reasons for the variability in composite strengths and fatigue lives(see chapter 6).4.1.4 Calculation of the tensile strength of a unidirectional composite As we see, damage builds up progressively in the composite until sufficient fibre breaks occur in onelocal region to constitute a crack which can then propagate catastrophically and cause fracture. Thisprogressive failure has been investigated by a variety of methods, including acoustic emission studies,and by microscopy or x-ray techniques. If we ignore the (low) matrix contribution in the strengthequation (4.1) we can see that the mean filament strength and the fibre bundle strength might well definethe upper and lower bounds on the strength of a unidirectional fibre composite: σB v f < σc < σ fu Vf ............................................................................................. [4.9]But there still remains the problem of knowing what is the relevant ‘test length’ for which we shouldchoose the value of σf u . The whole length of a fibre embedded in a composite matrix is never stresseduniformly, and it is usually assumed (Rosen, 1965) that the effective ‘test length’ of fibres breakingwithin a matrix is of the order of the critical length, lc, or 2δ (see Figure 4.8). Rosen’s cumulativeweakening-model assumes that fibre flaws are distributed randomly throughout the composite and itextends the fibre-bundle model to the situation inside the composite. As in the simple compositesimulation described above, fibre breaks occur singly and randomly throughout the material. The loadnear the breaks in the fibres must be redistributed because of the ineffective end sections, and thisredistribution will be controlled by the strength of the fibre/matrix interface and the relative stiffnessesof the fibre and matrix, as we have already seen. In the expression for the bundle strength (equation 4.7) the characteristic strength b relates towhatever fibre test gauge length has been used. However, for a given fibre population with shape factorm, the value of b appropriate to a ‘gauge length’ lc can be obtained by applying equation 4.10.Combining equations 4.7 and 4.10, therefore, we obtain an expression for the strength, σc*, of the bundlein the composite: −m 1 ⎛l ⎞ σc = b ⎜ c me ⎟ * ......................................................................................................... [4.10] ⎝L ⎠where the strength of the reinforcing filaments was determined on samples of gauge length L. The upperbound on composite strength is then equal to σf u Vf. Dividing this estimate of composite strength withthat predicted from the mean filament strength (ignoring any contribution from the weak matrix) weobtain the ratio: −1 ⎡ lc ⎤ m σ* ⎣ ⎢ L .m.e ⎥ ......................................................................................................... [4.11] ⎦ c = σ fu ⎛ 1⎞ Γ ⎜1+ ⎟ ⎝ m⎠ As we saw in chapter 3, the fibre critical length, lc, is determined by the elastic characteristics of thefibre and matrix and by the strength of the interfacial bond between the two. The fundamentalreinforcing potential of the fibres is therefore affected by a number of factors other than their nominaltensile strength. In Figure 4.11 the strength ratio of equation 4.13 is plotted as a function of the criticalaspect ratio, lc/d, for different values of the Weibull shape parameter and assuming a fixed fibre testlength (L) of 5cm. For many practical composites the values of m and lc/d fall within the ranges in thisgraph, and it is not surprising, therefore, that the strengths of some unidirectional composites may riseabove a mixture-rule prediction based on the single-fibre strength. An illustration of this coated-bundleeffect is shown by some results of Dickson (1980) in Figure 4.12. In this figure, the failure strains of the
chapter four Strength 68 bundles are plotted instead of stresses, and the 4 bundle failure load is used as an indicator of bundle size in order to avoid the tedious business fibre strength test gauge length = 5cm of counting large numbers of fine filaments. It 3 can be seen that the failure of dry bundles (filled m=5 symbols) is subject to substantial scatter, but that σc*/ σf m=7 the degree of variability falls as the bundle size m=9 2 increases. This is what would be expected of the bundle-failure model: the dry-bundle failure strain of 0.41% is predicted from the single- 1 filament data of Figure 4.7. By contrast, the variability of the resin-coated bundles, which resemble real composites, is much greater and not 0 markedly dependent on bundle size. The mean 0 20 40 60 80 100 failure strain of the resin-coated bundles is Critical fibre aspect ratio, l c/d. 0.55%, 20% greater than that of the dry bundles and over 95% of the dry bundles failed at strains Figure 4.11. Variation of predicted composite strength, below the mean coated-bundle failure strain. The σc*Vf, normalized with respect to the value predicted from mean filament failure strain, however, is 0.62% the mean fibre strength, σf Vf, as a function of the critical and it is therefore clear that although many of the aspect ratio, lc/d. resin-coated bundles do indeed fail above the line represented by σ∗ / σfu = 1 in Figure 4.11, on average they do not do so. c In practice experimental composite strengths are never as high as the Rosen model would lead us to expect. And although the model was reasonably successful in a number of cases, it is limited by the fact that it takes no account of the stress concentrations that result from single and multiple fibre breaks, ie. of the interactions between individual damage events which depend on the surface characteristics of the fibre, the interfacial adhesion, and the resin flexibility, as well as on the fibre strength statistics. It has also been suggested that the notional ‘test length’ of lc is far too small and that the Weibull model cannot be extrapolated to such small test lengths. Hughes et al (1980) and Harris et al (1992a) have shown, nevertheless, that for some types of carbon-fibre composite the extrapolated bundle strength gives good agreement with measured tensile strength values. 1.0 mean failure strain There are perhaps two extreme situations. If there of resin-coated bundles is a great deal of scatter in the strengths of individual 0.8 fibres, failures occur randomly throughout theFailure strain, % composite and are non-interacting. On the other hand, 0.6 if the fibre failure strength is very uniform, there will be a high degree of interaction between individual 0.4 fibre failures in one cross section of the composite. In large dry-bundle general, most composites will behave in a complex 0.2 failure strain fashion between these two extremes and it will usually be difficult to predict the composite strength predicted dry-bundle failure strain = 0.41% accurately. Bader (1980) has developed a model for 0 10 100 1000 the tensile failure of unidirectional composites which Bundle failure load, g (ie. increasing bundle size) suggests that the critical size of the group of fibres dry bundles which initiates failure is of the order of 9 fibres (ie. resin-coated bundles about three in a row in any given direction (cf. the results of Jamison described earlier) but that the final Figure 4.12. The breaking strains of fibre bundles failure sequence is determined by the relativecontaining different numbers of Courtauld HMS carbon fibres. The filled symbols are for dry bundles and the resistance of the laminate to splitting parallel to the open symbols are for resin-coated bundles. The fibres which occurs as a consequence of the shearbreaking load of the bundle is used as a rough indicator stress developed around the groups of failed fibres. of the number of fibres in the bundle (approx. 10g per Manders and Bader (1981) have also described a fibre). statistical model to predict the strengths of mixed-
chapter four Strength 69fibre (hybrid) composites in which they suggest that the critical number of fibre fractures is of the orderof three, and Curtis (1986) published details of a computer model for tensile failure of unidirectionalcomposites which showed the sequential development of fibre failures and suggested that four adjacentbroken fibres is the maximum stable group that could be tolerated in standard high-strength-fibrecomposites.4.1.5 Transverse strength The strengths of unidirectional composites are highly anisotropic.Perpendicular to the reinforcing fibres most composites are weak andfailure is controlled by rupture or plastic flow of the matrix, or byfibre/matrix decohesion: the precise mechanism will depend on thecapacity of the matrix for plastic deformation and the strength of thefibre/matrix bond. If the matrix is a metal or polymer, its intrinsicyield strength will govern the transverse behaviour of a compositecontaining only a few fibres. If this yielding is restricted to theligaments between the fibres, the transverse strength of thecomposite might be estimated from a crude rule-of-mixtures modelin which the deforming matrix cross-section is obtained from aknowledge of Vf and the reinforcement geometry. For the squarearray shown in Figure 4.13, for example, the effective volume Figure 4.13. Kies’s model (1962) forfraction of the deforming matrix normal to the fibres is: strain magnification during transverse loading of a unidirectional composite. 4Vf Vm (eff ) = 1 − πAssuming no contribution from the fibres, the transverse strength of the composite is then: ⎛ 4Vf ⎞ ......................................................................................................... [4.12] σt = σmy ⎜ 1− ⎜ ⎟ ⎝ π ⎟⎠ As the volume fraction increases, however, the relatively undeformable fibres impose an increasingdegree of constraint on the matrix. Contraction in the fibre direction (the width) is prevented, andextension under stress can only be accompanied by deformation in the thickness direction, ie. thedeformation is under plane-strain conditions. A consequence of this is that the effective yield strength ofthe matrix rises from the ‘free’ value of σmy to the plane-strain yield stress. 1.15σmy (Cottrell, 1964).Despite this, the transverse strengths of practical composites fall rapidly with increasing fibre contentwhile their axial strengths rise linearly, and even if corrections are made in equation 4.14 (vide Cooperand Kelly, 1969) to allow for the effect of apositive adhesive bond between the fibres and 1.0matrix, the degree of anisotropy of a 2024 aluminium/Nextelunidirectional composite rises dramatically with 0.8 T300 carbon/epoxyincreasing Vf, as illustrated in Figure 4.14. Twomaterials are represented in this figure, a typical σc / σt 0.6 σf /σm= 6.6MMC (mullite-fibre-reinforced aluminium) anda common epoxy-based CFRP, for which theratios of fibre strength to matrix strength are 0.4different by an order of magnitude (about 7 for σf /σm=88the MMC and 88 for the CFRP). A crude 0.2correction has been made to allow for the plasticconstraint just mentioned (the effective matrix 0yield strength increases in proportion to √(Vf)) 0 0.2 0.4 0.6 0.8but the effect is insignificant by comparison Fibre volume fraction, Vfwith the geometrical effect of equation 4.14.Figure 4.14 illustrates an important advantage of Figure 4.14. Variation of predicted ratio of composite transverse strength to axial strength with fibre content for two types of composite with different ratios of fibre-to-matrix strengths. The matrix strength varies from σmy at Vf = 0 to 1.15 σmy at Vf = 0.7.
chapter four Strength 70typical MMCs over reinforced plastics which derives from the much higher inherent matrix strengths ofthe former. Typical ratios of transverse to longitudinal strengths of GRP, for example, are only of theorder of 0.05 for glass/epoxy (Harris et al, 1979) and 0.04 for glass/polyester (Guild et al, 1982). Suchlow levels of transverse strength mean that unidirectional reinforced plastics are incapable of bearingtransverse loads, and even cross-plied laminates may develop cracks during processing as a result ofthermal stresses normal to the fibres if careful control is not exercised. Strain concentrations in the matrix may also lead to brittle failure at low strains, even in compositeswith otherwise ductile matrix materials. The magnitude of this strain concentration may be obtainedfrom an approximate elastic model by Kies (1962) which defines a strain magnification factor, SMF, dueto composite strains in a direction transverse to the fibres (Figure 4.13). For this simple rectangulararray, the increase in local matrix strain in the x direction, εm, as a fraction of the mean composite strain,εc, is given by the SMF: −1 εm ⎡⎛ a ⎞ ⎛ Em ⎞ ⎛ a ⎞ ⎤ ......................................................................... [4.13] SMF = =⎢ ⎜ ⎟ + 1− ⎥ ε c ⎣⎜ s ⎟ ⎝ E f ⎠ ⎜ s ⎟ ⎦ ⎝ ⎠ ⎝ ⎠ The geometrical ratio, s/a, defined in Figure 4.13, depends on the fibre diameter and volume fraction,and on the geometrical arrangement of the fibres. In typical GRP materials with 65vol% of 10μmdiameter fibres the strain magnification factor given by Kiess model would be about 5 for a hexagonalfibre array and 7.5 for a square array. Thus, even in resin matrices with failure strains of the order of 4%,transverse resin cracking perpendicular to the fibres couldoccur at applied composite strains as low as 0.5% at avery small percentage of the full composite potentialstrength. Indeed, in the Permali 0/90 GRP which we havealready used as an example in discussing elasticproperties, transverse cracking was shown to occur in the90° plies at strains as low as 0.2%, only a tenth of thecomposite failure strain (Harris et al, 1979): suchcracking is shown in the photomicrograph in Figure 4.15.And while this transverse cracking may not impair theload-bearing ability of the material in a major fibredirection, it could have serious consequences, if, forexample, the material were required to contain liquid or Figure 4.15. Photomicrograph of transverse-ply cracking in a 0/90 GRP laminate.gas under pressure. There is some doubt, however, whether failure in composites of high Vf ever occurs in the simplisticmanner described by these simple models for, as Bailey et al (1979) have shown, it is the fibre/matrixbond that is usually the weakest element and transverse cracking occurs by the linking up of localfibre/resin decohesion failures, which is how we also expect a ceramic- or glass-matrix composite to fail.The transverse strength of brittle-fibre/brittle-matrix laminates is probably best treated by a modifiedfracture mechanics approach where the critical flaw size is related to the transverse dimension of thefibres.
chapter four Strength 714.1.6 Orientation-dependence of composite strength When the fibres in a loaded unidirectional composite lie at an angle to the stress axis the effectivestrength of the composite is reduced. In chapter 3 we examined the variations of stress and strain asfunctions of orientation, and it is easy to see how some kind of failure criterion could be combined withthe stress or strain functions to provide indications of the variation of strength with orientation. Thestrength of a composite is highly dependent on the local damage mechanisms, however, and these mustchange as the active stress system affects different components of the composite. In our discussion of theaxial tensile strength, we emphasised the rôle of thefibres to the exclusion of all other effects. But whenthe level of shear stress builds up in a composite thiscan lead to failure modes of other kinds, includingfibre/matrix interfacial shear failure and interlaminarshear. And we have already discussed the possibilityof tensile failure of the interface or of the matrixbetween the fibres during transverse loading. It isvital in using composite strength models to ensurethat the appropriate failure mode is beingconsidered. This is shown by studying one of the Figure 4.16. Resolution of the force, F, acting on a composite of arbitrary orientation. The strength of thesimplest of the models, the maximum-stress theory composite in the fibre direction is σc.of Stowell and Liu (1961). The central assumption is that failure will occur when the stress in a given direction reaches somecritical value (ie. the critical stress for the operative failure mode). If the measured in-plane strengthproperties of a unidirectional composite lamina are the normal axial tensile strength, σc, the transversetensile strength, σt, and the in-plane shear strength, τc, the maximum-stress model is developed asfollows. Consider, first, the case where the angle between the stress and the fibres is relatively small, as shownin Figure 4.16, so that composite failure is still going to be dominated by fracture of the fibres. The fibretensile stresses reach the fibre fracture stress before any other failure event can occur. Resolving theapplied force, F, and the area over which it acts, we have: σc = Fcosθ/A1 = Fcosθ.cosθ/Ao = σθcos2θand hence the failure stress, σθ, of the composite at the angle θ to the fibre direction is given by: σθ = σcsec2θ........................................................................................................ [4.14] For larger values of θ, the shear component of stress acting at the fibre/matrix interface will graduallyincrease until shear failure occurs. Resolution again yields the angular-dependence of the compositestrength appropriate to an in-plane shear mode of failure: σθ = τc/sinθcosθ = 2τc.cosec2θ........................................................................... [4.15] At very large angles, the level of applied tensile stress resolved normal to the fibre/matrix interfaceresults in a failure passing partly through that interface and partly through the matrix between the fibres,which occurs at relatively low stresses, like interface shear failure. Further resolution leads to the result: σθ = σtcosec2θ .................................................................................................... [4.16] The three equations 4.16, 4.17 and 4.18 define the three régimes of failure of the maximum-stresscriterion and their predictions are in reasonably good agreement with experimental results for manyunidirectional composites. One difficulty with this model is that it is appropriate for unidirectional fibrecomposites only and cannot allow for constraints resulting from the presence of fibres at other angles (ie.in a real composite). It is therefore likely to underestimate real composite properties.
chapter four Strength 72 There are many other models of composite failure, and many arguments concerning the validity of the underlying reasoning. One example is that derived from the von Mises maximum-distortion-energy criterion for the failure of isotropic metals which was modified by Hill (1964) for anisotropic materials. The Hill argument was adapted by Azzi and Tsai (1965) for use with transversely isotropic laminates under plane stress, and in one of its forms it predicts the orientation dependence of composite strength as: 1 cos 4 θ sin 4 θ ⎛ 1 1 ⎞ = + + cos 2 θ sin 2 θ ⎜ 2 − 2 ⎟ .................................................. [4.17] σθ 2 σc 2 σt2 ⎝ τc σ c ⎠ where the stress terms are as already defined. 10 This model, which is almost universally known as the Tsai-Hill criterion, has the advantage σθ = σcsec2θ σc = 1.50GPa over the maximum-stress criterion that it is a σt = 0.04GPa Composite Strength, GPa mathematically continuous function, and the τc = 0.068GPa 1 σθ = σtcosec2θ two models are almost indistinguishable under the simple tensile conditions which we have been discussing, as shown in Figure 4.17. In σθ = 2τccosec2θ this graph, experimental results for σc , σt , and 0.1 τc for a standard CFRP material, T300/5208, have been used to generate the maximum-stress Tsai-Hill criterion and the Tsai-Hill failure criteria, and it can be Stowell and Liu model seen that they agree well except in the range 0.01 20° < θ < 40° and for this material even this 0 10 20 30 40 50 60 70 80 90 difference is relatively small. It is interesting to Orientation, θ, degrees note that for slight changes of θ away from 0° the maximum-stress model predicts a slight Figure 4.17. Comparison of the maximum-stress and Tsai- increase in strength as a consequence of the Hill failure criteria for a T300/5208 unidirectional resolution of forces. However, it is very carbon/epoxy composite difficult to manufacture composites with perfect 1.0 Si02/epoxy; Vf = 0.67 (Pabiot) fibre alignment and equally difficult to test them at a glass/polyester; Vf = 0.43 (Guild et al) precise angle to the fibres, so that experimental errors will make it almost impossible to distinguish Tensile strength, GPa between the two models at small θ. The Tsai-Hill criterion is a common feature of commercial 0.1 computer software programs for strength prediction (see section 4.4). The predictions of the Tsai-Hill criterion are compared in Figure 4.18 with strength measurements for two types of unidirectional 0.01 composite, SiO2/epoxy (Pabiot, 1972) and E- 0 30 60 90 Orientation, θ, degrees glass/polyester (Guild et al, 1982). The mean measured values of σc, σt, and τc for the SiO2/epoxyFigure 4.18. Comparison between experimental data and are similar to those for the T300/5208 CFRP the predictions of the Tsai-Hill criterion(full and dashed material just referred to, namely 1.46GPa, 0.32GPa,lines) for the orientation-dependence of the strength of a and 0.68GPa, respectively, while those for the lower ud SiO2/epoxy composite (Pabiot, 1971) and a ud E- Vf glass/polyester are proportionately lower. The glass/epoxy composite (Guild et al, 1982). comparison between theory and experiment for both kinds of material is seen to be excellent. 4.1.7 The strengths of multi-ply laminates. When a 0/90 (non-woven) laminate is stressed parallel to one set of fibres the transverse plies will begin to crack at low strain levels, as we have seen. This cracking will continue over a range of
chapter four Strength 73composite strains determined by the statistical spread of transverse strengths of the individual laminae,and each transverse lamina may crack many times, the crack spacing gradually being reduced until eachblock of transverse ply is too short to be cracked any further, as illustrated by Figure 4.15. Aveston et al(1980) have proposed that for 0/90 glass/resin laminates the spacing, c, of transverse ply cracks as afunction of applied stress, σa is given by the relationship: ELETbd2 ⎡ ε E ⎤ c=− ln ⎢1− Tu C ⎥ ................................................................................ [4.18] GTEC (b + d) ⎣ σa ⎦where EC , EL, and ET are the moduli of the composite and of the longitudinal and transverse plies, withrespect to the stress direction, GT is the shear modulus, and εTu is the failure strain of the transverse plies.The transverse plies are of thickness d while the longitudinal plies are of thickness b. Cracking of thetransverse plies could be supposed to start when 40the composite strain reaches the normal failurestrain, εTu, of the transverse plies. Youngs modulus, GPa 30 Transverse-ply cracking releases some of theinter-ply coupling constraint and residual thermalstresses, and impairs the load-bearing ability of the 20laminate. It is often assumed that the fully crackedtransverse plies no longer contribute to thestiffness of the laminate. On this basis, the 0° axial 10 0° orientationmodulus, E0, of the Permaglass XE6 laminate 45° orientationreferred to earlier should fall by about 45% after 0preloading whereas, as Figure 4.19 shows, the 0 20 40 60 80 100reduction in 0° stiffness after loading to 95% of the Stress, σ/σcfailure load in only about 11% and there is noreduction at all in the 45° stiffness. The fully-cracked transverse plies therefore continue to Figure 4.19. Elastic modulus of Permali XE6 non-woven glass/epoxy laminate as a function of pre-stress. Thecontribute to the stiffness of the damaged stress level is normalized with respect to the compositecomposite, both through direct stress transfer from failure stress, σc (results of Harris et al, 1979).the longitudinal plies and because of the lateral(Poisson) constraint they exert on the extensional strain of the longitudinal plies. The models of Bailey etal (1979) and Aveston et al (1980) predict that the critical strain for first cracking of the transverse pliesdepends on the ply thicknesses, and that the thinner the plies the higher the strains to which cracking isdeferred by the elastic constraint. Approximate estimates of the strengths of multi-ply laminates may be obtained by the use of theKrenchel model discussed in chapter 3, with the same values of the efficiency factor, ηθ, defined byequation 3.25, as were used to calculate elastic response. This factor is then used in a mixture-rulecalculation: σc = ηθσfu Vf + σm´(1 – Vf) ................................................................................... [4.19]The approach may again be criticized because it ignores contributions of fibres at 90° to the stress axisand elastic interactions between the individual anisotropic laminae, but these are less important incalculating the strength of a laminate than in determining its elastic properties. The choice of anappropriate value for σm´ is also of no great significance in a fibre-dominated laminate.
chapter four Strength 74 Another useful approximate approach is that known as the ‘Ten-Percent Rule’. Hart-Smith (1993)points out that while, in principle, fibre patterns could vary widely throughout any given structure,depending on requirements, practical aerospace laminates have for many years been designed within arelatively limited range of options. Theyare usually balanced laminates, with equalnumbers of +45° and –45° plies, and theratio of 0° and 90° plies varies toaccommodate local loads. Preferred fibre area of preferredarrangements usually fall within the fibre patternsshaded area surrounding the quasi-isotropic lay-up shown in the ternary quasi-isotropic lay-up‘phase diagram’ in Figure 4.20. In the ten- (25% 0; 25% 90; 50%percent rule, each 45° or 90° ply isconsidered to contribute one tenth of thestrength or stiffness of an axial (0°) ply tothe overall performance of the laminate.Justification for this lies in the fact thatthere is a rapid fall-off in both the strengthand stiffness of a unidirectional laminatewith orientation, as illustrated by Figure Figure 4.20. Preferred fibre patterns for aerospace composite3.12 (stiffness) and Figure 4.17 (strength). laminates (adapted from Hart-Smith, 1993).The effective properties at 45° and 90° aretherefore indeed very similar, although in reality the appropriate value for the anisotropy ratio may benearer to 4% than 10% for many unidirectional composites. Table 4.1. Prediction of laminate efficiencies by laminate theory and approximate methods. Laminate lay-up Comparison of laminate efficiencies predicted by laminate theory and approximate methods Laminate theory Krenchel factor Hart-Smith software 10% rule UD 1 1 1 (0,90)S (cross-ply) 0.530 0.500 0.550 (±45)S 0.139 0.250 0.100 [(±45,02)2]S 0.575 0.625 0.550 [(±45)2,03,90)]S 0.489 0.500 0.438 (0,±45,90)S (quasi-isotropic) 0.385 0.375 0.325 The ten-percent rule offers a rapid, and reasonably accurate, means of estimating the strength andstiffness of any practical laminate consisting only of 0, 45 and 90° plies, without the need for elaboratecalculations or extensive experimental evaluation of properties. For example, for a lay-up consisting of37.5% fibres in the 0° direction, 50% of ±45 fibres, and 12.5% of 90° fibres, a simple mixture-rule sumgives the laminate strength and stiffness in the 0° direction as (0.375 x 1 + 0.5 x 0.1 + 0.125 x 0.1) =0.438 times the value of the relevant property measured in axial tension on the unidirectional laminate.Table 4.1 gives a comparison of the predictions of the Krenchel and Hart-Smith methods for theefficiencies of some representative laminates, together with values obtained from analysis by laminate-theory software for T300/5208 carbon/epoxy composites. Except for the (±45)S laminate, the agreementis very good, despite the assumptions on which the approximate models are based. We saw in chapter 3 how the analytical procedures of the classical thin-laminate theory may be usedto determine the levels of stress and strain in a multi-ply laminate. If the level of stress in a ply at somepoint in the laminate exceeds the load-bearing ability of that ply, local failure will occur. Because of theway in which the microstructure controls the accumulation of damage in fibre composites, however, thecomposite rarely fails when the first ply breaks. The classical thin-laminate theory provides a means of
chapter four Strength 75estimating the laminate strength. Since all stresses in a loaded laminate can be calculated by the theory, asingle stress analysis serves to determine the stress field that causes failure in any one of the constituentlaminae by comparing the individual lamina stresses, σx, σy, τxy, with some suitable failure criterion,such as the Tsai-Hill model discussed in section 4.16. The thermal contraction stresses following curecan also be determined and included in the overall level of stress, mechanical plus thermal. If no laminaeare found to have failed following cure the computer program can adjust the external stress system untilthe first lamina fails according to the chosen failure criterion. This lamina is then eliminated, thestiffness matrices are recalculated to accommodate the redistributed loads and the cycle is repeated. Atthe point when the failure of one more lamina results in violation of the failure criterion for theremaining laminations, the composite is considered to have reached its macroscopic failure stress. Theprocedure is thus somewhat similar to that of calculating the strength of a fibre bundle. Hart-Smith(1996) has criticized this process of ply-by-ply decomposition, followed by assessment of each plyindependently from the others. He argues that such a process cannot be valid when matrix crackingaccompanies the deformation process, and he also considers that values of the transverse strengthobtained by measurements made on a single ply are not relevant for the failure of a 90° ply embedded ina laminate. The ply-discounting procedure is probably conservative, however — ie. it predicts lower strengthsthan actual values because even after a single lamina has failed one or more times it is still capable ofbearing load, the stresses in the neighbourhood of the break being diffused away into adjacent laminae inthe same manner as those surrounding a break in a single fibre. A central feature of analytical models and software for the prediction of the strength of laminates isthat they must depend on the use of an appropriate failure criterion. We have already discussed two ofthese, the maximum-stress and the Tsai-Hill (maximum-strain-energy) criteria, but there is currentlymuch disagreement about the validity of many of the commonly used models. It is necessary to makefurther reference to this problem, and we shall return to it in section 18.104.22.168.8 Short-fibre composites We saw in section 3.7 of chapter 3that if the fibres are short, stress must fibrebe transferred into them by shear and fibre strength tensiletheir ends are not fully loaded. Only if stress σa fibre is longer than the criticallength, lc, can it be broken by loadingthe composite and its full reinforcingpotential realized. To illustrate thisfurther, we consider three situations,where the fibres in the composite areassumed to be aligned and of uniformlengths which are less than, equal to, Figure 4.21. Simplified illustration of the variation of tensile stress inor greater than the critical length, as short fibres as a function of fibre length. σf is the fibre breaking stressshown in Figure 4.21. We also make and lc is the fibre critical length.the simplifying assumption that thetensile stress in the fibre builds up from the ends in a linear fashion, rather than as given by equation3.33, but this does not greatly affect the argument. In the case where l is equal to lc, the tensile breaking stress in the middle of the fibre can just bereached, and the fibre can therefore be broken, but the load-bearing ability of the whole composite mustbe less than that of a continuous-fibre composite containing an identical type of fibre. If the fibrestrength is σfu, ignoring statistical aspects of the problem, the average stress in each fibre of length lcwill be only ½σfu (middle sketch in Figure 4.21). Thus, in a longer fibre, such as that in the right-handsketch of this figure, there will be two inefficiently loaded end sections of total length lc in which theaverage stress is ½σfu and a central section of length (l – lc) in which the stress is σfu. By a rule-of-
chapter four Strength 76mixtures argument based on these lengths, then, the overall level of stress, σf , in a fibre of length l > lcwill be: [σfu(l – lc) + ½σfu lc]/lie. ( σ)f = σfu ⎛1− l c ⎞ ................................................................................................. [4.20] ⎜ ⎟ ⎝ 2l ⎠for the linear stress variation model illustrated above, where (1– lc/2l) represents an efficiency factor forlength. The mixture rule may then be modified to give the strength of the composite: ⎛ l ⎞ σc = σfu Vf ⎜1− c ⎟ + σ′ (1− Vf ) m [l ≥ l c ] .................................................. [4.21] ⎝ 2l ⎠This equation can be used to calculate the strengthening efficiency (the ratio σc/σfu) as a function of fibrelength (l/lc), as shown in Figure 4.22 for a typical composite. It can be seen that provided the fibrelength is about 10 times its critical length, some 95% of the strength obtainable in a continuous-fibresystem can be achieved with short, aligned fibres. The validity of this conclusion is not affected by thesimplistic stress-transfer model assumed above. The 0.8problem with discontinuous-fibre reinforcement, 0.668however, as we have suggested, is that it is verydifficult in conventional manufacturing processes to 0.6keep the fibres well aligned. σc / σfu 0.4 If the fibres are shorter than lc they cannot beloaded to their failure stress and the strength of the Vf = 0.65composite is then determined by the strength of the σfu = 2GPa 0.2fibre/matrix bond, not by the fibre strength. This is σm = 100MPasometimes the case in GRPs manufactured byinjection moulding, especially if the lengths of the 0fibres are reduced by damage during the 1 10 100 1000manufacturing process. The average stress in the l/ lcfibres can be estimated from the balance of forcesillustrated schematically in the diagram of Figure Figure 4.22. Efficiency of strengthening in short-fibre3.21. If the stress in the fibre is identified as (σ)f, the composites, as given by equation 4.23. 2maximum fibre tensile force, (σ)f.πd /4, is balancedby an internal frictional force which must exceed the fibre/resin bond strength, τi, or the matrix shearyield stress, τmy, if failure by a mechanism other than fibre failure is to occur. If we let this limiting shearstress be equal to τi (the more common failure mode) the force balance at failure will be: πdlτi πd2 ( σ )f = [( σ )f < σ fu ] 2 4and the average tensile stress in the fibre, (σ)f , is therefore: τil (σ)f = 2 (σ)f = 1 ............................................................................................ [4.22] dThe composite strength, from the mixtures rule, is therefore: ⎛ τl ⎞ σc = ⎜ i ⎟ Vf + σmu (1 − Vf ) [l < l c ] ........................................................ [4.23] ⎝ d ⎠
chapter four Strength 77where σmu is the matrix tensile strength. This 500relationship emphasises the importance of goodfibre/matrix bonding if reasonable strength levels 400 Tensile strength, MPaare to be obtained in short-fibre composites. If the Slope = τiVfbond is poor, a soft matrix like polyethylene or a 300 τ = 21MPapure metal like aluminium will deform readilyaround the more rigid fibres and the tensile 200strength falls as the fibre length is reduced. This is Short-fibre Cu/W compositesillustrated in Figure 4.23 by some tensile strength Vf = 0.5measurements on MMCs consisting of aligned 100 σmushort tungsten fibres in a matrix of pure copper(Harris and Ramani, 1975). The strength of these 0 0 10 20 30 40 50 60 70short-fibre composites only approaches that of a Fibre aspect ratio, l/dcontinuous-fibre composite at an aspect ratio ofabout 100. Since this is only about twice thecritical aspect ratio, lc/d, however, it appears that Figure 4.23. Relationship between the tensile strength and fibre aspect ratio in tungsten-wire/copper compositesthe stress transfer at the fibre ends is rather more containing short, aligned fibres (Harris & Ramani, 1975).efficient than is assumed by Figure 4.21. So far we have assumed the short fibres to have been arranged in a single direction, and comparisonswith the properties of unidirectional, continuous-fibre composites are therefore valid. The shorter thefibres, however, the more difficult it is to obtain good alignment, and without good alignment closepacking cannot be achieved. The strengths of short-fibre composites are therefore limited both by fibremisorientation and by the lower fibre contents than those which can be obtained in continuous-fibrecomposites in addition to the fibre-length effects already discussed. Methods of producing compositesreinforced with almost perfectly-aligned chopped fibres have been described by Parratt et al (1971) butshort-fibre composites are used most frequently as moulding materials. The polyester dough mouldingcompounds (DMCs, sometimes referred to as bulk moulding compounds) and sheet mouldingcompounds (SMC) are typical of thermo-set mouldings materials of this kind, while for injectionmoulding there is a wide range of glass-fibre-reinforced thermo-plastic composites available. The strengths of materials of this kind are hard to predict on the basis of equations 4.23 and 4.25because of the combination of variables, the uncertainty about parameters such as τi and lc (which aredifficult to measure for conditions appropriate to the real composite) and lack of knowledge of theeffects of processing on the strength of the reinforcing filaments. On the basis of assumptions relating toprobable values of lc and τi and with the application of a Krenchel factor of ηθ = 0.375 for randomly-oriented composites, Harris and Cawthorne (1974) estimated strengths for typical DMC and SMC thatwere well within the experimental scatter fortheir measured strength values (37MPa and 1.2100 MPa, respectively, for DMC with fibre size Frequency (normalized)15wt% of 6.4mm long fibres and SMC with 1.0 length coating25wt% of 50mm fibres in chopped-strand 0.8 a) 6mm solublemat). The strength of the DMC, with fibres b) 13mm solubleshorter than the probable critical length, is in 0.6 c) 13mm insolublefact no greater than that of the resin matrix,but its advantage lies in its much higher 0.4toughness, as we shall see in chapter 5. 0.2 One of the problems encountered in themanufacturing of short-fibre composites is 0that the fibres may sustain damage as a 0 5 10 15 20result of the mechanical processes involved. Fibre lengths, mmVery often the lengths of the filaments arereduced, either as a consequence of the Figure 4.24. Normalized distributions of the lengths of fibres extracted from moulded DMCs. The mean lengths of the fibresblending of the constituents in a thermoset after processing are: a) 1.63mm, b) 1.86mm, c) 3.10mm.
chapter four Strength 78moulding compound, or of the injection moulding of thermoplastic compounds through narrow dieopenings. And although the starting lengths of the fibre stock may initially be well above the criticallength, their lengths in the finished mouldings may be well below lc. In DMCs, the final fibre lengths arealso affected by the nature of the sizing compound used on the fibre tows. Figure 4.24 shows examplesof normalized length distributions for fibres extracted from polyester moulding compounds afterprocessing (Andrews, 1998). Three sets of data are included: two of them for fibres initially 6mm and13mm long coated with a soluble size, and the third for 13mm fibres with an insoluble size. It can beseen that when the size dissolves in the resin during processing, the fibre bundles become easilyseparated and they are reduced in length so as to have roughly the same modal value of length, onlyabout 1mm, whatever their initial length. If an insoluble size is used, the bundles do not filamentize toquite the same extent, but the modal length is only marginally greater. And although 1mm may be equalto or slightly greater than lc, a large fraction of the fibres are much shorter than this. In typical fibre-length distributions from injection moulded Nylon 66 with 15vol% of glass fibres, Bowyer and Bader(1972) showed that some 80% of the fibres were below the critical length, and they emphasised the needto control moulding procedures to minimize this processing damage. Some materials manufacturers havedeveloped commercial ‘long-fibre’ glass/thermoplastic moulding compounds to improve on theproperties of conventional mouldings: ICI’s Verton, containing 10mm long fibres, is an example of sucha material. Bowyer and Bader (1972) attempted to account for the effect of damage to fibres during the injectionmoulding of reinforced thermoplastics by studying the fibre length distributions in mouldings. They useda model in which contributions to composite strength from fibres of sub-critical and super-criticallengths were summed separately over the effective range of lengths : ⎡ τL ⎛ E ε d⎞ ⎤ σc = ηθ ⎢ ∑ i Vi + ∑ Ef εc ⎜ 1 − f c ⎟ Vj ⎥ + Emεc (1 − Vf ) ........................................... [4.24] ⎢ i d ⎜ 4L j τ ⎟ ⎥ ⎣ j ⎝ ⎠ ⎦The first summation represents the sub-critical fibre distribution, sub-fraction Vi with fibre lengthspectrum Li (l < lc), and corresponds to the first term in equation 4.25. The second summation gives thesuper-critical contribution, from sub-fraction Vj with fibre-length spectrum Lj (l > lc), and the third termis the usual matrix contribution. ηθ is the Krenchel factor, 0.375 for a planar-random moulding and 0.167 xy for 3-dimensional material. In this po on /e equation, τ represents the fibre/matrix 1.4 rb ca interfacial shear strength that we have S HT 1.2 xy previously called τi, the subscript having Tensile strength, GPa po y 1.0 s s/e pox xy been temporarily dropped to avoid gla on /e po S- rb l O /e 3 confusion with the summation indices, i 0.8 ca A 2 H M S and j. This model gave reasonable 0.6 ta l agreement with their experimental results ce olya M C C on glass-filled Nylon and polypropylene. 0.4 s/p r S M las ste rD -g lye ste 0.2 E po The strength of short-fibre composites lye po 0 is strongly affected by the fibre/matrix 0.5 0.5 0.5 0.14 0.25 0.25 0.12 bond strength, and since the reinforcing aligned random efficiency of short fibres is low, it is essential to ensure that they are as Fibre volume fraction strongly bonded as possible to the matrix. Figure 4.25. Tensile strengths of some short-fibre composites, The strengths of some typical short-fibre aligned and random. composites, commercial and experimental, are shown in Figure 4.25, together withthose of unreinforced matrix polymers. Improvements in strength by a factor of two or three areobtainable in practical moulding systems, but the strengths of these materials are very low bycomparison with those of continuous-fibre composites. By contrast, the well-aligned, short-fibrecomposites produced by Parratt and Potter (1980) can be seen from Figure 4.25 to have 60 to 70% of the
chapter four Strength 79strength of comparable continuous-fibre composites. The outstanding reinforcing potential of whiskersindicated in the table is not used in practice because of the cost of this kind of fibre. The effects of fibre characteristics anddistribution on the expected strengths ofaligned fibre composites are summarized in theschematic diagram of Figure 4.26. Increasingthe intrinsic fibre strength naturally increasesthe expected composite strength in the waysthat we have discussed in this chapter. But ifthe fibres are discontinuous, the reinforcingefficiency is reduced for two reasons: first, as aresult of the aspect-ratio effect described byequation 4.23 and, second, because the shorterthe fibres the more likely they are to bemisoriented, to a greater or lesser extent. This Figure 4.26. Schematic illustration summarising the effectsnot only results in a further efficiency loss from of choice and arrangement of fibres on the strengths of fibre-the orientation effect (Krenchel factor), but it reinforced composites.also limits the maximum fibre content that canbe incorporated into the composite since the closeness of packing is reduced.4.1.9 Hybrid composites As we saw in chapter 3 the elastic properties of hybrid composites can be calculated to within limitsacceptable for most design purposes by the application of well-established principles of compositemechanics and classical thin-laminate theory. But although elasticity calculations are largelyindependent of the nature of fibre distributions, predictions of properties such as strength, toughness, andfatigue behaviour are more difficult because they depend on micromechanisms of damage accumulationwhich, in turn, are determined by the construction of the laminate and the scale of dispersion of themixed fibres. At the grossest level of hybridization, strips of GRP incorporated into a CFRP laminate canact as efficient crack arresters (Bunsell and Harris, 1976; Sun and Luo, 1985), provided the width of thestrips is sufficient to dissipate the energy of a crack moving rapidly in the CFRP by localized debondingand splitting. The commonest type of hybrid, however, andthat which is most easily achieved in practice, ismade by laminating some balanced sequence of plieswithin each of which there is only a single species offibres. The composition-dependence of the strengthof a unidirectional composite of this kind is obtainedby analogy with the response of a single-fibrecomposite by considering the failure strains of thetwo separate constituents (Aveston and Kelly, 1979).When a small quantity of fibres with low failurestrain, εle, is added to a composite consisting offibres of high-failure-strain, εhe, the low-elongation(le) fibres will experience multiple failure before thefailure strain of the high-elongation (he) fibres isreached. By analogy with the case of a flexible resin Figure 4.27. Schematic representation of the variation ofcontaining only one species of brittle fibre, the the strengths of a family of unidirectional two-componentstrength of the hybrid composite, σH, will be given hybrid composites with proportions of the two constituents,at first (Figure 4.27) by the residual load-bearing referred to as the high-extensibility (he) and low- extensibility (le) materials.capacity of the he composite, assuming the lecomponent makes no contribution at all, ie. σH = σhu Vhe ......................................................................................................... [4.25]
chapter four Strength 80where Vhe is the volume fraction of the he component, Vhe + Vle = 1, and σhu is the strength of the pure hefibres. At the other extreme, if a small amount of he fibre is added to an le composite, the strength is againreduced because the he fibres cannot carry the load when the le component fails. Failure of the le fibrestherefore leads to single, catastrophic fracture of the composite. The hybrid strength in this mode is then: σH = σ’h Vhe + σlu Vle ............................................................................................ [4.26]where σlu is the strength of the pure le fibres, and the intercept of this line on the he axis (Vhe = 1) is thestress σ´h in the he component at the failure strain of the le component, equal to εluEh (εlu and εhu are thefailure strains of pure le fibres and the pure he fibres, 5 Failure strain, %respectively). The critical composition, Vcrit, for the 4 GRP/CFRPtransition from single to multiple fracture is found by 3 KFRP/CFRPsolving the simultaneous equations 4.27 and 4.28, whence: 2 1 σlu Vcrit = ..................................[4.27] 0 σ lu + σhu − εluEh 2 Tensile strength, GPaand this transition point also defines the hybridcomposition of minimum strength. Figure 4.28 illustrates 1that this simple model is adequate for two unidirectionalhybrid combinations, CFRP/GRP and CFRP/KFRP. It alsoshows that in the case of the KFRP/CFRP combination, forwhich the failure strains, εlu and εhu, are markedly 0 0 0.2 0.4 0.6 0.8 1.0different, the hybrid composite failure strain varies non-linearly with composition and falls below a straight line Composition, VCFRP /(VCFRP+ VGRP)joining εlu and εhu. This type of variation is characteristicand has given rise to the notion of ‘failure-strain Figure 4.28. Variation of tensile strength andenhancement’, also known as the ‘hybrid effect’. This idea failure strain with composition in ud hybridstems from the fact that since there is a continuous laminates of CFRP with GRP and with KFRP. The full lines in the lower figure represent equationsvariation of composite failure strain between the two end 4.27 and 4.28 for the two sets of strength data.points, some hybrid compositions must inevitably fail atstrains greater than the failure strain of the lower extensibility component, εlu. An analysis by Zweben(1977) shows that the failure process is affected by the statistical spread of failure strains of the two fibrespecies and predicts that the addition of he fibre to an le composite raises the strain level needed topropagate fibre breaks because the he fibres behave like crack arresters at a microstructural level. Thesituation becomes more complicated when the fibres are intimately mixed because micro-mechanisms offailure change as the pattern of nearest neighbours around a given fibre alters and the strength isgoverned by failure either of single fibres or of small bundles of fibres (Parratt and Potter, 1980).4.2 COMPRESSION STRENGTH Studies of the compression behaviour of compositeshave been complicated by the fact that when testingsmall, free blocks of material, failure modes occur whichare not necessarily determined by fibre behaviour, andthe compression strength of a composite often appears tobe lower than its tensile strength. As in the case of woodcompressed along the grain, longitudinal splitting and/orkinking of the sample often occur, as illustratedschematically in Figure 4.29, at stresses well below theequivalent tensile load-bearing ability of the composite. Figure 4.29. Schematic illustration of compression failure modes in unidirectional composites.
chapter four Strength 81 Measurements to obtain the true compression strength are difficult to carry out. A range of complexjigs has been developed for the purpose of preventing macroscopic (Euler) buckling of the sample during testing, but these often constrain the sample in an unnatural fashion, and it is uncertain whether the measured value of the compression strength is valid. Even after many precautions have been taken, measured compression strengths are often below the tensile strength of the same material, as shown by some experimental results for a variety of composites in Table 4.2. By contrast with polymer- and metal-matrix composites, however, the compression strengths of reinforced ceramics are often higher than their tensile strengths, presumably because the rigid ceramic matrix affords a much greater level of support to the fibres, allowing their reinforcing potential to be realized, whereas their tensile strengths are often determined by features other than the fibre strength (Harris et al, 1992b). This is shown by the data for the unidirectional SiC-reinforced calcium Figure 4.30. Microstructure of a aluminosilicate composite at the bottom of Table 4.2. In studying compression failure in a unidirectional glass/polyester compression behaviour, therefore, there is often uncertainty as to composite (the compression axis is whether an apparently low value of the compression strength is a vertical). reflection of material behaviour or a consequence of inappropriate testing procedures. Table 4.2. Experimental tension and compression strengths for various composite materials. Material Lay-up Vf Tensile Compression Ratio strength, σt strength, σc σc/σt GPa GPa GRP ud 0.6 1.3 1.1 0.85 CFRP ud 0.6 2.0 1.1 0.55 KFRP ud 0.6 1.0 0.4 0.40 HTA/913 (CFRP) [(±45,02)2]S 0.65 1.27 0.97 0.77 T800/924 (CFRP) [(±45,02)2]S 0.65 1.42 0.90 0.63 T800/5245 (CFRP) [(±45,02)2]S 0.65 1.67 0.88 0.53 SiC/CAS (CMC) ud 0.37 334 1360 4.07 SiC/CAS (CMC) (0,90)3S 0.37 210 463 2.20 Much effort has been expended on the development of compression test methods to overcome thisproblem. Devices commonly used include end-constraint techniques to prevent longitudinal splitting andlateral supports to prevent premature buckling, in addition to the more obvious precautionary measuresto align the stress axis accurately with the fibres. A recent study by Berg and Adams (1989) suggests thatmany of the observed discrepancies between published test results for composites occur as a result of testmethods. They carried out an evaluation of some of the commonly used anti-buckling test fixtures, andconcluded that a method developed at Illinois Institute of Technology (the IITRI fixture), which at thetime was an ASTM Standard test method, D 4310, was the most satisfactory method. By such means it ispossible to measure compression strengths almost equal to the tensile strength in composites other thanthose reinforced with Kevlar fibres, as demonstrated by Ewins and Ham (1973) for a series of carbon-fibre composites and, more recently, by Parry and Wronski (1982). Ewins and Ham suggested that themechanism of failure in CFRP is the same in both compression and tension modes and results from a 45°shear mechanism, but work by Parry and Wronski disagreed with this conclusion on the basis of studiesof the effect of superposed hydrostatic pressure on the compression behaviour. It does not follow,however, that for any given composite the ‘true’ compression strength must be the same as the tensilestrength.
chapter four Strength 82 Since it is not possible to attach any 0.8significance to the notion of ‘compression E-glass Compression strength, GPa HMS carbonstrength’ for a 10μm diameter fibre, when we 0.6 HTS carboninvestigate the effect of reinforcement on Kevlar-49compression strength we have to take the tensilestrength of the fibre as our point of reference. As a 0.4unidirectional composite is loaded in compression,the fibre axis being well-aligned with the stressaxis, the elastic models that we have already 0.2considered will apply and we would expect theinitial stiffness to be the same as the tensile 0stiffness, as discussed in chapter 3. But the fibres 0 0.2 0.4 0.6 0.8can only be maintained in good alignment by the Fibre volume fraction, Vfmatrix, which, in resin-based composites usuallyhas low shear stiffness, and when local shear or Figure 4.31. Variation of compression strength with fibretransverse tensile stresses become greater than the volume fraction in unidirectional composites of polyestermatrix can support, a crack may occur or a shear resin reinforced with carbon, glass and Kevlar-49 fibres (Martinez et al, 1981)(kink) band, like that shown in Figure 4.30, maydevelop and grow as the load increases. Flexiblefibres like glass or Kevlar-49 will usually bend or buckle in this kink band, while brittle fibres likecarbon will often fracture after the initial microbuckling has occurred. These instabilities then lead tooverall failure at stresses below the normal tensile strength of the material. Furthermore, since it isalmost impossible to obtain a unidirectional composite with perfectly aligned fibres — the fibres in mostpractical composites are likely to have small kinks or misalignments arising from manufacture — thesedefects will act as initiators for the microbuckling mechanisms. In an early model for compression strength, Rosen (1965) proposed that failure was initiated bymatrix instabilities that lead to co-operative, in-plane buckling of the reinforcement. The model wasdeveloped for lamellar composites with reinforcing plates, rather than fibres, and, except at low Vf, itpredicted failure by a shear mode at a stress: Gm ...................................................................................................... [4.28] σcomp = 1− Vfwhere Gm is the matrix shear modulus. The deficiency of the model, apart from the fact that it applies tothe buckling of plates, is apparent from the fact that σcomp → Gm as Vf → 0, and equation 4.30 consistently 3overestimates the compression strength of real fibre drawn wire Compression strength, GPacomposites. Lager and June (1969) suggested that out- annealed wireof plane buckling occurred in fibre composites, and 2proposed the use of an empirical ‘influence factor’ toobtain agreement between their results for wire tensileboron/epoxy composites and Rosen’s theory. This was strengths 1a logical idea, since the stored elastic energy in a fibrewhich buckles into a helix is bound to be lower thanthat in one constrained to preserve a planar buckledform. It was later demonstrated by de Ferran and 0 0 0.2 0.4 0.6 0.8 1.0Harris (1970) that helical buckling occurred in fibresextracted from compressed MMCs. They also showed Fibre volume fractionthat the compression strengths of steel-wire/resincomposites obeyed a mixture rule based on the tensile Figure 4.32. Compression strengths of steel-strength of the reinforcing wires, as illustrated in wire/polyester-resin composites (de Ferran andFigure 4.32. These results for two different species of Harris, 1970).steel wire reinforcements were in good agreement witha model of Hayashi and Koyama (1971) which allowed for the stress-dependence of the shear modulus.
chapter four Strength 83The implication was that in this case the fibres were controlling compression failure by virtue of theirinherent shear resistance which, in a ductile metal, is the same in compression as in tension. By contrast, Martinez et al (1981) have shown that in composites reinforced with much finerfilaments of carbon, glass and Kevlar-49 the compression strength appears not to be sensitive in anystraightforward fashion to either the strength or stiffness of the reinforcing filaments, as can be seenfrom Figure 4.31. The linear portions of the curves for glass and both varieties of carbon (high-strengthand high-modulus) are largely indistinguishable and extrapolate to stress levels at Vf = 1 of between 1.3and 1.4GPa, reasonable for the tensile failure of glass or HMS carbon, but only half what might havebeen expected for HTS carbon. The curve for the aramid composites lies well below those of the othercomposites, and the low strengths are inconsistent with the high tensile strength and stiffness of theKevlar-49 fibre itself. The curves for all of the composites are linear up to Vf values of only about 0.4,the deviations from linearity and subsequent downward trends implying changes in failure mode. Early models often assumed that fibre buckling was responsible for the compression yielding ofcomposites and that the Euler buckling theory for a column on an elastic foundation was a suitable basisfor calculating the composite compression strength. Since buckling would be controlled by fibremodulus and diameter, the results in Figure 4.31, representing fibres of roughly similar diameter buthaving a wide range of strengths and moduli, and the earlier results of de Ferran and Harris, representingexperiments with wires of different strengths but having identical moduli and diameters, offer no supportfor these ideas. A corollary of the buckling model was that fibres that were already misaligned or kinkedwould buckle more readily than misaligned fibres and that the apparently low compression strengths ofmany composites could be accounted for in this way. A series of experiments was therefore carried outby Martinez et al (1981) with composites in which the fibres were deliberately misaligned with respectto the stress axis by twisting the tows of fibre which were used to reinforce a polyester resin. In this waya known angle of deviation could be introduced. Their results showed that for misalignments up to 10°the compression strengths of brittle-fibre composites actually increased and in some cases did not fallbelow the aligned-fibre value until nearly twice this degree of misalignment. The increase can beexplained in purely geometric terms in the same way as the maximum-stress model of Stowell and Liu(qv) explains an initial increase in tensile strength with fibre misorientation. Although the results described above offer little support for the idea that fibre misalignment controlscompressive failure of unidirectional composites, a recent predictive model suggests otherwise. Barbero(1998) has derived an explicit mechanics-based model which is able to predict compression strengthwith good accuracy on the basis of a non-dimensional function: G12 χ= Ωτiiwhere G12 is the composite shear stiffness and τ11 its shear strength, while Ω is the standard deviation (indegrees) of the fibre misalignment. The advantage of this model is that values of all three terms in thedefinition of χ may be obtained from well-established experimental techniques. Agreement withexperimental data was good for a wide range of unidirectional composites, including glass- and carbon-fibre-reinforced polyesters, epoxies and thermoplastics. The factors other than fibre thickness which affect the compression strength are the matrix strengthand rigidity, and the interfacial bond strength. The more rigid the matrix, the greater the compressionstrength. Thus, ceramic- and metal-matrix composites are much stronger in compression than resin-basedcomposites. CMCs, in which the fibres and matrix often have similar levels of stiffness, may havecompression strengths that exceed their tensile strengths, as shown in Table 4.2. Most modernreinforcing fibres are only about 10-15µm in diameter. Boron, on the other hand, although not nowmuch used, is much thicker — about 40μm — and thicker fibres resist microbuckling much better thanthin ones, as predicted by the Euler theory. Boron-fibre-reinforced aluminium is currently the compositematerial having the highest ratio of compression strength to density. Curtis and Morton (1982) have
chapter four Strength 84shown that the compression strengths of multi-directional coupons of an unspecified CFRP materialwere markedly affected by fibre surface treatment, increasing by some 50% as the level of a commercialtreatment was increased from nothing to about 10% of the normal commercial level, and then remainingconstant, at which stage the measured strengths were only some 10% less than the tensile strength of thesame composite. This discrepancy could be removed, however, by taking into account small degrees ofeccentric loading in the test jig.4.2.1 Compression strength after impact We have seen that tensile loading introduces impacterdamage into a composite and that the damage +45accumulation process is partly responsible for -45 0 0determining the strength of the composite. It is one +45 -45of the perceived virtues of composite materials that 0 0they are tolerant of damage and that tensile damage 0 0does not seriously affect tensile load-bearing -45 +45ability, but a word of caution is necessary here. 0 0 -45Composite laminates in many external applications, +45especially in aircraft, are susceptible to impactdamage from low-velocity projectiles travelling 2cm scalenormal to the surface. The simplest, and most-oftenquoted, example is the damage caused by a spanner Figure 4.33. Damage map of the longitudinal section ofdropped by a person standing on an aeroplane a [(±45,02)2]S CFRP composite after it had received a low-velocity impact of energy 3J (Beheshty, 1997).wing. A tool weighing 1kg dropped from waistheight delivers a blow with about 10J of energy. In an impact between a round-ended projectile and aflat plate, tensile stresses may occur in the matrix and across the interlaminar planes of weakness. In alow-velocity impact the rate of build-up of the Hertzian contact stresses is high. Even a toughened epoxyresin may therefore appear to be brittle under such conditions and cracks may occur, as shown in Figure4.33, as planar cracks within the interlaminar regions and as transverse cracks in an apparently conicaldistribution spreading outwards through the composite away from the point of contact. The developmentof this kind of damage has been modelled by Davies et al (1995). If the impacter has sufficient energy,there may be serious surface cracking or spalling damage on the back face of the laminate, even whenthe damage on the impacted face is scarcely detectable, a condition referred to as BVID — barely-visibleimpact damage. The problem for users of composites is that although this kind of damage does notmarkedly affect the tensile strengths of most laminates, it has an adverse effect on the compressionstrength because the interlaminar cracks are able to extend as delaminations. The CAI, or compression- 1.5 after-impact, test has become a standard way of assessing the severity of damage induced by low- velocity impact events. An illustration of the tension effects of such impacts on the tension and Strength, GPa 1.0 compression strengths of a CFRP laminate is shown in Figure 4.34. For this fairly typical composite consisting of a high-strength fibre in a modified epoxy resin, an impact of only 5J 0.5 compression reduces the compression strength to some 32% of its initial value, while reducing the tensile strength by only 5 or 6%. Such a result has a 0 knock-on effect for other properties of the 0 1 2 3 4 5 6 material, such as the flexural response and Low-velocity impact energy, J fatigue behaviour. There are two aspects of the laminate structure that may be considered Figure 4.34. Effect of low-velocity impact damage on the responsible for this behaviour. First, the fact that residual tensile and compression strengths of a the matrix resin is an epoxy — even a so-called [(±45,02)2]S HTA/982 CFRP laminate (Beheshty & Harris, ‘modified’ one — which is naturally rate- 1997). sensitive means that the matrix is likely to become brittle at high rates of loading, and if the
chapter four Strength 85stresses are concentrated, either by the presence of notches or by the Hertzian contact effect, the rate isincreased even further. Second, if the laminate is manufactured from prepreg sheet, the interlaminarplanes form natural regions of weakness, as we have seen. Two possible solutions to this problem are a)to use a thermoplastic matrix instead of a thermoset, and b) to use woven-cloth reinforcement instead ofnon-woven fibres. An illustration of the power of this argument is given by some results ofGhaseminejad and Parvizi-Majidi (1990) who studied the impact behaviour and damage tolerance of twothermoplastic polyaryl resins, poly(ether ether ketone), known as PEEK, and poly(phenylene sulphide),or PPS, reinforced with woven carbon-fibre cloth. The compression strength after impact of the PEEK-based composite remained at 47% of the value for virgin material even after sustaining an impact of 29J. Guild et al (1993) developed a model for the reduction in compression strength of laminatesfollowing impact. The virtue of their model is that it is based on the premise that failure in post-impactcompression occurs as a consequence of the stress concentration that arises because of the presence of adamaged zone. It does not require the use of fracture-mechanics concepts which, as the authors pointout, is ruled out by the observed fact that materials whose fracture behaviour is characterized bydifferent values of the strain-energy release rates GIc and GIIc often show comparable performances inrespect of compression-after-impact. The model predicts, in agreement with experimental results, thatthe normalized compression-after-impact strength falls linearly with the width of the damage zone,whatever the material.4.3 SHEAR STRENGTH Most laminated continuous-fibre composites contain planes of weakness between the laminations andalong fibre/matrix interfaces. In shear the composite strength will be dominated by these weaknessesunless the stress direction intersects the fibres. Shear stresses at the interfaces between the plies canseldom be avoided by lay-up design because of the anisotropies of neighbouring plies, as discussed inchapter 3. These interlaminar shear stresses are usually high at edges, as shown by Pipes and Pagano(1970), and often give rise to delaminations which propagate into the composite from the edges,significantly reducing the laminate tensile strength (Pagano and Pipes, 1971). Delamination is a majorcause of failure in laminated composites, and one of the concerns of the designer is to ensure that shearstresses are diffused safely away from stressconcentration points. transverse section at AA Interlaminar shear failure is most readily seenin the three-point bending of short beams, amethod commonly used to measure what is interlaminarusually referred to as the interlaminar shear shear crackstrength, or ILSS, although this is often regardedas unsatisfactory because the state of stress isnot pure shear. In the diagram in Figure 4.35, ifthe level of horizontal shear stress at the mid-plane point M reaches the interlaminar shearstrength, τIL, of the composite before the tensile Figure 4.35. Schematic illustration of interlaminar shearstress level at T reaches the composite strength, failure in a unidirectional laminate.σc, then the beam will fail as shown. If the beamis longer than a certain critical length, however, it will fail in a normal bending mode by a tensile failureinitiating at the mid-point of the outer face. The variation in failure load as the span-to-depth ratio of thebeam increases is shown schematically in Figure 4.37. As long as the failure mode is interlaminar shear,the failure load is independent of length, but when the tensile failure mode predominates, the failure loadfalls rapidly in inverse ratio to the span of the beam. The critical span-to-depth ratio for the transition canbe found by equating the expressions for the tensile and shear stresses in the beam. The tensile stress at T is 3PL/2BD2, while the shear stress at the neutral plane is 3P/4BD (the standardformulae for the bending beam, with B = width, D = thickness, and L = length). Equating these, wehave:
chapter four Strength 86 σc 3PL 3P 2L ......................................................................................... [4.29] = = τIL 2BD2 4BD Dand the beam will therefore fail in interlaminar 30shear at the neutral plane if L/D < σc/2τIL. For atypical unidirectional CFRP laminate with σc ≈ 25 KIIc =A.τIL(v)1/61.5GPa and τIL ≈ 50MPa, a shear failure will occurin bending at span-to-depth ratios less than about 20 ILSS, MPa15:1, and when the short-beam shear test is used to dry 15evaluate the ILSS, it is usually recommended thata span-to-depth ratio of about 5 is used. wet 10 The interlaminar shear strength depends in part 5on the shear strength of the matrix and in part onthe shear resistance of the interface. The stronger 0 0 5 10 15the interfacial bonding, then, and the greater the Void content, vol%amount of interface relative to the amount ofmatrix, the greater will be the ILSS: the ILSS Figure 4.36. The effect of voids and moisture on thealmost always increases with fibre volume fraction interlaminar shear strength of a unidirectionalunless the level of fibre/matrix bonding is very carbon/epoxy laminate (Beaumont & Harris, 1972). Thelow. With modern carbon and glass fibres this dashed line represents a suggestion of Corten (1968) thatrarely occurs, however, because the reinforcing the effect of voids on ILSS may be represented by a constant value of the mode-II critical stress-intensity factorfibres are usually surface treated after manufacture and the voids as having the effect of cracks (see text).in order to improve the interfacial bond. In carbon-fibre composites it was long ago shown that the ILSS was roughly inversely related to the stiffness of thereinforcing fibres, which reflected the fact that both the fibre mechanical properties and their chemicalactivity (wettability) are determined by the level of heat-treatment they receive during processing. Interlaminar weakness is aggravated by the presence of voids or moisture in the resin, as shown inFigure 4.36. In some carbon/epoxy composites, for example, 10vol% of voids could reduce the ILSS bysome 25%: moisture absorption will reduce the intrinsic matrix strength and may also cause adeterioration in the interfacial bond strength, both of which will reduce the ILSS. Corten (1968)suggested that the effect of voids on the shear strength could be treated in terms of a fracture-mechanicsapproach (see chapter 5 for further information on fracture mechanics). If an increase in void content isnotionally equivalent, in terms of stress concentration, to an increase in crack size, and the equivalent crack dimension, a, is roughly proportional to the 100 cube root of the void content, 3√v, then an Flexural and shear failure loads, kN shear failure load expression for the mode II critical stress-intensity flexural failure load factor, KIIC, is: 10 tensile failure K IIc = τIL πa = Aτ6 v ....................[4.30] As the dashed line in Figure 4.36 shows, an 0 shear failure expression of this form fits the data very well down critical value of L/D to some threshold void content of about 1%. The constant, A, has a value of about 23 when the ILSS 0.1 is in MPa and v is in %). 0 10 20 30 Span-to-depth ratio, L/D Although an appreciation of the reasons for the weakness of composites in shear is of great Figure 4.37. Transition from shear to flexural (tensile) importance to the designer, it is not necessarilyfailure of a thin laminate plate in three-point bending asthe span-to-depth ratio, L/D, increases. The composite advantageous to use composites with the highest tensile strength for this sample is 750MPa and its obtainable shear strengths. Cracks running normal interlaminar shear strength is 50MPa. to fibres in a tension structure may pass at various times through fibres, resin and interface, but if
chapter four Strength 87nothing changes the crack path, a reasonably flat fracture surface may result and the composite will benotch-sensitive, even brittle. If the material has an interface of only moderate strength, however, cracksmay deviate through weak regions, such as the interlaminar planes, to become delaminations. As a result,a crack tip is effectively blunted and the material will appear tougher. Materials suppliers are required tomaintain a fine balance in controlling the fibre, matrix and interface properties in order to optimizestrength (tensile and shear) and toughness. An alternative approach to modifying the interfacial bondstrength is to improve the delamination resistance of a laminate by ‘stitching’ the laminae together withfibres running in the direction perpendicular to the plane of the laminate. This process has been shown(Dransfield et al, 1994) to improve both the ILSS (delamination resistance) and also the toughness of thecomposite, although Adanur et al (1995) have shown that there is a limiting stitch density beyond whichthese improvements are reversed. Another difficulty often faced by designers is that of assessing the reliability of a reported value ofthe shear strength of a composite, which we have previously termed τc. The short-beam shear testdescribed above is very easy to carry out and is very useful as an experimental tool. But although itforms the basis of an international standard test, the complex stress state involved makes it unsatisfactoryfor obtaining absolute values of the shear strength: τIL is not necessarily a good measure of τc. The idealmethod of measuring τc is perhaps by the torsion testing of thin-walled, hoop-wound tubes, as describedby Puck and Schneider (1969), which gives pure states of shear stress and strain in the tube wall.Alternative solutions have usually been sought, however, because of the time and expense involved incarrying out such tests. One such solution is the measurement of the intralaminar shear strength by thetensile testing of unidirectional test coupons at an angle to the fibres. Chamis & Sinclair (1972) showed,from a consideration of the relative stress and strain magnitudes in tensile test samples at various angles,θ, to the fibre direction, that the in-plane shear strain is a maximum when θ = 10° for typical CFRPlaminates. A tensile test on a unidirectional coupon cut at 10° to the fibres should therefore provide anaccurate measure of the intralaminar shear strength. The tensile stress normal to the fibres is not zero atthis angle, however, and locally the composite is effectively in a biaxial stress state. Hart-Smith (1996)argues that a tensile test on a ±45° laminate provides a more appropriate value of the in-plane shearstrength, and there is much current interest in the Iosipescu test (Iosipescu, 1967), a method involvingtransverse shear loading of deeply notched test beams which, when carried out with adequate controls,generates a state of pure shear and provides good values of shear stiffness, but which still leavessomething to be desired when used to obtain strength data (Pierron et al, 1996).4.3.1 The shear strength of the interfacial bond At several points in this book we refer to the importance of the fibre/matrix bond in determiningimportant physical properties of composites. The economic and safe exploitation of modern high-performance composites depends directly on our ability to employ the fibres in resin and other matricesin such a way as to permit the optimization of the major mechanical properties of the composite. Ourability to tailor composites to a given specification, and to predict accurately the properties ofmanufactured materials, calls for an understanding of the nature of the individual components and of themanner in which they interact when working in combination. Since much of this understanding hingeson characterization of the strength of the interface, it seems appropriate to digress briefly from dealingwith macroscopic properties in order to consider some of the methods that are used for determining thisall-important characteristic. One of the difficulties in making valid assessments of the interfacial shear strength, τi, is that thesimplest experimental methods involve interactions between single fibres and blocks or drops of resinrather than realistic composite structures. Some of the earliest experiments with single fibres embeddedin resin were carried out by Broutman and by McGarry (see Broutman, 1967). These were carried out onspecially shaped specimens which, when loaded in compression, caused shear or tensile debonding ofthe fibre from the matrix. These methods have largely been superseded, possibly because of thedifficulty of preparing the samples. A second problem is that the analysis of experimental data ofteninvolves oversimplified assumptions about the stress distribution along a fibre and about the manner ofinterfacial failure. Some of these limitations will be apparent in the following discussion of several of themore familiar test methods.
chapter four Strength 88 i) Values from macroscopic shear-strength measurements. It might be anticipated from the schematic illustration of an interlaminar shear failure shown in Figure 4.35 that, since this kind of failure is a mixed fracture passing partly through the matrix and partly through the interface, the ILSS would be a rule-of mixtures sum of the shear strengths of the matrix and the interface. It will not be a linear function of Vf, however, because the interface failure is associated with a non-planar surface area. As shown by Hancock and Cuthbertson (1970), the ILSS for a unidirectional composite would be given by: τIL = aiτi + (1 – ai)τm ....................................................................................... [4.31] where τm is the shear strength of the resin and ai is the fraction of the fracture surface area which consists of fibre/resin interface. Since ai → 1 in a composite of high Vf, this relationship may provide a useful first estimate of τi, but this simplified model is likely to be inadequate because of the shear-stress concentrations that result from the inhomogeneity of the material. The results of Iosipescu or other macroscopic shear tests could, of course, be analyzed in a similar manner to that described above. ii) Values from crack-spacing measurements. When dealing with brittle-matrix composites like CMCs, estimates of the value of τi may be made from observations of crack spacings in damaged composites. In such a composite the matrix is usually of lower extensibility than the fibres, so that when the composite is loaded in tension, multiple cracking of the matrix occurs until a limiting crack density is reached. The Aveston, Cooper and Kelly theory (Aveston et al, 1971, 1974, 1979), which is discussed in more detail in section 4.6, shows that the limiting crack separation in a brittle-matrix composite is between x and 2x, where ⎛V ⎞ ⎛σ r⎞ x′ = ⎜ m ⎟ . ⎜ mu ⎟ ..............................[4.32] ⎝ Vf ⎠ ⎝ 2τi ⎠ σmu being the failure stress of the unreinforced matrix and r the fibre radius. Aveston et al (1974) show that the mean crack spacing, s = 1.364x. Thus, for a typical mean crack spacing of the order c) single-fibre of 0.2mm in a SiC/CAS composite of Vf = 0.4, fragmentation (Harris et al, 1992b), x is about 0.15mm, and the τ i must therefore be about 3.5MPa if σmu is Figure 4.38. Schematic illustration of four of the most 100MPa. This low value is typical of many CMCs. common experimental methods for determining the interfacial shear strength. iii) Fibre pull-out tests. There are two main variants of this method, as illustrated in Figure 4.38a and b. In the first, single fibres of different lengths are embedded in resin and loads are applied. If the embedded length, l, is less than lc/2, the bond will be Fmax broken and the fibre extracted. When l > lc/2, the fibre will break outside the resin (see problem 14, Chapter 8). When the end of a fibre with l < lc/2 is loaded by pulling, Load the load increases to some maximum level at which the uncoated induced shear forces acting at the interface are able to silane coated initiate a debond and the load drops to some lower level as the debond rapidly propagates, as illustrated in Figure 4.39. The equilibrium state identified by the bottom of the load drop relates to a length of fibre separated from the Deflexion surrounding resin and an end ‘plug’ which maintains Figure 4.39. Load/deflexion curves obtained from contact and exerts an opposing frictional drag as thesingle-fibre pull-out experiments on glass/polyester applied force withdraws the fibre from the matrix. Thecomposites (Harris et al, 1975). The peak loads are peak load must reflect the strength of the combinednot directly comparable because the pulled lengths of fibre were different.
chapter four Strength 89chemical and physical bond, while the portion of the curve after the drop relates to the work of fibrepull-out. The interpretational problem associated with this test is that we have no easy means of knowingexactly what shear/debond condition the force Fmax or the load at the bottom of the load-drop shown inFigure 4.39 relate to. We do not know what the relative lengths of the plug and the ‘free’ portion of thefibre are, and we do not know how the shear stress varies in the plug region, nor how it changes as thepull-out process progresses. Fmax is often used to obtain an indirect estimate of the maximum interfacialshear stress required for debonding: τi = Fmax /πdl.................................................................................................... [4.33]and the area under the curve after the load drop has been equated with the work of fibre pull-out, whichprovides an estimate of the interfacial frictional stress. Outwater and Murphy (1969) and Gao et al(1988) adopted fracture-mechanics-based models to describe the debonding process, and while thesemay well offer more realistic models of the pull-out process, their implementation as tests fordetermining τi depends on knowing the critical strain-energy release rate for debonding Pitkethly and Doble (1989) pointed out that if equation 4.35 is applied to a long fibre then the shearstrength will be underestimated because a part of the fibre is included over which no stresstransfer is taking place. Ideally, the embedded fibre length should be as near to zero as possible,but for more manageable fibre lengths they took the value of the shear stress obtained fromequation 4.35 as an average value of the shear debond stress and applied a correction derivedfrom shear-lag theory to obtain a more realistic estimate of the maximum interfacial shearstrength. A recent critique of the test and its analysis has been given by DiFrancia et al (1996). Theycite values of the debonding shear strength for surface-treated carbon/epoxy combinations of about70MPa, compared to about 25MPa for untreated fibres. Qiu and Schwartz (1993) have tried toovercome the unrealistic condition of pull-out from a plain resin by designing micro-composite samplesin which the central fibre is withdrawn from a ‘composite’ consisting of seven fibres in resin.iv) Droplet-debond tests. In the droplet-debond test (Miller et al, 1991) a small droplet of resin issuspended on the fibre and, after curing, the fibre is withdrawn from the droplet (Figure 4.38b). Becausethe interfacial contact is small, there is a high probability that debonding will occur before fibre ruptureor matrix deformation. The interfacial shear strength is again calculated from the maximum debondingforce, Fmax, from equation 4.35. It is usually found that there is a high degree of variability in these tests(cv ≈ 20%), often as a consequence of the inherent non-uniformity of fibre surfaces. An accurateassessment of the area of the fibre perimeter within the droplet is required, and this is made either bywettability measurements or fibre diameter measurements. An accurate assessment of the embeddedlength is also sometimes difficult to obtain if there are marked menisci at the ends of the droplet andthese break off at an early stage in the test. Good instrumentation is needed if these dimensionalmeasurements are not to constitute a major source of error.v) Micro-indentation (or push-in) tests. This test was first proposed by Mandell et al (1980), anddescribed for use with CMCs by Marshall and Evans (1985). Analyses have also been given by Chenand Young (1991) and Ho and Drzal (1996). A cross-section is taken through a real composite andpolished by normal metallographic procedures. A very small diamond indenter, such as that in a micro-hardness testing machine, is then used to push one of the fibre ends into the body of the composite(Figure 4.38c). By choosing the load so that the indenter just contacts the matrix, an estimate of τi canbe obtained from the relationship: τi = F2/(4π2ur3Ef) ............................................................................................... [4.34]where r is the fibre radius and Ef is the fibre elastic modulus. F is the force applied to the fibre, and thisis calculated from the relationship:
chapter four Strength 90 F = 2a2HH being the fibre hardness which is obtained by indenting fibres under lower loads where no slidingoccurs, and a is the length of the diagonal of the indentation impression in the fibre. The term u is thedistance by which the fibre has been depressed at maximum load and is calculated from the dimensionsof the indentation in the fibre and matrix. Two common difficulties with this test are that it is hard toassess the effect of the sideways force exerted by the indenter normal to the direction of sliding, and it isoften difficult to obtain a realistic value of fibre ‘hardness’ because the structure (and therefore theproperties) of common fibres are often very variable through the cross section. More sophisticatedpurpose-built testing machines provide force/displacement information directly from sensitive transducerread-outs.vi) Single-fibre fragmentation tests. This test hasbecome one of the principal methods for assessing 1.2fibre/matrix interfacial characteristics. The method, Weibull parameters:introduced by Kelly and Tyson (1965), consists in 1.0 untreated oxidizedembedding a single fibre in a clear resin sample(Figure 4.38d) which is loaded in tension so as to 0.8 m 7 4.6 i/(N + 1) b 75 64cause the fibre to break down into successively a 0 0 0.6shorter lengths until all fragments have lengthsshorter than or equal to lc. To ensure that this 0.4process can be completed it is usually necessary toensure that the resin has a high failure strain, thus 0.2imposing a second element of artificiality on the test. 0The fragment lengths are measured with an optical 0 20 40 60 80 100microscope focused on the fibre within the resin (for Fragment aspect ratio, l/d.detailed descriptions, see, for example, Drzal et al,1982; Netravali et al, 1989; Feillard et al, 1994). Figure 4.40. Probability plot of fibre fragment aspect ratios from a single-fibre fragmentation test. Untreated and The principle of the test depends on the force- oxidized ENKA HTA carbon fibres.balance relationship between the critical aspect ratioof the fibre, lc/d, the fibre strength, σf, and the interfacial shear strength, τi, given by equation 3.30: lc σ = f ............................................................................................................. [4.35] d 2 τifor rigid/perfectly-plastic behaviour of the composite. In the use of the fragmentation test it is assumedthat the value of critical length obtained from the distribution of broken fibre lengths and the single-filament strengths obtained from single-filament tests may be used in this equation to obtain a value forthe interfacial shear strength. The situation is less simple than it appears, however. The distribution ofbroken fibre lengths is not independent of the fibre strength distribution, and assessment of a true valueof lc is not straightforward. Assuming a uniform interfacial strength and a fibre strength distribution with little dispersion aboutthe mean value, the shortest broken length that will be found should be equal to lc/2, and the longestobserved length will be just shorter than lc, the range of lengths being uniformly distributed betweenthese two extremes, provided the test has been continued to sufficiently large strains. Thus, it isfrequently assumed that the average observed broken length will be 3lc /4, and the value of the criticallength derived from such measurements is 4lmean/3. Two typical distributions of aspect ratios, l/d, ofcarbon-fibre fragments in epoxy resin are shown in Figure 4.40 (Harris et al, 1992a). They fit two-parameter Weibull distributions (see Appendix 2) with wide spreads. The shape factor, m, is about 6,which is similar to values obtained for the fibre strength distributions, as we saw in section 0. It can beseen that the effect of carrying out a commercial surface oxidation treatment on the fibre is to shift thedistribution of fragment lengths to the left, so that the characteristic length, obtained from the scale
chapter four Strength 91parameter, b, falls from about 525μm to about to 450μm as a result of this oxidation. Since both the fibrestrengths and the fragment lengths are distributed according to two-parameter Weibull models, it istherefore necessary to use a statistical approach in order to determine a cumulative distribution functionfor the interfacial shear strength, from which an average effective interfacial shear strength can beobtained. Table 4.3. Some published values of carbon/epoxy interfacial shear strength values measured by the single-fibre fragmentation test. Carbon-fibre/resin Fibre surface Reported value system treatment of τi , MPa HMU/828 none 6-14 HMS/828 commercial 20-47 AU/828 none 24 AS/828 commercial 74 AU4/828 none 29-36 AS4/828 commercial 47,48 T300/5208 none 39 T300/5208 commercial 49 In obtaining an estimate of the interfacial shear strength from equation 4.37, the usual assumption isthat the value of strength to be used in the equation is that which is characteristic of the fibre at a gaugelength equivalent to the critical length, lc. If we consider the process of fragmentation, either in a single-fibre composite or in a real composite, we see from the weakest-link model that each time a fibrefractures, the remaining pieces of the fibre must become stronger. During the fragmentation process,therefore, there will be a continuing change in the value of fibre strength that is actually affecting thefragmentation process and therefore a change in the balance of forces implied by equation 4.37. Thefinal fracture in a given piece of fibre, will occur when the fibre length, l, is somewhat greater than lcand somewhat less than 2lc, ie. lc < l < 2lc. Thus, the appropriate value of strength to use in equation4.37 will be that which is characteristic of a length of about 1.5lc, and this can be obtained from thestrength/length relationship of equation 4.10. Some typical experimental results for values of theinterfacial shear strength in carbon/epoxy systems are given in Table 4.3. These are taken frompublished papers, and full references may be found in Harris et al, 1992a. It is unlikely that the rigid/perfectly-plastic assumption is truly valid for resin-based composites.Lacroix et al (1992) have made a detailed critique of the method, arguing that lc may not be consideredto be a material constant, since it depends on the shear-stress-transfer model used. The Kelly and Tysonmodel(1965) which yields equation 4.37 is valid only for the condition of total debonding and fails todistinguish between the interfacial bond strength and the frictional shear strength. Predicted values of lcmay be lower than those characteristic of complete debonding if the interfacial bond strength issufficiently larger than the frictional shear stress. Despite the obvious experimental difficulties with thistest, the results in Table 4.3 are reasonably self-consistent, and the method can presumably be used forcomparative measurements, even though the absolute values of τi obtained from it may not be accurate.vii) Direct measurement by laser-Raman spectroscopy. This is essentially a means of measuring strainby monitoring the frequency of atomic vibrations in a crystalline material which can be probed byspectroscopic techniques such as Raman or IR spectroscopy. As atomic bond lengths increase underload, frequency shifts occur which are directly related to the applied load. The use of the laser Ramanmethod, which is widely applicable to materials such as commercial polymers and ceramics, does notrequire physical contact, unlike other strain-measuring techniques, and it is highly selective, beingcapable of probing areas as small as 1 or 2μm. Pioneering work in this field has been carried out byGaliotis and co-workers (1984, 1991).
chapter four Strength 92 It is commonly observed that the results obtained from many of the above tests show considerablevariability and there are also usually significant differences between the experimental estimates obtainedfrom the different tests, as shown by some results published by Herrera-Franco and Drzal (1991) (Table4.4). Table 4.4. A comparison of results of interfacial shear-strength measurements obtained by different test methods for AS4 carbon fibres in 828 epoxy resin (Herrera-Franco & Drzal, 1991) Experimental method τi, MPa Short-beam shear test (ILSS) 84.0 Iosipescu shear test 95.6 [±45]3s tension test 72.2 Droplet-debond test 50.3 Micro-indentation test 65.8 Single-fibre fragmentation test 68.34.4 FLEXURAL STRENGTH As discussed in section 4.3, we might expect that when a composite is loaded in bending it would failwhen the stress in the outer fibres on the tensile face reaches the normal composite tensile strength.However, early flexural tests often gave strength values that were considerably lower than the tensilestrength. One reason for this was that the loading points in flexural test rigs designed for metals oftencaused localized damage which initiated premature failures. But even when this defective test procedurewas rectified, low-stress failures still occurred. It was then considered that this was because in materialswith poor in-plane shear resistance and with compression strengths that were lower than the tensilestrengths, it was shear and/or compression damage modes that initiated the premature flexural failures.Controlled fibre surface treatments have now considerably improved both the interlaminar shear andcompression responses of many commercial materials, and it is usually possible to measure flexuralstrengths that are at least equal to the normal tensile strengths. Direct comparison of tension and flexural strength is somewhat complicated, however, by virtue ofthe statistical effect of the different stressed volumes in tensile and flexural test pieces. As discussed inAppendix 2 and illustrated by equation 4.10, the effective strength of a sample of small volume is greaterthan that of a larger sample. Thus, if two identically sized composite test pieces are tested in axialtension and in bending, the effective strength of the latter will be higher, even though the failure mode ineach case is simple tension, because the volume of the bend-test sample subjected to the highest stresslevel is much less than that in a tensile sample. The effect of such geometrical/statistical effects inceramics has been demonstrated by Davidge (1979). He shows that, for samples of similar volume, theratio of strengths measured in four-point bending and tension is a function only of the Weibull shapefactor, m, thus: 1 σ 4B ⎡ 4(m + 1)2 ⎤ ............................................................................................ [4.36] m =⎢ ⎥ σT ⎣ m+2 ⎦and for a given value of m the ratio of the three-point bend strength to the tensile strength is even greater. Measurements on a [(±45,02)2]S HTA/913 carbon/epoxy laminate gave values of 1.17±0.05,0.81±0.02, and 1.00±0.12GPa, respectively, for the axial tensile and compression strengths and the 4-point flexural strength (Hardiman, 1997). The Weibull shape factor for most good-quality CFRPmaterials is usually high, between 20 and 30, by comparison with common values for ceramics whichare less than 10. A mean value obtained at Bath for five other CFRP laminates of the same lay-up as theabove is 22, and the ratio given by equation 4.38 is therefore about 1.23. Thus, whereas the measuredtensile and flexural strengths are statistically almost identical, this apparent equivalence is accidentalsince, on this basis, we would have expected the flexural strength to be 23% higher than the tensilestrength, ie. about 1.44GPa, if the flexural failure is determined by the tensile strength. As it happens, the
chapter four Strength 93same factor applied to the experimental compression strength gives a value of 1.0GPa, which is equal tothe measured value of the flexural strength, even though the flexural failure of these samples was notapparently initiated on the compression face. We note, in passing, that for a group of SiC/CAS CMClaminates, the ratios of three-point-bend strength to tensile strengths were between 1.5 and 2.5,consistent with Weibull m values between 5 and 10. Attempts to reconcile the results of measurements ofthis kind with the simple statistical model are of course based on the assumption that the characteristicsof the critical flaws on the surface and in the volume of the material are identical, which may not be true.4.5 FAILURE CRITERIA FOR COMPLEX STRESSES For most practical purposes, designers require models of behaviour that can predict failure underrealistic combinations of stresses, rather than for the idealised uniaxial stress conditions under whichmost laboratory tests are carried out. There has been a great deal of research on complex-stress failurecriteria (twenty or more models have been proposed, although the differences between many of them arequite small: see the review by Owen and Found, 1972), and designers throughout the world remain indispute as to the ‘best’ method. A recent meeting organized jointly by the Institute of MechanicalEngineers and the Science & Engineering Research Council (now the Engineering and Physical SciencesResearch Council) in the UK (1991) exposed some of the areas of disagreement, and the Elsevier journalComposites Science and Technology has just published a Special Issue devoted to evaluating a widerange of popular failure criteria against validated experimental results*. The main difficulty in acceptingone or other of the common methods is that their validity can usually only be tested over limited rangesof combined stress because of the complexity and cost of the test samples and test procedures for suchexperiments — tubes under combined tension, torsion and internal pressure, for example. Most of theexisting failure criteria are in fact restricted to conditions of plane stress (thin plates) and some are onlyapplicable to orthotropic materials. We have noted in section 4.1.6 the differences between the maximum-stress criterion and themaximum-strain-energy criterion in predictions of the orientation-dependence of the strength of a singlelamina. The former takes into account that a unidirectional laminate will fail by different mechanisms atdifferent angles, but is not able to allow for interactions between failure modes or stresses. Thedisadvantage of the strain-energy approach is that it does not take account of different failure modes. Inits formal form it is an interactive model, although the interaction usually has to be allowed forempirically. The virtue of the strain-energy criterion in the eyes of many designers is that it isrepresented by a single equation instead of three (or five if compression failure is included). One of theearliest applications of the von Mises model was by Norris and McKinnon (1946) for GRP in planestress (ie. loading by stresses σ1 , σ2 , τ12, with all other stresses = 0) which predicts that failure willoccur when: 2 2 2 ⎡ σ1 ⎤ ⎡ σ2 ⎤ ⎡ τ12 ⎤ ⎢ ⎥ + ⎢ ⎥ + ⎢ ⎥ = 1 ....................................................................................... [4.37] ⎣ σc ⎦ ⎣ σt ⎦ ⎣ τc ⎦the stresses σc, σt, and τc being the composite failure stresses in tension, compression and shear, asdefined in section 4.16. In this form no interaction effects are allowed for. The later model of Azzi andTsai (1965), a development of which we have already met, took into account interaction effects betweenthe in-plane normal stresses: 2 2 2 2 ⎡ σ1 ⎤ ⎡ σ1σ2 ⎤ ⎡ σ2 ⎤ ⎡ τ12 ⎤ ............................................................................ [4.38] ⎢ ⎥ +⎢ ⎥ + ⎢ ⎥ + ⎢ ⎥ =1 ⎣ σc ⎦ ⎣ σc σt ⎦ ⎣ σt ⎦ ⎣ τc ⎦although in many situations the second term is relatively small and is often ignored, when the equationreverts to equation 4.39. Like the maximum-stress theory, these quadratic models are also extendible__________________________________________________________________________________* Failure criteria in fibre-reinforced polymer composites, Editors MJ Hinton, P Soden and AS Kaddour, Comp Sci &Technol, 58, July 1998, 999-1254.
chapter four Strength 94into the second, third and fourth quadrants of the (σ1,σ2) plane-stress framework, provided appropriatevalues of the compression strengths are used. Predictions of strength for off-axis loading can be obtainedby substituting the stress definitions used for the maximum-stress model (equations 4.16-4.18) intoequation 4.39, when the form of the maximum-strain-energy criterion given in equation 4.19 isrecovered. Eckold et al (1978) have developed a laminate theory for the prediction of failure envelopes forfilament-wound structures under biaxial loads. They predict failure, from a maximum-stress criterionrather than an interaction model, in a ply-by-ply analysis which allows for progressive failure of thelaminate, for shear non-linearity, and for different properties in tension and compression. The compositeis assumed to be composed of a series of homogeneous orthotropic plies, as is usual in laminate theorycalculations. Good agreement between predictions and experimental results was obtained. Although single-expression models like equation 4.39 are easy to work with mathematically, they aresubject to the very serious criticism that they are truly appropriate only for homogeneous materials anddo not take account of the different physical failure modes that occur in composites as the relativeorientations of the stress and symmetry axes change. Homogenisation methods of this kind result insingle elliptical failure envelopes which can apparently be defined from only three or four data pointsobtained under straightforward experimental conditions. But they are incapable of distinguishingbetween fibre and matrix failures, or allowing for alternative matrix damage processes, such as crackingand ductile shear failure. Hart-Smith has been particularly vociferous in condemning the quadraticmodels used by Tsai and his collaborators (and embodied in most of the currently available computerdesign software). He maintains (1991) that it is scientifically incorrect to use polynomial interactionfailure models whenever the mechanism of failure of the laminate changes with stress and maintains thatseparate failure criteria are needed for the fibres, the matrix and the interface. He has argued (1991, forexample) for the adoption of a maximum-shear-stress (Tresca) model because it automatically introducestruncations related to changes in failure mode which the quadratic models do not, and satisfactorilyexplains in-plane laminate test data in all of the stress quadrants.4.6 THE STRENGTH OF CERAMIC-MATRIX COMPOSITES Because of the brittleness of the matrices of CMCs, their response to stress differs considerably fromthat of reinforced plastics and metals. The matrix cracks at low stresses relative to the final failure stress,gradually transferring all responsibility for load bearing to the reinforcing fibres. Stress/strain curves forsome unidirectional and cross-plied (0,90)3S laminates of SiC/CAS are shown in Figure 4.41. The right-hand section of this figure shows the normal axial stress/strain curves, while the left-hand section showsthe variation of the transverse strains duringloading. 500 The axial stress/strain relationships for 400 (0) 12the unidirectional and (0,90)3s laminates Stress, MPashow similar features, with a predominantly 300linear initial portion, a marked knee, analmost linear second stage with a much 200reduced slope, followed by a third non- (0,90) 3Slinear region in which the average slope 100increases again. The knee indicates the onsetof major matrix cracking. 0 -0.5 10 x ε 22 0 0.5 1.0 ε 11 The transverse strains exhibit unusualvariations: they begin in the normal manner Longitudinal and transverse strains, %by showing a reduction in lateral dimensionthat is proportional to the load — normal Figure 4.41. Longitudinal and transverse strains as a function ofPoisson contraction — but the direction of stress for unidirectional and cross-plied composites of SiC/CASthis strain is subsequently reversed and (Harris et al, 1992b). The transverse strains are multiplied by ten to increase visibility on the graph.
chapter four Strength 95eventually becomes positive. This type of behaviour has been observed for a number of CMCs andalthough various explanations have been put forward it seems likely that the reversal is due to a gradualrelease of residual thermal stresses as matrix cracking develops. From an energy-based model, Aveston et al (1971) and Budiansky et al (1986) show that the stress atwhich matrix cracking should occur, σmc, is given by: 1 ⎡ 12τi γ m Vf2E f (1 − ν c )2 ⎤ 3 Ec ............................................................... [4.39] 2 σmc =⎢ ⎥ ⎦ (1 − ν c ) 2 2 ⎣ rVmEcEmwhere τi is the interfacial shear strength, r is the fibre radius, and νc is composite major Poisson ratio.The two unknowns in this equation are γm, the matrix fracture energy, and τi, the interfacial shearstrength. Estimates of the value of τi are often found from observations of crack spacing in damagedcomposites which, in a brittle/brittle system, is inversely related to the strength of the interfacial bond.When the fibres have a greater failure elongation than the matrix, which is almost always the case inCMCs, multiple cracking of the matrix occurs during loading until a limiting crack density is reachedwhere the crack spacing is between x´ and 2x´. The condition for multiple fracture is that: σfu > σmu Vm + σf′ Vf ............................................................................................. [4.40]where σmu is the matrix tensile strength and σf′ is the fibre stress at the matrix failure strain. The crackspacing is obtained from a force balance between tensile force in the fibres and shear force at theinterface as: ⎛V ⎞ ⎛σ r⎞ x′ = ⎜ m ⎟ . ⎜ mu ⎟ ............................................................................................ [4.41] ⎝ Vf ⎠ ⎝ 2τi ⎠σmu being the failure stress of the unreinforced matrix and r the fibre radius. The cracking stresspredicted by equation 4.41 is often very low by comparison with the normal composite tensile strength.For example, Evans et al (1991) quote a range of 140-160MPa for SiC/CAS composites for which thetensile strength may well be of the order of 1GPa, and acoustic emission studies have shown thatsubstantial sub-critical matrix cracking occurs at stresses well below the level predicted by equation 4.41(Harris et al, 1992b). The ACK model was used to predict the stress/strain curves for a number of fibre-reinforced cement-matrix composites with a considerable degree 600of accuracy (Aveston et al, 1994). The ud SiC/CAS data σfuVfpredicted curve follows three distinct, linear 500 ACK modelstages as shown in Figure 4.42. The first stage slope = EfVfhas a slope which is given by the usual rule of 400 Stress, MPamixtures, Ec = Ef Vf + Em(1 - Vf), and rises εmuto a stress level σmc at the first matrix cracking 300 Eoεmustrain, εmc. The second stage is horizontal and 200 εmu(1 + α/2)corresponds to a strain range during whichmatrix cracking continues at constant stress 100until a saturation level is reached at a strain slope = EfVf + EmVm (mixtures rule)εmc(1 + 0.66α), α being the weighted modulus 0ratio, EmVm/EfVf. The plateau joins the third 0 0.2 0.4 0.6 0.8 1.0section which is of slope EfVf, representing a Strain, %fibre-only contribution, and the failure point isreached at a stress level σfuVf. Figure 4.42. Illustration of the model of Aveston et al (1974) to predict the shape of the stress/strain curve for a ceramic- Not all CMC stress/strain curves are so matrix composite. α is the ratio Em Vm/Ef Vf.
chapter four Strength 96well predicted by the ACK model, however. Figure 4.42 also includes the stress/strain curve for theunidirectional SiC/CAS laminate referred to in Figure 4.41. It can be seen that matrix cracking, signalledby the deviation from linearity of stage 1 of the curve, starts well below the predicted level and the stresscontinues to rise as the cracking proceeds, rather than remaining constant. The slope of the third stage ofthe curve falls well below the predicted fibre-only contribution, and final failure occurs below thepredicted failure stress. Possible explanations of this are that the fibres have been damaged by themanufacturing process, or sustain damage as matrix cracking proceeds, perhaps as a result of dynamiccrack-growth effects not envisaged in the ACK model.4.7 REFERENCES TO CHAPTER 4 Adanur S, Tsao YP and Tam CW, 1995, Compos Engg, 5, 1149-1158. Andrews KE, 1998, unpublished results, Department of Materials Science & Engineering, University of Bath. Aveston J, Cooper GA and Kelly A, 1971, Proc NPL Conference on Properties of Fibre Composites NPL Teddington, (IPC Science & Technology Press, Guildford, UK), 15-26. Aveston J, Mercer RA and Sillwood JM, 1974, Proc NPL Conference on Composites - Standards, Testing and Design, (IPC Science & Technology Press, Guildford, UK), 93-102. Aveston J and Kelly A, 1979, Proc Roy Soc (Lond), A366, 599-623. Aveston J, Kelly A and Sillwood JM, 1980, Proc. ICCM3 (Paris) Advances in Composite Materials vol.1, (Pergamon, Oxford), Azzi VD and Tsai SW, 1965, Exp Mechanics, 5, 283-288. Bader MG, 1988, Sci & Engg of Compos Mater, 1, 1-11. Bailey JE, Curtis PT and Parvizi A, 1979, Proc Roy Soc, A366, 599-623. Barbero EJ, 1998, J Compos Mater, 32, 483-502. Berg JS and Adams DF, 1989, J Compos Technol & Research, 11, 41-46. Bowyer WH and Bader MG, 1972, J Mater Sci, 7, 1315-1321. Broutman LJ, 1967, Modern Composite Materials (Editors LJ Broutman and RH Krock), (Addison-Wesley Reading Mass), 391 et seq. Budiansky B, Hutchinson and JW, Evans AG, 1986, J Mech Phys Solids, 34, 167-189. Bunsell AR and Harris B, 1976, Proc ICCM1: First Int Conference on Composite Materials (editors E Scala E Anderson, I Toth and BR Noton), (AIME New York), 174-190. Chamis CC and Sinclair JH, 1977, Exper Mechanics, 17, 339-346. Chen EJH and Young JC, 1991, Compos Sci & Technol, 42, 189-206. Cooper GA and Kelly A, 1969, Interfaces in Composites STP 452, (American Society for Testing and Materials, Philadelphia, USA), 90-106. Corten HT, 1968, in Fundamental Aspects of Fibre Reinforced Plastics (edited by RT Schwartz and HS Schwartz), (Wiley/Interscience, New York), 89-128. Cottrell AH, 1964, The Mechanical Properties of Matter, (John Wiley and Son, NY). Curtis PT and Morton J, 1982, The effect of fibre surface treatment on the compressive strength of CFRP laminates (RAE Technical Report 82047), (Ministry of Defence Procurement Executive, UK). Curtis PT, 1986, Compos Sci & Technol, 27, 63-86. Davidge RW, 1979, Mechanical Behaviour of Ceramics, (Cambridge University Press, Cambridge). Davies GAO and Zhang X, 1995, Int J Impact Engng, 16, 149-170. de Ferran EM and Harris B, 1970, J Compos Mater, 4, 62-72. Dickson RF, 1980, The Strength of Fibre Bundles, (unpublished results, School of Materials Science, University of Bath). DiFrancia C, Ward TC and Claus RO, 1996, Composites, A27, 597-612. Dransfield K, Baillie C and Mai YW, 1994, Compos Sci & Technol, 50, 305-317. Drzal LT, Rich MJ and Lloyd P, 1982, J Adhesion, 16, 1-30. Eckold GC, Leadbetter D, Soden PD and Griggs PR, 1978, Composites, 9, 243-246.
chapter four Strength 97 Ewins PD and Ham AH, 1973, The nature of compressive failure in unidirectional CFRP (Technical Report 73057), (Ministry of Defence Procurement Executive, UK). Feillard P, Désarmot G and Favre JP, 1994, Compos Sci & Technol, 50, 265-279. Fukuda H and Kawata K, 1977, Fibre Sci and Technol, 10, 53-63. Galiotis C, Young RJ, Yeung P and Batchelder DN, 1984, J Mater Sci, 19, 3640-3684, Galiotis C, 1991, Compos Sci & Technol, 42, 125-150. Gao YC, Mai YW and Cotterell B, 1988, Zeit für Angewandte Math und Phys, 39, 550-572. Ghaseminejhad MN and Parvizi-Majidi A, 1990, Composites, 21, 155-168. Guild FJ, Harris B and Wills AJ, 1982, J Acoustic Emission, 1, 244-250. Guild FJ, Hogg PJ and Prichard JC, 1993, Composites, 24, 333-339. Hancock P and Cuthbertson RC, 1970, J Mater Sci, 5, 762-768. Hardiman SJ, 1997, Unpublished results, School of Materials Science, University of Bath. Harris B and Cawthorne D, 1974, Plastics and Polymers, 42, 209-216. Harris B and Ramani SV, 1975, J Mater Sci, 10, 83-93. Harris B, Guild FJ and Brown CR, 1979, J Phys D: Applied Phys, 12, 1385-1407. Harris B, Braddell OG, Lefebvre C and Verbist J, 1992a, Plast Rubb & Compos: Processing & Applic, 18, 221-240. Harris B, Habib FA and Cooke RG, 1992b, Proc Roy Soc (Lond), A437, 109-131. Hart-Smith LJ, 1991, in Proceedings of a meeting on Failure of Polymeric Composite Structures: Mechanisms and Criteria for the Prediction of Performance, St Albans, UK, September 1991, (SERC/IMechE London), 19-31. Hart-Smith LJ, 1993, Aerospace Materials, 5 (part 2), 10-16. Hayashi T and Koyama K, 1971, Proc Int Conference on Mechanical Behaviour of Materials, Kyoto, Japan, (Japanese Society for Materials Science), vol. 5, 104-112. Herrera-Franco PJ and Drzal LT, 1992, Composites, 23, 2-27. Hill R, 1948, Proc Roy Soc (Lond), A193, 281-297. Ho H and Drzal LT, 1996, Composites, A27, 961-971. Hughes JD, Morley H and Jackson EE, 1980, J Phys D: Appl Phys, 13, 921-936. Iosipescu N, 1967, J Mater, 2, 537-566. Jamison RD, 1985, Compos Sci and Technol, 24, 83-99. Kelly A and Tyson WR, 1965, J Mech Phys Solids, 13, 329-350. Kies JA, 1962, Maximum strains in the resin of fibre-glass composites: Report 5752, (US Naval Research Laboratory). Lacroix T, Tilmans B, Keunings R, Desaeger M and Verpoest I, 1992, Compos Sci & Technol, 43, 379-387. Lager JR and June RR, 1969, J Compos Mater, 3, 28-56. Mandell JF, Chen JH and McGarry FJ, 1980, Adhesion & Adhesives, 1, 40-44. Manders PW and Bader MG, 1981, J Mater Sci, 16, 2246-2256. Marshall DB and Evans AG, 1985, J Amer Ceram Soc, 68, 225-231. Martinez GM, Piggott MR, Bainbridge DMR and Harris B, 1981, J Mater Sci, 16, 2831-2836. Miller B, Gaur U and Hirst DE, 1991, Compos Sci & Technol, 42, 207-219. Netravali AN, Topoleski LTT, Sachse WH and Phoenix SL, 1989, Compos Sci & Technol, 35, 13-29. Norris CB and McKinnon PF, 1946, US Forest Products Laboratory Report no. 1328, (US Forest Products Laboratory). Outwater JO and Murphy MC, 1969, Proc 24th Annual Tech Conference of Reinforced Plastics/Composites Institute of SPI, paper 11C. Owen MJ and Found MS, 1972, Solid/Solid Interfaces: Faraday Special Discussions no. 2, (Chemical Society London), 77-89. Pabiot J, 1971, Composite Materials: Conference proceedings number 63 (AGARD/NATO Neuilly Paris), paper 6.
chapter four Strength 98 Pagano NJ and Pipes RB, 1971, J Compos Mater, 5, 50-57. Parratt NJ and others, 1971, New Technology (May issue), (Department of Trade and Industry, London). Parratt NJ and Potter KD, 1980, in Advances in Composite Materials (Proc ICCM3), vol. 1 (editors AR Bunsell , C Bathias, A Martrenchar, D Menkes and G Verchery), (Pergamon, Oxford), 313-326. Parry TV and Wronski AS, 1982, J Mater Sci, 17, 893-900. Pierron F and Vautrin A, 1996, in Realising their Commercial Potential: Proc 7th European Conference on Composite Materials (ECCM7), (Woodhead Publishing, Abington, UK , and EACM, Bordeaux), vol 2 119-124. Pipes RB and Pagano NJ, 1970, J Compos Mater, 4, 538-548. Pitkethly MJ and Doble JB, 1989, in Proceedings of an International conference on Interfacial Phenomena in Composite Materials ‘89 (editor FR Jones), (Butterworths, London), 35-43, Puck A and Schneider W, 1969, Plastics & Polymers, 37, 33-34. Qiu YP and Schwartz P, 1993, Compos Sci & Technol, 48, 5-10. Rosen BW, 1965, Fibre Composite Materials: Proc ASM Conference, October 1964 (American Society for Metals, Ohio), 37-87. Stowell EZ and Liu TS, 1961, J Mech Phys Solids, 9, 242. Sun CT and Luo J, 1985, Compos Sci & Technol, 22, 121-134. Weibull W, 1951, J Appl Mech (Trans ASME), 73, 293-297. Zweben C, 1977, J Mater Sci, 12, 1325-1337.
5 FRACTURE AND TOUGHNESS OF COMPOSITES5.1 STRUCTURAL ASPECTS OF COMPOSITES FAILUREM any reinforced plastics consist of brittle fibres, such as glass or carbon, in a weak, brittle polymer matrix, such as epoxy or polyester resin. An important characteristic of these composites, however, is that they are surprisingly tough, largely as a result of their heterogeneous nature and construction. During deformation, micro-structural damage iswidespread throughout the composite, as we saw in chapter 4, but much damage can be sustained beforethe load-bearing ability is impaired. Beyond some critical level of damage, failure may occur by thepropagation of a crack which usually has a much more complex nature than cracks in homogeneousmaterials. Crack growth is inhibited by the presence of interfaces, both at the microstructural levelbetween fibres and matrix, and at the macroscopic level as planes of weakness between separate laminaein a multi-ply laminate. The fracturing of a composite therefore involves not only the breaking of theload-bearing fibres and the weak matrix, but a complex combination of crack deviations along theseweak interfaces. For similar reasons, even all-brittle ceramic/ceramic composites can also exhibittoughnesses which are orders of magnitude higher than those of unreinforced ceramics. The microstructural inhomogeneity and anisotropy of fibre composites are together responsible forthe fact that the fracture of these materials is rarely a simple process. Although the complex combinationof micro-failure events that leads to deterioration of load-bearing ability, or to destruction, can often giverise to surprisingly high levels of toughness, the same complexity makes it difficult or impossible to useprocedures based on fracture mechanics for design purposes. There have been many theoretical andexperimental studies of cracking in composites and of the mechanisms by which toughening is achieved,but there is still a large measure of disagreement about the contributions to the overall toughness of thevarious processes by which cracks are stopped or hindered. This is probably because of the greatdiversity of composite types that have been studied. The toughness of a composite is derived from manysources, and the relative magnitudes of the separate contributions depend not only on the characteristicsof the components, but also on the manner in which they interact. There is thus no simple recipe forpredicting the toughness of all composites. The lay-up geometry of a composite strongly affects crackpropagation, with the result that some laminates appear to be highly notch-sensitive whereas others aretotally insensitive to the presence of stress concentrators. The selection of resins and fibres, the mannerin which they are combined in the lay-up, and the quality of the manufactured composite must all becarefully controlled if optimum toughness is to be achieved. Furthermore, materials requirements forhighest tensile and shear strengths of laminates are sometimes incompatible with requirements forhighest toughness. Final selection of a composite for a given application is often therefore a matter ofcompromise. In this chapter we examine the cracking of a composite at various structural levels. We begin byconsidering how the behaviour of a crack in the matrix phase is modified by the presence of reinforcingfilaments and how the mechanical characteristics of the fibres themselves affect cracking of thecomposite. These effects are distinct from those related to true composite action in which it is theinterfacial discontinuity between fibres and matrix that controls crack propagation. At the macroscopiclevel there are other discontinuities, the interfaces between laminae for example, or the resin-rich zonesaround the boundaries of fibre tows, and these discontinuities also affect crack growth.5.1.1 Fracture formalisms The Griffith model of fracture of cracked brittle solids (1920) has had far reaching consequences fordesigners, specifically in having laid the foundations of modern fracture mechanics as couched in termsof the familiar stress-based stress-intensity factor, K, and the associated energy-based parameter, G, thestrain-energy release rate. With appropriate modifications to the basic concepts and definitions ofGriffith (see, for example, Atkins and Mai, 1985; Broek, 1986), we arrive at design methods that canreasonably account for modest levels of non-linear, inelastic behaviour in a variety of homogeneous
chapter five Toughness 100brittle and semi-brittle materials — ceramics, metals, and even plastics. It was natural, therefore, thatmany attempts should have been made to apply the same concepts to fibre composites in order to obtaindesign data that could be directly compared with those already in use for conventional engineeringmaterials. And, despite the limitations imposed by the microstructural complexity of composites, by thescale of those structural features relative to the crack geometry, and by the distributed patterns ofdamage, there has been a measure of success. However, it is now apparent that the stress-intensity factoris not an appropriate design parameter for use with fibre composites, except for situations where adelamination crack spreads between the plies of a conventional laminate (see Hashemi et al, 1990, forexample). The stress approach is dubious because it is unable to account for mechanistic input in the way thatan energy-based approach can, and perhaps the most successful early studies of composite toughnesshave been those based on the Orowan fracture-energy development of the Griffith model (see McGarryand Mandell, 1972, and Phillips, 1972, for example). Measurements of the fracture energy, or work offracture, γF, provided information which related in a fairly obvious way to the observed fractureprocesses, permitted comparisons of the performance of different materials, and encouraged deductionsto be made as to the likely effects of materials/processing parameters on the behaviour of a givencomposite system. Unfortunately, although some early attempts to correlate γF with the conventionalfracture toughness parameters were moderately successful, γF cannot be thought of as a design parameteralthough it fulfils an important rôle in furthering our understanding of composites fracture processes.The fracture energy idea has also led to the development of the concept of crack-resistance curves (Rcurves) which have particular relevance to materials like composites where sub-critical cracking andprogressive failure are common features (Gurney and Hunt, 1967; Mai et al, 1976). In this book, in orderto preserve the analogy with the Griffith surface energy, γS, we define γF as the total energy absorbedduring the complete failure process divided by twice the sample cross-sectional area: it is thus half thevalue of R or G, as usually defined.5.2 FRACTURE PROCESSES IN COMPOSITES As a starting point, we take the simple, Griffith planar-crack model and the knowledge that duringcrack extension an irreversible process takes place in which the net change in the stored elastic energy ofthe whole system (testing machine plus sample) caused by an increment of crack growth serves toprovide the energy, γS, needed to produce new surfaces plus the energy, γF, required to activate any otherdeformation or damage mechanism that must operate in order for the crack to grow. The second of thesecontributions is minute in bulk glass where crack-tip plastic deformation is very limited (though still anorder of magnitude greater than γS,) but is much greater in metallic or polymeric solids where extensiveplastic or viscoelastic deformation may lead to the development of a sizeable plastic zone ahead of thecrack. This concept of a ‘process’ zone near the crack tip in which we encounter a variety of deformation orfailure events all drawing on the energy of the system is familiar in ceramics where the events inquestion may include a distribution of subcritical micro-cracks, crack deviation, and crack blunting.Ceramic composites are designed to add other, perhaps more effective, damage mechanisms. Anexample of a particulate ceramic composite is the family of partially stabilized zirconias, or PSZmaterials which, on account of their improved intrinsic toughness, may provide a better starting point asa matrix for subsequent fibre reinforcement in CMCs (Evans et al, 1981; Garvie, 1985).5.2.1 Matrix effects In practical fibre composites the proportion of fibres present will vary between about 10% (in DMCs,for example) and 70% (in high-performance CFRP). Crack-resistance effects directly attributable to thematrix material may not therefore be significant except perhaps in composites reinforced with relativelylow volume fractions of short fibres. Three specific matrix effects might be listed, however: i) The effective toughness of a non-brittle matrix, such as a metal or thermoplastic, will be reduced by the presence of a high Vf of rigid, brittle fibres or particles as a result of plastic
chapter five Toughness 101 constraint which leads to triaxial tensile stress components in the matrix. A cermet, or metal- bonded ceramic, is a good example of this. ii) The effective toughness of a soft, flexible matrix may be increased by the presence of a low Vf of rigid particles or fibres because a high overall stress level on the composite may then be required to generate a critical degree of crack opening in the stiffened matrix (Harris, 1980). iii) The effective toughness of a low-toughness matrix may be increased by the presence of fibres or particles as a result of the slowing up of cracks in the neighbourhood of the filler. The toughness of certain brittle plastics for example, shows a strong dependence on the crack speed, often linked to changes in the crack face roughness — the slower the crack, the rougher the crack face and the higher the associated work of fracture (Harris, 1980).5.2.2 Fibre effects Certain types of fibres such as the drawn steel wires used for reinforcing concrete, the polyestertextile fibres used to reinforce rubber tyres, or the aromatic polyamide fibres used in high-performancelaminates, may be classified as ‘tough’ because they are capable of extensive non-elastic deformationafter yielding. Familiar mechanisms of deformation in such fibres are plastic necking in metal wires anddrawing or inter-fibrillar splitting in polymer fibres. Such fibres often show high tolerance of detects andsurface damage, by contrast with brittle fibres like glass or carbon. A bundle of such fibres possesses alarge fracture energy, and a substantial portion of this fracture energy can be transferred into a compositecontaining the bundle. Fibres such as glass, carbon and boron, whichhave high breaking strengths and failure strains(when undamaged) have very low intrinsicfracture energies, of the order of only 10-100Jm-2, and their failure is governed by thestatistical nature of flaw distributions. These lowfracture energies make no direct usefulcontribution to the composite work of fracture,even though each fibre may break many times(multiple cracking). But as a result of thismultiple cracking, damage is widespread, crackpaths in composites become complex, and it isthis that results in very high values of the work Figure 5.1. Schematic illustration of the way in which fibresof fracture. in a plastically deforming metal-matrix composite constrain the plastic deformation of the matrix.5.2.3 Simple fibre/matrix addition effects When fibres are incorporated into a matrix of any kind the separate phases may be able to contributetheir individual levels of toughness to the composite in an additive fashion, or they may not, dependingon the kind of interaction that occurs and on the level of constraint that is set up as a result of thedifferences in their properties. Early studies (Cooper and Kelly, 1969; McGuire and Harris, 1974) ofmetal-matrix composites in which the reinforcements were also metallic, showed that the specificfracture energy of the composite, (γF)c, could be obtained as a mixture-rule sum of the fracture energiesof the individual components: (γF)c = (γF)m(1 – Vf) + (γF)fVf ...............................................................................[5.1]where the subscripts c, m and f refer, as usual, to the composite, matrix and fibres, provided account wastaken of the fact that the presence of the stiffer fibres caused the extent of matrix plastic deformation tobe localized in the neighbourhood of the crack plane. Typically, a metal filament like tungsten or cold-drawn steel undergoes plastic deformation which is concentrated within a volume of the order of onefibre diameter, d, in height on either side of the final break, as illustrated schematically in Figure 5.1. Ifthe fibre failure stress and strain are σfu and εfu, respectively, the fibre fracture energy is therefore
chapter five Toughness 102roughly equal to 2d.σfuεfu.πd2/4 per fibre, which amounts to 2dVf σfuεfu for the total fibre contribution.The matrix contribution is likewise obtained from the stress/strain product for the matrix, σmuεmu, and thedeforming volume which is determined by the geometry of fibre/matrix distribution and the size of thedeformation zone in the fibre. An estimate of this component (Cooper and Kelly, op cit) gives d(1 –Vf)2Vf–1σmuεmu, and the total work of fracture for the composite is then: (γF)c = 2dVf σfuεfu + d(1 – Vf)2Vf–1σmuεmu, ............................................................... [5.2] The terms in d and Vf modify the plastic work terms (stress x strain) to take into account thelocalization of the plastic deformation. Both matrix and fibres are subject to large local deformation, anddebonding may also occur. This decohesion relaxes some of the triaxiality that would otherwise prevail at the interface. Failure to debond would cause conditions approaching plane strain throughout the composite and failure surfaces would have the appearance of a flat brittle-looking failure rather than the tougher, pseudo-plane-stress tensile failure of the locally separated components shown in Figure 5.2. There is also evidence that the strain to failure of a metal wire embedded with good wetting in a ductile metal matrix is rather higher than that of an identical isolated wire, perhaps because a strong fibre/matrix bond delays the onset of localized necking in the fibre. Estimates given by equation 5.2 are in reasonable agreement with measured values in composites where the interfacial bond is not very strong so that decohesion is able to occur and the two components can deform in an unconstrained fashion. Modern composites rarely contain metallic reinforcements, however, and the more usual situation is that the stiffness Figure 5.2. Tensile failure surface of a ratio, Ef/Em, is very high. This reduces the deforming volumetungsten-wire/aluminium composite, showing plastic deformation of both fibres and matrix of even a highly deformable matrix and limits the extent to (McGuire, 1972) which it can contribute its plastic work to the toughness of the composite. When we consider that a composite such as aGRP, in which both fibres and matrix are brittle (with fracture energies of the order of 0.5 and 100Jm-2,respectively), may exhibit a work of fracture of the order of 105Jm-2, it is clear that estimates based onthe intrinsic toughnesses of the components have no relevance to real behaviour. It is in the specialnature of composite action that the behaviour of individual components is dramatically modified; newdamage mechanisms are introduced which drain energy from the system and in doing so contribute tothe composite toughness, or crack-growth resistance. This is one reason for the success of GRP and otherhigh-performance reinforced plastics, and it is the driving force for the intensive search for toughness inceramic-matrix composites.5.3 TOUGHNESS DERIVING FROM COMPOSITE ACTION5.3.1 Toughening mechanisms in fibre-reinforced plastics We have seen, for a simple case, how estimates of the energy required for deformation mechanismsassociated with the matrix and fibres provide reasonable models of macroscopic toughness. In real fibrecomposites, however, the microstructural inhomogeneity and anisotropy cause the failure process to bevery complex, and the combination of microfailure events — sometimes interacting, sometimes not —that leads ultimately to ‘destruction’ can often give rise to high levels of fracture energy. We should beclear that by using the γF definition of toughness we are begging a number of questions. The engineerused to dealing with K or G will usually be interested only in events up to maximum load. Unlikemetals, most high-performance composites do not exhibit work-hardening phenomena and the load-bearing ability of a component may fall quite rapidly after peak load, even though the deteriorationprocess may be gradual, and much energy may be required to complete the destruction process, asillustrated schematically in Figure 5.3. Such a composite would have a high work of fracture, and be
chapter five Toughness 103 valuable for many applications where energy absorption rather than load- bearing ability (or strength) is called for. There are also composites in which, as in plastically deforming metals, a process zone develops and increases in size as a single crack grows and the ‘toughness’, now defined as a crack- growth resistance, R, increases. Low-energy failures of the kind implied by a rule-of-mixtures equation (5.1) for a brittle/brittle composite rarely occur in modern engineering laminates Figure 5.3. Schematic stress/strain curves illustrating different except, for example, in certain types of classes of brittle/tough behaviour. GRP under the combined action of stress and an aggressive environment (stress corrosion, as in Figure 5.4, for example), although it was a common feature of early CFRP in which the commercial fibre surfaces were often over-treated. Such failures are rare, partly because the interface will usually modify the mode of crack propagation and partly because of the statistical variation of fibre strengths. At any fibre break the load is shed back, via the matrix, to the neighbouring fibres, so that the stresses in these adjacent fibres will be concentrated somewhat above the average fibre stress level, as illustrated by Figure 4.8 in chapter 4. It is statistically unlikely, however, that there will be weak spots at the same points in these neighbouring unbroken fibres, and in the early stages of deformation fibre failures are widely distributed throughout the stressed volume. If the fibre/matrix bond is not too strong some relaxation of the stresses around the broken fibre ends can occur and this, together with local creep relaxation in the matrix, will help to reduce Figure 5.4. Brittle fibre-to-fibre failure in a high- the level of stress concentration in neighbouring fibres.performance GRP pultruded rod exposed to stress- corrosion conditions in dilute hydrochloric acid Thus, in many modern composites a great deal of fibre solution. damage may occur before the number of fibre breaks in any cross-section reduces the load-bearing ability of that cross-section below the current level of applied load. At this point we have, effectively, a crack nucleus of critical size which could propagate rapidly to cause failure of the composite, and the simple cross- section argument should be modified to include the effect of the crack-tip stress concentration. If the fibre/matrix bond is too strong, however, this prevents relaxation, so that failure of whole bundles of fibres can occur, the crack spreading from one fibre to the next via the matrix with little or no deviation at the interface, in the brittle mode described earlier. A detailed study of tensile failure due to inter-fibre stress transfer within the axial plies of notched laminates has been made by Potter (1978). Practical fibre-reinforced plastics consist of relatively brittle resins (γF values of a few hundred to a few thousand Jm-2) reinforced with strong, brittle fibres which may be very stiff (eg. carbon) or less stiff (eg. glass or aramid polymers). The failure strains of these fibres are generally less than that of the matrix. The fibres may be continuous and straight, continuous and woven, or chopped and randomly dispersed. When a continuously reinforced composite laminate is loaded, the weaker fibres in the distribution begin to break at relatively low loads, and this damage is distributed throughout the material, as illustrated in chapter 4. A brittle fibre fracture is a process which requires an amount of energy ½σfu εfu per unit volume. If we allow all of the fibres in a 0.7Vf carbon-fibre composite to break once, with a deforming volume of the order of d3, their net contribution to the composite fracture energy can only be of the order of 1Jm-2. Because of the statistical distribution of fibre strengths, each fibre may break many times before the composite fails, but even if, in a 10cm long sample, say, each fibre could be
chapter five Toughness 104completely broken down to pieces of nearcritical length (about 0.5mm in a CFRP), thetotal available fracture work from this sourcestill amounts to only a few hundred Jm-2. In order to distinguish the separate micro-mechanisms of toughening it is convenient toconsider a rather artificial model in which a elastic straincrack travelling in the matrix approaches an in fibreisolated fibre (Figure 5.5).The crack iseffectively halted by the fibre (picture b), first,because the higher stiffness of the fibre inhibitsfurther opening of the matrix crack, and second,because the strength of the fibre is too high topermit of its being broken by the level of stresscurrently concentrated at the tip of the matrixcrack. Further crack opening may occur if thelocal shearing force acting at the fibre/matrix Figure 5.5. Schematic illustration of the stages in crackinterface is sufficiently high to allow the fibre to growth in a fibre composite (see text for explanation).become locally debonded. This debonding isalso encouraged by the fact that there may be a significant level of transverse tensile stress concentrationahead of the crack tip, parallel with the crack plane, as shown by the work of Cook and Gordon (1964). The overall consequence is that debonding may occur, the debonded fibre will extend elastically, andsubsequent further crack opening can take place during which the matrix slides relative to the fibre(stage c): all of these processes require energy. The crack may progress past a number of fibres in this 3 way, leaving them unbroken in its wake and for fibres: a given fibre/matrix/interface system there may be some equilibrium state where a stable spacing = 5mm number of these bridging fibres continue to K, MPa.√m 2 support part of the load, modifying the thermodynamic driving force for crack growth. This fibre bridging is thus a further toughening mechanism. Its effect is illustrated in Figure 1 5.6. These are results of a simple double- plain resin cantilever beam (DCB) experiment on a polyester resin sample containing a single array of glass fibres spaced as indicated in the figure 0 0 50 100 150 200 (Harris and Ankara, 1978). The crack propagates through the array, and the unbroken Crack length, mm fibres behind the crack tip provide a closure force which opposes the applied stress, so Figure 5.6. Plot of K against crack length during a test on a double-cantilever beam sample of polyester resin containing reducing the driving force for crack growth, an a linear array of glass fibres 5mm apart (Harris and Ankara, idea proposed very early on by Romualdi and 1978). Batson (1963) for the toughening effect in fibre-reinforced cement. The apparenttoughness is defined in the graph in terms of a notional ‘stress-intensity factor’, K = σ√a, a being thelength of the crack, and σ the applied stress.
chapter five Toughness 105 Figure 5.7. Photographs of fibre pull-out in a carbon-fibre-reinforced epoxy composite (right) and a SiC-fibre-reinforced glass-ceramic. The magnifications may be judged from the fibre diameters, carbon 7μm and SiC 15μm The extent of this increase in crack resistance as the crack extends, which is commonly termed ‘R-curve behaviour’, may be limited or extensive, depending on the material. At some point, however, therising load on a bridging fibre must reach a level at which the fibre will break (stage d in Figure 5.5).During loading, the fibre will have been released by Poisson contraction from contact with the matrixover a debonded length that will depend on the interfacial bond strength, and a weak spot may beencountered anywhere within this length (or just outside it, where contact and frictional grip is being re-established). When the fibre failure occurs away from the crack plane, the stored elastic energy isreleased and the fibre expands to regain contact with the matrix. Many of the broken fibres will thereforeremain bridging the crack, and the embedded ends must be pulled out of the matrix holes in order forfurther crack opening to occur (stage e). This fibre ‘pull-out’ makes further demands on the energy ofthe system, and leads to the characteristic brush-like failures of many types of composite, as shown inFigure 5.7. Since the earliest years of research on fracture-energy mechanisms in composites, there havebeen strong disagreements about the major contributing factors. McGarry and Mandell (1972), forexample, were categoric that the primary source of toughening in glass-fibre/resin composites was thework necessary to break the fibres in a damage zone at the crack tip, and that contributions from thematrix toughness, fibre debonding or splitting, and fibre pull-out were negligible. Outwater and Murphy(1969) were equally convinced that it was the debonding process that was the major contributor, whileother researchers believe that fibre pull-out is dominant (Harris et al, 1975). The truth is not easy tounravel, especially when several mechanisms, which may be inter-dependent, may be making similarcontributions, and it is in any event clear that different situations occur in different kinds of composites.We now examine the major mechanisms in a little more detail in order to see how simple energyconsiderations may offer guidance in designing composite materials.22.214.171.124 Fibre/resin debonding Glass fibres are coated prior to incorporation in the resin matrix with a complex mixture that includesa coupling agent, usually an organo-silane, the purpose of which is to encourage wetting and theestablishment of a direct chemical bond between the glass surface and the resin molecular network. Nosuch direct bond can easily be produced between a carbon fibre and the resin, so that the coating whichis put on carbon fibres is merely a size which assists handling and encourages wetting-out duringcomposite manufacture. However, carbon-fibre surfaces are also usually treated, by chemical,electrochemical, or plasma methods, to modify their surface chemistry and so further enhance wetting.Depending on the type of fibre, then, and the type and level of coating or surface treatment, the degree ofactual chemical bonding between fibre and resin and the efficacy of any purely physical bond may varyimmensely from system to system. There is uncertainty about the exact nature of the interface infibre/resin composites (Drzal et al, 1982, 1983; Kardos, 1985) and in this discussion of debonding weshall therefore adopt a very simple approach.
chapter five Toughness 106 As discussed in section 4.3.1, when the end of afibre, of length less than half the critical transferlength, lc, which is embedded in a block of curedresin, is loaded by pulling (Figure 5.8a), the loadincreases to some maximum level at which theinduced shear forces acting at the interface are ableto initiate a debond and the load drops to some lowerlevel as the debond rapidly propagates. The peakload must reflect the strength of the combinedchemical and physical bond, and the shadedtriangular area on the diagram in Figure 5.8brepresents the elastic energy that was needed tocause the debond, ie. the debond energy. The fibre isnot free, however, because the cured resin has Figure 5.8. A simple pull-out experiment. As theshrunk onto the fibre during the curing process and embedded fibre is loaded (a), the resultingduring cooling from the cure temperature. As a load/deflexion curve frequently resembles that shownconsequence, further work is needed to withdraw the in (b).fibre completely from the resin block, and the fullloading curve is as shown in Figure 5.8b. The magnitude of the debonding energy can be roughly assessed (Harris et al, 1975) by assumingthat it is equivalent to the energy released when the fibre finally breaks. If a fibre debonds to a totaldistance ½ldb on either side of the crack face, the stored elastic energy released at fibre fracture is likelyto be somewhat greater than ½(σ2fu /Ef).(πd2/4).ldb. If N fibres break in the cross section of thecomposite, the debonding contribution to the composite fracture work, wdb, normalized with respect tothe sample cross-sectional area, 2A, is: w db Nπd2σ2 l db .................................................................................................[5.3] = fu 2A 16AEfand since the fibre volume fraction Vf = Nπd2/4A, we obtain the debond component of the work offracture: Vf σfu l db ..............................................................................................[5.4] 2 (γ F )debond = 4EfThis is an under-estimate, since it assumes that the fibre/resin interfacial shear strength falls to zero afterdebonding and that the fibre is not strained outside the debonded region, neither of which is likely to bevalid. In their early attempt to assess the work of debonding, Outwater and Murphy (1969) treated theproblem as a fracture-mechanics case of the propagation of a mode-II shear crack along a cylindricalinterface. For a long fibre of diameter d embedded in a block of matrix, as in Figure 5.8a, and debondedover a distance x from the surface, the stress needed to continue the debonding process is given by: 4 τx 8E f GIIi σ fu = + ........................................................................................[5.5] d dwhere τ is the sliding friction stress operating between fibre and matrix in the region already debonded,and the second term is the energy required to break the bond, GIIi being the fracture surface energy of theinterface in shear. The condition for the start of debonding is given, when τ = 0, as:
chapter five Toughness 107 8E f GIIi σ fu = .....................................................................................................[5.6] d It is evident that there is a limiting fibre diameter, 8EfGIIi/σ2fu, equivalent to equation 5.3 modified soas to relate to the debonded surface area of the fibre, above which the fibres will break before they candebond. In such circumstances a crack would propagate cleanly through fibres and matrix, with nodeviation, resulting in a flat fracture face, such as that shown in Figure 5.9, and a very low fractureenergy. Such a situation could occur if the fibre/matrixbond were excessively strong, and fibre surfacetreatments therefore need to be carefully controlled sothat they are neither too weak (low G → low compositetoughness) nor too strong (no debonding → lowtoughness). The interface would be likely to have afracture energy intermediate between that for a resinfracture and that for the failure of a glass/resin adhesivebond, say a few hundred Jm-2. But Outwater and Murphymeasured values of about 4kJm-2 for GIIi forglass/polyester models, which suggests that simplemode-II cracking is not occurring during the debondingprocess. Kelly (1970) considered the debonding energyto be small, although more recent work by Wells and Figure 5.9. Flat surface topography of a typical brittleBeaumont (1985) suggests that it could be a major composite fracture. The material is a unidirectionalcontributor to toughening. carbon/epoxy composite containing plasma-treated fibres. The effect of debonding is to permit a large increasein the volume of fibre that is under stress and, therefore, the amount of stored elastic energy that issubsequently released when the fibre fails. Harris (1980) suggested that it may well be this consequenceof debonding rather than the debonding itself that adds substantially to the composite fracture energy. Ithas also been suggested that in glass/polyester model composites the overall fracture energy is relativelylittle affected by the ease or difficulty of debonding (Harris and Ankara, 1978), presumably because thearea under the tail of the load/deflexion curve in Figure 5.8b is usually substantially greater than that inthe debonding triangle indicated.126.96.36.199 Frictional work following debonding As implied by equation 5.5, after debonding has taken place the fibres and matrix move relative toeach other as crack opening continues, and work must be done against frictional resistance during theprocess. The magnitude of this work is hard to evaluate because we do not know with any certainty whatlevel of friction force is operating. The work expended will result from the action of the interfacialfrictional force over a distance equal to the differential displacement of fibre and resin which Kelly(1970) suggested was roughly the product of the debonded length and the differential failure strain,ldbΔε. In early composites, the matrix failure strains were usually much less than those of the fibres, andΔε could be taken as being approximately equal to εfu. If the initial friction force, τi πd.½ldb, acts in eachdirection from the crack face over a distance ½εfu ldb, the post-debond friction work is (Harris et al,1975): ⎛ 2τ πdl db ⎞⎛ ε ful db ⎞ .................................................................................[5.7] w pdb = ⎜ i ⎟⎜ 2 ⎟ ⎝ 2 ⎠⎝ ⎠per fibre. Normalizing again with respect to the sample cross-sectional area, the contribution to the workof fracture is therefore: Nτi πdl 2 ε fu ( γ F )post −debond = db ..............................................................................[5.8] 4A
chapter five Toughness 108for N fibres in the cross-section, and again converting to Vf, we have: Vf τil2 εfu ( γF )post−debond = db ..................................................................................... [5.9] dSubstituting reasonable values for the parameters (Vf = 0.6, τi = 40MPa, ldb ≈ 10d to 50d, d = 7μm, andεfu ≈ 1.5%), the contribution varies between 250Jm-2 to 6.3kJm-2. For modern fibre/resin combinationswith toughened resins, the resin failure strain may well be much closer to that of the fibre, and the netcontribution to toughening from this source would then become almost insignificant. It is interesting tonote that Marston et al (1974) had some success in attempting to account for the fracture energies ofvarious types of composite by associating the surface energy of the debonded interface with the actualdebonded surface area. They generalized the Outwater debonding model and showed how interfacialshear strength might be tailored to obtain reasonable levels of toughness while maintaining rule-of-mixtures strengths in boron/epoxy and carbon/epoxy composites.188.8.131.52 Fibre pull-out The pull-out work has long been considered to be of great significance in providing toughness incomposites, and the earliest solutions were given by Cottrell (1964) and Kelly (1973). When a fibre endof length x is pulled from the matrix, the effective friction force, τi πd(x/2), acts over the distance x to dowork ½τiπdx2. Since x is normally considered to vary between 0 and ½lc (where lc is the critical fibrelength), the mean work done in pulling N fibres out to a maximum distance ½lc over the composite crosssection is: lc / 2 ∫ x 2dx w pull−out = 1 2 Nπdτi 0 .............................................................................. [5.10] lc / 2 ∫ 0 dxThe pull-out contribution to the work of fracture is then: Nτi πdl 2 Vf τil 2 ( γF )pull−out = c = c ............................................................................[5.11] 48A 12dThe relationship given in section 4.1.9 of chapter 4: l c σfu = d 2τibetween fibre strength, σfu, effective interfacial bond strength, τi, fibre critical length, lc, and fibrediameter, d, which was derived by Kelly and Tyson (1965) for metallic composites without interfacialchemical bonding, may be used to write equation 5.11 in slightly different form: Vf σ fu l c ( γ F ) pull − out = .........................................................................................[5.12] 24 For typical values (Vf = 0.6, σfu = 3GPa, lc ≈ 10d to 50d), this amounts to between 5 and 25kJm-2,clearly a potentially powerful source of toughening. We see from equations 5.11 and 5.12 that control ofthe interface characteristics in a composite of given fibre/matrix composition is vitally important indesigning toughness into a system. An illustration is shown in the results of some crack growthexperiments of the kind referred to earlier (cf. Figure 5.6) in which the surfaces of glass fibres weretreated in various ways prior to embedding in polyester DCB samples. The curves in Figure 5.11 againshow the increase in apparent toughness as a crack passes through an array of fibres (R curves), and it
chapter five Toughness 109 can be seen the results are not entirely in accord with conventional ideas. It is true that all of the fibre- containing samples develop crack resistances greater than that of the plain resin. But the toughening effect is considerably greater when the fibre surfaces are pristine than when they are coated with a silane coupling agent, applied in practice to improve the fibre/matrix bond, and the highest toughness is obtained with a fibres that have been damaged by environmental contamination prior to embedment in the resin. 3 The parameters σfu, τi and lc are not damaged fibres independent, and there are limits to the extent to clean fibres which the interfacial bond strength and the pull- silane-coated out length (which is related to lc) can be varied. ItKeff, MPa√m 2 fibres has been shown, for example, that as the fibre/resin bond strength is gradually increased by fibre surface treatments, the work of fracture first increases and then decreases as the initial 1 improvement with increasing τi is replaced by a plain resin deterioration as lc becomes very small. This is illustrated in Figure 5.10 by some early results for 0 carbon/polyester composites in which the fibres 0 5 10 15 have been exposed to a range of chemical Crack length, cm treatments which have modified the strength of the interfacial bond. The effects of those treatments Figure 5.11. Notional stress-intensity factor, Keff, as a are also reflected in changes in the interlaminarfunction of crack length for plain polyester resin and three shear strength of the composite (qv, chapter 4), and composite samples (DCBs) containing glass fibres with this property is used as the abscissa in the graph. different surface treatments (Harris et al, 1975). Early commercial fibre surface treatments were sometimes carried to excess in the drive to raise the composite shear resistance, with the consequence that many brittle structural failures were encountered (the datum point at the extreme right of the graph was for a commercial treatment). Modern treatments are designed to optimize strength and toughness. Beaumont and Phillips (1972) showed very early on that in carbon-fibre-reinforced plastics, untreated fibres produced composites that were notch- insensitive, whereas treated fibres, especially the somewhat over-treated fibres of that time, led to notch sensitivity. There have been many studies of the effects of interface control in modifying the toughness of composites, and it has often been observed that attempts to improve the work of fracture (as opposed to the notional fracture-mechanics KC value) often resulted in a reduction in strength. Atkins (1974) 50 showed, however, that if reinforcing filaments were treatments to γF ∝ (τi)-1 Work of fracture, γF , kJm -2 made to have random alternating sections of high 40 increase bonding and low interfacial bond strength (giving locally silicone oil to reduce bonding low and high interfacial toughness) a desirable 30 combination of strength and toughness could still be untreated achieved. The strongly bonded regions ensured that 20 fibre the fibre strength could be utilized and the weakly bonded regions, randomly arranged in the paths of untreated fibre, 10 composite exposed running cracks, provided the source of debonding to steam and pull-out energy. In fact, it was possible to 0 achieve fracture energies of the order of 300kJm-2 in 0 0.02 0.04 0.06 0.08 0.10 0.12 0.14 boron/epoxy composites containing ‘barber’s pole’ Reciprocal ILSS, m2 MN-1 release-agent coatings without loss of strength relative to composites with uncoated fibres. Figure 5.10. Effect of fibre surface treatments in modifying the work of fracture and the interlaminar shear strength of carbon-fibre/polyester composites The simple models for debonding and pull-out (Harris et al, 1971) described above both make the incorrect assumption that the fibre strength has a unique
chapter five Toughness 110value, σfu, having been originally derived, like many of the early theoretical studies of compositesbehaviour, for metal-fibre/metal-matrix systems. Wells and Beaumont (1985) and Thouless and Evans(1988) have recognized that the statistical distribution of fibre strengths must be taken into account inattempting to determine the location of a fibre failure (and hence the pull-out length) and its relationshipwith the fibre, matrix and interface properties. In a composite containing fibres at angles to apropagating crack, extra work may be needed to withdrawthe fibres (Harris and Ankara, 1978; Harris 1980; Helfet andHarris, 1972; Piggott, 1970 and 1974). The sources of thisextra work will depend on the constituents of the composite.Ductile or tough fibres, like metal wires or polymerfilaments, will be capable of deforming inelastically in order Figure 5.12. Model for the plastic shearingto follow the more complex pull-out path without breaking. during pull-out of a fibre lying at an angle to the crack plane.A metal filament that is capable of work-hardening, like asteel wire in concrete, may contribute a considerable level ofplastic deformation work to the overall composite toughness by being forced to deform first one way andthen another, as illustrated in Figure 5.12. Results of Morton and Groves (1974) support those of Helfetand Harris in demonstrating that a higher angle of misorientation leads to a higher pull-out stress. Theydeveloped plastic-hinge models to determine extra plastic work and showed that the pull-out force was amaximum at an angle, θ, of 45°. Piggott (1970, 1974) suggested that the apparent strength of brittle fibres would be reduced by thebending process, although the extent of the strength loss was smaller the softer (or more ductile) thematrix resin since the bending fibres can cause the matrix to yield at the corners formed by theintersections of the fibre holes and crack faces. However, in recent work Khatibzadeh and Piggott (1997)has carried out more detailed studies of the effect of loads applied at an angle, and has found that theapparent strength of brittle fibres is actually initially increased as the angle between fibres and crackplane increases. At larger angles, though, the combination of geometric effects and mechanical damageto the fibres will offset the gains described above and the overall work of pull-out will be reduced. For a brittle-fibre composite, Piggott (1974) 700 fibre spacing = 10mmproposed that the work of fracture of a compositecontaining fibres at an angle θ to the crack plane γF, Jm-2was given by: 600 plain resin value = 350Jm-2 (γF)θ = (γF)0(1 – Btan θ)............[5.13] 500where (γF)0 is the work of fracture of a composite K, MPa.√m 1.5with the fibres normal to the crack plane and the fibre spacing = 30mmparameter B, which is determined by the force 1.0exerted by the fibres on the matrix, is related to theratio of the matrix yield strength to the fibre 0.5tensile strength, τmy/σfu. For ductile fibres, the plain resin value = 0.5MPa.√mfracture work increases with increasing angle 0 0 10 20 30 40provided the breaking stress of the fibre is notexceeded. Some examples of the effect of fibre Angle between loading direction and fibres, θ oorientation for metallic and glass fibres in modelcomposites are shown in Figure 5.13. The results Figure 5.13. Effect of the angle, θ, between the fibrefor the steel-wire/PMMA composites are presented direction and the crack plane on the resistance to crackas work-of-fracture versus angle, while those for propagation for a) steel wires in PMMA, and b) glassthe glass/polyester, following the style of Figure fibres in polyester resin. The test samples were double cantilever beams with a single row of spaced fibres5.6, are given as K (= σ√c). It can be seen that for (Harris, 1980). The dashed curve in the lower plotboth cases the composite toughness first increases represents the Piggott model of equation 5.13, with (γF)0 =with θ and then falls as the angle increases. 1.16 and B = 0.78.
chapter five Toughness 111Although the Piggott model is for work of fracture rather than K, the data agree reasonably well withequation 5.13, as shown, with values of (γF)0 of 1.16 and B = 0.78. The disagreement at small anglesclearly relates to the issue of whether or not the apparent strength of the glass fibres increases for smalldeviations of alignment. 30 If the fibres are discontinuous, as in a DMC, forexample, the situation is changed since the length of Work of fracture, γF , kJm -2 25the fibre and its orientation may affect the pull-out w = 0.5lc2behaviour. In a composite containing aligned, short 20fibres with lengths shorter than lc, the toughness 15increases with increasing length since the fibrescannot be broken by the external forces and 10 w = 10 + 90/lincreasing their length increases the extent to which 5 aligned fibresthey can be pulled from the matrix. From equation random fibres5.11, it can be seen that the fracture work will be 0 0 5 lc 10 15 20 25 30proportional to the square of the fibre length for l < Fibre length, mmlc. Beyond the critical length, however, a proportionof those bridging a matrix crack will have an end Figure 5.14. Variation of work of fracture with fibrewithin ½lc of the plane of fracture and these will length in random and aligned composites of choppedpull out: the rest can fracture and, as a result, the steel wires in polyester resin. The fibre volume fractionamount of pull-out work required is reduced (Cooper is 0.1. (Helfet and Harris, 1972).and Kelly, 1969; Harris and Ramani, 1975), thefracture work being inversely proportional to the fibre length. Thus, for a given system, the toughestcomposites will be those with fibres with lengths equal to lc, but, in order to achieve this benefit,strength and stiffness would have to be sacrificed. If the fibres are randomly oriented instead of beingaligned, the effects described above are less clear cut. The combined effects of fibre length andorientation on the work of fracture of some model steel-wire/polyester composites are shown in Figure5.14. The simple model for the effect of fibre length is not entirely satisfactory, since the proportionality -1constant for the experimental l relationship shown in this figure is lower than that calculated by Helfetand Harris (op cit), and the two curves do not intersect at precisely the experimental value of the fibrecritical length, but the argument is at least mechanistically reasonable. We would normally expect composite toughness to be raised by increasing the fibre volume fraction,by using fibres of larger diameter, or by using stronger fibres. Contrary to expectation however,improving the fibre/matrix bond will usually reduce the toughness because it inhibits debonding andtherefore reduces pull-out (Beaumont and Harris, 1972). Detailed analysis of the individual energy-absorbing mechanisms that are believed to contribute tothe overall toughness of reinforced plastics is useful, as we have said, for guiding us in the design ofcomposites that may be expected to show improved mechanical properties, particularly in respect ofcombined strength and toughness. But it is easy to develop an over-simplified view of compositebehaviour, especially when the analysis is carried out on model systems which are deliberately designedto prevent interaction of microfailure events.5.3.2 Toughness of hybrid composites When more than one species of fibre is embedded in a single resin, the behaviour of the resultinghybrid composite may not be easy to predict from simple models. Early experiments withglass/carbon/resin composites led Harris and Bunsell (1975) to conclude that the work of fracturemeasured by notched impact followed a simple mixture-rule variation with composition (proportions ofCFRP and GRP), as shown in Figure 5.15, regardless of the distribution of the two constituent fibres.But more detailed work on carbon/glass and carbon/Kevlar hybrids suggested that this may not alwaysbe the case. Anstice and Beaumont (1983), for example, showed that the presence of the carbon fibres, asan ‘environment’, as it were, for the glass filaments, effectively modified the debond and pull-outlengths of the glass so as to reduce the overall hybrid fracture energy below that predicted by the mixture
chapter five Toughness 112rule. Stefanidis et al (1985) reported similar 200results from impact-energy values for Work of fracture, γF, kJm 2carbon/Kevlar hybrids. These are examples of a 150negative ‘hybrid effect’. An interesting effect that is often overlooked is 100that since cracks propagating in laminatedcomposites may be forced to travelsimultaneously through two materials — eg. two 50 GRP/CFRP composites (polyester matrix)plies of different orientation, or two similarlyoriented plies of different composites (in a hybrid)— which have different intrinsic fracture 0 0 20 40 60 80 100toughnesses, this will constrain the crack andmodify the material’s apparent resistance to crack Composition, vol% of CFRP in compositegrowth. When a crack is forced to move with acommon front through a sandwich consisting of a Figure 5.15. Work of fracture, measured by notched Charpywell-bonded high-toughness and low-toughness impact tests, for hybrid CFRP/GRP composites (Harris and Bunsell, 1975).pair of layers, since the composite fails at acommon displacement, the failure strain for thetougher ply will be reduced and that of the less-tough ply will be increased. Guild et al (1978) showedby a simple mechanics analysis that the value of the fracture energy of the composite, (γF)c, would be themixture-rule average, ie.: (γF)c = ½[(γF)L + (γF)H].......................................................................................... [5.14]of the toughness of the low- and high-toughness components, (γF)L and (γF)H. Rewriting this in terms ofthe strain-energy release rate, G (= 2γF), given by the compliance relationship: P 2 ⎛ dC ⎞ G= ⎜ ⎟ ................................................................................................... [5.15] 2 ⎝ dA ⎠Awhere (dC/dA)A is the rate of change of compliance with crack area, A, it is then easy to show that thecracking load for the composite beam, PC, is given by: Pc2 = 1 2 ( PL + PH ) ............................................................................................[5.16] 2 2from which we conclude that the composite cracking load, and therefore the related critical stress-intensity factor, KC, must always be greater than a simple mixture-rule sum such as that given for (γF)c.Atkins and Mai (1976) showed that the cracking load is given by the volume-fraction sum only whenthere is no bond between the components. This is an example of an apparent synergistic effect, asdiscussed above and in chapter 4, where the composite appears to perform better than would be expectedfrom simple mixture-rule considerations.5.3.3 Toughness of laminated structures184.108.40.206 Delamination In discussing these microstructural failure events we have taken a simplified view of failure, butfrequently there are further complications which may swamp the effects just described. The debondingprocess is effectively a localized crack-blunting and crack-deviation mechanism, and the growing crackdescribed above may in fact change planes rather than always continuing on the same plane. Multiplecracks may also be distributed throughout the process zone. But in most practical composites, there is theadded complexity of laminate structure. A laminate is constructed from groups of individualunidirectional plies which are laid at various angles, depending upon design requirements, or from layersof woven cloth laid at various angles to the main stress axes. The tension/shear coupling effects
chapter five Toughness 113discussed in chapter 3 cause shear stresses to be developed in the plane of the laminate, especially nearfree edges, when the material is stressed. And since interlaminar planes in non-woven composites arealways planes of weakness, the interlaminar shear stresses may easily become large enough to disrupt ordelaminate a composite well before its overall tensile strength is reached. A crack travelling through agiven ply may therefore find it energetically favourable to deviate along an interlaminar plane: undersuch circumstances, considerations of fibre debonding and pull-out are of little significance. Although the specific fracture energy for splitting is low (of the same order as that of the resin, ie. afew hundred Jm-2), the total area of delaminated surfaces created may be very large, so that the netcontribution of a delamination to the overall composite γF may be substantial. Aveston (1971) hasanalysed the work of fracture that may be available when the destruction of a bending beam occurs by aprocess of repeated fracture arrest and delamination. From strain-energy considerations, he has shownthat the total work for a single delamination may be three times the normal stored elastic energy to peakload, even in all-brittle composite systems. Most prepreg laminated composites exhibit multipledelamination, with consequent further increases in fracture work. But delaminations of this kind are notalways able to travel unhindered through fibre-free planes of weakness in modern composites becausethe manufacturing process has usually forced the original pre-preg layers into reasonably good contact,and it is often found that, after some degree of splitting, fibres lying partially across the splitting planeexert a bridging effect in the form of a tied zone. 1.2Crack propagation then becomes increasingly Fractional change in toughnessdifficult as the delamination extends. An 1.0indication of the relative degrees of resistance toimpact damage can be seen in Figure 5.16. Test 0.8coupons of a quasi-isotropic carbon-fibrelaminate and a woven-roving glass/epoxy 0.6composite were subjected to repeated impacts by 0.4a round-nosed tup, the samples being supportedby a solid steel backing during the impacts, and 0.2 CFRP (quasi-isotropic laminate)the residual levels of toughness were determined GRP (woven-roving/epoxy)as a function of cumulative incident energy. It 0can be seen that the prepregged CFRP material 0 100 200 300begins to lose toughness following the initial Cumulative incident impact energy, Jimpact, whereas the woven GRP compositeretains a very high level of toughness after many Figure 5.16. Effect of repeated impact on the notchedimpacts. This is of course one of the reasons tensile strength of a quasi-isotropic carbon/epoxy laminatewhy crash helmets made of this kind of GRP and a woven-roving glass/epoxy laminate (Harris et al,composite perform so much better than cheaper, 1991).unreinforced polycarbonate helmets. Since delamination appears to be advantageous in improving the overall toughness of composites, itis natural that much attention should have been paid to methods of increasing the work of delamination,as characterised by both the mode-I (tensile) strain-energy release rate, GIC, and the mode-II (shear)characteristic, GIIC (O’Brien, 1982; Hashemi et al, 1990). Results obtained from these two types ofmeasurement sometimes appear to give contradictory indications. Various methods have been tried toincrease the work of delamination, including: 1. modification of the matrix resin chemistry to increase the basic toughness of the resin. Alternatively, the use of intrinsically tough thermoplastic matrix polymers like PEEK and other polyaryls is advantageous, but calls for somewhat more complex manufacturing processes, 2. modification of the matrix by the incorporation of ‘flexibilizers’ — a process akin to that used in the production of high-impact polystyrene or ABS. Liquid CTBN rubber added to an epoxy resin results in a tougher, phase-separated structure containing rubber particles, but the hot-wet properties of a material are often reduced by ‘flexibilization’,
chapter five Toughness 114 3. modification of the resin by the incorporation of particles, whiskers or chopped fibres into the resin, usually in the interlaminar regions of a laminate, 4. interleaving with inert, usually soft, polymer films, 5. through-thickness stitching of the laminate. The first three of these bring about some improvement, but the degree of improvement is rarelysufficiently great to make much difference to the overall composite toughness. Srivastava and Harris(1994), for example, showed that by the incorporation of a number of types of particulate material intothe interlaminar planes of a cross-plied CFRP laminate both the mode-I and mode-II delaminationtoughnesses could be increased. GIC was approximately doubled, from about 0.6kJm-2 to roughly1.3kJm-2, and GIIC was increased from about 120Jm-2 to about 200Jm-2. These improvements, which werea maximum at particle addition levels of about 3%, falling back thereafter towards the original levels,were greater the higher the rigidity of the particulate additive. The resultant improvements in laminatetoughness were much smaller, however, amounting to only about a 25% increase in the un-notchedimpact strength. If the composite laminae are deliberately separated by interleaving with inert films which can act asdelamination initiators, the tied zone caused by fibre bridging can no longer form, but the extra energy ofdelamination contributes to toughening instead. Favre (1977) showed that the fracture energy of CFRPlaminates may be increased in proportion to the number of deliberately introduced delaminationinitiators such as films of aluminium foil or polyimide resin bonded between the carbon/epoxy laminae.Altus and Ishai (1990) also demonstrated the value of this process of ‘interleaving’ by observing theeffects of soft interleaved layers on delamination. They considered that delamination was triggered bytransverse ply cracking, and that, up to a certain level of thickness, the presence of soft layers reducesstress associated with transverse cracks and hence delays the start of delamination. Sela and Ishai (1989),in a useful review of interlaminar toughening methods, showed that interleaving markedly improved thecompression-after-impact strength (CAI) of laminates, but has the disadvantage that it brings a weightpenalty because of the concomitant reduced stiffness. The net Vf is lower than in an equivalentcomposite with no interleaving, so that additional plies have to be used to maintain design requirements.They also recommend selective interleaving as a useful compromise. Mai (1993) shows that the use ofplastic interleaving in which the film is perforated so as to allow intermittent separation of the compositelaminae leads to significant increases in toughness without the concomitant loss in tensile strength whichaccompanies the incorporation of non-perforated interleaving films. This effect is seemingly analogousto that of intermittent fibre coating described in section 220.127.116.11. We saw in section 4.3 of chapter 4 that third-direction stitching was a useful means of improving theinterlaminar shear strengths of laminates by its effect in improving the delamination resistance.Dransfield et al (1994) showed that stitching was able to improve some mechanical properties such asthe delamination resistance and the compression-after-impact strength, but that it may cause degradationof other properties as a result of the creation of pockets of resin or the breakage of load-bearing fibres.Adanur et al (1995) had recognised the problem of the fibre damage caused by the stitching process, andthey describe an improved stitching method to reduce it. Materials produced by the improved methodthen exhibited reduced delamination and increased shear strength and impact energy up to a critical levelof stitch density. It is interesting to note that Mouritz et al (1997) found that stitching increased themode-I delamination resistance but not the mode-II resistance. They also noted that the fibre damagecaused by stitching led to reductions in the flexural properties, including the ILSS, especially underimpact conditions. The interlaminar fracture toughness of composites often shows R-curve behaviour — an increase incrack resistance as an interlaminar crack grows — as a result of the effect of fibres bridging the growingcrack behind the moving crack tip. Truss et al (1997) demonstrated that the misalignment of short fibresin a discontinuously reinforced laminate added to this fibre-bridging effect, increasing the fracturetoughnesses for both initiation and growth of interlaminar and intralaminar cracks.
chapter five Toughness 118.104.22.168 Transverse-ply cracking In the case of an orthogonally laminated composite (eg. of [(0,90)n]S lay-up, or similar), loading alongone of the principal axes will cause cracking of the transverse plies at relatively low strains. In a typicalGRP laminate, for example, this cracking, which is easily detected by techniques such as acousticemission monitoring, may begin at strains as low as 0.2%, depending on the thicknesses and distributionof the plies and the resin toughness (Garrett and Bailey, 1977; Harris et al, 1979) and continue to strainsof about 1% — perhaps half the overall composite failure strain — leaving the transverse pliescompletely cracked into blocks of lengths of the order of the plythickness, as shown in Figure 4.15 of chapter 4. This crackingoccurs partly through the weak fibre/matrix interface and partlythrough the matrix resin, as shown schematically in Figure 5.17and it reduces the composite stiffness. If a 10cm x 2cm x 3mmstrip of a six-ply (0,90)3S composite were loaded until each of the90° plies was fully cracked, with a crack spacing of about0.5mm, and if the γF value for transverse-ply cracking were ofthe order of 200Jm-2, there would be about 0.012m2 of cracksurface, and this would require 2.4J of energy. Normalized with Figure 5.17. Schematic illustration of therespect to twice the sample cross-sectional area, this provides crack path during transverse crackingabout 20kJm-2. This is no doubt a vast over-estimate, but it through the matrix and interface.certainly suggests that transverse-ply cracking may not be anegligible contribution to the composite work of fracture.5.4 TOUGHNESS OF PRACTICAL REINFORCED PLASTIC LAMINATES The fracture energy of laminated composites depends strongly on both the ply stacking sequence andon the arrangement of the reinforcing fibres in the individual plies. The degree of anisotropy of theimpact fracture energy of some typical high-quality E-glass/epoxy laminates is shown in Figure 5.18(Harris, 1980). The high degree of anisotropy of the unidirectional composite is indicated by the ratio ofabout 100: 1 between the extreme values for cracking normal to and parallel with the fibres. The fractureenergy for unconstrained cracking in the transverse direction, approximately 2kJm-2, is some four or fivetimes higher than typical values for cracking of unreinforced resin, an increase partly due to the greatercomplexity of the crack path and partly to the higher fracture surface energy of the fibre/resin interface.For the 0/90 non-woven laminate, which has about the same Vf as the unidirectional composite andcontains approximately equal proportions of 250fibres in the two directions, the fracture energy Work of fracture, γF , kJm -2in the two orthogonal directions is roughly half unidirectional, Vf = 0.64that of the unidirectional composite. This 200 0/90 non-woven, Vf = 0.63implies that it is the crack/fibre interaction in the 0/90 woven, Vf = 0.47longitudinal plies that determines the overall 150toughness of the 0/90 laminate, although thismay be an over-simplification since we observerelatively little reduction in γF at angles other 100than 0° and 90° where the fracture within theplies must be more complex. The woven-cloth 50laminate, which has a somewhat lower Vf has awork of fracture only one quarter that of the 0non-woven 0/90 laminate and it is more nearly 0 30 60 90isotropic, showing a slight increase in γF at 45°to the fibre directions. It is interesting to note Orientation, θ°that the orientation-dependence of the fractureenergy, like those of the elastic modulus and Figure 5.18. Orientation dependence of the work of fracturetensile strength, can be represented by an of some GRP laminates. The data were obtained from notched Charpy impact tests (Harris, 1980).expression of the form:
chapter five Toughness 116 1 a cos 4 θ b sin 4 θ = + + csin 2 θ cos 2 θ ........................................................[5.17] ( γ F )θ ( γ F )0 ( γ F )90and the fitted curves in Figure 5.18 have this form, although we make no attempt to interpret the valuesof the constants a, b and c in terms of physical mechanisms. The differences in γF levels between these threematerials and the degree of anisotropy exhibited by each ofthem cannot be explained on the basis of either fibre Vf orelastic modulus variations. Perhaps the most significantdifference between the macroscopic fracture patterns ofthese three composites relates to the volume of materialcomprising the fracture zone (Figure 5.19). In theunidirectional and non-woven 0/90 composites thecontinuity of fibres results in an extensive damage zonearound the notch tip, whereas in a woven-cloth laminatethe damage zone is much more restricted. Fracture of a0/90 non-woven laminate at other than a right angle to thefibre direction occurs by transverse fracture of the two sets Figure 5.19. Damage accompanying fracture ofof plies, interlaminar shearing failure between the plies, the notched Charpy samples of the GRPand final separation by a type of pulling-out of the laminates for which the fracture energies are shown in Figure 5.18. In sequence, left to right,interlocked plies. The more localized failure of a woven- unidirectional, 0/90 non-woven, and 0/90 woven.cloth laminate involves fracture and pulling-out of stubbybundles of fibres, mostly less than 10 fibre diameters in length, the shortness of these pull-outspresumably being due to the high local curvature of the filaments in the woven cloth. These effects ofstyle of reinforcement on fracture energy are ascribed to the fact that woven reinforcement constrains theextension of the damage zone and serves to transfer the stress in a manner analogous to that whichoccurs with thin interspersed plies in a non-woven laminate. The tighter the weave, the lower thetoughness. McGarry et al (1976) have discussed in detail the factors affecting the toughness of practicallaminates. They describe the development of a damage zone ahead of a crack which like the plastically-yielded zone in a metal, helps to relax the high stresses concentrated at the crack tip. For practicalreinforced plastics the damage zone is a region containing intra-ply cracks propagating parallel to the fibres and inter-ply delaminations, and its size and shape exert an important influence 1.0 on the resistance of the laminate to crack HMS [(±45)2]S propagation. Sharp cracks in a ply are Strength ratio, σn / σun HTS unidirectional 0.8 effectively blunted by the intra-ply cracks HMS [(0,90)2]S so that failure requires a higher applied 0.6 stress, but final failure is still determined by the stress distributions outside the damage 0.4 region. un-notched strengths: 1.00GPa Growth of a crack through the thickness 0.2 0.60GPa of a laminate is inhibited by the 0.08GPa development of the delaminated region 0 0 0.2 0.4 0.6 0.8 1.0 between cracked and uncracked plies. As a Notch depth ratio, 2a/W consequence, certain types of laminate construction may be highly notch-sensitive Figure 5.20. Notch sensitivity of some CFRP laminates (data of whereas others may be completely Lee and Phillips, 1981). The stresses are the nominal failure insensitive to the presence of notches. Thus, stresses, σn (peak load divided by sample cross-section area) notched CFRP laminates with ±45 lay-up normalized with respect to the un-notched strength, σun . They fail at net section stresses higher than their are plotted as a function of ratio of the notch length, 2a, to the specimen width, W. Two types of carbon fibre, high-strength un-notched failure stress, σc, whereas 0/90 (HT) and high-modulus (HM), both surface treated, are represented.
chapter five Toughness 117 laminates fail at net section stresses much 1.0 lower than σc. The ±45 laminates are, of Percentage of 0o plies course, much weaker than the 0/90 laminates 17% despite their lack of notch sensitivity. 0.8 25% Strength ratio, σn / σun Grouping of the plies so as to reduce the 50% effective number of interfaces between 0.6 100% differently-oriented plies reduces the notch insensitive: efficiency of stress transfer from ply to ply σn/σun = [1 - d/2W] and dramatically increases the fracture 0.4 toughness of the laminate. An illustration of the differing degrees of notch-sensitivities of 0.2 notch sensitive: some practical CFRP laminates is shown in σn/σun = Kt-1 Figure 5.20 (Lee and Phillips, 1981). In this 0 diagram, the straight line represents the 0 0.2 0.4 0.6 0.8 1.0 behaviour of a material that is completely Ratio of hole diameter to sample width, d/W insensitive to the presence of a notch, in this case a composite of lay-up [(±45)2]S. The Figure 5.21. Results of Soutis (1994) for the compression extent to which the experimental strengths of T800/924 CFRP laminates of various lay-ups measurements of notched strength (shown containing holes. Kt = 3 for a circular hole in an infinitely large here normalized with respect to the un- plate. notched strength) fall below the straight line is then an indication of notch sensitivity. A more systematic analysis of the effect of lay-up in one specific material, a T800/924 carbon/epoxy system (Soutis, 1994), shows quite clearly how increasing the percentage of 0°plies increases the notch sensitivity (Figure 5.21). The test pieces used by Soutis contained circular holes rather than notches, but the effect is similar to that shown by Lee and Phillips. In Figure 5.21 the straight line again represents notch-insensitive behaviour, and the bottom curve, which is effectively a lower bound to the experimental curves, identifies the fully-notch-sensitive definition of the stress concentration for a circular hole, Kt (equal to 3 for a circular hole in an infinite plate). 5.4.1 Short-fibre composites Thermoset and thermoplastic moulding compounds containing randomly arranged chopped fibres, usually glass, are cheap materials which are finding wide-spread use in mainly non-load-bearing applications. Although the stiffnesses of these materials are usefully greater than those of the base resins from which they are compounded, their strengths are rarely much higher than those of the plain (filled) matrices. An important virtue of such materials, however, apart from their cheapness and mouldability, is that they are substantially tougher than unreinforced polymeric materials on account of the toughening mechanisms described above. They are roughly isotropic, and the lack of obvious planes of weakness such as occur in prepreg laminates means that the cracking process resembles that in 5 γFγF , kJm-2 and KQ , MPa.√m conventional homogeneous materials more KQ than that in anisotropic laminates. Because of 4 lp their structure and composition their behaviour is more matrix- and interface- 3 dominated than that of higher-performance Pull-out length, lp, mm composites. Polyester dough-moulding 2 2.0 compounds provide a useful example of the behaviour of this kind of composite. Some 1 1.0 measurements of the work of fracture, γF, and the candidate critical stress-intensity factor, 0 0 KQ, for a typical DMC are shown in Figure -50 0 50 100 150 200 5.22 (Harris and Cawthorne, 1974). The work Temperature, °C of fracture of the compound is of the order of 2 kJm-2, much greater than that of theFigure 5.22. Temperature-dependence of the fracture energy, critical polyester/chalk-filler material which stress intensity, and fibre pull-out length for DMC (Harris and Cawthorne, 1974)
chapter five Toughness 118constitutes the matrix. It is interesting to note thatthe two fracture parameters behave quite differently 12as functions of temperature, and are clearly not γF , kJm-2 and KQ , MPa.√m 10 γFmeasuring the same property even though we use KQboth to refer to toughness. The KQ values fall 8linearly with increasing temperature, presumablybecause KQ is influenced by the material strength 6which falls markedly over the temperature rangeshown. On the other hand, γF shows classical tough- 4brittle transformation behaviour, the transition 2occurring roughly in the region of the matrix glass-transition temperature. Thus, the fact that the matrix 0is becoming less brittle is dominating the variation -6 -4 -2 0of this property. The figure also shows the observed Log(cross-head speed, m.s-1)fibre pull-out lengths, and it can be seen that thesevary with temperature in roughly the same way as Figure 5.23. Variation of work of fracture and criticalthe γF values. It should be recalled, with reference to stress intensity with testing speed (three-point bendFigure 5.3, that KQ relates only to behaviour as far as tests) for a polyester dough-moulding compound (DMC) at room temperature (Harris and Cawthorne, 1974)the peak load, whereas γF includes the work requiredfor the whole failure process. In matrix-dominated materials the measured values of toughnessparameters are also more rate-dependent than those in fibre-dominated composites. Figure 5.23 shows,for example, how the two fracture parameters vary with testing speed in notched three-point bend tests.In this case, γF is much more sensitive than KQ, but both increase with testing speed.5.4.2 Design of damage-tolerant composites Lee and Phillips (1981) have given some rules-of-thumb for the design of damage-tolerantcomposites. The requirements are: i) The fibre/matrix bond strength is most important and must be optimized: too strong a bond results in brittle composites. ii) The composite needs to store large amounts of strain energy, ½σf εf, so high-strength, intermediate-modulus, or high-failure-strain fibres are required. iii) Thick plies delaminate more easily and reduce interactions between adjacent cracked and uncracked plies, thereby increasing toughness. But there is a need to compromise because thick plies increase the susceptibility to transverse cracking, and hence reduce fatigue and environmental resistance. iv) The stacking sequence needs to be arranged so as to encourage delaminations between shear cracks in 45° plies adjacent to load-bearing 0° plies (eg. as in (±45,02)S structures) in order to increase notched strength by protecting the 0° plies. By contrast, if delamination is suppressed (as in [0,±45,0]S structures) then the shear cracks which form in 45° plies at low stresses have a detrimental effect on the 0° fibres, leading to brittle behaviour. v) The style of reinforcement is important: cloth limits the size of the damage zone, rendering the composite more brittle. vi) 45° plies are weak but notch insensitive. They can therefore be used as crack arrestment strips in a laminate normally reinforced with 0° load-bearing plies. Mai (1993) has also given a valuable summary of the idea of developing high fracture toughness incomposites by engineering the interfaces in the composite at several levels which encapsulates some ofthe main ideas presented in the foregoing sections.5.5 TOUGHNESS OF CERAMIC-MATRIX COMPOSITES The current high level of interest in ceramic-matrix composites has largely been generated by users ofmaterials in high-temperature applications for which existing metallic alloys are increasingly becoming
chapter five Toughness 119border-line candidates. In most of the CMCs that have been studied hitherto, both fibre and matrix arerefractory in nature and therefore brittle. Practical applications consequently depend on the ability ofthese brittle/brittle combinations to exhibit energy-absorbing mechanisms which are more efficient thanthose associated with simple failure of the matrix and the fibres. In typical CMCs, by contrast with reinforced plastics, the stiffnesses of the reinforcing and matrixphases are often quite similar, although the strength and failure strain of the fibre will almost always behigher than those of the matrix. Many of the mechanisms of energy absorption that have already beendescribed for polymer composites will also occur in CMCs, but the consequence of the extremebrittleness of the matrix — ie. multiple matrix cracking — is to modify in some respects the extent towhich these other toughening mechanisms can operate. Hillig (1987), following Cottrell (1964), hassummarized the situation for CMCs with reference to the expression for the fracture energy (in terms ofthe critical strain-energy release rate, G): U max Gc = 2 ∫0 σdU ....................................................................................................5.17)where U is the non-elastic displacement relative to the bulk material at the crack plane under criticalconditions for crack propagation, and σ is the corresponding stress level in that plane. A large value ofGc results from a combination of a high crack-tip stress and a broad process zone, which sets the guidingprinciples for the development of successful CMCs. The extent of the process zone can be modified, aswith reinforced plastics, by the provision of a group of energy-absorbing mechanisms which, in ceramicmaterials, will include incipient microcracking, crack deflexion and branching, fibre/matrix debonding,and fibre pull-out.5.5.1 Matrix cracking One of the seminal treatments of the failure of CMCs was that of Aveston and co-workers (1971,1973, 1974) which led to what is now almost universally referred to as the Aveston-Cooper-Kelly, orACK, model. It is an energy-balance model set up to explain the multiple fracture of CMCs and isfrequently used to predict the occurrence of the first crack as a design parameter. In composites of thiskind first cracking may be more important than the notional strength. The ACK model starts from theassumption that a crack cannot form in the matrix unless the work done by the applied stress is greaterthan the increase in elastic strain energy of the composite plus the fracture surface work of the matrix perunit area of cross section. The model takes into account the work done by the applied stress on thecomposite body, the work expended in debonding the fibres from the matrix, the matrix fracture energy(usually negligible), the friction work expended as the matrix and fibres slide past each other, thedecrease in the elastic strain energy of the matrix, and the increase in the strain energy of the fibres. Thefriction stress controlling the interfacial sliding is assumed to be constant and characteristic of thesystem. After cracking of the matrix, the bridging fibres are then assumed to carry the entire loadformerly shared with the matrix. A brief introduction to the derivation of the ACK model is given insection 4.6 of chapter 4. We refer again, briefly, to matrix cracking in section 22.214.171.124.5.2 Fibre bridging In order for crack bridging to occur and contribute to composite toughening, it is essential that thefibres debond at the interface in preference to fracturing at the crack front. When this condition issatisfied, the rate of load transfer from fibres to matrix is determined by the frictional resistance tosliding at the interface. If τi is high, load transfer is efficient, and the load in the fibre decays rapidly withdistance from the crack face. The statistical nature of the strengths of brittle fibres then results in theoccurrence of fibre failures mainly in locations close to the crack face, thereby reducing the potentialpull-out contribution to toughening. A low level of frictional resistance thus promotes toughness and, asin polymer-matrix composites, control of the interface is therefore of paramount importance indetermining the composite fracture resistance. In a review of the mechanical behaviour of CMCs, Evansand Marshall (1989) point out that in order for debonding to occur instead of fibre fracture, the ratio ofthe interface fracture energy, GIC, to that of the fibre, Gfc, should be less than about 0.25, although, as
chapter five Toughness 120they pointed out, there was at the time no experimental validation of this requirement. The effect ofbridging fibres on the composite toughness can be modelled (Romualdi and Batson, 1963; Marshall etal, 1985) by considering the stresses in the fibres as crack-surface closure tractions which reduce thestresses at the crack tip.5.5.3 Fibre pull-out The fabrication of CMCs almost alwaysinvolves the use of high temperatures and/orpressures in order to achieve good levels ofdensity and uniform microstructures, and underconventional processing conditions this may leadto interfacial reactions which can result inreductions in the strength of the reinforcingfilaments, increases in the interfacial bond Figure 5.24. Schematic illustration of a unidirectionalstrength, and the build-up of differential thermal CMC composite after loading so that the matrix is crackedstresses. These effects, as we have already seen, into small blocks surrounded by an array of longitudinalshould result in marked reductions in the level of and transverse cracks. See text for explanation.toughness that can be contributed to the compositethrough the pull-out and other mechanisms. Further exposure to elevated temperatures during servicewill also lead to deterioration. Results that have been reported range from composites where the bond isso strong that little or no pull-out can occur to systems where the bonding is so weak that the matrix cancompletely disintegrate, leaving dusty bundles of bare fibres. Neither of these extremes offers a usefulengineering composite, and it is clear that control of the interface is therefore just as important an issuein CMCs as in reinforced plastics and metal-matrix composites. A good deal of early research on CMCs related to composites with glass or glass-ceramic matricesreinforced with carbon or SiC fibres which were manufactured by slurry impregnation and hot-pressing.In much of this work, the composites produced exhibited works of fracture of the order of 3-10kJm-2.Examples were the work of Phillips (1972, 1974a) on borosilicate glass and a low-expansion lithiumalumino-silicate (LAS) glass-ceramic reinforced with high- and low-modulus carbon fibres. The fractureenergies of the composites were related to differences in the fibre/matrix bond strength and the simplepull-out model described earlier appeared to account for the greater part of the measured toughnessvalues. Subsequent CMC development, particularly in the USA, concentrated on glass and glass-ceramicsystems reinforced with Nicalon SiC fibres which have been reported on extensively by Prewo and hisco-workers (1980, 1982a, 1982b) who gave fracture energy values of about 30kJm-2. Values of γF forSiC/Pyrex composites were also published by Ford et al (1987) who showed that, depending on heat-treatment conditions, the same composite could have a fracture toughness as low as 2kJm-2, with littlepull-out, or as high as 25kJm-2 when the interfacial bond strength was optimized. When the samematerial was heat treated so as to cause extensive delamination, γf values over 40kJm-2 were obtained. One of the difficulties in using a simple model such as that of equation 5.12 for CMCs is that it isoften impossible to know exactly what is the strength of the fibre after it has undergone the rigours of themanufacturing process. In resin-based or glass-based composites it is possible to dissolve away thematrix and carry out strength measurements on the filaments so as to obtain their true strength in situ,but in composites with more resistant matrices it is impossible to do this without the fibre sustainingfurther damage. To remove glass or a silica-based ceramic from a Nicalon-fibre composite, for example,it is necessary to use hydrofluoric acid or similar aggressive chemicals, and since Nicalon itself containssome SiO2 it is likely that some attack of the fibres will also occur. For a SiC/CAS composite of Vf about0.4 manufactured by Corning, experimental measurements gave values of γF of about 50kJm-2 (Harris etal, 1992). Scanning electron microscope pictures showed pull-out lengths of about 2-3 fibre diameters,so the contribution of fibre pull-out to the toughness, from equation 5.12, is only about 5kJm-2, if thefibre strength is about 1.5GPa (a value assumed from the measured strengths of extracted fibres). Harriset al showed that a substantial part of the remaining fracture energy of the SiC/CAS composite couldhave been contributed by the multiple transverse and longitudinal matrix cracking which occurs duringdeformation, reducing the matrix to a series of roughly equi-axed blocks as shown schematically in
chapter five Toughness 121 1.0 Figure 5.24. From an estimation of the total crack surface area in a typical cracked sample, it was 0.8 (0,±45)2S deduced that the contribution of matrix cracking (±45,0,90)S to the composite work of fracture must be about 0.6 (90,0,±45)S 250γm, where γm, the specific work of fracture ofσN /σo the matrix is about 50Jm-2. This works out at 0.4 about 30kJm-2 which, together with the pull-out work and other small contributions, approximates 0.2 reasonably well to the measured value. 0 5.6 APPLICATION OF FRACTURE MECHANICS -1 0 1 2 3 TO COMPOSITES Log(R) 5.6.1 Strength of notched composites andFigure 5.25. Predicted values of the ratio of notched to un- notch sensitivitynotched strengths of three types of laminate as a function of hole radius (Pipes et al, 1979). The fitted curve is a Before discussing the possibility of applying a sigmoidal (Boltzmann) curve. fracture-mechanics formalism to composites behaviour it is instructive to consider a number ofattempts that have been made to model strength of composites containing holes or notches. In the firstplace, experimental work, like that of Waddoups et al (1971) on (0,±45)2S CFRP laminates,demonstrated that the notched composite strength is often strongly dependent on the size of the hole. Inorder to explain observed notch strengths, it is necessary to know the stress distribution in the vicinity ofthe notch and to assume that failure occurs when the stress at some distance from the notch (known asthe point-stress criterion) or the mean stress in a given region in the neighbourhood of the notch (theaverage-stress criterion) reach the un-notched tensile strength of the laminate. Whitney and Nuismer(1974) used a two-parameter model, arguing that while the stress-concentration factor is the same forholes of different sizes in an infinite plate, the stress gradient is different for each. Thus large stresses arelocalized more closely to the edge of a small hole than a large hole, and a critical defect is more likely tooccur in a region of high stress for a large hole. The 2-parameter point-stress and average-stress modelsare both capable of predicting observed notch size without recourse to fracture-mechanics methods. A 3-parameter ‘classical elasticity’ model involving a transposition procedure proposed by Pipes et al (1979)was also successful in being able to predict notched strength versus notch radius relationships for quasi-isotropic laminates of any stacking sequence, given the relationship for a single sequence, as illustratedin Figure 5.25. Potter (1978) considers that microcracks that form in the damage zone near a notch as aresult of over-stressing do not inevitably lead to failure, and may even act as stress-relievers. Then,although the composite may exhibit linear-elastic behaviour, the notched laminate may fail at a stressgreater than that indicated by the linear elastic stress concentration — ie. it will show a notch-size effect.Potter showed that tensile fracture is governed by inter-fibre stress transfer within the axial plies, andthat limitations on the extent of this stress transfer imposed by matrix strength and fibre/matrix bondstrength result in ‘large’ and ‘small’ notch effects. ‘Large’ notches initiate a sequential fibre failureprocess in the axial plies, and their effect is predictable by orthotropic laminate analysis, assuminginhomogeneity. In the neighbourhood of ‘small’ notches on the other hand, fibre failures in the 0° pliesdo not initiate this sequential fibre failure process, but form stable damage zones such as we havealready discussed, which consist of matrix and fibre/matrix interface failures propagating parallel to thefibres and inhibiting inter-fibre stress transfer. ‘Small’ notches become ‘large’ when the notch geometryis modified in an appropriate way by the developing damage zone. Early work on unidirectional epoxy-based composites reinforced with high-modulus carbon and with low-modulus SiO2 suggested that thereis a logarithmic relationship between the fracture energy and the radius of the notch tip in Charpy impacttests, as shown in Figure 126.96.36.199.2 The application of fracture mechanics Fracture mechanics is universally accepted as a useful discipline for characterising the toughness ofmaterials that are homogeneous and isotropic on the macroscopic scale — materials like metals and
chapter five Toughness 122alloys. In the field of composites, however, there is serious doubt about whether the additionalcomplexities of heterogeneity and anisotropy do not preclude the practical application of fracturemechanics. Early questions that were asked in this context (Sih, 1979) are: • Is it feasible to use the same test procedures (such as critical stress-intensity and compliance measurements) to characterize composite toughness? • Can the basic equations of fracture mechanics be modified to include inhomogeneity and anisotropy? • To what extent is crack propagation (when it occurs in an appropriate manner) controlled by initial crack geometry, loading, and material orientation? • What kinds of theoretical and experimental investigations are needed to develop predictive techniques to forecast composite behaviour? Much experimental and theoretical work has indeed been published about a wide variety ofcomposite types. but it is still far from clear whether fracture mechanics is or is not a useful investigativetool and predictive model (see, for example,Sendeckyj, 1975, and Sih and Tamuzs, 1979). 200 It is well known that certain composite or Work of fracture, γF, kJm-2laminate types give results which can apparentlybe treated by linear-elastic fracture mechanics, or 100extensions of it, whereas others cannot. Severaldistinct types of composite stress/strain behaviour SiO2/epoxy; slope 0.15 50may be observed, for example, as shown in Figure carbon/epoxy; slope 0.095.3. The linear, or non-tough, kind of behaviour,undesirable in engineering structures, is mostlikely to allow the application of fracture 20mechanics whereas the toughest kind of behaviour,in which the material retains a substantial degree 10of ‘post-failure’ integrity involving highly 0.05 0.1 0.2 0.5 1 2complex deformation and cracking mechanisms, Notch root radius, mmseems least likely to obey fracture-mechanicsprinciples. And in the failure of such a desirable Figure 5.26. The effect of notch acuity on measured worksengineering material, we have to ask whether the of fracture for unidirectional carbon/epoxy and SiO2/epoxymore important parameter is that representing the composites (Ellis and Harris, 1973)initial crack-growth resistance — G or K — or thetotal fracture work, γF. The spreading of a delamination crack is perhaps the simplest mode of crackingin a laminate, and is satisfactorily modelled, both for simple crack growth and for fatigue, by linear-elastic fracture mechanics, as shown by Vancon et al (1984). On the other hand, the rupturing of anotched unidirectional GRP rod, which may involve the total disintegration of the resin matrix over alarge part of the sample volume, will be too complex to treat by the usual models. Furthermore, as wehave seen, for any given laminate it is sometimes possible to change from one extreme type of fracturebehaviour to another simply by arranging the plies in different ways.5.6.3 Application to specific composites In seeking to apply fracture mechanics to composite materials we are, in essence, attempting to definea fracture criterion that concerns only the macroscopic behaviour of the material in the presence ofnotches, flaws or other design features that are large by comparison with the fibre diameter. At first sightthis does not appear to be feasible because the fracture behaviour of composites can be considerablymodified by the presence of weak interfaces, and the mode of crack propagation does not seem to satisfythe conditions laid down for the application of fracture mechanics. Experimental results seem to suggesthowever that under some circumstances fracture-mechanics ideas can be used. Wu (1968) showed that afracture-mechanics approach to the propagation of cracks in homogeneous, isotropic plates could beapplied in a limited way to unidirectionally-reinforced plastics. He determined the critical stress for the
chapter five Toughness 123propagation of cracks of various lengths parallel with the fibres under tension and shear loadingconditions, and showed that for each case a relationship of the form k = σ∞√(πa) accurately fitted theresults, k being a constant, a the crack length, and σ∞ the fracture stress. He also showed that theinteraction of stress-intensity factors for combined conditions (tensile and shear mode) was welldescribed by a relationship of the form 2 K I ⎛ K II ⎞ +⎜ ⎟ = 1 ...............................................................................................[5.18] K Ic ⎝ K IIc ⎠This empirical relationship was not in agreement, however, with a general theoretical one given by Parisand Sih (1965) for anisotropic materials: 2 2 ⎛ K I ⎞ ⎛ K II ⎞ ⎜ ⎟ +⎜ ⎟ = 1 .........................................................................................[5.19] ⎝ K Ic ⎠ ⎝ K IIc ⎠although both could be considered to be specific cases of a more general power-law model. Sanford andStonesifer (1971) measured the fracture toughness and strain-energy release rate, G, of several types ofglass-fibre/epoxy composites and showed that G is a bulk property of the material, independent of themode of loading. For combined tension and shear they give G = GI + GII ................................................................................................................... [5.20]so that fracture toughness properties for the in-plane forward-shear mode, which are experimentallymuch more difficult to measure than those in tension, could be deduced in a straightforward mannerfrom opening-mode results. Since G and K are not independent properties of the material, and can bewritten G c = CK c .........................................................................................................[5.21] 2C being an elastic compliance property. Equation 5.21 can be given in the alternative form C1K1 + C2K2 = cons tan t ...............................................................................[5.22] 2 2which is more in keeping with the expression of Paris and Sih. C1 and C2 are functions of the elasticcompliances for the material, viz. 1 1 ⎛ C1 ⎞ 2 ⎛ E1 ⎞ 4 ...................................................................................................[5.23] ⎜ ⎟ =⎜ ⎟ ⎝ C2 ⎠ ⎝ E 2 ⎠where E1 and E2 are the elastic moduli in the longitudinal and transverse directions, respectively. Thefull form of equation 5.21 for opening-mode cracks in a rectilinearly anisotropic body (as opposed to aninhomogeneous composite) has been given by Sih, Paris and Irwin (1965): 1 ⎛ S S ⎞ ⎡⎛ S ⎞ ⎛ 2S + S66 ⎞ ⎤ .....................................................[5.24] 1 1 2 2 2 G Ic = K 2 ⎜ 11 22 ⎟ ⎢⎜ 22 ⎟ + ⎜ 12 Ic ⎟⎥ ⎝ 2 ⎠ ⎢⎝ S11 ⎠ ⎝ 2S11 ⎣ ⎠⎥⎦On making the appropriate substitutions for the Sij in terms of the engineering elastic constants (seechapter 3), and ignoring a small term involving Poisson’s ratio, we obtain:
chapter five Toughness 124 1 1 ⎞ ⎡⎛ E1 ⎞ E1 ⎤ .................................................................. [5.25] 1 1 2 2 ⎛ 2 2 G Ic = K Ic ⎜ ⎟ ⎢⎜ ⎟ + ⎥ ⎝ 2E1E 2 ⎠ ⎢⎝ E 2 ⎠ 4G12 ⎥ ⎣ ⎦This equation can be presented in a form analogous to the conventional fracture-mechanics relationshipfor isotropic materials, viz.: K2 Gc = Ic (isotropic solids) .................................................................... [5.26] E K2 Gc = Ic (orthotropic materials ).......................................................... [5.27] E effectivethe effective modulus thus being the reciprocal of the bracketed terms in equation 5.25. It was suggestedin the First Edition of this book (page 75) that for orthotropic composites with a strong anisotropic axis,such as CFRP, the effective modulus could be approximated by 2√(E1G12). Closer inspection of thefunction defined in equation 5.25, however, suggests that this is invalid and that for most practicalpurposes the value of the transverse modulus, E2, is a better approximation. From their work on stress concentrations in flawed (0,±45)2S carbon/epoxy laminates referred to inthe previous section, Waddoups et al (1971) concluded that the experimental behaviour of theirlaminates, when tested without deliberately introduced notches, was consistent with predictions of afracture-mechanics analysis for a crack dimension of approximately 1mm, even though nomacroscopically detectable crack was present. This and other treatments, including that of Whitney andNuismer (op cit), therefore gives rise to the concept of an energy-intense region at each crack tip whichleads to an empirical extension of isotropic linear-elastic fracture mechanics in which the fracturetoughness, KC, for an infinite body under tensile load containing an internal crack of length 2a is givenby Kc = σ√[π(a + rρ)]......................................................................................................... [5.28]where rρ is the dimension of the energy-intense region at the crack tip, referred to in other formalizationsas the process zone: rρ is treated as a disposable parameter and is evaluated from experimental data.Similar approaches have been followed by Owen and Rose (1973) for glass/polyester composites, and byBeaumont and Phillips (1972) who suggested that the damage zone consists largely of material in whichthe fibres were debonded from the resin. Owen and Bishop (1972) have found that as far as the fracture-mechanics approach is concerned this zone can be treated in the same way as the plastic zone in metallicmaterials, and they used measured values of the zone size to correct Kc results obtained from a variety ofGRP laminates. By determining the fracture toughness of plates up to 105mm wide in this way they wereable to show that Kc could be considered to be a genuine material parameter for design purposes. Thework of Owen and his co-workers has largely been carried out by testing wide, notched plates in tension.One of the difficulties in comparing results obtained by different investigators, however, is that thevarious test methods are sometimes found to give quite different data, and it is not clear what type of testcan be said to give absolute values. Phillips (1974b) measured G and K values for 0/90 carbon/epoxy and carbon/glass composites andconcluded that KC was independent of crack size and could therefore be used to predict compositestrength. A fracture-mechanics analysis gave fracture energies that agreed quite well with those obtainedby other methods, indicating the validity of the Griffith-Irwin criterion for crack-propagation normal tofibres. He obtained KC values of 6-25 MPa√m for various CFRP materials, GC being between 1 and 20kJm-2. For the carbon-fibre/glass material he obtained a KC value of about 10 MPa√m and a GC of about2 kJm-2.
chapter five Toughness 125 In attempting to use the concept of KC for a unidirectional GRP, Barnby and Spencer (1976) showedthat the compliance calibration is significantly different from that for a continuous elastic medium, and isnon-conservative (ie. the error goes the wrong way). With an experimental calibration involving afourth-order polynomial they obtained KC values of about 15MPa√m, similar to those of Owen and Rose(1973), but observed that the failure mode was not transverse to the fibres. An example of what can be achieved by a fracture-mechanics type of analysis applied to a series ofcarbon-fibre laminates is illustrated by some work reported by Dorey (1977). He shows that when anattempt is made to compare a range of laminate lay-ups having different notch sensitivities,measurements of the apparent fracture toughness, KC = σc√(πa), give results that were stronglydependent on the test-panel width and the notch length and acuity, and which do not therefore permit ofeasy evaluation of the relative toughness of different laminates. By contrast, when the results areadjusted by the application of a sample finite-width correction factor, α, and the damage-zone sizecorrection factor, rρ, of equation 5.28: Kc = ασ√[π(a + rρ)] ....................................................................................................... [5.29]the resulting values become independent of notch and sample geometry and can therefore be used tomake comparisons of materials characteristics such as resin type, ply distribution and layer thickness.His results illustrate the wide variations in fracture toughness that may be observed in any given class ofcomposites as a result of the use of different resins and alternative arrangements of the plies in (0,±45)laminates. Bishop and McLaughlin (1979), working with laminates similar to those of Dorey, summarized thematerials characteristics that affect the toughness of this type of composite. They showed that the notch-sensitivity of a (0,±45) CFRP laminate in tension can be reduced by avoiding too high a bond strength,since in general all lay-ups tend to become brittle if the bond strength is too high. At modest levels ofinterfacial bonding, increases in toughness can be obtained by selecting ply angles and stackingsequences, and by increasing the thickness of the plies. Thicker plies tend to delaminate more readilythan thin plies. Thus, increasing the laminate thickness by repeating the basic stacking sequence has littleeffect on failure characteristics, but increasing the thickness of the layers leads to more delamination andshear cracking, so that toughness is increased. Laminates with four-ply layers, for example, had notchedtensile strengths some 50% greater than similar laminates with single-ply layers. The load-carryingability of 0° plies is increased by shear splitting (in the 0° plies), but is reduced by cracks in adjacent 45°plies: 0/45 ply interactions are of course reduced when delamination occurs. Thus, even if fibres, resins,and bond strengths are pre-selected on the basis of some optimisation procedure for strength andstiffness, further optimisation for improvements in toughness can still be done in terms of fibre angles,stacking sequences and ply thickness. Some conclusions from work by Wang et al (1975) on through-thickness cracks in cross-pliedlaminates may serve as a summary of these ideas. It is clear that the stress field round a crack is severelymodified by the introduction of damage consisting of sub-cracks parallel to the fibres in each ply. A corezone can be defined around the main crack tip such that outside this zone the stress field is undisturbedwhile inside the zone the stress field is relaxed by high levels of inter-laminar stress that are present.Mixed-mode crack propagation is therefore automatically implied. These sub-cracks serve a functionsimilar to the plastic zone in metals, and crack resistance results from reduction of the in-plane stressfield at the main crack tip. The relaxed core zone is embedded in a stress field at the main crack tipwhich is unaltered by the sub-cracks, and the in-plane stresses follow a classical r-½ stress singularity inthe near-crack-tip region.5.7 CONCLUSION
chapter five Toughness 126 Under some circumstances, linear-elastic fracture mechanics can be used directly. Typically thisapplies to brittle composites with high fibre/resin bond strengths and brittle matrices. In such materialscrack paths may be planar, or nearly so, and damage zones small (eg. ≤ 1mm), and the effects ofcomposite heterogeneity are not apparent. Similarly, it is likely that in random composites like chopped-strand-mat laminates or in short-fibre moulding compounds like DMC and SMC, anisotropy will not bea problem and fracture mechanics may be used. It has also been observed that for specific cases of cracksrunning parallel with the fibres (in a unidirectional laminate) or delaminating cracks in a complexlaminate, crack growth appears to obey fracture-mechanics requirements. In such cases as these the modified fracture mechanics can often be used for cracking under both monotonic and cyclic loading conditions. By contrast, in tough composites damage is complex and single-crack failure may not occur. In cases where a single crack does propagate, a plastic- zone or process-zone correction factor may work, but very large samples are often needed to obtain sensible results. Low Vf composites are also likely to cause difficulties because the assumption of structural uniformity is no longer valid. An important generalisation is that generalisations should not be made! There is always likely to be Figure 5.27. Schematic illustration of the general relationship between fracture toughness and uncertainty over the question of validity of LEFM for strength for families of metallic materials. any given case. Designers dealing with metallic materials 100recognise that, in general, high toughness andhigh strength are mutually exclusive Toughness, KQ , MPa.√m 80characteristics of materials, and that there isroughly an inverse relationship betweentoughness and strength. This is illustrated 60schematically in Figure 5.27. Markedlycontrasting behaviour in composites was shown 40by Harris et al (1988) who examined many regression line:published and unpublished results, obtained over 20 KQ = 65σfa 15-year period, for a wide variety of composite (R = 0.933; n = 67)types. The range of materials included moulding 0compounds, cross-plied and quasi-isotropic 0 0.5 1.0 1.5laminates, unidirectional composites, glass, Tensile strength, GPacarbon, Kevlar-49 and hybrid laminates, andglass- and ceramic-matrix composites. They Figure 5.28. Relationship between apparent toughnesses,showed that it was possible to plot measured KQ, of a wide variety of composite materials and their tensilevalues of K (the candidate fracture toughness, strengths. The dashed lines are prediction bands at the 90%KQ), measured in tension, against the tensile level (Harris et al, 1988).fracture stress and show, as seen in Figure 5.28,that there is a reasonably good linear relationship between the two. Clearly a substantial amount ofscatter is to be expected, given the different experimental and analytical methods used by the largenumber of authors whose work appears on this diagram, but the correlation is statistically significant. Acrude analysis on the basis of the familiar approximate relationship: KQ ≈ 1.2.σc √(πa)................................................................................................. [5.30]indicates that the intrinsic crack dimension for all of this diverse range of materials is about 1 mm, whichis identical with the result of Waddoups et al (1971) for one specific laminate. A similar result was also
chapter five Toughness 127shown by Wetherhold et al (1986). We may suppose then that the conclusion of Waddoups et al isgenerally valid and a crack-tip process zone of the order of 1mm across forms near cracks in mostcomposites prior to failure. This is of the order of 100 fibre diameters for composites like GRP andCFRP, but it is clear from the results of Jamison referred to in Chapter 4 that crack nuclei of this size arenever found in practice. It appears, nonetheless, that regardless of the apparent notch-sensitivity orotherwise of fibre composites, the micro-structural features which determine their resistance to crackpropagation also control their fracture behaviour in the absence of deliberately introduced notches.5.8 REFERENCES TO CHAPTER 5 Adanur S, Tsao YP and Tam CW, 1995, Compos Engg, 5, 1149-1158. Altus E and Ishai O, 1990, Compos Sci & Techol, 39, 13-27. Anstice PD and Beaumont PWR, 1983, J Mat Sci Letters, 2, 617-622. Atkins AG and Mai YW, 1976, Int J Fracture, 12, 923-924. Atkins AG, 1974, Nature, 252, 116-118. Atkins AG and Mai YW, 1985, Elastic and Plastic Fracture, (Ellis Horwood, Chichester, UK). Aveston J, 1971, Proc NPL Symposium on The Properties of Fibre Composites (IPC Science & Technology Press, Guildford, UK), 63-73. Aveston J, Cooper GA, Kelly A, 1971, Proc NPL Conference on The Properties of Fibre Composites (IPC Science & Technology Press, Guildford, UK), 15-26. Aveston J and Kelly A, 1973, J Mater Sci, 8, 352-362. Aveston J, Mercer RA and Sillwood JM, 1974, Proc NPL Conference on Composites - Standards, Testing and Design, (IPC Science & Technology Press, Guildford, UK), 93-102. Bailey JE, Curtis PT and Parvizi A, 1979, Proc Roy Soc (London), A366, 599-623. Barnby JT and Spencer B, 1976, J Mater Sci, 11, 78-82. Beaumont PWR and Harris B, 1972, J Mater Sci, 7, 1265-1279. Beaumont PWR and Phillips DC, 1972, J Compos Mater, 6, 32-46. Bishop SM and McLaughlin KS, 1979, RAE ( Farnborough) Technical Report TR 79051. Broek D, 1986, Elementary Engineering Fracture Mechanics, (Martinus Nijhoff, Dordrecht, Netherlands). Cook J and Gordon JE, 1964, Proc Roy Soc (Lond), A282, 508-520. Cooper GA and Kelly A, 1967, J Mech Phys Solids, 15, 279-298. Cooper GA and Kelly A, 1969, in Interfaces in Composites STP 452, (American Society for Testing and Materials, Philadelphia, USA), 90-106. Cooper GA, 1970, J Mater Sci, 5, 645-654. Cottrell AH, 1964, Proc Roy Soc (Lond), A282, 2-9. Dorey G, 1977, Damage Tolerance In Advanced Composite Materials, RAE (Farnborough) Technical Report TR 77172. Dransfield K, Baillie C and Mai YW, 1994, Compos Sci & Technol, 50, 305-317. Drzal LT Rich MJ and Lloyd P, 1982, J Adhesion, 16, 1-30. Drzal LT Rich MJ, Koenig MF and Lloyd P, 1983, J Adhesion, 16, 133-152. Ellis CD and Harris B, 1973, J Compos Mater, 7, 76-87. Evans AG, Marshall DB and Burlingame NH, 1981, Advances in Ceramics, 3, 202-216. Evans AG, Zok FW and Davis J, 1991, Compos Sci and Technol, 42, 3-25. Evans AG and Marshall DB, 1989, Acta Metall, 37, 2567-2583. Favre JP, 1977, J Mater Sci, 12, 43-50. Ford BA, Cooke RG and Newsam S, 1987, Brit Ceram Proc, 39, 229-234. Garrett KW and Bailey JE, 1977, J Mater Sci, 12, 157-168 and 2189-2193. Garvie RC, 1985, J Mater Sci, 20, 3479-3486. Gerberich WW, 1971, J Mech Phys Solids, 19, 71-88. Griffith AA, 1920, Proc Roy Soc (Lond), A221, 163-198.
chapter five Toughness 128 Guild FJ, Atkins AG and Harris B, 1978, J Mater Sci, 13, 2295-2299. Gurney C and Hunt J, 1967, Proc Roy Soc (Lond), A299, 508-524. Harris B, Beaumont PWR and de Ferran EM, 1971, J Mater Sci, 6, 238-251. Harris B and Cawthorne D, 1974, Plastics & Polymers, 42, 209-216. Harris B and Bunsell AR, 1975, Composites, 6, 197-199. Harris B and Ramani SV, 1975, J Mater Sci, 10, 83-93. Harris B, Morley J and Phillips DC, 1975, J. Mater. Sci, 10, 2050-2061. Harris B and Ankara AO, 1978, Proc Roy Soc (Lond), A359, 229-250. Harris B, Guild FJ and Brown CR, 1979, J Phys D: Applied Phys, 12, 1385-1407. Harris B, 1980, Metal Science, 14, 351-362. Harris B, Dorey SE and Cooke RG, 1988, Compos Sci & Technol, 31, 121-141. Harris B, Chen AS, Coleman SL and Moore RJ, 1991, J Mater Sci, 26, 307-320. Harris B, Habib FA and Cooke RG, 1992, Proc Roy Soc (Lond), A437, 109-131. Hashemi S, Kinloch AJ and Williams JG, 1990, Proc Roy Soc (Lond), A427, 173-199. Helfet JL and Harris B, 1972, J Mater Sci, 7, 494-498. Hillig WB, 1987, Annual Rev of Mater Sci, 17, 341-383. Kardos JL, 1985, in Molecular Characterisation of Interfaces (editors H Ishida and G Kumar) Polymer Science & Technology, 27, (Plenum Press NY), 1-11. Kelly A and Tyson WR, 1965, J Mech Phys Solids, 13, 329-350. Kelly A, 1970, Proc Roy Soc (Lond), A319, 95-116. Kelly A, 1973, Strong Solids (second edition), (University Press Cambridge). Khatibzadeh M & Piggott MR, 1997, Compos Sci & Technol, 58, 497-504. Lee RJ and Phillips DC, 1981, Proc First International Conference on Composites Structures, Paisley, Scotland (editor IH Marshall), (Applied Science Publishers, London), 536-554. Mai YW, Atkins AG and Caddell RM, 1976, Int J Fracture, 12, 391-407. Mai YW, 1993, Proc 3rd Japan International SAMPE Symposium, Advanced Materials — New Processes and Reliability (Editors T Kishi, N Takeda and Y Kagawa) Dec 1993 Chiba, Japan, (Japan Chapter of SAMPE, Tokyo), vol 2, 2099-2107. Marshall DB, Cox BN and Evans AG, 1985, Acta Metall, 33, 2013-2021. Marston TU, Atkins AG and Felbeck DK, 1974, J Mater Sci, 9, 447-455. McGarry FJ and Mandell FJ, 1972, Proc 27th Annual Technical Conference of Reinforced Plastics/Composites Institute of SPI, (Society for Plastics Industry New York), Paper 9A. McGarry FJ, Mandell FJ and Wang SS, 1976, Polymer Eng Sci, 16, 609-614. McGuire MA and Harris B, 1974, J Phys D: Appl Physics, 7, 1788-1802 Morton J and Groves GW, 1974, J Mater Sci, 9, 1436-1445. Morton J and Groves GW, 1976, J Mater Sci, 11, 617-622 Mouritz AP, Gallagher J and Goodwin AA, 1997, Compos Sci & Technol, 57, 509-522. O’Brien TK, 1982, in Damage in Composite Materials (editor KL Reifsnider) ASTM STP 775, (American Society for Testing and Materials, Philadelphia, USA), 140-167. Outwater JO and Murphy MC, 1969, Proc. 24th Annual Technical Conference, Reinforced Plastics/Composites Inst. of SPI, paper 11C. Outwater JO and Murphy MC, 1973, Proc. 28th Annual Technical Conference, Reinforced Plastics/Composites Inst. of SPI, paper 17A. Owen MJ and Bishop PT, (1972), J Phys D: Appl Physics, 5, 1621-1636. Owen MJ and Rose RG, (1973), J Phys D: Appl Physics, 6, 42-53. Paris PC and Sih GC, 1965, Fracture Toughness Testing and its Applications, ASTM STP 381, 30-81. Phillips DC, 1972, J Mater Sci, 7, 1175-1191. Phillips DC, 1974(a), J Mater Sci, 9, 1847-1854. Phillips DC, 1974(b), J Compos Mater, 8, 130-141.
chapter five Toughness 129 Phillips MG, 1981, Composites, 12, 113-116. Piggott MR, 1970, J Mater Sci, 5, 669-675. Piggott MR, 1974, J Mech Phys Solids, 22, 457-468. Pipes RB, Weatherhold RC and Gillespie JW, 1979, J Compos Mater, 13, 148-160. Potter RT, 1978, Proc Roy Soc (Lond), A361, 325-341. Prewo KM, 1982(b), J Mater Sci, 17, 2371-2383. Prewo KM and Brennan JJ, 1980, J Mater Sci, 15, 463-468. Prewo KM and Brennan JJ, 1982(a), J Mater Sci, 17, 1201-1206. Romualdi JP and Batson GB, 1963, J Eng Mech Div Proc Am Soc Civil Eng, 89, 147-168. Sanford RJ and Stonesifer FR, 1971, J Compos Mater, 5, 241-245. Sela N and Ishai O, 1989, Composites, 20, 423-435. Sendeckyi GP (editor), 1975, Fracture Mechanics of Composites, ASTM STP 593, (American Society for Testing and Materials, Philadelphia, USA). Sih GC Paris PC and Irwin GR, 1965, Int J Fract Mech, 1, 189-203. Sih GC, 1979, Proc. First USA/USSR Symposium on Fracture of Composite Materials, (GC Sih and VP Tamuzs, editors), Riga 1978, (Sijtoff and Noordhoff, Netherlands). Soutis C, 1994, Compos Engg, 4, 317-327. Srivastava VK and Harris B, 1994, J Mater Sci, 29, 548-553. Stefanidis S, Mai YW and Cottrell B, 1985, J Mater Sci Letters, 4, 1033-1035. Thouless MD and Evans AG, 1988, Acta Metall, 36, 517-522. Truss RW, Hine PJ and Duckett RA, 1997, Composites, 28A, 627-636. Vancon M, Odorico J and Bathias C, 1984, Comptes Rendus des Quatrièmes Journées Nationales sur les Composites (JNC4), (Editions Pluralis, Paris), 93-120. Waddoups ME, Eisenmann JR and Kaminski BE, 1971, J Compos Mater, 5, 446-454. Wang SS, Mandell JF and McGarry FJ, 1975, in Fracture Mechanics of Composites (editor GP Sendeckyj ), ASTM STP 593, 36-85. Wells J and Beaumont PWR, 1985, J Mater Sci, 20, 1275-1279. Wetherhold RC and Mahmoud MA, 1986, Mater Sci and Engg, 79, 55-65. Whitney JM and Nuismer RJ, 1974, J Compos Mater, 8, 253-265. Wu E, 1968, in Composite Materials Workshop ( editors. SW Tsai et al), (Technomic Press, Stamford, Conn., USA).
6. FATIGUE BEHAVIOUR OF FIBRE COMPOSITES6.1 INTRODUCTIONO ur familiarity with fatigue failure is so closely linked with the behaviour of isotropic, homogeneous, metallic materials that we have tended to treat modern fibre composites as though they were metals. The test methods used to study fatigue in metals have also been applied to composites, and the interpretation of the results of such tests has often been clouded by ourperception of what constitutes metallic fatigue failure. It is natural that a designer wanting to substitute acomposite for a metal component should want to test the new material by applying a cyclic loadingrégime of the same kind as the component would be required to sustain in service in order to prove thatthe composite will perform as well as the metal. But it must not be assumed, a priori, that there is someuniversal mechanism by which fluctuating loads will inevitably result in failure at stresses below thenormal monotonic failure stress of the material. Fatigue of metals accounts for a high proportion of engineering failures and has been intensivelystudied for more than a century. Design data have been accumulated for every conceivable engineeringmetal and alloy, and the engineer has access to a comprehensive set of rules, some empirical and somebased on scientific understanding, with which to cope with any given design requirement, although somedesigners often choose to ignore these rules. Fatigue in metals progresses by the initiation of a singlecrack and its intermittent propagation until catastrophic failure. This occurs with little warning and littlesign of gross distortion, even in highly ductile metals, except at the final tensile region of fracture. Inordinary high-cycle (low-stress) fatigue, where stress levels away from the crack tip are low, theproperties of the metal remote from the crack are only slightly changed during fatigue. It is not a generalfeature of fatigue in metals and plastics that the strength of the material is reduced by cyclic loading,although work-hardening or work-softening may occur in metals undergoing low-cycle (high-stress)fatigue. The usual effect of fatigue at low stresses is simply to harden the metal slightly. Generallyspeaking, a stronger material will have a higher fatigue resistance, the fatigue ratio (fatigue limit dividedby tensile strength) being roughly constant. It is not uncommon for users of composite materials, even in the aerospace industry, to express thebelief that composite materials — specifically, carbon-fibre-reinforced plastics — do not suffer fromfatigue. This is an astonishing assertion, given that from the earliest days of the development ofcomposites, their fatigue behaviour has been a subject of serious study, and what is usually implied isthat, because most CFRP are extremely stiff in the fibre direction, the working strains in practicalcomponents at conventional design stress levels are usually far too low to initiate any of the localdamage mechanisms that might otherwise have led to deterioration under cyclic loads. The idea of using composites, especially CFRP, only at very low working strains raises two importantissues. The first is the obvious one that by using expensive, high-performance materials at smallfractions of their real strength, we are over-designing or, in more cost-conscious terms, we are usingthem uneconomically. The second is that since anisotropy is a characteristic that we accept and evendesign for in composites, a stress system that develops only a small working strain in the main fibredirection may easily cause strains normal to the fibres or at the fibre/resin interface that may be highenough to cause the kind of deterioration that we call fatigue damage. In designing with composites,therefore, we cannot ignore fatigue. And it follows directly that, in addition to needing to understand themechanisms by which fatigue damage occurs in composites, we need access to procedures by which thedevelopment and accumulation of this damage, and therefore the likely life of the material (orcomponent) in question, can be reliably predicted. In this chapter, we shall concentrate mainly on the fatigue behaviour of polymer-matrix composites.Since the majority of accessible research studies have concerned these materials, it is inevitable that evena general picture of composites fatigue will be substantially coloured by our knowledge of fibre-
chapter six Fatigue e 131reinforced plastics (FRPs). Specific reference to metal- and ceramic-matrix composites will be madeafter a discussion of FRPs.6.2 DAMAGE IN COMPOSITES Unlike metals, composite materials are inhomogeneous (on a gross scale) and anisotropic. Theyaccumulate damage in a general rather than a localizedfashion, and failure does not always occur by thepropagation of a single macroscopic crack. The micro-structural mechanisms of damage accumulation,including fibre breakage and matrix cracking,debonding, transverse-ply cracking, and delamination,occur sometimes independently and sometimesinteractively, and the predominance of one or othermay be strongly affected by both materials variablesand testing conditions. At low monotonic stress levels, or early in the life Figure 6.1 Degradation of composite strength byof a composite subjected to cyclic loading, most types wear-out until the residual strength, σR, falls from theof composite sustain damage, and this damage is normal composite strength, σc, to the level of thedistributed throughout the stressed region, as fatigue stress, at which point failure occursdescribed in chapter 4, section 4.1.3. The damage doesnot always immediately reduce the strength of the composite although it often reduces the stiffness. Suchstrength reductions as might occur (in a process described as wear-out) are sometimes off-set in the earlystages of life by slight increases in strength, known as wear-in. These increases may be caused by suchmechanisms as improved fibre alignment which results from small, stress-induced, viscoelastic or creepdeformations in the matrix. At a later stage in the life the amount of damage accumulated in some regionof the composite may be so great that the residual load-bearing capacity of the composite in that regionfalls to the level of the maximum stress in the fatigue cycle and failure ensues, as shown schematically inFigure 6.1. This process may occur gradually, when it is simply referred to as degradation, orcatastrophically, when it is termed sudden-death. Changes of this kind do not necessarily relate to thepropagation of a single crack, and this must be recognized when attempting to interpret compositesfatigue data obtained by methods developed for metallic materials. When a pre-existing crack is present in a composite it may or may not propagate under the action of a cyclic load, depending upon the nature of the composite. In a metal-fibre/metal-matrix composite the fibre itself will be subject to conventional fatigue processes. Planar (or near-planar) crack propagation can occur with both fibres and matrix exhibiting normal signs of fatigue, as shown in Figure 6.2, and the material behaves simply like a homogeneous metal of higher strength than the unreinforced matrix. In highly anisotropic composites of high Vf the crack will often refuse to propagate normal to the fibres (mode 1) but will be diverted into a splitting mode. In composites like unidirectional CFRP this may result in a brittle, end-to-end splitting failure which simply eliminates the crack (Figure 6.3) while in a metal- matrix composite the splitting will be preceded by a localized but elongated region of intense plastic Figure 6.2. Fatigue fracture surface of an MMC deformation (McGuire and Harris, 1974). By contrast,consisting of tungsten filaments in an Al/4%Cu matrix showing brittle fracture of both fibres and matrix in GRP laminates containing woven-roving or(McGuire and Harris, 1974). Compare with Figure 5.2 chopped-strand mat reinforcement crack tip damage which shows a tensile fracture surface of the same composite.
chapter six Fatigue e 132may remain localized by the complex geometry longitudinal splittingof the fibre array and the crack may proceedthrough this damaged zone in a fashionanalogous to the propagation of a crack in aplastically-deformable metal (Owen and stressBishop, 1974).6.2.1 Definition of failure and Figure 6.3 End-to-end splitting parallel to fibres in a unidirectional composite, resulting in effective removal ofexperimental scatter the stress concentrator. Smith and Owen (1968) have demonstratedthe extent to which variability affects the results of fatigue tests and have emphasised the value ofreplicate testing. This variability stems not only from the statistical nature of the progressive damagewhich leads to fracture of a composite, but more particularly from the variable quality of commercialcomposite materials. They have also pointed out that in many kinds of composite the number of cycles tocomplete separation of the broken halves of a sample is a definition of failure that becomes quitemeaningless if the sample has lost its integrity and its ability to sustain an applied stress as a result ofextensive resin cracking, arguing the need for careful (and relevant) definition of the failure criterion.They have nevertheless shown that designs based on the use of debonding or the onset of resin crackingas failure criteria would drastically impair the economic use of GRP.6.3 REVIEW OF SOME CLASSICAL FATIGUE PHENOMENA6.3.1 Stress/life curves A good deal of the work that has been done on the fatigue of fibre composites reflects the much moreextensive body of knowledge relating to the fatigue of metals, and this is not altogether unreasonablesince the established methods of accumulating and analysingmetallic fatigue data provided a reliable means of describingfatigue phenomena and designing against fatigue. Theformidable treatise of Weibull (1959), for example, is avaluable source book for modern workers on compositesfatigue. The danger was, and is, in making the assumption thatthe underlying mechanisms of material behaviour that give riseto the stress/life (S/N or σ/logNf) curve are the same in metalsand composites (see Ashby and Jones, 1980, for a descriptionof the various kinds of metallic fatigue). Figure 6.4 Schematic illustration of the features of an S/N curve (sometimes Before the development of fracture mechanics and its use in referred to as a Wöhler diagram).treating metallic fatigue as a crack-growth problem, the onlyavailable design information on fatigue behaviour was the σ/logNf curve (Figure 6.4). It representeddirectly the perceived nature of fatigue in terms of experimental results, but gave no indication of themechanisms of fatigue damage, of the presence or behaviour of cracks, or of changes in thecharacteristics of the material as a consequence of the fatigue process. The curve represents the stress tocause failure in a given number of cycles, usually either the mean or median life of a series of replicatetests at the same stress. Despite the anomaly (from a mathematical viewpoint) of plotting the dependentvariable on the abscissa rather than vice versa, the σ/logNf curve is nevertheless a useful starting pointfor the designer, provided due attention has been paid to the statistical aspects of data generation, so thatthe apparently simple failure envelope which it defines is associated with failure probabilities rather thanwith some simplistic fail/no-fail criterion. It can then be used, as many designers prefer, without anyconsideration of the underlying fatigue damage mechanisms, despite the availability of rather betterfracture-mechanics methods. There is logic in using the semi-logarithmic form of the σ/logNf plot but there is no reason forsupposing a priori that the failure envelope would be linear on a log-log plot (Basquin’s Law formetals). Some stress/life plots are linear on both kinds of plot, some on neither. The knowledge that for
chapter six Fatigue e 133bcc metals and alloys such as steels, the σ/logNf curve flattened out at long lives (>107 cycles, say) andgave rise to a fatigue limit, or endurance limit, σe, which could be explained in terms ofdislocation/solute-atom models, and that the fatigue ratio, σt/σe, (σt is the monotonic tensile strength)was roughly constant for a given class of alloys, gave confidence to users of this kind of design data.Finally, there was no general idea that the metallic σ/logNf curve should necessarily extrapolate back toa stress level which was related to any monotonic strength property of the material (at Nf = 1 cycle, forexample).6.3.2 Constant-life diagrams In order to use stress/life information for design purposes, a common procedure was to cross-plot thedata to show the expected life (or expected stress for some particular probability of failure) for a givencombination of the alternating component of stress, σalt, defined as half the stress range, ½(σmax – σmin),and the mean stress, σm, which is ½(σmax + σmin). envelope representingThe stress ratio, R, is σmin/σmax. In metallic a given life or lifefatigue it was frequently assumed that fractioncompression stresses were of no significancebecause they acted only to close fatigue cracks,unlike tensile forces. Master diagrams of thiskind are presented in a variety of forms, all moreor less equivalent, but the most familiar is thatwhich is usually referred as the Goodman factored linediagram (Figure 6.5). For design purposes, itwas useful to have an equation to represent thefail/safe boundary in this diagram, and it is thelinear relationship of Figure 6.5 that isassociated with the name of Goodman (1899) Figure 6.5 Schematic illustration of a constant-life oralthough others have been proposed, including Goodman diagram. The stress σe is the endurance or fatiguethe earlier parabolic relationship of Gerber limit, and σt is the material tensile strength.(1874). The linear and parabolic ‘laws’ havebeen modified to include safety factors on one or both of the stress components. An important question,for metals as well as for composites, relates to the minimum amount of test data that is needed to definethe failure envelope with a level of reliability sufficient for engineering design of critical components.6.3.3 Statistical aspects of the analysis of fatigue data The mechanical properties of practical composites are almost always variable as a consequence of thevariability of the material quality. It is not surprising, therefore, that the variability of the fatigueresponse of a composite is even greater than that associated with metallic materials. Stress/life data maybe obtained by testing single samples at many different stress levels, or by carrying out replicate tests atrather fewer stresses: the latter is usually considered to be the more satisfactory method because itprovides statistical information at each stress, and provides probability/stress/life curves in addition tomedian-life or mean-life curves. One of the problems is to know how many replicate tests should be done at each stress level since,given the cost of fatigue-testing programmes, the smaller the number of tests that can be used toestablish a ‘safe’ σ/logNf curve, the better. From a statistical point of view it is usually accepted that atleast 20 replicate tests may be necessary before the user can have any confidence in a statistical analysisof results (see, for example, Lee et al, 1997). But when stress/life curves are required at, say, fivedifferent R ratios, even five tests at each stress level may be all that can be provided in a reasonableamount of time, especially at long lives. A variety of distributions have been used to characterize fatigue lives, but the three-parameterWeibull function, described in Appendix 2, is usually considered to be the most appropriate model forthis purpose. The form of the cumulative distribution function used for fatigue is:
chapter six Fatigue e 134 ⎡ ⎛ Nf − a ⎞ m ⎤ P(Nf ; a, b, m ) = 1 − exp⎢− ⎜ ⎟ ⎥ ..................................................................... 6.1) ⎢ ⎝ b ⎠ ⎥ ⎣ ⎦where P is the probability of a life Nf, and a, the location parameter, defines a number of cycles forwhich there is zero probability of failure. For metallic materials, the value of the shape parameter, m, isoften in the range 2 < m < 6 (Freudenthal and Gumbel, 1953), whereas several recent studies of CFRPfatigue suggest that for these materials 1 < m < 2 (Whitney, 1981; Harris et al, 1997). It is interesting tonote that for an m value of unity the Weibull model reduces to a simple exponential distribution. Theexponential distribution, which is sometimes used to model distributions of failure times for thereliability of a product, governs systems where age has no influence on the probability of failure. If acomponent survives for a length of service t, the probability of failure within a subsequent time intervalfrom t to (t + Δt) is λΔt, where λ is a constant for all t. Thus, failure is a random event, and the systemdoes not deteriorate as a result of service. We would not normally consider this as being applicable to thefatigue failure of reinforced plastics for which it is known that residual performance is certainly reducedas a result of the accumulation of damage. One reason why the data may appear to fit an exponentialdistribution is that the range of lives at a given stress level is often very wide, spreading sometimes overtwo decades or more. Whereas when viewed by eye on a logarithmic life axis this may not appear tooserious, when considered in the Weibull analysis as a linear function, Nf , rather than as a logarithmicfunction, logNf, the range could thus easily be judged to be bounded at the lower extreme at Nf = 0, andhence the distribution may appear exponential. In reality, the shape of the Weibull distribution changesfrom being of classical exponential form to being peaked over a very small range of values of m between1 and 2. Although we often work in terms of median or mean lives when discussing fatigue data, it isimportant to recognize that to the designer of critical structures, such as aircraft components, therequirements are much more restrictive, and it is likely that the desired failure probability for such astructure would be at a very low level, say 5%, instead of the 50% level implied by the median life. Aneven more appropriate ‘life’ parameter may be the minimum extreme value obtained from an applicationof the theory of extreme values (Castillo, 1988). Extreme-value models are appropriate models fordescribing many engineering phenomena and systems where the relevant parameters are thecharacteristic largest and characteristic smallest values of a distribution. For example, in the case of thelife of a gas-turbine disc fitted with a large number of blades, the turbine life is determined by the life ofthe shortest-lived blade — a ‘weakest-link’ model. Such a model, referred to as a Type III asymptotemodel, is also applicable to the fatigue behaviour of engineering materials. One of the characteristics of the Weibull model is what is known as its reproductive property (Bury,1975). A consequence of this property is that for a population of results that is well modelled by theWeibull distribution certain other features of the population, such as the minimum extreme values, willalso be described by a Weibull distribution. Put more formally, the exact distribution of the smallestobservations in sets of data that are described by a Weibull model also fits a Weibull model. Thus, if wehave replicate data sets of fatigue lives at a given stress and R ratio which is described by the two-parameter version of equation 6.1 (see Appendix 2), with shape parameter m and scale parameter b (abeing equal to 0), the smallest observations of these data sets also exhibit a Weibull distribution similarto that of the parent distribution and with the same value of the shape factor, m, but rescaled by n1/m. Thecharacteristic minimum value for a test sample of n tests will therefore be (b/n1/m) and the modal value ofthe distribution (ie. the most probable value) will be given by: 1 b ⎛ 1⎞m ⎜1 − ⎟ nm ⎝ m⎠ 1If, on the other hand, the desired level of failure probability happens to be the 5% level (q = 0.05), thenthe appropriate value of ‘life’ is given by:
chapter six Fatigue e 135 1 ⎡ ⎛ 1 ⎞ ⎤m b ⎢ln⎜ ⎟⎥ ⎣ ⎝ 1 − q⎠ ⎦ Thus, from a series of replicate data sets of fatigue lives at various cyclic stress levels, a stress/life/probability (or S/N/P) diagram resembling that shown in Figure 6.6 may be drawn, provided the distribution parameters, b and m, can be obtained for each data set. From a design point of view, the lower curve in this diagram, scatter in representing some given failure strength probability, is clearly of more scatter in fatigue lives interest to the engineer than any other part of the data, but it can only be obtained by statistical means which requires reliable values of the two distribution parameters, b and m. This, in turn, calls for replicate data sets of at least 20 test results for each stress level and R ratio, a requirement which carries with it a serious time/cost disincentive. Figure 6.6 Effects of variability in strength and fatigue life on the definition of However, Whitney (1981) has the σ/logNf curve. The scatterband of lives is jointly defined by the upper suggested that where only small and lower probability limits of the fatigue data sets and the monotonic numbers of life values are strength distribution. available at a number of different stress levels, the data may be pooled to give an overall value of the Weibull shape parameter, m, this value then being used to obtain working stress/loglife curves for any given failure probability. This is done by normalising each test-stress data set with respect to either the characteristic life, b (the scale factor of the Weibull distribution for the data set) or the median life for the data set, pooling all data sets for all stress levels and all R ratios, and then re-ranking them in order to allot a new failure probability function to each point (see Appendix 2 for a discussion of ranking methods). The virtue of this procedure is that a much larger population is being used to derive the value of the Weibull shape parameter and calculations of an expected life based on that m value will be much more reliable than ones obtained from the much smaller data sets for 2 each individual stress level. The Weibull distribution for a pooled fatigue data set for a 1 carbon-fibre composite laminate is shown in 0 Figure 6.7. The shape parameter for the pooledLn[-ln(1 - P)] -1 data is 1.1, and is similar to values obtained for other CFRP laminates by, for example, Whitney -2 (1981) and Harris et al (1997). The value of m -3 obtained in this way can then be used, as shown above, to derive stress/life curves for desired -4 failure probability levels -5 slope, m = 1.1 -6 6.3.4 Cumulative damage laws -5 -4 -3 -2 -1 0 1 2 3 In most fatigue environments the mean and Ln(Nf) alternating stress amplitudes vary and may be presented as a spectrum of the frequency of Figure 6.7. Two-parameter Weibull plot for pooled, occurrence of different stress levels. The conceptnormalized fatigue data for a [(±45,02)2]S T800/5245 CFRP of deterioration as a result of damage laminate. The pooled data are for all stress levels at 5 different R ratios (Gathercole et al, 1994). accumulation within the material with stress cycling is used in combination with the notion of residual strength, and the damage is quantified such that a parameter Δ represents the fraction of
chapter six Fatigue e 136catastrophic damage sustained after n cycles (where n < Nf ) so that at failure Δ = 1 and n = Nf. Thus, Δirepresents the fractional damage after cycling at a stress σi for a fraction of life ni/Ni. Various proposalsfor damage laws have been derived, the most common of which is the Palmgren-Miner linear damagerule (Miner, 1945). The accumulation of damage is supposed to be linear with number of cycles, and isapparently independent of the value of the stress: Δ = n/N .................................................................................................................. 6.2)Thus, if the load spectrum is divided into blocks with ni cycles at stress levels σi, then equation 6.2applies incrementally to each block and the total damage is the sum of the individual ‘block’ damages,irrespective of the order of their application, so that: ni Δ= ∑N ( = 1 for failure) ................................................................................. 6.3) i This well-known, though rarely obeyed, rule was originally proposed for the prediction of the life ofmetallic components undergoing fatigue, and although it is a standard feature of text-book presentationsof fatigue it has always been viewed with great suspicion by designers because it is often found to givenon-conservative results, ie. to predict lives greater than those observed experimentally. The simpleconcept of damage defined by equation 6.3 is not, of course, a mechanistic concept. It has been appliedto many kinds of engineering materials, regardless of the actual nature of the damage mechanisms thatcontribute to the gradual deterioration and ultimate failure of an engineering component subject to cyclicloading. The simplest step forward from the linear damage rule is to look for non-linear functions that stillemploy the damage parameter Δ, as defined by equation 6.3. In the Marco-Starkey (1954) model, forexample, a simple non-linear presentation suggests an equation of the form: Δ = (n/N)β ............................................................................................................... 6.4)where β is a function of stress amplitude. The condition for failure when Δ = 1.0 is satisfied and theMiner rule is a special case of this law with β = 188.8.131.52 FATIGUE OF REINFORCED PLASTICS6.4.1 Constant-stress fatigue curves The dominant damage mechanisms in FRP vary both with the nature of the composite (the particularcombination of fibres and matrices, reinforcement lay-up, etc.), and with the loading conditions (tension,bending, compression, etc.), and results for any one material under a given stress condition may appearto fit no general pattern. This is easily illustrated with reference to the gradual accumulation of resultsand materials development over the last two decades or so. First, the forms of stress/life curves for various kinds of GRP have long been familiar to researchers,as was the fact that the fall of the curve with reducing stress was considerable. This fall, or averageslope, is an indication of the fatigue resistance of the material, a more rapid fall being indicative of agreater susceptibility to fatigue damage. Mandell (1982) attempted to show that fatigue damage in GRPmaterials can be explained simply in terms of a gradual deterioration of the load-bearing fibres. Heanalyses a great range of experimental data to demonstrate that the behaviour of composites with long orshort fibres, in any orientation, and with any matrix, can be explained in this way. He does this byeffectively forcing σ/logNf curves to fit a linear law of the form: σ = σt – BlogNf ...................................................................................................... 6.5)
chapter six Fatigue e 137where σ is the peak cyclic (tensile stress), σt is the monotonic tensile fracture stress, Nf is the fatigue lifeof the material at stress σ, and B is a constant, as illustrated in Figure 6.8. For a wide and disparate rangeof GRP materials, including moulded reinforced thermoplastics, Mandell obtained a constant value ofabout 10 for the ratio σt/B, with very little spread. In principle, the idea that the controlling mechanismin fatigue of composites is the gradual deterioration of the load-bearing fibres is logical and inevitable.What controls the actual life of any given sample or composite type is simply the manner in which othermechanisms, such as transverse-ply cracking in 0/90 laminates, or local resin cracking in woven-clothcomposites, modify the rate of accumulation of damage in the load-bearing fibres. Nevertheless, a singlemechanistic model which includes randomly-reinforced dough-moulding compounds and injection- moulded thermoplasts as well as woven and non-woven laminates is unexpected. 1500 The σ/logNf curves for many GRP Tensile strength, σt , MPa materials are not linear, however, as illustrated by the selection of data for a 1000 group of glass-fibre composites shown in Figure 6.9. With GRP there are two factors which complicate the appearance 500 of the stress/life curves. As a consequence σt /B = 10.4 of the high failure strain of the glass fibres and their sensitivity to moisture, 0 i) the tensile strengths of GRP materials 0 50 100 150 are sensitive to strain-rate and Slope of stress/loglife curve, B, MPa/decade temperature, and ii) during cycling at large strains there is Figure 6.8. Relationship between composite tensile strength and usually a significant rise in temperature the slope of the fatigue σ/logNf curve (after Mandell, 1982). Data as a result of hysteretic heating which points taken from the literature represent a wide range of GRP is not easily dissipated by the non- composites. conducting constituents of the GRP.The consequences of this have been demonstrated by Sims and Gladman (1978). First, when fatigue testsare carried out at constant frequency over the whole stress range of interest, the deformation rate isusually considerably greater than the rates normally used for measuring the monotonic strength, and as aresult, since it is common for the strength to be included, as shown in Figure 6.9, as the point on theextreme left of the σ/logNf curve (ie. notionally 2.0at Nf = 0.5 for a repeated tension test, or Nf = unidirectional [(0,90)2]S (prepreg)0.25 for a fully reversed tension/compression [(±45,02)2]Stest) that measured strength is often actually 1.5 Peak stress, GPa 0/90 (woven)lower than a value measured at the fatigue-test chopped-strand matfrequency. Second, if tests are run at constant dough moulding compound 1.0frequency, the effective strain rate at each stresslevel will be different (higher at lower stresses),and the measured life values for each stress will 0.5not be associated with a common base-line ofmaterial behaviour: ie. the fatigue curve willrefer to a range of stresses, σ, which are 0 -1 0 1 2 3 4 5 6 7 8proportions of a variable material property, say LogNfσt( ε ), instead of the material property that we &normally define as the strength, σt. And third, Figure 6.9. Stress/loglife curves for a range of GRP materialsas the peak stress level falls and the life of the at an R ratio, σ /σ , of 0.1. Data points are omitted for min maxsample extends, the degree of hysteretic heating clarity, but may be found in the original diagram (Harris,rises, and the effective baseline strength of the 1994). The stress for a ‘life’ of 0.5 cycles is the monotonicmaterial therefore also falls, so reversing the tensile strength measured at a loading rate equivalent to that used for the fatigue tests.effect of the higher effective deformation rate.
chapter six Fatigue e 138 As Sims and Gladman pointed out, the only way to avoid the effects of these interacting processes is to ensure that all σ/logNf curves for GRP materials are determined at a fixed rate of load application (RLA), that the material strength is measured at the same RLA, and that the hysteretic effects are either eliminated or accounted for. These corrections can make substantial differences to the shapes of stress/life curves and to the validity of the design data obtained from them: many otherwise curved σ/logNf graphs are also rendered more linear by these corrective measures. By contrast with GRP, carbon-fibre composites are largely rate insensitive and because they deform less than GRP under working loads and are reasonably highly conducting, hysteretic heating effects are usually insignificant (Jones et al, 1984). Some of the earliest CFRP, reinforced with the HM (high- modulus, or Type 1) species of carbon fibre had such low failure strains that fatigue experiments in tension were extremely difficult to carry out, and some of the first tension σ/logNf curves published (Beaumont and Harris, 1972; Owen & Morris, 1972) were almost horizontal. The S/N line hardly fell outside the scatterband of measurements of the monotonic tensile strength, the fatigue response being effectively dominated by tensile failure of the fibres alone and the slight reduction in resistance after 106 or 107 cycles appeared to be a result of small viscoelastic (creep) strains rather than to cycling effects per se (Fuwa et al, 1975). Only in torsion or bending tests was the slope of the σ/logNf increased as these different stress systems allowed other damage mechanisms to occur. A very small failure strain is often a disadvantage in engineering materials (some of the early CFRPs were extremely brittle) and developments in carbon-fibre manufacture led to materials that possessed higher failure strains (lower elastic moduli), although these improvements were often offset by concomitant reductions in strength. By the end of the 1970s, the most common polyacrylonitrile-based fibres, designated HMS, HTS and XAS, covered a range of moduli from about 400GPa down to 200GPa, and the tensile stress/loglife data for these materials fell approximately on straight lines with slopes which increased with decreasing fibre stiffness (Sturgeon, 1973). This is roughly in accord to with the Mandell model except that Mandell’s correlation was with composite strength rather than stiffness. Increasing awareness on the part of designers of the qualities of fibre composites, and of carbon-fibre composites in particular, resulted in demands for fibres with combinations of strength and stiffness which were different from those which characterized the earlier materials. A particular call was for higher failure strains in association with high strength, and these demands led to developments in carbon-fibre manufacture and the availability of a much wider range of fibre characteristics. The fatigue performance of composites based on these newer fibres is clearly different from that of earlier CFRP, as illustrated by the range of results shown in Figure 6.10. These data are all for composites with the lay-up [(±45,02)2]s and the curves are polynomial fits to experimental data. Perhaps the most notable feature of this collection of data is that the monotonic strength characteristics of the reinforcing fibres are not directly translated into the fatigue response, ie. the strongest fibres do not always generate the most 1.75 fatigue-resistant composites. And whereas the earliest of CFRP composites had approximately 5 IM7/977 7 6 T800/924 linear, or even slightly upward turning σ/logNf 1.50 curves, the newer, increasingly ‘high-Peak stress, GPa 7 T800/5245 6 performance’ composites show downward 5 curvature. We note that none of these curves for 1.25 4 3 the newer materials has reached any kind of 2 stable fatigue limit within the convenient 1 XAS/914 1.00 2 XAS/913 laboratory test window extending to 107 cycles. 3 HTA/913 1 4 T800/6367 This downward curvature also occurs in 0.75 composites reinforced with Kevlar-49 aromatic 0 1 -1 2 3 4 5 6 7 8 LogNf polyamide (aramid) fibres (Jones et al, 1984; Fernando et al, 1988). Typical behaviour of aFigure 6.10. Median stress/loglife curves at R = 0.1 for seven cross-plied KFRP composite is compared with varieties of carbon-fibre composite, all with the lay-up those of similar GRP and CFRP materials in [(±45,02)2]S (Harris et al, 1997). Figure 6.11, plotted here in terms of initial peak
chapter six Fatigue e 139strain, rather than stress. The composites are comparable in every respect except for the reinforcingfibres. The performance of the KFRP over the first three decades is similar to that of the CFRP on anormalized basis in that the slopes of the strain/life curves are similar. At maximum cyclic strain (orstress) levels only marginally below the tensile-failure scatter band, however, the fatigue resistancedeteriorates rapidly, and a change in controlling failure mode occurs. At the highest stress levels (firstthree or four decades in Figure 6.11) failure of the KFRP occurs by the normal fibre-dominated failureprocess. At lower stresses, however, (much larger numbers of cycles) the internal structural weaknessesof the aramid filaments are exposed to the effectsof the cyclic stress and the fibres themselves 5exhibit much lower fatigue resistance. This GRPapparent weakness can be overcome to some 4 Initial tensile strain, %extent by preventing complete unloading of thecomposite between cycles. Effectively, the down- 3 KFRPturn of the σ/logNf curve, which is not seen in the0/90 CFRP in Figure 6.11, can be delayed by 2raising the minimum cyclic stress level. 1 These results for carbon, glass and aramid CFRPlaminates illustrate very well a strain-control 0model of fatigue proposed by Talreja (1981). He -1 0 1 2 3 4 5 6 7 8suggests that the strain/loglife curves for polymer- LogNfmatrix composites may be thought of in terms ofthree régimes within which separate mechanisms Figure 6.11. Strain/life curves for [(0,90)2]S laminates ofcontrol fatigue failure. At high stress levels fibre composites reinforced with HTS carbon, Kevlar and E-breakage occurs (with or without interfacial glass fibres in a Code-69 epoxy resin (Fernando et al, 1988: repeated tension fatigue, R = 0.1: RH = 65%).debonding) which leads to failures within thenormal tensile failure scatter band of the 0° plies.At lower cyclic stress levels, however, although statistical fibre breakage still occurs, it does not lead sorapidly to composite destruction and other competing mechanisms then have time to occur. These othermechanisms — matrix cracking, interfacial shear failure, etc. — can then influence the overall damagestate provided the composite working strain level is sufficiently high, and the slope of the strain/loglifecurve therefore begins to fall. There is, however, some notional fatigue-limit strain for the matrix itselfand if working strains do not rise above this level the composite should not, in principle, fail in fatigue.The strain/loglife curve ought therefore to flatten out again and something in the nature of an endurancelimit should be observed. Whether or not some or all of these stages are observed will clearly depend onthe characteristics of the constituents and the lay-up geometry. In Figure 6.11, where the influence of thefibre deformation characteristics is more visible than in a stress/life plot, it can be seen that high workingstrains in the GRP prevent the establishment of stage 1 of the Talreja model, the curve moving almostimmediately into stage 2, whereas the higher stiffness of the Kevlar fibre delays this transition in thearamid composites. Working strains in the CFRP are rarely sufficiently high as to exceed the matrixfatigue limit and so the strain/life curve (like the σ/logNf curve) retains the low slope, characteristic ofstage 1, for the entire stress range shown. It can be seen from the shapes of the σ/logNf curves forvarious CFRP materials in Figure 6.10 that many of these high-performance composites exhibit similarfeatures in tensile fatigue, regardless of the specific nature of the degradation mechanisms, although theextent to which some or all of the stages of Talreja’s model are visible within a practical experimentaltest window depends on the nature of the constituents and of the fibre/matrix bond.6.4.2 Materials factors affecting fatigue behaviour of reinforced plastics Brittle fibres like glass, boron and carbon should not show the characteristic weakness of metalsunder fatigue loading conditions. Composites containing them should also, therefore, in principle, befatigue resistant if the fibres carry the major part of the load and provided the reinforcing phase is not soextensible as to permit large elastic or viscoelastic deformations of the matrix as a function of time.These conditions are fulfilled when composites unidirectionally reinforced with high-modulus fibres likecarbon or boron are tested in repeated tension, and their σ/logNf curves are, in general, very flat. Ascycling continues, however, even small viscoelastic movements in the resin lead to local redistributions
chapter six Fatigue e 140of stress which permit some random fibre damage to occur, and similar damage will occur in theneighbourhood of any stress concentrations. As a function of time, then, rather than as a function of thenumber of stress reversals, damage levels will build up to some critical level when the compositestrength is no longer above the peak cyclic stress level, and failure will occur. When the stress is not simply tensile, uniaxial, and aligned with the fibres more severe loads areplaced on the matrix and the fatigue resistance of the composite is reduced. This occurs in simpleflexural fatigue (Beaumont and Harris, 1972) and tension/compression loading of undirectionalcomposites, and also in fatigue tests on any kind of laminated materials. Ramani and Williams (1976),for example, tested 18-ply, (0,±30) carbon/epoxy laminates in various combinations of axialtension/compression cycling and showed an increasingly adverse effect on fatigue resistance as thecompressive stress component was increased. Kunz and Beaumont (1975) and Berg and Salama (1972)showed that fatigue cracks propagated in CFRP during purely compressive cycling through thespreading of zones of fibre buckling failure. As we saw in chapter 4, compressive buckling is acharacteristic mode of failure in fibre-reinforced materials of many kinds and it is usually initiated bylocal matrix shear failures, sometimes associated with debonding in imperfectly bonded composites.Ramani and Williams observed extensive shear damage resulting from matrix shear and frominterlaminar and interfacial weakness. Compression and shear stress systems will 200 also be likely to be even more damaging to composites containing aramid fibres than to CFRP CFRP or GRP, as indicated by the poor Peak stress, MPa 150 GRP KFRP compression response of KFRP described in chapter 4. The shear weakness is also clearly 100 manifested in tensile fatigue of ±45 KFRP laminates, by comparison with similar samples 50 of CFRP and GRP, as shown in Figure 6.12. In this mode of stressing the matrix and interface would normally be expected to dominate 0 -1 0 1 2 3 4 5 6 7 8 composite behaviour, the fibre characteristics LogN f playing little part. This is demonstrated in Figure 6.12 by the CFRP and GRP results, but Figure 6.12. Stress/loglife curves for the same materials as the intrafibrillar weakness of the aramid fibre those of Figure 6.11 but tested at 45°to the main fibre results in a considerable reduction in composite directions: R = 0.1; RH = 65% (Jones et al, 1984) fatigue resistance, and microscopic observations of KFRP samples that have failedin this mode clearly show the kinking and splitting of the fibres resulting from this weakness (Figure6.13). Similarly, when tested in torsion the weak parts of a composite (ie. the resin and the interface) areloaded directly by the shear forces the strength and rigidity of the fibres contributing relatively little tofatigue resistance and the torsional rigidity of the material falls substantially during cycling. Sometypical shear strain/loglife curves for two types ofunidirectional carbon/epoxy composites are shown inFigure 6.14 (Phillips and Scott, 1976). The curves wereobtained under constant angular (torsional) cyclingconditions and the fatigue life is defined as the number ofcycles to the occurrence of cracking. There is much evidence from fatigue tests on reinforcedplastics that the matrix and interface are the weak links asfar as fatigue resistance is concerned. It appears that lowerreactivity resins give better low-stress fatigue life in GRP,the optimum resin content being between 25 and 30 vol.%,although variations in resin content affect the fatigue Figure 6.13. Splitting and kinking damage instrength at 106 cycles hardly at all by comparison with Kevlar-49 fibres after fatigue cycling (Fernando et al, 1988)
chapter six Fatigue e 141their effect on tensile strength (Owen,1970). By contrast, variations in resin 0.06properties appear to have little effect on the epoxy resinfatigue strength of CFRP (Owen and Morris, 0.05 Shear strain amplitude1970). Any materials treatment or 0.04processing that can improve the resistance of HT-carbon/epoxythe matrix to crack propagation or the 0.03interfacial adhesion is likely to improvefatigue properties. Conversely, exposure of 0.02reinforced plastics to water often results in HM-carbon/epoxysome degree of plasticization of the matrix 0.01and weakening of the interfacial bond, andin GRP and aramid-fibre composites it may 0 -1 0 1 2 3 4 5also affect the performance of the fibres LogNfthemselves (Jones et al, 1984). It followsthat the fatigue of almost all FRP will beenvironment sensitive, the least sensitive carbon/epoxy 6.14. Strain/loglife curves for unidirectional Figure composites together with that of the unreinforcedbeing those consisting of moisture-resistant matrix resin. The reinforcements are type 1 (high-modulus)plastics like the polyaryls (PEEK, etc.) and type 2 (high-strength) carbon. The curves were obtainedreinforced with carbon fibres which are under constant angular (torsional) cycling conditions. Thethemselves insensitive to degradation in fatigue life is defined as the number of cycles to the occurrence of cracking. (Phillips and Scott, 1976)moist atmospheres (Dickson et al, 1985). For manufacturing reasons (eg. to secure good ‘drape’ characteristics when doubly curved surfacesare required) there is considerable advantage in using woven fabrics as reinforcements. Some of theeffects of this on strength and toughness have already been seen in previous chapters, and it would beexpected that these effects might follow through into the fatigue response. Curtis and Moore (1985)showed that both the monotonic tensile strength and the fatigue strengths of CFRP laminates reinforcedwith woven fabric were significantly poorer than the properties of similar materials made with non-woven fibres, largely as a consequence of the distortion in the load-carrying 0° fibres and the stressesinduced at weave cross-over points. However, when the fabric was oriented at 45° to the loadingdirection both tensile and fatigue performances were slightly better than for non-woven material.184.108.40.206 Hybrid Composites The simplest expectation for the fatigue stress/life curve of a hybrid laminate would be that it wouldfall between those of the two single-fibre components, but published results do not offer an obviouspicture on which to base predictive models. It would be expected that the overall fatigue response woulddepend upon the extent to which the particular fibre mix controlled strain levels in the composites, and,if aramid fibres were involved, on the extent to which the intra-fibrillar weakness of that fibre wasexposed to the stress. Some early experiments by Phillips et al (1976) on woven-cloth GRP/CFRPlaminates suggested that adding CFRP to GRP improves its fatigue resistance more or less in proportionto the amount of CFRP added, ie. in accordance with the rule of mixtures. Hofer et al (1978) also foundthat the fatigue stress of unidirectional HTS-carbon/S-glass hybrids obeyed the rule of mixtures when inthe as-manufactured state, but showed a positive deviation from linear when the composites werehygrothermally aged. Fernando et al (1988) found that the failure stresses for lives of 105 and 106 cyclesfor unidirectional carbon/Kevlar-49/epoxy hybrids were linear functions of composition for bothrepeated tension and tension/compression loading. But since the tensile strengths of the same series ofhybrids were given by the failure-strain model (Chapter 4, section 4.19), the fatigue ratio (fatigue stressfor a given life divided by the tensile failure stress) showed a marked positive deviation from the linearweighting rule. The same workers (Dickson et al, 1989) found that unidirectional CFRP/GRP fatiguestrengths fell above a linear relationship, and the fatigue ratio therefore showed an even more markedpositive synergistic effect. This suggests that factors controlling monotonic tensile (and compression)failure do not necessarily continue to determine failure under cyclic loading conditions, and that forfatigue applications there appear to be positive benefits in using hybrids in place of single-fibrecomposites.
chapter six Fatigue e 14220.127.116.11 Short-fibre composites Although the fatigue resistance of high-Vfcomposites reinforced with continuous, 2.5aligned, rigid fibres is usually high, short-fibrecomposites of all kinds are much less resistant 2.0 long fibresto fatigue damage because the weaker matrix Peak stress, GPais required to sustain a much greater 1.5proportion of the fluctuating load. Localfailures are easily initiated in the matrix and 1.0 short fibresthese can destroy the integrity of thecomposite even though the fibres remain 0.5intact. The interface region is particularlysusceptible to fatigue damage since the shearstresses at the interface may be reversing their 0 -1 0 1 2 3 4 5 6 7 8direction at each cycle and there is always a LogNfhigh shear stress concentration at fibre ends. Itis also possible that in both random and Figure 6.15. Stress/loglife data for unidirectional composites ofaligned short-fibre composites the ends of XAS/914 carbon/epoxy laminates reinforced with continuousfibres and weak interfaces can become sites and discontinuous fibres (R = 0.1) (Harris et al, 1990).for fatigue-crack initiation. The beneficial effects of short fibres in materials like injection-moulding compounds have been well-known for 40 years or more, and although increases in strength in such materials are modest, increases intoughness are much greater for the reasons discussed in Chapter 5. Since fatigue resistance depends inpart on strength and in part on crack resistance, it would therefore be expected that these benefits wouldbe advantageously translated into fatigue response. Lomax and O’Rourke (1966) reported that theendurance limit of polycarbonate at two million cycles is increased by a factor of seven when thepolymer is filled with 40vol.% of 6.4mm long glass fibres. Lavengood and Gulbransen (1969)determined the number of cycles to failure of short-fibre boron/epoxy composites and found that forcycling at any given fraction of the failure stress the fatigue life increased rapidly with fibre aspect ratio,levelling off at l/d ratios of about 200. This therefore represents a critical aspect ratio above which thefatigue strength is a constant proportion of the flexural strength, as shown in Figure 6.16. These authorsalso studied the behaviour of aligned asbestos/epoxy composites and found them to behave in roughlythe same way as boron/epoxy composites containing 25mm-long fibres. Owen et al, (1969) showed thatthe fatigue strength at a million cycles of polyesterresin reinforced with random glass-fibre mat varied 106between 15 and 45% of the ultimate tensilestrength. Huffine et al (1973) studied the tension Fatigue life, Nf cyclesand flexural fatigue behaviour of glass/epoxycomposites containing 44 vol.% of aligned E-glass 105fibres 12.5mm long. Their results suggested thatthis material was potentially useful for dynamic 60%structural applications since it appeared to have anendurance limit of 40% of the ultimate tensile 104 70% 80%strength. 90% A comparison of the relative fatigue responses 103 1of composites containing continuous and 10 102 103discontinuous fibres is shown in Figure 6.15. The Aspect ratio of fibreresults are for unidirectional composites of thesame carbon/epoxy system, XAS/914, in which the Figure 6.16. Fatigue life versus aspect ratio for an appliedwell-aligned prepreg for the short-fibre material, stress of the indicated percentage of the composite tensilecontaining chopped fibres 3mm long, was strength. The materials are short-fibre-reinforcedproduced by the glycerol-alignment method boron/epoxy composites; repeated tension (Lavengood &described in Chapter 2: the fibre volume fraction is Gulbransen, 1969).
chapter six Fatigue e 1430.35. The continuous-fibre laminate was produced from normal commercial prepreg. It can be seen thatalthough the strength of the short-fibre composite is much lower than that of the continuous-fibrelaminate, its fatigue response, as characterized by the slope of the σ/logNf curve, is better. In fact, if thefatigue data are all normalized with respect to the monotonic tensile strengths of the two materials, therate of fall-off is much greater for the conventional laminate. Working with similar aligned short-fibrecomposites, Moore (1982) also found that the fatigue behaviour of these materials compared favourablywith those of continuous-fibre composites, although progressive cracking occurred from the fibre endsand fibre surface effects appeared to give more problems. It is assumed, therefore, that less fibre damageresulting from fatigue can occur if the fibres are already short, and the short-fibre ends apparently do notact as sources of excessive damage. It is not certain what the effect of fibre length would be in alignedcomposites such as these, but Hitchen et al (1995) have shown that in random-short-fibre carbon/epoxycomposites the fatigue life is independent of fibre length at any stress level. They also showed that themore flexible the matrix, the shorter the fatigue life. Friedrich et al (1986) found that the incorporationof short glass or carbon fibres into PEEK to produce injection-moulding compounds produced onlyslight improvements in the fatigue and fracture toughness of this material. Harris et al (1977) studied the fatigue behaviour of commercial polyester DMC in both the dry andwet-aged conditions and for samples with drilled holes. Their results were characterized by a good dealof scatter, but indicated that in the low-stress (long-life) range the effects of moisture and stressconcentrations were less marked than in the higher stress range. They showed that when their resultswere normalized by dividing by tensile strength, the σ/logNf curve for the DMC fell only slightly morerapidly than the curves for other types of GRP (see Figure 6.9). Atzori et al investigated the effects of awide range of material and environmental variables on the fatigue behaviour of moulding compoundsand developed a rule for estimating the fatigue strength from the monotonic tensile strength that was amodification of that of Mandell described in section 0. In some cases the fatigue resistance of the matrix plastic has been found to be diminished byreinforcement with short fibres. For example, Shaver and Abrams (1971) found that randomly reinforcedglass/Nylon composites had only half the endurance of the unfilled polymer. It should also be noted thatthe fatigue behaviour of most reinforced plastics will always be worse when the material is exposed to awet environment.6.4.3 Other factors affecting the fatigue of reinforced plastics18.104.22.168 Machines and specimens Testing machines of most kinds have been used for reinforced plastics, but testing rates must usuallybe carefully chosen to avoid excessive temperature increases caused by hysteretic heating. Heatdissipation by conduction is poor in many reinforced plastics, and even in CFRP it may be too low toprevent some temperature rise. In polymeric materials, quite small temperature increases maysignificantly change the mechanical properties, and excessive heating will also lead to thermaldegradation. Recommendations of appropriate testing methods for reinforced plastics have been made byOwen (1970). Choice of appropriate specimen shape is strongly influenced by the characteristic natureof the composite being tested and has given rise to some difficulties. Early attempts to use test specimenssimilar to those used for metals led to unrepresentative modes of failure in composites that (a) werehighly anisotropic and (b) had relatively low in-plane shear resistance, although techniques for testingmost kinds of GRP had been early established by Boller (1959, 1964). Much early work was carried out on waisted samples of the conventional kind, and designs wereadapted for unidirectional CFRP and similar composites by using long samples with very large radii andrelatively little change in cross-section in the gauge length. An alternative approach that has been used toprevent the familiar shear splitting in composites of low shear resistance (illustrated in Figure 6.3) was toreduce the sample thickness rather than the width, but this has now been almost universally supersededby the technique of using parallel-sided test coupons with end-tabs, either of GRP or soft aluminium,bonded onto the samples for gripping. Carefully done, this eliminates the risk of grip-damage (and
chapter six Fatigue e 144resultant premature failure) without introducing significant stress concentrations at the ends of the testlength and failures can usually be expected to occur in the test section. Although sample size can have significant effects on the fracture toughness of metals it is not usuallyconsidered that fatigue tests on very small samples are likely to be unrepresentative of the material as awhole. In composite materials, however, the inhomogeneity resulting from the fibre distribution may begreat enough to influence the fatigue response of a sample the size of which is comparable with the scaleof the inhomogeneity. Thus, in woven-roving laminates, the width of a test piece should be sufficientlygreat to include several repeats of the weaving pattern. Similarly, a test piece for a hybrid laminate mustbe an order of magnitude or so greater than the scale of the hybridization.22.214.171.124 Frequency and related effects Testing has often been carried out at the highest testing rate that could be used without causingexcessive heating of the sample. But even in CFRP, which are fairly good conductors, the occurrence ofprogressive damage, leading to lower stiffness and larger strains during a test, will give rise to hystereticheating which may affect fatigue behaviour. In the presence of pre-existing design features like holes, orof growing cracks, high local temperature rises may occur at quite modest applied loads, as shown inFigure 6.17. The use of available σ/logNf fatigue data for many reinforced plastics for design purposes istherefore complicated by uncertainty about the separate effects of frequency and autogenous heating ofsamples tested at different rates — an uncertainty that is exacerbated by the high degree of scatternormally found in fatigue-test results for these materials. Normalization of test data in terms of themonotonic tensile strength is also likely to lead to confusion because of the strong temperature- and rate-dependence of the monotonic mechanical properties of some reinforced plastics (particularly GRPs). As mentioned earlier, Sims and Gladman (1978, 1980) have attempted to resolve the problem bystudying the tensile and repeated tension (R = 0.1) behaviour of glass/epoxy laminates at constant rate ofstress application instead of constant testfrequency, a procedure which avoids the confusion 50of the varying loading rate in conventionalconstant-frequency sine-wave fatigue-test routines. 30Hz 40 stress ratio,By monitoring the specimen temperature rises R = 0.067 ΔT, deg. Cduring tests at different rates of loading, they were 30able to show that the temperature-dependence ofthe composite tensile strength transposed directly 20to the fatigue strength. They showed that fatiguetests at different rates could be normalized with 10Hzrespect to the tensile strength measured at the 10 3Hzsame rate of stress application to give a single, 1Hzlinear, master fatigue curve. The corrections make 0 2 3 4 5substantial differences to the interpretation offatigue results, especially at longer lives. Their LogNmodel is valid for materials of variousconstructions and is also able to take into account Figure 6.17 . Rise in sample temperature during cycling at different frequencies: 8-ply ±45 CFRP laminate (Sun andthe effects of moisture in modifying the tensile Chan, 1979)properties.126.96.36.199 Effects of holes and notches There has been some disagreement about the effects of holes and notches on fatigue resistance ofcomposites, perhaps because we are often tempted to generalize about the class of materials we call‘composites’ which, in reality, encompasses a wide range of materials of very different character. A briefsurvey of some of the available results will illustrate the danger in such generalisation. Boller (1957, 1964) found that in GRP sharp notches were more detrimental than drilled holes, butthat notches in general had little effect on fracture strength because of the large number of debondingsites present in the material to begin with. He also showed that small holes had no effect on long-life
chapter six Fatigue e 145fatigue behaviour, presumably because progressive damage quickly removed the stress concentrationdue to the hole. Studies of the notch sensitivity of GRP by Prabhakaran and Sridhar (1975) confirm thatvalues of the fatigue strength reduction factor, Kf, fell during cycling. Owen and Bishop (1972), on the other hand, showed that holes are effective in initiating fatiguedamage although they do not always affect final failure. They found that a circular hole acts as a stressconcentrator at the onset of damage with reduction of the fatigue strength by a factor between 2 and 4 inmany GRP materials and up to 10 in unidirectional GRP. They were also able to predict the fatiguestress for the onset of damage fairly accurately from a knowledge of the properties of plain samples anda stress analysis of the hole. Shütz and Gerharz (1977) showed that the notch sensitivity of(02,±45,02,±45,90)S carbon/epoxy laminates changed during cycling in such a way as to eliminate thestress concentration almost completely, whereas the opposite effect occurs during the fatigue cycling ofmetals. This progressive neutralisation of notches, which is often accompanied by an increase in residualstrength, occurs by a variety of splitting mechanisms, especially longitudinal splits in 0° plies tangentialto the hole. The accompanying reduction in notch sensitivity can even lead to fractures away from thecross-section containing the hole. This effect has also been observed in random, short-fibre compositessuch as polyester moulding compounds (DMC) (Harris et al, 1977). More recent work on DMCs andSMCs by Atzori et al (1994) also suggest that the fatigue properties of notched samples are similar tothose of un-notched ones. Curtis and Moore (1985) showed that woven-fabric CFRP composites wereslightly more notch-sensitive in fatigue than non-woven composites. Xiao and Bathias (1994) showedthat the fatigue ratio of woven-fabric-reinforced glass/epoxy composites was unaffected by the presenceof notches. And Kawai et al (1996), comparing the behaviour of Nylon and epoxy composites reinforcedwith woven carbon fibres, found that un-notched samples of the carbon/Nylon had a higher fatiguestrength that the carbon/epoxy material, whereas when notches were introduced, the relativeperformance of the two materials was reversed. The crack-stopping ability of composites, which results from their inhomogeneity on a fine scale (thefibre/matrix interface) and on a gross scale (laminated structure) makes it difficult in many cases toapply a fracture mechanics approach to fatigue testing and design. The difficulty is most acute withunidirectional composites or laminates pressed from preimpregnated sheets of continuous and non-woven fibres. Stress concentrating effects of notches and holes may be almost completely eliminated bylarge-scale splitting in the 0° and 45° plies and by delaminations between the plies, the net result oftenbeing disintegration of the composite. In laminates containing woven cloth or CSM, however, or inmouldings containing random chopped fibres, the scale of this damage is limited by the structure of thecomposite and cracks and notches will often propagate in a more normal fashion, especially in wideplates. Owen and Bishop (1974) have shown that it is possible to use a fracture-mechanics approach,based on the Paris power law: da = A( ΔK )p ......................................................................................................... 6.6) dN relating crack growth rate, da/dN, to the range of stress intensity factor, ΔK, for some GRP laminates.The exponent, p, in this relationship was 12.75 for CSM/polyester composites and 6.4 for plain-weavefabric GRP, a substantial difference not accounted for by the different tensile strengths of the twomaterials. To overcome the problem of accurately defining crack length, a compliance calibration wasused to determine an equivalent crack length, a procedure somewhat similar to that of using a plastic- orprocess-zone size correction when applying fracture mechanics to other materials. For constant load-range cycling Owen and Bishop constructed log(ΔK) versus N curves which were initially flat but turnedup rapidly at certain critical levels. This instability defined a ‘fatigue life’ when the cyclic ΔK levelreached the value of KC for ordinary monotonic crack growth. Underwood and Kendall (1975) also used a fracture-mechanics approach to study the growth of adamage zone during the fatigue of notched GRP laminates. They obtained much lower values of theParis-law exponent, p, — 2.5 for 0/90 laminates and 4 for (0,±60) laminates — much closer to the valuesnormally obtained for metallic materials. They found that their results were best described by linear plots
chapter six Fatigue e 146of ΔK versus cycles-to-failure which extrapolated back to the monotonic fracture toughness values. Theyobserved that, depending on the type of material, large diffuse damage zones could increase the residualstrength, while small, sharply defined zones would reduce it. Vancon et al (1984) have shown that for the very much simpler case of propagation of delaminationcracks in multi-ply laminates, fracture mechanics methods and the Paris power law are straightforwardlyapplicable.188.8.131.52 Effect of stress system and the stress ratio, R Although interpretation of the results of testscarried under axial loading conditions (ie. 2.5repeated tension, repeated compression, andmixed tension/compression) are perhaps the 2.0 Peak stress, GPamost straightforward to interpret, a good deal of flexuretesting has also been done in other modes, 1.5including shear (torsion) and flexure. Whathappens in any kind of test, however, depends 1.0sensitively on the structure of the composite and tensionmanner in which the applied load develops 0.5stresses within the material. In a unidirectionalrod subjected to torsion, for example, it is the 0matrix and interface, both sources of weakness -1 0 1 2 3 4 5 6 7 8in reinforced plastics, that determine the fatigue LogNfresponse: the fibres play little part (Beaumontand Harris, 1972; Phillips and Scott, 1976). The Figure 6.18. Comparison of stress/loglife data for asituation is similar when a ±45 laminate is tested unidirectional XAS/913 laminate tested in tension and flexurein repeated tension, as we saw earlier. In flexural (Charrière, 1985).tests, the stress distribution varies across thethickness of the sample and it would be expected that the performance of the material in this mode oftesting would be controlled by the maximum tension and compression stresses on the sample faces. Inearly tests on high-stiffness materials (see Beaumont and Harris, 1972, for example) it was oftenobserved that the flexural fatigue behaviour was markedly poorer than that obtained in repeated tension.This was presumably because in some of these tests, especially those conducted on small test pieces,significant levels of interlaminar shear loading could be generated, and the final fatigue failure of thesample was initiated prematurely by interface or matrix damage. In larger samples of more moderncomposites, the flexural fatigue response may be very similar to that obtained in tension, as illustrated inFigure 6.18, a further indication of the fact, mentioned in chapter 4, that compression failures rarely occur in the flexural loading of thin laminates, 2.0 despite their known weakness under direct R= compression loading conditions. 1.5 +0.5 Peak stress, GPa The effects of direct compression loading are 1.0 +0.1 -0.3 best illustrated by the use of stress/loglife curves 0.5 -0.6 at different R ratio, such as the family of curves -1.0 in Figure 6.19. These median-life curves are -1.5 0 plotted in terms of peak stress as a function of logNf and compression stresses are represented -0.5 +10 as negative. Note that an R ratio of 0 represents cycling between 0 and some positive stress level -1.0 -1 0 1 2 3 4 5 6 7 8 (ie. ideal repeated-tension, or T/T, cycling) but it LogNf is usual to retain a small positive load at the bottom of the cycle in order to avoid theFigure 6.19. Median stress/loglife) curves for a [(±45,02)2]S possibility of any overshoot into compression: T800/5245 laminate at various R ratios (Gathercole et al, hence the use of an R ratio of 0.1 to represent1994). The plotted curves are best-fit polynomial curves of T/T cycling. Similarly, an ideal repeated- second or third order.
chapter six Fatigue e 147compression cycle would have an R ratio of ∝, which complicates the mathematical handing of R ratios,so a small negative load is usually retained at the top of a C/C cycle: hence the R ratio of 10 in Figure6.19. An R ratio of –1 represents a fully reversed T/C cycle. It is interesting to note that the median σ/logNf curves for repeated tension (T/T) and repeatedcompression (C/C) extrapolate back to the related monotonic tension and compression strength values,and when the two sets of median-life data are normalized with respect to those strength values there is ahigh degree of correspondence between them. As the compression component of cycling increases (Rincreasingly negative) the stress range, 2σalt , to which the sample is subjected must at first increase, sothat if the data were plotted as stress range versus loglife the data points for R = –0.3 would thenapparently lie above those for R = +0.1. This is a familiar feature of fatigue in fibre composites, and itleads to the notion that some element of compression load in the cycle can apparently improve thefatigue response. It also results in a well-known aspect of composites fatigue, viz. that master diagramsof the constant-life, or Goodman, variety are displaced from the symmetrical location about R = –1 (ie.the alternating-stress axis) (Owen & Morris, 1972; Schütz and Gerharz, 1977; Kim, 1988). It hasrecently been shown (Harris et al, 1997) that the effects of R ratio can be illustrated by presenting thefatigue data on a normalized constant-life diagram by means of the function: a = f (1 − m)u (c + m)v ............................................................................................ 6.7)where a = σalt/σt, m = σm/σt and c = σc/σt(definitions of σalt and σm were given in section 0,and σt and σc are the monotonic tensile and Normalised alternating stress, acompressive strengths, respectively). The stress 0.8function, f, depends on the test material, and inparticular on the value of the ratio σc/σt, and the 0.6exponents u and v, usually quite close to eachother in value, are functions of logNf. Since this is 0.4a bell-shaped function, it is more akin, as a failurecriterion, to the old parabolic Gerber relationship 0.2(1874) than to the more frequently used linearGoodman law (1899). The extreme values of m for 0.03 1.0a = 0 are 1 on the tension side of the ordinate and 4 0.5 m 5 0 0.0 ess, 6 n str–c on the compression side: the mean stress range LogN 7 -1.0 -0.5 d mea alise fis thus (1 + c). The setting up of this parametric No rmform of the constant life curve is in fact a doublenormalisation with respect to the monotonic Figure 6.20. Constant-life curves for a T800/924 CFRPtensile strength of the hybrid material. A family of laminate of [(±45,02)2]S construction (Gathercole et al,curves representing different constant values of 1994).life, plotted as a three-dimensional diagram, is shown in Figure 6.20. There are naturally HTA/913 differences between the shapes of constant- E-glass/913 life curves for different kinds of composite. R = -1.0 0.8 5 -0.3 Figure 6.21, for example, shows curves for Nf = 10 cycles -1.5 0.6 CFRP (HTA/913) and GRP (E-glass/913) +0.1a laminates of identical lay-up and matrix 0.4 +10 resin for a life of 105 cycles. It can be seen that the GRP curve is much more 0.2 asymmetric than that for the carbon composite, and that its maximum, which is 0 -1.0 -0.5 0 0.5 1.0 lower than that for the CFRP, lies to the left m rather than to the right of the alternating- Figure 6.21. Constant-life plots for HTA/913 CFRP and E- stress axis. These differences may all beglass/913 GRP laminates of [(±45,02)2]S construction for a life of 105 cycles (Beheshty et al, 1999).
chapter six Fatigue e 148 ascribed to the difference in the reinforcing fibres. 6.4.4 Damage accumulation and residual strength The progressive damage which occurs in a composite sample during fatigue will affect the mechanical properties of the material to an extent which depends on the composition and lay-up of the composite and on the mode of testing. In a unidirectional, high-modulus CFRP, for example, there may be no significant changes in composite stiffness prior to failure (Beaumont & Harris, 1972). By contrast, in cross-plied (0/90) GRP and CFRP laminates transverse-ply cracking Figure 6.22. X-ray photograph of a 0/90 carbon-fibre/PEEK composite after 8.5 x105 occurs early in the life fatigue cycles in repeated tension at a peak stress of 200MPa (Dickson et al, 1985). of the sample, causing a significant stiffness reduction, perhaps of the order of 10%. Thereafter, for the greater part of the life following this initial deterioration there may be little further change in stiffness (although longitudinal cracks may appear as a result of the lateral constraint imposed by the transverse plies) 800 until close to failure when the elastic modulus falls rapidly (Reifsnider and AE Acoustic emission, events Jamison, 1982: Poursartip and Beaumont, 600 1982). An illustration of the extent of this progressive damage is shown in the x-ray photograph of Figure 6.22, showing both Youngs modulus, GPa 400 80 transverse and longitudinal cracking in a 0/90 laminate of XAS-carbon/PEEK after E cycling in repeated tension. We note that 200 70 even the use of a high-toughness matrix like PEEK does not eliminate this 0 60 cracking. Boniface and Ogin (1989) have 0 1 2 3 4 5 shown that this kind of transverse-crack Log N growth can be satisfactorily modelled by the Paris relationship (equation 6.6) with Figure 6.23. Reduction in stiffness and accompanying acoustic exponents, p, between 2 and 6. When the emission in the early stages of fatigue cycling of a reinforcement is in the form of a woven [(±45,02)2]S XAS/914 CFRP laminate at a stress ratio, R = 0.1 (Chen & Harris, 1993) fabric, the occurrence of transverse-ply cracking is hindered, and the changes in stiffness accompanying cycling are less marked. And even in laminates containing only ±45 and 0° plies, there 1.2 may be no fall in stiffness until near to failure, as strength illustrated by some typical experimental results for a 1.0 scatterbandResidual stress, GPa [(±45,02)2]S CFRP laminate shown in Figure 6.23. 0.8 The microstructural damage events which lead to these changes are readily monitored by means of 0.6 Peak stress, such methods as acoustic emission monitoring (Fuwa MPa et al, 1975; Chen and Harris, 1993), as shown in this 0.4 200 figure. 300 0.2 400 S/logNf curve We referred earlier to the ‘wear-out’ model of 500 0 fatigue damage. It is a matter of common experience -1 0 1 2 3 4 5 6 7 8 that both the rigidities and strengths of composite LogNf materials are affected adversely by repeated loading as damage accumulates in the material. In someFigure 6.24. Residual strength curves for samples of 0/90GRP laminate subjected to fatigue cycling at an R ratio of circumstances, both strength and stiffness may 0.1 and various stress levels (Adam et al, 1986).
chapter six Fatigue e 149initially increase slightly as the fibres in off-axis plies or slightly misaligned fibres in 0° plies re-orientthemselves in the visco-elastic matrix under the influence of tensile loads, but the dominating effect isthat due to the accumulating damage in the material. The deterioration during cycling usually dependson the stress as shown in Figure 6.24: the higher the peak stress, the earlier the deterioration starts. Inaccordance with the wear-out model, the end-point of each residual-strength curve lies on the normalσ/logNf curve for the material. In their work on the comparable group of CFRP, GRP and KFRP cross-plied laminates alreadyreferred to, Adam et al (1986) found that the shapes of the residual strength curves for all three materialswere similar and could be represented by an interaction curve of the form: ta + sb = 1............................................................................................................... 6.8)where t is a function of the number of cycles, n, sustained at a given stress, σmax, for which the expectedfatigue life is Nf : log n − α t= ...................................................................................................... 6.9) log Nf − αThe constant α is equal to log(0.5) and simply accounts for the fact the normal strength of the materialcorresponds to the lower limit of the cycles scale at ½ cycle. The normalized residual strength ratio, s, isdefined as: σ R − σ max s= ....................................................................................................6.10) σ t − σ maxwhere σt is again the monotonic tensile strength of the material and σR is the residual strength aftercycling at a peak fatigue stress σmax. The exponents a and b are materials- and environment-dependentparameters which may have physical significance although they must be obtained by curve fitting. Forrate-sensitive materials like GRP and KFRP, σt and σR must be determined at the same loading rate asthat used for the fatigue cycling. The loss in strength due to cycling, (σt – σR), may then be regarded as adamage function: 1 Δ = 1 − s = (1 − t a ) b …………............ 6.11) 1.0 The shape of the curve can, in principle, vary from 0.8a linear form (with a = b = 1), through a circular Stress ratio, squadrant for powers of two, to an extremely angular ta + sb = 1variation for very high powers. Since both the gradual 0.6wear-out and ‘sudden-death’ type of behaviour can be a baccommodated within a single general model, a CFRP (1.8 23.1) 0.4 KFRP (1.8 5.2)treatment of this kind has advantages over non- GRP (1.5 4.8)normalising procedures. Despite apparent mechanistic 0.2dissimilarities in the fatigue behaviour of the threetypes of composite studied in this work, the residualstrength results suggested that a common mechanism 0 0 0.2 0.4 0.6 0.8 1.0of damage accumulation led to final failure since the Cycle ratio, tdamage law of equation 6.8, with suitably chosenvalues of a and b, fits all of the data for all three Figure 6.25. Normalized residual strength curves formaterials, as shown in Figure 6.25. Having established three comparable 0/90 laminates consisting of HTSthe values of a and b for a given material, the residual carbon, Kevlar-49 and E-glass fibres in a commonstrength for any fatigue stress can then be evaluated: epoxy resin (Adam et al, 1986). The values of the exponents for the fitted curves are shown in brackets.
chapter six Fatigue e 150 σR = (σ t − σ max )(1 − ta ) + σ max …..……........... 6.12) 1 b 1.8 S/logNf curve 1.6 R = +0.1 or, alternatively, the remaining life, (Nf – n) can be Peak stress, GPa 1.4 estimated. It seems unlikely that a single mathematical model could cope with the whole 1.2 range of composite types and lay-ups available, and 1.0 although this model requires validation for each system of interest — materials, lay-ups, stress 0.8 1 2 3 4 5 systems — this validation would be reasonably 0.6 lines showing onset of specific damage mechanisms economical of test time and material, given that the interaction curve could be deduced from relatively 0.4 -1 0 1 2 3 4 5 6 7 8 few data. LogN The foregoing discussion suggests that the Figure 6.26. Schematic damage mechanism maps for a changes in mechanical properties of fatigued T800/5245 [(±45,02)2]S CFRP laminate tested in repeated composites may be caused by a single damage tension fatigue (R = 0.1) (Chen & Harris, 1993). mechanism, but this is unlikely to be the case. Key: 1 = fibre fracture in 0° plies; 2 = matrix cracks in Detailed studies of the damage processes occurring outer 45° plies; 3 = fibre drop-out; 4 = matrix cracks in inner 45° plies; 5 = delamination at 0/45 interfaces. during cycling of CFRP materials (Chen & Harris, 1993) show that sequences of damage occur throughout life, and these sequences can be mapped, as shown in Figure 6.26, on a conventional σ/logNf diagram. The supposition is that each damage- mechanism curve, including the final failure curve (σ/logNf curve), represents part of an S-shaped decay curve of the kind postulated by Talreja (1981), although in the experimental window we see only a part of each curve. It is also supposed that at sufficiently low stresses, corresponding to the notional endurance limit, all curves will flatten out and converge at large numbers of cycles. One of the problems of developing damage-growth models for life- 6 prediction purposes (see section 0) is that the damage development laws are likely to be 5 different for each specific damage mechanism and will be structure-dependent, as illustrated by the Crack density, mm -1 4 inner 45° plies results of crack-density measurements shown in Figure 6.27. The measurements were made on a 3 T800/5245 CFRP laminate of [(±45,02)2]S lay-up, outer 45° plies 2 and it can be seen that the development of cracks in the outer (unconstrained) and inner 1 (constrained) 45° plies proceeds at quite different rates and that the saturation levels for the two 0 types of crack are also quite different 0 20 40 60 80 100 Percentage of life, % Howe & Owen (1972) studied the accumulation of damage during cyclic loading Figure 6.27. Density of cracks in 45° plies in a [(±45,02)2]S with the object of obtaining useful workingT800/5245 CFRP laminate during cycling at a peak stress of 1GPa and an R ratio of 0.1 (Grimm, 1996). relationships of the Miner-rule type, that might be used in design. They used optical microscopy to study the development of debonding sites and resin cracks in CSM/polyester composites. They suggested that although debonding did not itself cause reductions in strength it served to initiate resin cracks which did weaken the material. For resin cracking they proposed a non-linear damage law, independent of stress level, which gives the damage, Δ, as ⎡ ⎛ n⎞ ⎛ n⎞ ⎤ 2 Δ= ∑ ⎢ ⎝ N⎠ ⎝ N⎠ A ⎜ ⎟ + B⎜ ⎟ ⎥ ...........................................................................................6.13) ⎢ ⎣ ⎥ ⎦ where n is the number of cycles sustained by the composite at a stress level which would normally cause failure after N cycles, and A and B are constants. B is negative and Δ is equal to unity at failure. They
chapter six Fatigue e 151used a modification of this law to predict residual strength after cycling of CSM/polyester laminates, thisstrength being dependent upon the growth of resin cracks.6.4.5 Fatigue under conditions of variable stress: block loading Although studies of damage accumulation processes have been correlated moderately satisfactorilywith fatigue testing régimes involving a limited number of stress levels, it is even more necessary tomake good correlations when variable-amplitude or flight-loading sequences are used for practicaldesign purposes. Shütz and Gerharz (1977) have reported results of life-prediction experiments with HT-carbon/epoxy laminates of 0.4Vf and (02,±45,02,±45,90)S construction. They used flight-spectrum teststypical of the conditions at an aircraft wing root, and they also obtained conventional fatigue data at arange of different R values from which they made Miner-rule life predictions at two mean stress levelsfor comparison with the variable-amplitude test results. The linear-damage rule predicted lives up tothree times those actually measured — far too wide a margin for comfortable design work — and theyconcluded that this was probably due to damage contributed by low-load cycles in the compressiveregion which is not accounted for in the Miner estimate. In some more recent experiments, Adam et al (1994) carried out some simple four-unit block loadingsequences on samples of a [(±45,02)2]s T800/5245 CFRP laminate. They first carried out a series of all-tension (TTTT) experiments for which the numbers of cycles at each of the stress levels were chosen sothat the block should account for 20% of the lifetime of the specimen if Miners rule were to be obeyed.Each unit in the sequence should therefore have contributed 5% of the total damage to failure. Since thecontribution to the total life of the specimen by each of the units within the block programme is 5% ofthe median life, each block of four units therefore had a notional Miner number, M, of 0.2, ie. n1 n2 n3 n4 + + + = M = 0.2 ..................................................6.14) m(N1 ) m(N2 ) m(N3 ) m(N4 )where ni is the number of cycles in the unit and m(Ni) is the median life at that particular stress level. IfMiners rule is followed, the block should repeat itself 5 times before failure occurs. Following the firstall-tension (TTTT) series, the next stage was to introduce a compressive element into the loadingsequence so as to construct TTCT blocks. It is logical to assume that if the life data for a given constant stress level are randomly distributedthen the Miner sum, M, defined by equation 6.14, should be similarly distributed, regardless of whetherthe mean value or median value of M is equal to unity. The Miner sums from all six groups for eachsequence were therefore pooled and analysed in terms of the Weibull model, discussed earlier, whichshowed that there was a marked difference between the mean values of the Miner number for the twogroups of tests, 1.1 for the TTTT sequence, and 0.36 for the TTCT sequence. To all intents andpurposes, then, the Miner rule is valid for all-tension block-loading sequences for this material, and theeffect of introducing a single compression block into an otherwise all-tension group was clearly highlydamaging, Miners law no longer being obeyed and by a substantial margin, the mean life having beenreduced by some 60% as a result of the substitution. Similarly, the substitution of a repeated tension unitinto an all-compression sequence also resulted in a marked reduction in the mean Miner sum. It thereforeappears to be the stress reversal as such which is damaging rather than the actual sequence or the actualstress levels. This has serious consequences for designers since most practical cycling régimes, are likelyto include stress excursions into both tension and compression. This is certainly true of the familiar‘FALSTAFF’ and other load-spectrum sequences used in the laboratory to represent actual lifeconditions for aircraft components.6.4.6 Life prediction There have been many attempts to develop life-prediction methods for reinforced-plastics, but thecomplexity of the response of these materials to stress makes it very difficult to develop universallyapplicable models. Some of the established methods are based on structural models, while others are lessspecific. Most of the structurally based procedures depend on modelling the degradation of material
chapter six Fatigue e 152properties as a consequence of microstructural damage (eg. Lee et al, 1989; Hwang and Han, 1989) andmany are based on the concept of a ‘characteristic damage state’ (CDS) developed by Reifsnider and co-workers (see, for example, Reifsnider et al, 1979). Many of these methods involve both statistical andlaminate-theory analyses and give reasonably good predictions. But many require a good deal of priordata determination and are structure-specific. It is beyond the scope of this book to treat this subject inany detail, but we shall refer to two recent approaches which appear to have some generality. The first is based on the constant-life analysis referred to in section 0. Equation 6.7 is a parametricdescription of the stress/R-ratio/life ‘environment’ for composite fatigue which appears to be valid for awide variety of material types and structures (Harris et al, 1997). In this equation: a = f (1 − m)u (c + m)vof which the terms have already been defined, the shape and location of the fatigue ‘surface’ aredetermined by four parameters, the compression and tensile strengths (which define c), the exponents uand v, and the factor f. Since c is a material property and the alternating and mean components of stress(a,m) are normalized with respect to the tensile strength, u, v and f must be obtained by a parametricanalysis of fatigue data sets. The exponents u and v (both functions of fatigue life) are usually verysimilar in value, unless the constant-life curves are very asymmetric, and for a wide range of CFRPmaterials are close to 2. And the parameter f is an inverse-power function of the ratio of the compressionstrength to the tensile strength, ie. of c, of the form (Beheshty and Harris, 1999): f = Ac − p .............................................................................................................6.15)where A and p are functions of life. The (a,m) data may be obtained from median-life fatigue results, or,by pooling fatigue data sets as described earlier to obtain valid statistical information, they may bechosen to represent any required failure probability. If no information other than the tensile andcompression strengths is available for a given composite, a preliminary attempt can still be made topredict stress/life curves on the basis of accumulated data for other related materials. A limited fatigue-test programme can then be carried out to provide stress/life data at three or four stresses at, say, three Rratios and the predictions of the model will become gradually more refined and reliable. The virtue ofthis method is that it can provide designers with useful design information at very early stages in thedevelopment of new materials, before detailed descriptions of the fatigue response have becomeavailable, as shown by Harris et al (1997). While this may well be all that is necessary for non-criticalapplications, in the case of critical applications such as aircraft structures it would of course always benecessary to confirm predictions from any model before a design could be validated. The proceduredescribed above requires data specific to a given type of reinforcing fibre. It appears from these resultsthat stress/life curves for materials damaged by low-velocity impact can also be predicted from data forthe undamaged laminate provided the changes in the tensile and compression strengths caused by theimpact damage are known (Beheshty & Harris, 1999). Although a high level of understanding of the mechanisms of fatigue damage accumulation and theeffects of this damage on the ability of a material or structure to sustain the service loads for which itwas originally designed is of importance to materials developers, it must be said that the designerhimself has little interest in the actual physical mechanisms of degradation. What he needs is simply away of analysing available data to predict the likelihood of failure under a specified set of conditions. Inrecent years artificial neural networks (ANNs) have emerged as a new branch of computing suitable forapplications in a wide range of fields. They offer a means of dealing with many multi-variate propertiesfor which there is no exact analytical model and fatigue seems to be the kind of materials property that issuitable for ANN analysis. Neural networks provide a compact way of coping with the large amounts ofcharacterization data generated in the study of a multi-variate dependent property such as fatigue. Theyalso provide a very simple means of assessing the likely outcome of the application of a specified set ofconditions, precisely what is required by a designer who needs to make safe use of complex fatigue datafor complex materials like composites.
chapter six Fatigue e 153 An ANN is a type of computer programme that can be ‘taught’ to emulate the relationships betweensets of input data and corresponding output data and the results of a characterization programme cantherefore be ‘learnt’ by the network and patterns in the data can be established. Once the network hasbeen ‘trained’ it can be used to predict the outcome of a particular set of input parameters. Unlike othertypes of analysis there is no need to know the actual relationship between inputs and outputs and thequestion of determining physical laws and relationships need not be addressed. The network simplycompares patterns of inputs with those it has been ‘taught’ and provides an output which takes fullaccount of its accumulated ‘experience’. It is a highly developed interpolation system and its outputsprovide a good indication of the certainty of an outcome, a property which may be a useful indicator ofwhere additional experimental information is required. The ability to signal the ‘certainty’ of theoutcome is particularly important for materials like composites for which the fatigue response is oftenhighly variable even when the monotonic strength properties of the same material may be quite closelydefinable. As we have seen, fatigue in composites involves many variables, including a variety of materialscharacteristics (eg. fibre/resin mix, lay-up, moisture content) as well as the specific fatigue variables(mean and alternating stresses, variable stress characteristics, etc.), all of which may be treated as inputsto an ANN. One of the first questions that arises relates to the issue of what constitutes ‘failure’. It ismore likely to be the minimum life in a data set than the medianor mean life, and it is important to decide whether the inputshould simply be the lowest value of life recorded in a data set,or some value estimated from the application of extreme-valuetheory (Castillo, 1988), as discussed earlier. Some recent resultsobtained by Lee et al (1995, 1999) suggest that the ANNapproach may provide a useful method of fatigue data analysisand life prediction.6.5 FATIGUE OF METAL-MATRIX COMPOSITES Much early work on MMCs related to metals reinforced with residualfibre stresshigh-strength metallic wires like tungsten and cold-drawn steel.These were essentially model composites, and were rapidly residual matrix stresssupplanted as experimental materials by modern aluminium andtitanium alloys mostly reinforced with boron, carbon and SiCfibres of various kinds. Nevertheless, some of the early results Figure 6.28. Schematic illustration of theprovide useful insights into the fatigue response of this kind of first tensile stress/strain cycle of a metal-material. It will be appreciated that in a metal/metal system, matrix composite loaded beyond the matrix yield stress, ie. into the elastic-plasticboth components will be susceptible to conventional fatigue range.failure, whereas in a metal/ceramic system, only the matrix willbe susceptible. However, since metallic fatigue is essentially a brittle-failure process, the difference maynot be great. When a composite with a low-yield-stress matrix is cycled in repeated tension, the matrix will besubjected to a more complex stress régime than the level of external applied stress would suggest.During the first cycle, shown schematically in Figure 6.28, in the régime where both fibres and matrixdeform elastically, the initial elastic modulus of the composite, usually designated EI, is given by thenormal rule of mixtures. At the yield point of the matrix, at the strain εmy, the composite deforms elasto-plastically with a somewhat lower stiffness (a constant EII if we assume linear work-hardening behaviourin the matrix) while the fibres continue in their elastic state and the matrix deforms irreversibly. Onreversing the sense of the applied deformation, the composite describes a hysteresis loop, as shown,while the matrix and fibres unload elastically. The matrix reaches a zero-stress state at a finite level ofstrain, and the stresses in the constituents will reach an equilibrium state at the point X, the fibres beingin tension and the matrix in compression, as shown, and the composite is left with a permanent strain.Further cycling in repeated tension will result in entirely elastic loading and unloading of both fibres andmatrix from this new stress state (Dvorak and Tarn, 1975). However, if the stress cycle is fully reversed
chapter six Fatigue e 154(ie. for R = –1), with the matrix stress exceeding the matrix yield stress in each direction, energy willcontinue to be dissipated in the material until the plastic strain range has been reduced as a result ofcyclic work-hardening. The effect of the elasto-plastic stress cycle in the matrix may be substantial andcould lead to over-ageing in a peak-aged aluminium matrix, for example, perhaps resulting in more rapidwork-hardening and crack growth than would occur in purely elastic cycling. Thus, although it might atfirst sight be expected that in a metal/metal system the fatigue response should be predictable by amixtures-rule model for the fatigue stress for a given number of cycles, for example: σc(Nf) = σf(Nf)Vf + σm(Nf)(1 – Vf)..........................................................................6.16)the low-cycle fatigue of the matrix may prevent this. McGuire and Harris (1974) studied the fatigueresponse of unidirectional composites consisting of a tungsten-wire-reinforced aluminium alloy(Al/4%Cu) produced by vacuum diffusion bonding, and their results show the effects of heat treating the matrix alloy to peak hardness or over-ageing it to 10 produce a brittle matrix state. Their σ/logNf curves showed that increasing Vf increased the Normalised stress range fatigue resistance of the composite, and this increase in fatigue resistance seemed to be a direct result of the increased strength of the 1 composite since if their stress/life data for each Al alloy matrix composite composition are normalized by Vf = 0.07 dividing the cyclic stress-range values by the 0.12 appropriate sample tensile strength the points for 0.24 all of the composites and the unreinforced matrix fall on a single line which appears to obey 0.1 Basquin’s Law very well (Figure 6.29). Both 1 2 3 4 5 6 7 matrix and fibres exhibit distinctive signs of LogNf fatigue failure, as shown in Figure 6.2, in clear contrast with the normal tensile fracture mode of Figure 6.29. Normalized stress/loglife data for an Al/4%Cu both constituents. The composites with the alloy and three composites containing tungsten wirereinforcement (McGuire and Harris (1974). The data are for higher cyclic work-hardening rate (peak aged)reversed axial tension/compression cycling (R = -1) and the possessed the better fatigue resistance, but the stress ranges for the data points are normalized with fatigue stresses (for Nf = 107 cycles) for both respect to the tensile strength of each material. heat-treatment conditions fell well below the mixture-rule prediction of equation 6.16. In othermetal/metal systems including steel/silver and tungsten/copper (Courtney & Wulff, 1966) andtungsten/silver (Morris & Steigerwald, 1967) it was shown that the fatigue ratio actually decreased withincreasing fibre content. 1.0 McGuire and Harris also carried out low-cyclefatigue experiments at constant total strain range, and Power-law exponent, -qin these tests the composites showed work-hardening 0.8and work-softening characteristics that were affected normal range forby matrix plastic properties. The observed changes did 0.6 metallic materialsnot indicate any difference in the nature ofdeformation, however, and the exponent, q, in the 0.4Manson-Coffin law relating plastic strain range to thenumber of cycles to failure: 0.2 peak-aged matrix over-aged matrix Δε p N q = constant ………………… 6.17) f 0 0 0.05 0.10 0.15 0.20 0.25 Fibre volume fraction, Vffell smoothly with increasing Vf from valuescharacteristic of conventional metallic materials, of theorder of 0.5, to something like half that value at Vf ≈ Figure 6.30. Variationfor the Coffin-Manson exponent, q, with fibre content of W/Al-Cu composites in low-0.2, as shown in Figure 6.30. This indicates that the cycle fatigue (McGuire & Harris, 1974).
chapter six Fatigue e 155improvement in fatigue properties results from the effect of 100the reinforcing fibres in limiting the composite plastic strain matrix n=5range of the matrix. Vf = 0.07 Vf = 0.12 The matrix plastic strain range has been identified by Vf = 0.22 da/dN, m/cycleseveral workers as being the key parameter determining thefatigue characteristics not only of metal/metal systems, butalso of metals reinforced with brittle ceramic fibres like 10carbon and silica. The work of Baker and co-workers, forexample (Baker, 1966; Baker et al, 1966), suggested that inboth types of system, fatigue failure occurred mainly by thegrowth of matrix or interface cracks, linking via fracturedfibres in the case of brittle-fibre systems, and that the maineffect of the reinforcing fibres in improving fatigue 1resistance was to reduce the matrix plastic-strain range. 10 20 50 100Courtney & Wulff (1966) invoked a fatigue model due to Stress intensity, Δσ.√a, MPa.√mOrowan (1939) which also ascribed the fatigue failure (ofW/Cu and steel/Ag) to matrix cracking resulting from cyclic Figure 6.31. Paris law plots for fatigue crackwork-hardening as a result of the elastic-plastic deformation growth in W/Al-Cu composites (Harris et al, 1976). The average slope of the curves isdescribed above. Lee and Harris (1974), working with about 5.tungsten/copper composites, commented on an associatedeffect, recalling the work of Kelly & Lilholt (1969) who showed that during the deformation of anMMC, the stress levels in the matrix were often considerably greater than would be predicted by the ruleof mixtures, probably because of the highly perturbed and constrained state of stress in the matrixadjacent to the fibres. The difference between the resulting enhanced matrix flow stress and theunconstrained matrix yield stress increases as Vf increases and as the fibre diameter decreases. The resultduring fatigue is to reduce both the matrix ductility and the matrix plastic strain-range, and therebyincrease the composite life. By contrast with some of the other results referred to above, they showedpositive deviations from the mixtures rule between 4 and 20%, the greater deviations being associatedwith finer reinforcing filaments. Leddet and Bunsell (1979), studying the fatigue of 100 boron/aluminium-alloy composites in rotating Stress-intensity factor, KQ or ΔK KQ bending, have shown that fibre/matrix interactions 80 caused by heat treatment change the mechanisms which lead to progressive deterioration during 60 ΔK cycling. They suggested that with a soft matrix the predominant damage mechanism is fatigue cracking 40 cyclic: overaged in the matrix parallel to the fibres and originating cyclic: peak aged 20 tension: overaged from initial fibre fractures. In a slightly harder matrix tension: peak aged cracks propagate through the matrix and around the 0 fibres without causing fibre failure, but in a highly 0 0.1 0.2 0.3 0.4 work-hardening matrix successive fibre failure can Fibre volume fraction, Vf occur. The fatigue behaviour of B/Al composites depends on the intrinsic matrix mechanical properties Figure 6.32. Variation of effective stress intensity factor with fibre content for monotonic and cyclic but is controlled by the fibre strength. loading conditions (McGuire and Harris, 1974 and 1976). By contrast with reinforced plastics, crack growth from pre-existing notches often occurs normally incomposites MMCs. Harris et al (1977) showed this to be the case with composites of Vf up to 0.22, butin samples with 37 vol.% of reinforcement the closely-spaced fibres led to the development of a highlylocalized plastic zone parallel with the fibres that inhibited planar crack growth and encouraged the samekind of longitudinal splitting that occurs in unidirectional reinforced plastics. For their W/Al materials,the crack growth rate, da/dN, correlated well with a stress-intensity-range parameter, similar to ΔK, ofthe form σ√a, following the Paris Law (equation 6.6), as illustrated in Figure 6.31. The slopes of the
chapter six Fatigue e 156 curves, p, for different composites were identical with Log(crack growth rate), da/dN in m/cycle 10 that for the unreinforced matrix, about 5. These p -6 5 results again indicate that fatigue response was determined simply by the strength and work- 0 plain copper 0 Vf 0.05 0.10 hardening ability of the matrix, without significant -7 differences in the controlling damage mechanism. It is Cu/6%W clear that the matrix alloy work-hardens sufficiently to cause fibre failure, but by a conventional fatigue Cu/9%Cu mechanism rather than brittle (tensile) failure. Similar -8 effects of work-hardening behaviour would not necessarily have occurred had the fibres been non- Paris law slope, p metallic. A comparison between the results shown in -9 Figure 6.31 and the stress-intensity factor 0.75 1.00 1.25 1.50 LogΔK, ΔK in MPa.√m measurements for crack propagation in the same materials under monotonic loading shows the extent Figure 6.33. Paris-law plots for fatigue crack to which cyclic loading conditions are more damagingpropagation in composites consisting of short, aligned (Figure 6.32).tungsten fibres in copper (Harris and Ramani, 1975). Crack propagation in some unidirectional short- fibre Cu/W composites shows slightly different features (Figure 6.33). In this case, the slope for the matrix is much higher than that for the Al/4%Cu alloy in Figure 6.31, about 10 instead of 5, and the intrinsic fatigue resistance of the copper is thus much lower. Addition of a small volume fraction of tungsten filaments nevertheless reduces the slope to the same level as that for the Al/W composites. The curious feature of this graph, however, is that for initial cracks below some threshold level, the short fibres actually cause the growing cracks to slow down as their lengths increase before conventional Paris-law behaviour is established. Similar results have been reported by Bowen (1993) and Barney et al (1993) for titanium-alloy MMCs and by Pegoretti & Ricco (1999) for composites of polypropylene reinforced with short glass fibres. Bowen suggests an approach to the prediction of this crack-arrest mechanism. 6.6 FATIGUE OF CERAMIC-MATRIX COMPOSITES Although it has traditionally been considered that ceramics do not suffer from fatigue, this view may have arisen partly because of the difficulty of carrying out fatigue tests on brittle materials and partly because fatigue phenomena may easily be obscured by the high level of variability associated with brittle failure. Certainly, fatigue crack growth phenomena have been observed in a variety of 1.1 brittle materials and a range of mechanisms, Normalised modulus, E/Eo including microcracking, small-scale plasticity 1.0 unidirectional resulting from dislocation movements and stress- 0.9 peak stress induced phase transformations, have been (% of invoked to explain the observations (Suresh et al, 0.8 failure stress) 1988). Nevertheless, although fine-scale effects 0.7 (0,90)3S 57% such as these will certainly occur in ceramic- matrix composites, especially those reinforced 0.6 with particulate fillers or fine whiskers, the 0.5 35% results of fatigue in continuous-fibre CMCs are on a much larger scale and are due largely to 0.4 1 10 100 1000 cracking. Ritchie et al (1993) have suggested that Cycle number, N cyclic fatigue in low-ductility materials such as these is conceptually distinct from metallic Figure 6.34. Effect of repeated